#------------------------------------------------------------------------------
#$Date: 2017-02-07 17:13:06 +0200 (Tue, 07 Feb 2017) $
#$Revision: 191892 $
#$URL: file:///home/coder/svn-repositories/cod/cif/2/10/35/2103541.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2103541
loop_
_publ_author_name
'Pavlovska, A.'
'Werner, S.'
'Maximov, B.'
'Mill, B.'
_publ_section_title
;
 Pressure-induced phase transitions of piezoelectric single crystals
 from the langasite family: La₃Nb~0.5~Ga~5.5~O₁₄ and
 La₃Ta~0.5~Ga~5.5~O₁₄
;
_journal_issue                   6
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              939
_journal_page_last               947
_journal_paper_doi               10.1107/S0108768102010273
_journal_volume                  58
_journal_year                    2002
_chemical_formula_sum            'Ga5.5 La3 Nb0.5 O14'
_chemical_formula_weight         1070.65
_chemical_name_systematic        ?
_space_group_IT_number           150
_symmetry_space_group_name_Hall  'P 3 2"'
_symmetry_space_group_name_H-M   'P 3 2 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            1
_cell_length_a                   8.069
_cell_length_b                   8.069
_cell_length_c                   5.062
_cell_measurement_temperature    293(2)
_cell_volume                     285.4
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_pressure         7.8E+6
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.808
_diffrn_measured_fraction_theta_max 0.808
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71070
_diffrn_reflns_av_R_equivalents  0.0626
_diffrn_reflns_av_sigmaI/netI    0.0406
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_k_min       -10
_diffrn_reflns_limit_l_max       6
_diffrn_reflns_limit_l_min       -6
_diffrn_reflns_number            1553
_diffrn_reflns_theta_full        27.89
_diffrn_reflns_theta_max         27.89
_diffrn_reflns_theta_min         4.97
_exptl_absorpt_coefficient_mu    24.287
_exptl_crystal_density_diffrn    6.229
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             474
_refine_diff_density_max         1.479
_refine_diff_density_min         -1.854
_refine_diff_density_rms         0.455
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.06(11)
_refine_ls_extinction_coef       0.166(17)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.028
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     39
_refine_ls_number_reflns         400
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.028
_refine_ls_R_factor_all          0.0446
_refine_ls_R_factor_gt           0.0446
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1000P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1081
_refine_ls_wR_factor_ref         0.1081
_reflns_number_gt                400
_reflns_number_total             400
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            sn0021-7.8cad4.cif
_cod_data_source_block           7.8cad4
_cod_depositor_comments
;
The _diffrn_ambient_pressure was taken from the original data block
header, after comparison with the paper text and supplementary
material.

Saulius Gra\<zulis
;
_cod_original_formula_sum        'Ga5.50 La3 Nb0.50 O14'
_cod_database_code               2103541
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'y, x, -z'
'-y, x-y, z'
'-x+y, -x, z'
'-x, -x+y, -z'
'x-y, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
La1 La 0.42902(13) 0.0000 0.0000 0.0237(5) Uani 1 2 d S
Ga1 Ga 0.0000 0.0000 0.0000 0.0249(8) Uani 0.50 6 d SP
Nb Nb 0.0000 0.0000 0.0000 0.0249(8) Uani 0.50 6 d SP
Ga2 Ga 0.3333 0.6667 0.5294(6) 0.0230(7) Uani 1 3 d S
Ga3 Ga 0.7657(3) 0.0000 0.5000 0.0256(6) Uani 1 2 d S
O1 O 0.3333 -0.3333 0.173(4) 0.026(4) Uani 1 3 d S
O2 O 0.4535(17) 0.3071(19) 0.317(3) 0.039(3) Uani 1 1 d .
O3 O 0.7830(16) -0.1449(14) 0.243(3) 0.035(3) Uani 1 1 d .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
La La -0.2871 2.4523 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Nb Nb -2.0727 0.6215 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ga Ga 0.2307 1.6083 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O3 La1 O3 67.2(6) 5_665 3_545
O3 La1 O2 140.5(4) 5_665 3_655
O3 La1 O2 106.0(5) 3_545 3_655
O3 La1 O2 106.0(5) 5_665 5_655
O3 La1 O2 140.5(4) 3_545 5_655
O2 La1 O2 102.0(6) 3_655 5_655
O3 La1 O1 123.6(3) 5_665 .
O3 La1 O1 79.6(3) 3_545 .
O2 La1 O1 90.9(4) 3_655 .
O2 La1 O1 72.7(5) 5_655 .
O3 La1 O1 79.6(3) 5_665 2_655
O3 La1 O1 123.6(3) 3_545 2_655
O2 La1 O1 72.7(5) 3_655 2_655
O2 La1 O1 90.9(4) 5_655 2_655
O1 La1 O1 154.08(8) . 2_655
O3 La1 O2 64.5(4) 5_665 6
O3 La1 O2 80.1(4) 3_545 6
O2 La1 O2 154.9(2) 3_655 6
O2 La1 O2 63.3(5) 5_655 6
O1 La1 O2 65.9(5) . 6
O1 La1 O2 124.8(5) 2_655 6
O3 La1 O2 80.1(4) 5_665 .
O3 La1 O2 64.5(4) 3_545 .
O2 La1 O2 63.3(5) 3_655 .
O2 La1 O2 154.9(2) 5_655 .
O1 La1 O2 124.8(5) . .
O1 La1 O2 65.9(5) 2_655 .
O2 La1 O2 137.5(5) 6 .
O3 La1 Ga2 111.0(3) 5_665 2_556
O3 La1 Ga2 85.7(3) 3_545 2_556
O2 La1 Ga2 31.1(3) 3_655 2_556
O2 La1 Ga2 130.0(3) 5_655 2_556
O1 La1 Ga2 110.4(4) . 2_556
O1 La1 Ga2 64.9(4) 2_655 2_556
O2 La1 Ga2 165.7(3) 6 2_556
O2 La1 Ga2 32.2(2) . 2_556
O3 La1 Ga2 85.7(3) 5_665 1_544
O3 La1 Ga2 111.0(3) 3_545 1_544
O2 La1 Ga2 130.0(3) 3_655 1_544
O2 La1 Ga2 31.1(3) 5_655 1_544
O1 La1 Ga2 64.9(4) . 1_544
O1 La1 Ga2 110.4(4) 2_655 1_544
O2 La1 Ga2 32.2(2) 6 1_544
O2 La1 Ga2 165.7(3) . 1_544
Ga2 La1 Ga2 160.49(4) 2_556 1_544
O3 La1 Ga1 33.6(3) 5_665 .
O3 La1 Ga1 33.6(3) 3_545 .
O2 La1 Ga1 129.0(3) 3_655 .
O2 La1 Ga1 129.0(3) 5_655 .
O1 La1 Ga1 102.96(4) . .
O1 La1 Ga1 102.96(4) 2_655 .
O2 La1 Ga1 68.7(2) 6 .
O2 La1 Ga1 68.7(2) . .
Ga2 La1 Ga1 99.754(19) 2_556 .
Ga2 La1 Ga1 99.755(19) 1_544 .
O3 La1 Nb 33.6(3) 5_665 .
O3 La1 Nb 33.6(3) 3_545 .
O2 La1 Nb 129.0(3) 3_655 .
O2 La1 Nb 129.0(3) 5_655 .
O1 La1 Nb 102.96(4) . .
O1 La1 Nb 102.96(4) 2_655 .
O2 La1 Nb 68.7(2) 6 .
O2 La1 Nb 68.7(2) . .
Ga2 La1 Nb 99.754(19) 2_556 .
Ga2 La1 Nb 99.755(19) 1_544 .
Ga1 La1 Nb 0.0 . .
O3 Ga1 O3 84.7(6) 4_665 6_455
O3 Ga1 O3 85.2(5) 4_665 1_455
O3 Ga1 O3 107.6(8) 6_455 1_455
O3 Ga1 O3 107.6(8) 4_665 5_665
O3 Ga1 O3 85.2(5) 6_455 5_665
O3 Ga1 O3 162.9(7) 1_455 5_665
O3 Ga1 O3 162.9(7) 4_665 2_545
O3 Ga1 O3 85.2(5) 6_455 2_545
O3 Ga1 O3 84.7(6) 1_455 2_545
O3 Ga1 O3 85.2(5) 5_665 2_545
O3 Ga1 O3 85.2(5) 4_665 3_545
O3 Ga1 O3 162.9(7) 6_455 3_545
O3 Ga1 O3 85.2(5) 1_455 3_545
O3 Ga1 O3 84.7(6) 5_665 3_545
O3 Ga1 O3 107.6(8) 2_545 3_545
O3 Ga1 La1 42.4(3) 4_665 2
O3 Ga1 La1 42.4(3) 6_455 2
O3 Ga1 La1 98.5(3) 1_455 2
O3 Ga1 La1 98.5(3) 5_665 2
O3 Ga1 La1 126.2(4) 2_545 2
O3 Ga1 La1 126.2(4) 3_545 2
O3 Ga1 La1 98.5(3) 4_665 .
O3 Ga1 La1 126.2(4) 6_455 .
O3 Ga1 La1 126.2(4) 1_455 .
O3 Ga1 La1 42.4(3) 5_665 .
O3 Ga1 La1 98.5(3) 2_545 .
O3 Ga1 La1 42.4(3) 3_545 .
La1 Ga1 La1 120.0 2 .
O3 Ga1 La1 126.2(4) 4_665 4
O3 Ga1 La1 98.5(3) 6_455 4
O3 Ga1 La1 42.4(3) 1_455 4
O3 Ga1 La1 126.2(4) 5_665 4
O3 Ga1 La1 42.4(3) 2_545 4
O3 Ga1 La1 98.5(3) 3_545 4
La1 Ga1 La1 120.0 2 4
La1 Ga1 La1 120.0 . 4
O3 Ga1 O2 68.3(5) 4_665 2
O3 Ga1 O2 51.6(4) 6_455 2
O3 Ga1 O2 146.4(4) 1_455 2
O3 Ga1 O2 50.7(4) 5_665 2
O3 Ga1 O2 115.1(5) 2_545 2
O3 Ga1 O2 111.6(4) 3_545 2
La1 Ga1 O2 47.9(2) 2 2
La1 Ga1 O2 79.65(19) . 2
La1 Ga1 O2 148.2(2) 4 2
O3 Ga1 O2 51.6(4) 4_665 3
O3 Ga1 O2 68.3(5) 6_455 3
O3 Ga1 O2 50.7(4) 1_455 3
O3 Ga1 O2 146.4(4) 5_665 3
O3 Ga1 O2 111.6(4) 2_545 3
O3 Ga1 O2 115.1(5) 3_545 3
La1 Ga1 O2 47.9(2) 2 3
La1 Ga1 O2 148.2(2) . 3
La1 Ga1 O2 79.65(19) 4 3
O2 Ga1 O2 95.8(4) 2 3
O3 Ga1 O2 111.6(4) 4_665 5
O3 Ga1 O2 50.7(4) 6_455 5
O3 Ga1 O2 68.3(5) 1_455 5
O3 Ga1 O2 115.1(5) 5_665 5
O3 Ga1 O2 51.6(4) 2_545 5
O3 Ga1 O2 146.4(4) 3_545 5
La1 Ga1 O2 79.65(19) 2 5
La1 Ga1 O2 148.2(2) . 5
La1 Ga1 O2 47.9(2) 4 5
O2 Ga1 O2 101.8(3) 2 5
O2 Ga1 O2 63.6(4) 3 5
O3 Nb O3 84.7(6) 4_665 6_455
O3 Nb O3 85.2(5) 4_665 1_455
O3 Nb O3 107.6(8) 6_455 1_455
O3 Nb O3 107.6(8) 4_665 5_665
O3 Nb O3 85.2(5) 6_455 5_665
O3 Nb O3 162.9(7) 1_455 5_665
O3 Nb O3 162.9(7) 4_665 2_545
O3 Nb O3 85.2(5) 6_455 2_545
O3 Nb O3 84.7(6) 1_455 2_545
O3 Nb O3 85.2(5) 5_665 2_545
O3 Nb O3 85.2(5) 4_665 3_545
O3 Nb O3 162.9(7) 6_455 3_545
O3 Nb O3 85.2(5) 1_455 3_545
O3 Nb O3 84.7(6) 5_665 3_545
O3 Nb O3 107.6(8) 2_545 3_545
O3 Nb Ga3 31.5(3) 4_665 4_665
O3 Nb Ga3 114.2(3) 6_455 4_665
O3 Nb Ga3 86.7(4) 1_455 4_665
O3 Nb Ga3 98.4(4) 5_665 4_665
O3 Nb Ga3 160.3(4) 2_545 4_665
O3 Nb Ga3 54.0(4) 3_545 4_665
O3 Nb Ga3 114.2(3) 4_665 1_454
O3 Nb Ga3 31.5(3) 6_455 1_454
O3 Nb Ga3 98.4(4) 1_455 1_454
O3 Nb Ga3 86.7(4) 5_665 1_454
O3 Nb Ga3 54.0(4) 2_545 1_454
O3 Nb Ga3 160.3(4) 3_545 1_454
Ga3 Nb Ga3 145.18(3) 4_665 1_454
O3 Nb Ga3 54.0(4) 4_665 1_455
O3 Nb Ga3 98.4(4) 6_455 1_455
O3 Nb Ga3 31.5(3) 1_455 1_455
O3 Nb Ga3 160.4(4) 5_665 1_455
O3 Nb Ga3 114.2(3) 2_545 1_455
O3 Nb Ga3 86.7(4) 3_545 1_455
Ga3 Nb Ga3 62.43(6) 4_665 1_455
Ga3 Nb Ga3 106.49(7) 1_454 1_455
O3 Nb Ga3 98.4(4) 4_665 4_664
O3 Nb Ga3 54.0(4) 6_455 4_664
O3 Nb Ga3 160.4(4) 1_455 4_664
O3 Nb Ga3 31.5(3) 5_665 4_664
O3 Nb Ga3 86.7(4) 2_545 4_664
O3 Nb Ga3 114.2(3) 3_545 4_664
Ga3 Nb Ga3 106.49(7) 4_665 4_664
Ga3 Nb Ga3 62.43(6) 1_454 4_664
Ga3 Nb Ga3 145.18(3) 1_455 4_664
O3 Nb Ga3 160.4(4) 4_665 2_545
O3 Nb Ga3 86.7(4) 6_455 2_545
O3 Nb Ga3 114.2(3) 1_455 2_545
O3 Nb Ga3 54.0(4) 5_665 2_545
O3 Nb Ga3 31.5(3) 2_545 2_545
O3 Nb Ga3 98.4(4) 3_545 2_545
Ga3 Nb Ga3 145.18(3) 4_665 2_545
Ga3 Nb Ga3 62.43(6) 1_454 2_545
Ga3 Nb Ga3 145.18(3) 1_455 2_545
Ga3 Nb Ga3 62.43(6) 4_664 2_545
O3 Nb Ga3 86.7(4) 4_665 2_546
O3 Nb Ga3 160.4(4) 6_455 2_546
O3 Nb Ga3 54.0(4) 1_455 2_546
O3 Nb Ga3 114.2(3) 5_665 2_546
O3 Nb Ga3 98.4(4) 2_545 2_546
O3 Nb Ga3 31.5(3) 3_545 2_546
Ga3 Nb Ga3 62.43(6) 4_665 2_546
Ga3 Nb Ga3 145.18(3) 1_454 2_546
Ga3 Nb Ga3 62.43(6) 1_455 2_546
Ga3 Nb Ga3 145.18(3) 4_664 2_546
Ga3 Nb Ga3 106.49(7) 2_545 2_546
O1 Ga2 O2 115.6(5) 1_565 6_566
O1 Ga2 O2 115.6(5) 1_565 5_666
O2 Ga2 O2 102.7(6) 6_566 5_666
O1 Ga2 O2 115.6(5) 1_565 2_556
O2 Ga2 O2 102.7(6) 6_566 2_556
O2 Ga2 O2 102.7(6) 5_666 2_556
O1 Ga2 O1 179.999(6) 1_565 1_566
O2 Ga2 O1 64.4(5) 6_566 1_566
O2 Ga2 O1 64.4(5) 5_666 1_566
O2 Ga2 O1 64.4(5) 2_556 1_566
O1 Ga2 La1 134.80(4) 1_565 1_566
O2 Ga2 La1 58.2(5) 6_566 1_566
O2 Ga2 La1 44.5(4) 5_666 1_566
O2 Ga2 La1 109.0(5) 2_556 1_566
O1 Ga2 La1 45.20(4) 1_566 1_566
O1 Ga2 La1 134.80(4) 1_565 2_556
O2 Ga2 La1 44.5(4) 6_566 2_556
O2 Ga2 La1 109.0(5) 5_666 2_556
O2 Ga2 La1 58.2(5) 2_556 2_556
O1 Ga2 La1 45.20(4) 1_566 2_556
La1 Ga2 La1 75.83(6) 1_566 2_556
O1 Ga2 La1 134.80(4) 1_565 4_666
O2 Ga2 La1 109.0(5) 6_566 4_666
O2 Ga2 La1 58.2(5) 5_666 4_666
O2 Ga2 La1 44.5(4) 2_556 4_666
O1 Ga2 La1 45.20(4) 1_566 4_666
La1 Ga2 La1 75.83(6) 1_566 4_666
La1 Ga2 La1 75.83(6) 2_556 4_666
O1 Ga2 O3 65.4(2) 1_565 3
O2 Ga2 O3 57.5(5) 6_566 3
O2 Ga2 O3 101.3(5) 5_666 3
O2 Ga2 O3 151.9(5) 2_556 3
O1 Ga2 O3 114.6(2) 1_566 3
La1 Ga2 O3 78.8(2) 1_566 3
La1 Ga2 O3 99.93(18) 2_556 3
La1 Ga2 O3 154.6(2) 4_666 3
O1 Ga2 O3 65.4(2) 1_565 1_565
O2 Ga2 O3 151.9(5) 6_566 1_565
O2 Ga2 O3 57.5(5) 5_666 1_565
O2 Ga2 O3 101.3(5) 2_556 1_565
O1 Ga2 O3 114.6(2) 1_566 1_565
La1 Ga2 O3 99.93(18) 1_566 1_565
La1 Ga2 O3 154.6(2) 2_556 1_565
La1 Ga2 O3 78.8(2) 4_666 1_565
O3 Ga2 O3 103.8(3) 3 1_565
O1 Ga2 O3 65.4(2) 1_565 4_665
O2 Ga2 O3 101.3(5) 6_566 4_665
O2 Ga2 O3 151.9(5) 5_666 4_665
O2 Ga2 O3 57.5(5) 2_556 4_665
O1 Ga2 O3 114.6(2) 1_566 4_665
La1 Ga2 O3 154.6(3) 1_566 4_665
La1 Ga2 O3 78.8(2) 2_556 4_665
La1 Ga2 O3 99.93(18) 4_666 4_665
O3 Ga2 O3 103.8(3) 3 4_665
O3 Ga2 O3 103.8(3) 1_565 4_665
O1 Ga2 La1 41.83(3) 1_565 1_565
O2 Ga2 La1 96.5(4) 6_566 1_565
O2 Ga2 La1 86.4(5) 5_666 1_565
O2 Ga2 La1 156.2(5) 2_556 1_565
O1 Ga2 La1 138.17(3) 1_566 1_565
La1 Ga2 La1 92.971(7) 1_566 1_565
La1 Ga2 La1 139.611(7) 2_556 1_565
La1 Ga2 La1 139.611(7) 4_666 1_565
O3 Ga2 La1 39.71(18) 3 1_565
O3 Ga2 La1 64.9(2) 1_565 1_565
O3 Ga2 La1 105.2(2) 4_665 1_565
O3 Ga3 O3 132.6(8) . 6_556
O3 Ga3 O2 102.1(7) . 3_655
O3 Ga3 O2 108.3(5) 6_556 3_655
O3 Ga3 O2 108.3(5) . 5_656
O3 Ga3 O2 102.1(7) 6_556 5_656
O2 Ga3 O2 99.1(9) 3_655 5_656
O3 Ga3 O3 73.5(6) . 4_765
O3 Ga3 O3 77.4(6) 6_556 4_765
O2 Ga3 O3 79.1(5) 3_655 4_765
O2 Ga3 O3 177.8(5) 5_656 4_765
O3 Ga3 O3 77.4(6) . 2_646
O3 Ga3 O3 73.5(6) 6_556 2_646
O2 Ga3 O3 177.8(5) 3_655 2_646
O2 Ga3 O3 79.1(5) 5_656 2_646
O3 Ga3 O3 102.7(4) 4_765 2_646
O3 Ga3 Nb 109.7(5) . 1_656
O3 Ga3 Nb 35.0(3) 6_556 1_656
O2 Ga3 Nb 142.9(4) 3_655 1_656
O2 Ga3 Nb 88.8(5) 5_656 1_656
O3 Ga3 Nb 91.9(3) 4_765 1_656
O3 Ga3 Nb 38.7(3) 2_646 1_656
O3 Ga3 Nb 35.0(3) . 1_655
O3 Ga3 Nb 109.7(5) 6_556 1_655
O2 Ga3 Nb 88.8(5) 3_655 1_655
O2 Ga3 Nb 142.9(4) 5_656 1_655
O3 Ga3 Nb 38.7(3) 4_765 1_655
O3 Ga3 Nb 91.9(3) 2_646 1_655
Nb Ga3 Nb 106.49(7) 1_656 1_655
O3 Ga3 O1 160.5(5) . 2_656
O3 Ga3 O1 62.6(4) 6_556 2_656
O2 Ga3 O1 58.7(6) 3_655 2_656
O2 Ga3 O1 75.0(4) 5_656 2_656
O3 Ga3 O1 102.9(3) 4_765 2_656
O3 Ga3 O1 121.8(4) 2_646 2_656
Nb Ga3 O1 89.3(3) 1_656 2_656
Nb Ga3 O1 136.9(2) 1_655 2_656
O3 Ga3 O1 62.6(4) . .
O3 Ga3 O1 160.5(5) 6_556 .
O2 Ga3 O1 75.0(4) 3_655 .
O2 Ga3 O1 58.7(6) 5_656 .
O3 Ga3 O1 121.8(4) 4_765 .
O3 Ga3 O1 102.9(3) 2_646 .
Nb Ga3 O1 136.9(2) 1_656 .
Nb Ga3 O1 89.3(3) 1_655 .
O1 Ga3 O1 106.2(2) 2_656 .
O3 Ga3 O3 88.0(6) . 5_766
O3 Ga3 O3 44.9(3) 6_556 5_766
O2 Ga3 O3 134.7(5) 3_655 5_766
O2 Ga3 O3 119.6(5) 5_656 5_766
O3 Ga3 O3 61.5(4) 4_765 5_766
O3 Ga3 O3 47.5(3) 2_646 5_766
Nb Ga3 O3 32.9(2) 1_656 5_766
Nb Ga3 O3 74.6(2) 1_655 5_766
O1 Ga3 O3 107.3(3) 2_656 5_766
O1 Ga3 O3 144.2(2) . 5_766
O3 Ga3 O3 44.9(3) . 3_645
O3 Ga3 O3 88.0(6) 6_556 3_645
O2 Ga3 O3 119.6(5) 3_655 3_645
O2 Ga3 O3 134.7(5) 5_656 3_645
O3 Ga3 O3 47.5(3) 4_765 3_645
O3 Ga3 O3 61.5(4) 2_646 3_645
Nb Ga3 O3 74.6(2) 1_656 3_645
Nb Ga3 O3 32.9(2) 1_655 3_645
O1 Ga3 O3 144.2(2) 2_656 3_645
O1 Ga3 O3 107.3(3) . 3_645
O3 Ga3 O3 45.2(4) 5_766 3_645
Ga2 O1 La1 110.1(4) 1_545 .
Ga2 O1 La1 110.1(4) 1_545 2_545
La1 O1 La1 108.9(4) . 2_545
Ga2 O1 La1 110.1(4) 1_545 4_655
La1 O1 La1 108.9(4) . 4_655
La1 O1 La1 108.9(4) 2_545 4_655
Ga2 O1 O2 146.8(3) 1_545 6
La1 O1 O2 62.3(4) . 6
La1 O1 O2 52.0(4) 2_545 6
La1 O1 O2 102.7(7) 4_655 6
Ga2 O1 O2 146.8(3) 1_545 5_655
La1 O1 O2 52.0(4) . 5_655
La1 O1 O2 102.7(7) 2_545 5_655
La1 O1 O2 62.3(4) 4_655 5_655
O2 O1 O2 56.7(5) 6 5_655
Ga2 O1 O2 146.8(3) 1_545 2_545
La1 O1 O2 102.7(7) . 2_545
La1 O1 O2 62.3(4) 2_545 2_545
La1 O1 O2 52.0(4) 4_655 2_545
O2 O1 O2 56.7(5) 6 2_545
O2 O1 O2 56.7(5) 5_655 2_545
Ga2 O1 O2 32.2(3) 1_545 6_556
La1 O1 O2 96.7(3) . 6_556
La1 O1 O2 88.3(3) 2_545 6_556
La1 O1 O2 141.6(7) 4_655 6_556
O2 O1 O2 114.6(4) 6 6_556
O2 O1 O2 148.64(15) 5_655 6_556
O2 O1 O2 148.64(15) 2_545 6_556
Ga2 O1 O2 32.2(3) 1_545 5_656
La1 O1 O2 88.3(3) . 5_656
La1 O1 O2 141.6(7) 2_545 5_656
La1 O1 O2 96.7(3) 4_655 5_656
O2 O1 O2 148.64(15) 6 5_656
O2 O1 O2 114.6(4) 5_655 5_656
O2 O1 O2 148.64(16) 2_545 5_656
O2 O1 O2 54.9(6) 6_556 5_656
Ga2 O1 O2 32.2(3) 1_545 2_546
La1 O1 O2 141.6(7) . 2_546
La1 O1 O2 96.7(3) 2_545 2_546
La1 O1 O2 88.3(3) 4_655 2_546
O2 O1 O2 148.64(16) 6 2_546
O2 O1 O2 148.64(15) 5_655 2_546
O2 O1 O2 114.6(4) 2_545 2_546
O2 O1 O2 54.9(6) 6_556 2_546
O2 O1 O2 54.9(6) 5_656 2_546
Ga2 O1 O3 83.6(4) 1_545 3_545
La1 O1 O3 48.1(2) . 3_545
La1 O1 O3 82.1(2) 2_545 3_545
La1 O1 O3 156.9(5) 4_655 3_545
O2 O1 O3 67.5(4) 6 3_545
O2 O1 O3 96.0(4) 5_655 3_545
O2 O1 O3 124.0(6) 2_545 3_545
O2 O1 O3 56.1(4) 6_556 3_545
O2 O1 O3 85.2(4) 5_656 3_545
O2 O1 O3 111.0(6) 2_546 3_545
Ga2 O1 O3 83.6(4) 1_545 4_655
La1 O1 O3 156.9(5) . 4_655
La1 O1 O3 48.1(2) 2_545 4_655
La1 O1 O3 82.1(2) 4_655 4_655
O2 O1 O3 96.0(4) 6 4_655
O2 O1 O3 124.0(6) 5_655 4_655
O2 O1 O3 67.5(4) 2_545 4_655
O2 O1 O3 85.2(4) 6_556 4_655
O2 O1 O3 111.0(6) 5_656 4_655
O2 O1 O3 56.1(4) 2_546 4_655
O3 O1 O3 118.76(15) 3_545 4_655
Ga2 O1 O3 83.6(4) 1_545 .
La1 O1 O3 82.1(2) . .
La1 O1 O3 156.9(5) 2_545 .
La1 O1 O3 48.1(2) 4_655 .
O2 O1 O3 124.0(6) 6 .
O2 O1 O3 67.5(4) 5_655 .
O2 O1 O3 96.0(4) 2_545 .
O2 O1 O3 111.0(6) 6_556 .
O2 O1 O3 56.1(4) 5_656 .
O2 O1 O3 85.2(4) 2_546 .
O3 O1 O3 118.76(15) 3_545 .
O3 O1 O3 118.76(15) 4_655 .
Ga2 O1 Ga2 180.0 1_545 1_544
La1 O1 Ga2 69.9(4) . 1_544
La1 O1 Ga2 69.9(4) 2_545 1_544
La1 O1 Ga2 69.9(4) 4_655 1_544
O2 O1 Ga2 33.2(3) 6 1_544
O2 O1 Ga2 33.2(3) 5_655 1_544
O2 O1 Ga2 33.2(3) 2_545 1_544
O2 O1 Ga2 147.8(3) 6_556 1_544
O2 O1 Ga2 147.8(3) 5_656 1_544
O2 O1 Ga2 147.8(3) 2_546 1_544
O3 O1 Ga2 96.4(4) 3_545 1_544
O3 O1 Ga2 96.4(4) 4_655 1_544
O3 O1 Ga2 96.4(4) . 1_544
Ga2 O1 O2 78.2(4) 1_545 4
La1 O1 O2 94.1(2) . 4
La1 O1 O2 43.3(2) 2_545 4
La1 O1 O2 149.9(3) 4_655 4
O2 O1 O2 70.6(4) 6 4
O2 O1 O2 125.7(4) 5_655 4
O2 O1 O2 105.1(4) 2_545 4
O2 O1 O2 48.6(4) 6_556 4
O2 O1 O2 103.2(5) 5_656 4
O2 O1 O2 85.1(4) 2_546 4
O3 O1 O2 48.9(3) 3_545 4
O3 O1 O2 69.9(3) 4_655 4
O3 O1 O2 158.9(6) . 4
Ga2 O1 O2 101.8(4) 1_544 4
Ga2 O1 O2 78.2(4) 1_545 3_655
La1 O1 O2 43.3(2) . 3_655
La1 O1 O2 149.9(3) 2_545 3_655
La1 O1 O2 94.1(2) 4_655 3_655
O2 O1 O2 105.1(4) 6 3_655
O2 O1 O2 70.6(4) 5_655 3_655
O2 O1 O2 125.7(4) 2_545 3_655
O2 O1 O2 85.1(4) 6_556 3_655
O2 O1 O2 48.6(4) 5_656 3_655
O2 O1 O2 103.2(5) 2_546 3_655
O3 O1 O2 69.9(3) 3_545 3_655
O3 O1 O2 158.9(6) 4_655 3_655
O3 O1 O2 48.9(3) . 3_655
Ga2 O1 O2 101.8(4) 1_544 3_655
O2 O1 O2 116.0(2) 4 3_655
Ga2 O1 O2 78.2(4) 1_545 1_545
La1 O1 O2 149.9(3) . 1_545
La1 O1 O2 94.1(2) 2_545 1_545
La1 O1 O2 43.3(2) 4_655 1_545
O2 O1 O2 125.7(4) 6 1_545
O2 O1 O2 105.1(4) 5_655 1_545
O2 O1 O2 70.6(4) 2_545 1_545
O2 O1 O2 103.2(5) 6_556 1_545
O2 O1 O2 85.1(4) 5_656 1_545
O2 O1 O2 48.6(4) 2_546 1_545
O3 O1 O2 158.9(6) 3_545 1_545
O3 O1 O2 48.9(3) 4_655 1_545
O3 O1 O2 69.9(3) . 1_545
Ga2 O1 O2 101.8(4) 1_544 1_545
O2 O1 O2 116.0(2) 4 1_545
O2 O1 O2 116.0(2) 3_655 1_545
Ga2 O1 Ga3 62.4(3) 1_545 2_546
La1 O1 Ga3 77.78(11) . 2_546
La1 O1 Ga3 72.47(11) 2_545 2_546
La1 O1 Ga3 171.8(6) 4_655 2_546
O2 O1 Ga3 84.5(3) 6 2_546
O2 O1 Ga3 125.7(3) 5_655 2_546
O2 O1 Ga3 132.4(4) 2_545 2_546
O2 O1 Ga3 30.5(2) 6_556 2_546
O2 O1 Ga3 78.4(5) 5_656 2_546
O2 O1 Ga3 83.5(5) 2_546 2_546
O3 O1 Ga3 30.2(2) 3_545 2_546
O3 O1 Ga3 93.4(3) 4_655 2_546
O3 O1 Ga3 130.4(5) . 2_546
Ga2 O1 Ga3 117.6(3) 1_544 2_546
O2 O1 Ga3 29.5(2) 4 2_546
O2 O1 Ga3 87.6(3) 3_655 2_546
O2 O1 Ga3 129.0(5) 1_545 2_546
Ga2 O1 Ga3 62.4(3) 1_545 .
La1 O1 Ga3 72.47(11) . .
La1 O1 Ga3 171.8(6) 2_545 .
La1 O1 Ga3 77.78(11) 4_655 .
O2 O1 Ga3 132.4(4) 6 .
O2 O1 Ga3 84.5(3) 5_655 .
O2 O1 Ga3 125.7(3) 2_545 .
O2 O1 Ga3 83.5(5) 6_556 .
O2 O1 Ga3 30.5(2) 5_656 .
O2 O1 Ga3 78.4(5) 2_546 .
O3 O1 Ga3 93.4(3) 3_545 .
O3 O1 Ga3 130.4(5) 4_655 .
O3 O1 Ga3 30.2(2) . .
Ga2 O1 Ga3 117.6(3) 1_544 .
O2 O1 Ga3 129.0(5) 4 .
O2 O1 Ga3 29.5(2) 3_655 .
O2 O1 Ga3 87.6(3) 1_545 .
Ga3 O1 Ga3 100.3(4) 2_546 .
Ga2 O1 Ga3 62.4(3) 1_545 4_655
La1 O1 Ga3 171.8(6) . 4_655
La1 O1 Ga3 77.77(11) 2_545 4_655
La1 O1 Ga3 72.47(11) 4_655 4_655
O2 O1 Ga3 125.7(3) 6 4_655
O2 O1 Ga3 132.4(4) 5_655 4_655
O2 O1 Ga3 84.5(3) 2_545 4_655
O2 O1 Ga3 78.4(5) 6_556 4_655
O2 O1 Ga3 83.5(5) 5_656 4_655
O2 O1 Ga3 30.5(2) 2_546 4_655
O3 O1 Ga3 130.4(5) 3_545 4_655
O3 O1 Ga3 30.2(2) 4_655 4_655
O3 O1 Ga3 93.4(3) . 4_655
Ga2 O1 Ga3 117.6(3) 1_544 4_655
O2 O1 Ga3 87.6(3) 4 4_655
O2 O1 Ga3 129.0(5) 3_655 4_655
O2 O1 Ga3 29.5(2) 1_545 4_655
Ga3 O1 Ga3 100.3(4) 2_546 4_655
Ga3 O1 Ga3 100.3(4) . 4_655
Ga2 O1 O3 118.8(3) 1_545 5_665
La1 O1 O3 27.25(18) . 5_665
La1 O1 O3 81.8(3) 2_545 5_665
La1 O1 O3 122.4(6) 4_655 5_665
O2 O1 O3 40.1(4) 6 5_665
O2 O1 O3 60.2(4) 5_655 5_665
O2 O1 O3 92.9(6) 2_545 5_665
O2 O1 O3 93.3(3) 6_556 5_665
O2 O1 O3 108.5(3) 5_656 5_665
O2 O1 O3 148.2(5) 2_546 5_665
O3 O1 O3 37.2(4) 3_545 5_665
O3 O1 O3 129.9(4) 4_655 5_665
O3 O1 O3 108.5(3) . 5_665
Ga2 O1 O3 61.2(3) 1_544 5_665
O2 O1 O3 72.0(3) 4 5_665
O2 O1 O3 69.4(3) 3_655 5_665
O2 O1 O3 162.9(6) 1_545 5_665
Ga3 O1 O3 65.69(16) 2_546 5_665
Ga3 O1 O3 98.87(17) . 5_665
Ga3 O1 O3 158.08(16) 4_655 5_665
Ga2 O1 O3 118.8(3) 1_545 6_445
La1 O1 O3 122.4(6) . 6_445
La1 O1 O3 27.25(18) 2_545 6_445
La1 O1 O3 81.8(3) 4_655 6_445
O2 O1 O3 60.2(4) 6 6_445
O2 O1 O3 92.9(6) 5_655 6_445
O2 O1 O3 40.1(4) 2_545 6_445
O2 O1 O3 108.5(3) 6_556 6_445
O2 O1 O3 148.2(5) 5_656 6_445
O2 O1 O3 93.3(3) 2_546 6_445
O3 O1 O3 108.5(3) 3_545 6_445
O3 O1 O3 37.2(4) 4_655 6_445
O3 O1 O3 129.9(4) . 6_445
Ga2 O1 O3 61.2(3) 1_544 6_445
O2 O1 O3 69.4(3) 4 6_445
O2 O1 O3 162.9(6) 3_655 6_445
O2 O1 O3 72.0(3) 1_545 6_445
Ga3 O1 O3 98.87(17) 2_546 6_445
Ga3 O1 O3 158.08(16) . 6_445
Ga3 O1 O3 65.69(16) 4_655 6_445
O3 O1 O3 98.7(4) 5_665 6_445
Ga2 O1 O3 118.8(3) 1_545 2_645
La1 O1 O3 81.8(3) . 2_645
La1 O1 O3 122.4(6) 2_545 2_645
La1 O1 O3 27.25(18) 4_655 2_645
O2 O1 O3 92.9(6) 6 2_645
O2 O1 O3 40.1(4) 5_655 2_645
O2 O1 O3 60.2(4) 2_545 2_645
O2 O1 O3 148.2(5) 6_556 2_645
O2 O1 O3 93.3(3) 5_656 2_645
O2 O1 O3 108.5(3) 2_546 2_645
O3 O1 O3 129.9(4) 3_545 2_645
O3 O1 O3 108.5(3) 4_655 2_645
O3 O1 O3 37.2(4) . 2_645
Ga2 O1 O3 61.2(3) 1_544 2_645
O2 O1 O3 162.9(6) 4 2_645
O2 O1 O3 72.0(3) 3_655 2_645
O2 O1 O3 69.4(3) 1_545 2_645
Ga3 O1 O3 158.08(16) 2_546 2_645
Ga3 O1 O3 65.69(16) . 2_645
Ga3 O1 O3 98.87(17) 4_655 2_645
O3 O1 O3 98.7(4) 5_665 2_645
O3 O1 O3 98.7(4) 6_445 2_645
Ga2 O1 Ga3 137.11(17) 1_545 2_545
La1 O1 Ga3 57.6(3) . 2_545
La1 O1 Ga3 52.8(3) 2_545 2_545
La1 O1 Ga3 112.8(6) 4_655 2_545
O2 O1 Ga3 10.4(3) 6 2_545
O2 O1 Ga3 62.5(4) 5_655 2_545
O2 O1 Ga3 66.9(4) 2_545 2_545
O2 O1 Ga3 105.1(2) 6_556 2_545
O2 O1 Ga3 140.1(3) 5_656 2_545
O2 O1 Ga3 146.5(3) 2_546 2_545
O3 O1 Ga3 57.2(3) 3_545 2_545
O3 O1 Ga3 99.7(3) 4_655 2_545
O3 O1 Ga3 128.3(4) . 2_545
Ga2 O1 Ga3 42.90(17) 1_544 2_545
O2 O1 Ga3 63.5(3) 4 2_545
O2 O1 Ga3 100.9(3) 3_655 2_545
O2 O1 Ga3 134.9(4) 1_545 2_545
Ga3 O1 Ga3 74.70(12) 2_546 2_545
Ga3 O1 Ga3 129.86(18) . 2_545
Ga3 O1 Ga3 129.86(18) 4_655 2_545
O3 O1 Ga3 32.7(2) 5_665 2_545
O3 O1 Ga3 66.0(3) 6_445 2_545
O3 O1 Ga3 100.8(5) 2_645 2_545
Ga2 O1 Ga3 137.10(17) 1_545 1_554
La1 O1 Ga3 52.8(3) . 1_554
La1 O1 Ga3 112.8(6) 2_545 1_554
La1 O1 Ga3 57.6(3) 4_655 1_554
O2 O1 Ga3 66.9(4) 6 1_554
O2 O1 Ga3 10.4(3) 5_655 1_554
O2 O1 Ga3 62.5(4) 2_545 1_554
O2 O1 Ga3 146.5(3) 6_556 1_554
O2 O1 Ga3 105.1(2) 5_656 1_554
O2 O1 Ga3 140.1(3) 2_546 1_554
O3 O1 Ga3 99.7(3) 3_545 1_554
O3 O1 Ga3 128.3(4) 4_655 1_554
O3 O1 Ga3 57.2(3) . 1_554
Ga2 O1 Ga3 42.90(17) 1_544 1_554
O2 O1 Ga3 134.9(4) 4 1_554
O2 O1 Ga3 63.5(3) 3_655 1_554
O2 O1 Ga3 100.9(3) 1_545 1_554
Ga3 O1 Ga3 129.86(18) 2_546 1_554
Ga3 O1 Ga3 74.70(12) . 1_554
Ga3 O1 Ga3 129.86(18) 4_655 1_554
O3 O1 Ga3 66.0(3) 5_665 1_554
O3 O1 Ga3 100.8(5) 6_445 1_554
O3 O1 Ga3 32.7(2) 2_645 1_554
Ga3 O1 Ga3 72.2(3) 2_545 1_554
Ga2 O1 Ga3 137.10(17) 1_545 4_654
La1 O1 Ga3 112.8(6) . 4_654
La1 O1 Ga3 57.6(3) 2_545 4_654
La1 O1 Ga3 52.8(3) 4_655 4_654
O2 O1 Ga3 62.5(4) 6 4_654
O2 O1 Ga3 66.9(4) 5_655 4_654
O2 O1 Ga3 10.4(3) 2_545 4_654
O2 O1 Ga3 140.1(3) 6_556 4_654
O2 O1 Ga3 146.5(3) 5_656 4_654
O2 O1 Ga3 105.1(2) 2_546 4_654
O3 O1 Ga3 128.3(4) 3_545 4_654
O3 O1 Ga3 57.2(3) 4_655 4_654
O3 O1 Ga3 99.7(3) . 4_654
Ga2 O1 Ga3 42.90(17) 1_544 4_654
O2 O1 Ga3 100.9(3) 4 4_654
O2 O1 Ga3 134.9(4) 3_655 4_654
O2 O1 Ga3 63.5(3) 1_545 4_654
Ga3 O1 Ga3 129.86(18) 2_546 4_654
Ga3 O1 Ga3 129.86(18) . 4_654
Ga3 O1 Ga3 74.70(12) 4_655 4_654
O3 O1 Ga3 100.8(5) 5_665 4_654
O3 O1 Ga3 32.7(2) 6_445 4_654
O3 O1 Ga3 66.0(3) 2_645 4_654
Ga3 O1 Ga3 72.2(3) 2_545 4_654
Ga3 O1 Ga3 72.2(3) 1_554 4_654
Ga2 O1 O3 52.3(2) 1_545 5_666
La1 O1 O3 63.6(3) . 5_666
La1 O1 O3 103.3(2) 2_545 5_666
La1 O1 O3 147.5(4) 4_655 5_666
O2 O1 O3 100.6(3) 6 5_666
O2 O1 O3 115.2(3) 5_655 5_666
O2 O1 O3 157.2(5) 2_545 5_666
O2 O1 O3 33.5(3) 6_556 5_666
O2 O1 O3 53.2(4) 5_656 5_666
O2 O1 O3 83.2(5) 2_546 5_666
O3 O1 O3 33.2(4) 3_545 5_666
O3 O1 O3 117.5(4) 4_655 5_666
O3 O1 O3 99.8(4) . 5_666
Ga2 O1 O3 127.7(2) 1_544 5_666
O2 O1 O3 60.5(3) 4 5_666
O2 O1 O3 57.9(3) 3_655 5_666
O2 O1 O3 130.6(5) 1_545 5_666
Ga3 O1 O3 31.03(16) 2_546 5_666
Ga3 O1 O3 69.8(3) . 5_666
Ga3 O1 O3 110.7(5) 4_655 5_666
O3 O1 O3 66.49(17) 5_665 5_666
O3 O1 O3 129.90(11) 6_445 5_666
O3 O1 O3 129.90(12) 2_645 5_666
Ga3 O1 O3 90.38(15) 2_545 5_666
Ga3 O1 O3 113.55(14) 1_554 5_666
Ga3 O1 O3 159.5(2) 4_654 5_666
Ga2 O1 O3 52.3(2) 1_545 6_446
La1 O1 O3 147.5(4) . 6_446
La1 O1 O3 63.6(3) 2_545 6_446
La1 O1 O3 103.3(2) 4_655 6_446
O2 O1 O3 115.2(3) 6 6_446
O2 O1 O3 157.2(5) 5_655 6_446
O2 O1 O3 100.6(3) 2_545 6_446
O2 O1 O3 53.2(4) 6_556 6_446
O2 O1 O3 83.2(5) 5_656 6_446
O2 O1 O3 33.5(3) 2_546 6_446
O3 O1 O3 99.8(4) 3_545 6_446
O3 O1 O3 33.2(4) 4_655 6_446
O3 O1 O3 117.5(4) . 6_446
Ga2 O1 O3 127.7(2) 1_544 6_446
O2 O1 O3 57.9(3) 4 6_446
O2 O1 O3 130.6(5) 3_655 6_446
O2 O1 O3 60.5(3) 1_545 6_446
Ga3 O1 O3 69.8(3) 2_546 6_446
Ga3 O1 O3 110.7(5) . 6_446
Ga3 O1 O3 31.03(16) 4_655 6_446
O3 O1 O3 129.90(11) 5_665 6_446
O3 O1 O3 66.49(17) 6_445 6_446
O3 O1 O3 129.90(11) 2_645 6_446
Ga3 O1 O3 113.55(14) 2_545 6_446
Ga3 O1 O3 159.5(2) 1_554 6_446
Ga3 O1 O3 90.38(15) 4_654 6_446
O3 O1 O3 86.6(4) 5_666 6_446
Ga2 O1 O3 52.3(2) 1_545 2_646
La1 O1 O3 103.3(2) . 2_646
La1 O1 O3 147.5(4) 2_545 2_646
La1 O1 O3 63.6(3) 4_655 2_646
O2 O1 O3 157.2(5) 6 2_646
O2 O1 O3 100.6(3) 5_655 2_646
O2 O1 O3 115.2(3) 2_545 2_646
O2 O1 O3 83.2(5) 6_556 2_646
O2 O1 O3 33.5(3) 5_656 2_646
O2 O1 O3 53.2(4) 2_546 2_646
O3 O1 O3 117.5(4) 3_545 2_646
O3 O1 O3 99.8(4) 4_655 2_646
O3 O1 O3 33.2(4) . 2_646
Ga2 O1 O3 127.7(2) 1_544 2_646
O2 O1 O3 130.6(5) 4 2_646
O2 O1 O3 60.5(3) 3_655 2_646
O2 O1 O3 57.9(3) 1_545 2_646
Ga3 O1 O3 110.7(5) 2_546 2_646
Ga3 O1 O3 31.03(16) . 2_646
Ga3 O1 O3 69.8(3) 4_655 2_646
O3 O1 O3 129.90(12) 5_665 2_646
O3 O1 O3 129.90(11) 6_445 2_646
O3 O1 O3 66.49(17) 2_645 2_646
Ga3 O1 O3 159.5(2) 2_545 2_646
Ga3 O1 O3 90.38(15) 1_554 2_646
Ga3 O1 O3 113.55(14) 4_654 2_646
O3 O1 O3 86.6(4) 5_666 2_646
O3 O1 O3 86.6(4) 6_446 2_646
Ga2 O1 Nb 100.7(2) 1_545 .
La1 O1 Nb 45.37(5) . .
La1 O1 Nb 71.29(11) 2_545 .
La1 O1 Nb 146.4(6) 4_655 .
O2 O1 Nb 49.6(3) 6 .
O2 O1 Nb 84.6(4) 5_655 .
O2 O1 Nb 106.2(5) 2_545 .
O2 O1 Nb 71.1(2) 6_556 .
O2 O1 Nb 102.4(3) 5_656 .
O2 O1 Nb 125.3(5) 2_546 .
O3 O1 Nb 17.9(3) 3_545 .
O3 O1 Nb 115.4(2) 4_655 .
O3 O1 Nb 125.8(2) . .
Ga2 O1 Nb 79.3(2) 1_544 .
O2 O1 Nb 49.1(2) 4 .
O2 O1 Nb 78.8(2) 3_655 .
O2 O1 Nb 164.2(2) 1_545 .
Ga3 O1 Nb 41.79(4) 2_546 .
Ga3 O1 Nb 106.02(9) . .
Ga3 O1 Nb 136.59(19) 4_655 .
O3 O1 Nb 24.62(15) 5_665 .
O3 O1 Nb 95.4(2) 6_445 .
O3 O1 Nb 123.2(4) 2_645 .
Ga3 O1 Nb 39.30(8) 2_545 .
Ga3 O1 Nb 90.6(2) 1_554 .
Ga3 O1 Nb 110.9(3) 4_654 .
O3 O1 Nb 51.09(14) 5_666 .
O3 O1 Nb 106.1(2) 6_446 .
O3 O1 Nb 133.5(3) 2_646 .
Ga2 O1 Ga1 100.7(2) 1_545 .
La1 O1 Ga1 45.37(5) . .
La1 O1 Ga1 71.29(11) 2_545 .
La1 O1 Ga1 146.4(6) 4_655 .
O2 O1 Ga1 49.6(3) 6 .
O2 O1 Ga1 84.6(4) 5_655 .
O2 O1 Ga1 106.2(5) 2_545 .
O2 O1 Ga1 71.1(2) 6_556 .
O2 O1 Ga1 102.4(3) 5_656 .
O2 O1 Ga1 125.3(5) 2_546 .
O3 O1 Ga1 17.9(3) 3_545 .
O3 O1 Ga1 115.4(2) 4_655 .
O3 O1 Ga1 125.8(2) . .
Ga2 O1 Ga1 79.3(2) 1_544 .
O2 O1 Ga1 49.1(2) 4 .
O2 O1 Ga1 78.8(2) 3_655 .
O2 O1 Ga1 164.2(2) 1_545 .
Ga3 O1 Ga1 41.79(4) 2_546 .
Ga3 O1 Ga1 106.02(9) . .
Ga3 O1 Ga1 136.59(19) 4_655 .
O3 O1 Ga1 24.62(15) 5_665 .
O3 O1 Ga1 95.4(2) 6_445 .
O3 O1 Ga1 123.2(4) 2_645 .
Ga3 O1 Ga1 39.30(8) 2_545 .
Ga3 O1 Ga1 90.6(2) 1_554 .
Ga3 O1 Ga1 110.9(3) 4_654 .
O3 O1 Ga1 51.09(14) 5_666 .
O3 O1 Ga1 106.1(2) 6_446 .
O3 O1 Ga1 133.5(3) 2_646 .
Nb O1 Ga1 0.0 . .
Ga2 O1 Nb 100.7(2) 1_545 1_655
La1 O1 Nb 71.29(11) . 1_655
La1 O1 Nb 146.4(6) 2_545 1_655
La1 O1 Nb 45.37(5) 4_655 1_655
O2 O1 Nb 106.2(5) 6 1_655
O2 O1 Nb 49.6(3) 5_655 1_655
O2 O1 Nb 84.6(4) 2_545 1_655
O2 O1 Nb 125.3(5) 6_556 1_655
O2 O1 Nb 71.1(2) 5_656 1_655
O2 O1 Nb 102.4(3) 2_546 1_655
O3 O1 Nb 115.4(2) 3_545 1_655
O3 O1 Nb 125.8(2) 4_655 1_655
O3 O1 Nb 17.9(3) . 1_655
Ga2 O1 Nb 79.3(2) 1_544 1_655
O2 O1 Nb 164.2(2) 4 1_655
O2 O1 Nb 49.1(2) 3_655 1_655
O2 O1 Nb 78.8(2) 1_545 1_655
Ga3 O1 Nb 136.59(19) 2_546 1_655
Ga3 O1 Nb 41.79(4) . 1_655
Ga3 O1 Nb 106.02(9) 4_655 1_655
O3 O1 Nb 95.4(2) 5_665 1_655
O3 O1 Nb 123.2(4) 6_445 1_655
O3 O1 Nb 24.62(15) 2_645 1_655
Ga3 O1 Nb 110.9(3) 2_545 1_655
Ga3 O1 Nb 39.30(8) 1_554 1_655
Ga3 O1 Nb 90.6(2) 4_654 1_655
O3 O1 Nb 106.1(2) 5_666 1_655
O3 O1 Nb 133.5(3) 6_446 1_655
O3 O1 Nb 51.09(14) 2_646 1_655
Nb O1 Nb 116.66(14) . 1_655
Ga1 O1 Nb 116.66(14) . 1_655
Ga2 O1 Ga1 100.7(2) 1_545 1_655
La1 O1 Ga1 71.29(11) . 1_655
La1 O1 Ga1 146.4(6) 2_545 1_655
La1 O1 Ga1 45.37(5) 4_655 1_655
O2 O1 Ga1 106.2(5) 6 1_655
O2 O1 Ga1 49.6(3) 5_655 1_655
O2 O1 Ga1 84.6(4) 2_545 1_655
O2 O1 Ga1 125.3(5) 6_556 1_655
O2 O1 Ga1 71.1(2) 5_656 1_655
O2 O1 Ga1 102.4(3) 2_546 1_655
O3 O1 Ga1 115.4(2) 3_545 1_655
O3 O1 Ga1 125.8(2) 4_655 1_655
O3 O1 Ga1 17.9(3) . 1_655
Ga2 O1 Ga1 79.3(2) 1_544 1_655
O2 O1 Ga1 164.2(2) 4 1_655
O2 O1 Ga1 49.1(2) 3_655 1_655
O2 O1 Ga1 78.8(2) 1_545 1_655
Ga3 O1 Ga1 136.59(19) 2_546 1_655
Ga3 O1 Ga1 41.79(4) . 1_655
Ga3 O1 Ga1 106.02(9) 4_655 1_655
O3 O1 Ga1 95.4(2) 5_665 1_655
O3 O1 Ga1 123.2(4) 6_445 1_655
O3 O1 Ga1 24.62(15) 2_645 1_655
Ga3 O1 Ga1 110.9(3) 2_545 1_655
Ga3 O1 Ga1 39.30(8) 1_554 1_655
Ga3 O1 Ga1 90.6(2) 4_654 1_655
O3 O1 Ga1 106.1(2) 5_666 1_655
O3 O1 Ga1 133.5(3) 6_446 1_655
O3 O1 Ga1 51.09(14) 2_646 1_655
Nb O1 Ga1 116.66(14) . 1_655
Ga1 O1 Ga1 116.66(14) . 1_655
Nb O1 Ga1 0.0 1_655 1_655
Ga2 O1 Ga1 100.7(2) 1_545 1_545
La1 O1 Ga1 146.4(6) . 1_545
La1 O1 Ga1 45.37(5) 2_545 1_545
La1 O1 Ga1 71.29(11) 4_655 1_545
O2 O1 Ga1 84.6(4) 6 1_545
O2 O1 Ga1 106.2(5) 5_655 1_545
O2 O1 Ga1 49.6(3) 2_545 1_545
O2 O1 Ga1 102.4(3) 6_556 1_545
O2 O1 Ga1 125.3(5) 5_656 1_545
O2 O1 Ga1 71.1(2) 2_546 1_545
O3 O1 Ga1 125.8(2) 3_545 1_545
O3 O1 Ga1 17.9(3) 4_655 1_545
O3 O1 Ga1 115.4(2) . 1_545
Ga2 O1 Ga1 79.3(2) 1_544 1_545
O2 O1 Ga1 78.8(2) 4 1_545
O2 O1 Ga1 164.2(2) 3_655 1_545
O2 O1 Ga1 49.1(2) 1_545 1_545
Ga3 O1 Ga1 106.02(9) 2_546 1_545
Ga3 O1 Ga1 136.59(19) . 1_545
Ga3 O1 Ga1 41.79(4) 4_655 1_545
O3 O1 Ga1 123.2(4) 5_665 1_545
O3 O1 Ga1 24.62(15) 6_445 1_545
O3 O1 Ga1 95.4(2) 2_645 1_545
Ga3 O1 Ga1 90.6(2) 2_545 1_545
Ga3 O1 Ga1 110.9(3) 1_554 1_545
Ga3 O1 Ga1 39.30(8) 4_654 1_545
O3 O1 Ga1 133.5(3) 5_666 1_545
O3 O1 Ga1 51.09(14) 6_446 1_545
O3 O1 Ga1 106.1(2) 2_646 1_545
Nb O1 Ga1 116.66(14) . 1_545
Ga1 O1 Ga1 116.66(14) . 1_545
Nb O1 Ga1 116.66(14) 1_655 1_545
Ga1 O1 Ga1 116.66(14) 1_655 1_545
Ga2 O1 Nb 100.7(2) 1_545 1_545
La1 O1 Nb 146.4(6) . 1_545
La1 O1 Nb 45.37(5) 2_545 1_545
La1 O1 Nb 71.29(11) 4_655 1_545
O2 O1 Nb 84.6(4) 6 1_545
O2 O1 Nb 106.2(5) 5_655 1_545
O2 O1 Nb 49.6(3) 2_545 1_545
O2 O1 Nb 102.4(3) 6_556 1_545
O2 O1 Nb 125.3(5) 5_656 1_545
O2 O1 Nb 71.1(2) 2_546 1_545
O3 O1 Nb 125.8(2) 3_545 1_545
O3 O1 Nb 17.9(3) 4_655 1_545
O3 O1 Nb 115.4(2) . 1_545
Ga2 O1 Nb 79.3(2) 1_544 1_545
O2 O1 Nb 78.8(2) 4 1_545
O2 O1 Nb 164.2(2) 3_655 1_545
O2 O1 Nb 49.1(2) 1_545 1_545
Ga3 O1 Nb 106.02(9) 2_546 1_545
Ga3 O1 Nb 136.59(19) . 1_545
Ga3 O1 Nb 41.79(4) 4_655 1_545
O3 O1 Nb 123.2(4) 5_665 1_545
O3 O1 Nb 24.62(15) 6_445 1_545
O3 O1 Nb 95.4(2) 2_645 1_545
Ga3 O1 Nb 90.6(2) 2_545 1_545
Ga3 O1 Nb 110.9(3) 1_554 1_545
Ga3 O1 Nb 39.30(8) 4_654 1_545
O3 O1 Nb 133.5(3) 5_666 1_545
O3 O1 Nb 51.09(14) 6_446 1_545
O3 O1 Nb 106.1(2) 2_646 1_545
Nb O1 Nb 116.66(14) . 1_545
Ga1 O1 Nb 116.66(14) . 1_545
Nb O1 Nb 116.66(14) 1_655 1_545
Ga1 O1 Nb 116.66(14) 1_655 1_545
Ga1 O1 Nb 0.0 1_545 1_545
Ga2 O1 La1 29.82(12) 1_545 1_556
La1 O1 La1 80.3(3) . 1_556
La1 O1 La1 122.1(4) 2_545 1_556
La1 O1 La1 122.1(4) 4_655 1_556
O2 O1 La1 129.1(3) 6 1_556
O2 O1 La1 123.5(3) 5_655 1_556
O2 O1 La1 173.9(3) 2_545 1_556
O2 O1 La1 34.3(3) 6_556 1_556
O2 O1 La1 25.4(3) 5_656 1_556
O2 O1 La1 61.7(4) 2_546 1_556
O3 O1 La1 61.9(3) 3_545 1_556
O3 O1 La1 111.7(5) 4_655 1_556
O3 O1 La1 79.0(4) . 1_556
Ga2 O1 La1 150.19(12) 1_544 1_556
O2 O1 La1 79.9(3) 4 1_556
O2 O1 La1 53.2(3) 3_655 1_556
O2 O1 La1 104.1(4) 1_545 1_556
Ga3 O1 La1 53.3(2) 2_546 1_556
Ga3 O1 La1 49.8(2) . 1_556
Ga3 O1 La1 92.2(4) 4_655 1_556
O3 O1 La1 92.0(2) 5_665 1_556
O3 O1 La1 142.2(4) 6_445 1_556
O3 O1 La1 115.5(2) 2_645 1_556
Ga3 O1 La1 119.01(6) 2_545 1_556
Ga3 O1 La1 116.65(6) 1_554 1_556
Ga3 O1 La1 166.8(3) 4_654 1_556
O3 O1 La1 28.82(18) 5_666 1_556
O3 O1 La1 78.8(3) 6_446 1_556
O3 O1 La1 58.7(2) 2_646 1_556
Nb O1 La1 79.75(14) . 1_556
Ga1 O1 La1 79.75(14) . 1_556
Nb O1 La1 91.39(17) 1_655 1_556
Ga1 O1 La1 91.39(17) 1_655 1_556
Ga1 O1 La1 129.4(3) 1_545 1_556
Nb O1 La1 129.4(3) 1_545 1_556
Ga2 O1 La1 29.82(12) 1_545 2_546
La1 O1 La1 122.1(4) . 2_546
La1 O1 La1 80.3(3) 2_545 2_546
La1 O1 La1 122.1(4) 4_655 2_546
O2 O1 La1 123.5(3) 6 2_546
O2 O1 La1 173.9(3) 5_655 2_546
O2 O1 La1 129.1(3) 2_545 2_546
O2 O1 La1 25.4(3) 6_556 2_546
O2 O1 La1 61.7(4) 5_656 2_546
O2 O1 La1 34.3(3) 2_546 2_546
O3 O1 La1 79.0(4) 3_545 2_546
O3 O1 La1 61.9(3) 4_655 2_546
O3 O1 La1 111.7(5) . 2_546
Ga2 O1 La1 150.18(12) 1_544 2_546
O2 O1 La1 53.2(3) 4 2_546
O2 O1 La1 104.1(4) 3_655 2_546
O2 O1 La1 79.9(3) 1_545 2_546
Ga3 O1 La1 49.8(2) 2_546 2_546
Ga3 O1 La1 92.2(4) . 2_546
Ga3 O1 La1 53.3(2) 4_655 2_546
O3 O1 La1 115.5(2) 5_665 2_546
O3 O1 La1 92.0(2) 6_445 2_546
O3 O1 La1 142.2(4) 2_645 2_546
Ga3 O1 La1 116.65(6) 2_545 2_546
Ga3 O1 La1 166.8(3) 1_554 2_546
Ga3 O1 La1 119.01(6) 4_654 2_546
O3 O1 La1 58.7(2) 5_666 2_546
O3 O1 La1 28.82(18) 6_446 2_546
O3 O1 La1 78.8(3) 2_646 2_546
Nb O1 La1 91.39(17) . 2_546
Ga1 O1 La1 91.39(17) . 2_546
Nb O1 La1 129.4(3) 1_655 2_546
Ga1 O1 La1 129.4(3) 1_655 2_546
Ga1 O1 La1 79.75(14) 1_545 2_546
Nb O1 La1 79.75(14) 1_545 2_546
La1 O1 La1 51.0(2) 1_556 2_546
Ga2 O1 La1 29.81(12) 1_545 4_656
La1 O1 La1 122.1(4) . 4_656
La1 O1 La1 122.1(4) 2_545 4_656
La1 O1 La1 80.3(3) 4_655 4_656
O2 O1 La1 173.9(3) 6 4_656
O2 O1 La1 129.1(3) 5_655 4_656
O2 O1 La1 123.5(3) 2_545 4_656
O2 O1 La1 61.7(4) 6_556 4_656
O2 O1 La1 34.3(3) 5_656 4_656
O2 O1 La1 25.4(3) 2_546 4_656
O3 O1 La1 111.7(5) 3_545 4_656
O3 O1 La1 79.0(4) 4_655 4_656
O3 O1 La1 61.9(3) . 4_656
Ga2 O1 La1 150.18(12) 1_544 4_656
O2 O1 La1 104.1(4) 4 4_656
O2 O1 La1 79.9(3) 3_655 4_656
O2 O1 La1 53.2(3) 1_545 4_656
Ga3 O1 La1 92.2(4) 2_546 4_656
Ga3 O1 La1 53.3(2) . 4_656
Ga3 O1 La1 49.8(2) 4_655 4_656
O3 O1 La1 142.2(4) 5_665 4_656
O3 O1 La1 115.5(2) 6_445 4_656
O3 O1 La1 92.0(2) 2_645 4_656
Ga3 O1 La1 166.8(3) 2_545 4_656
Ga3 O1 La1 119.01(6) 1_554 4_656
Ga3 O1 La1 116.65(6) 4_654 4_656
O3 O1 La1 78.8(3) 5_666 4_656
O3 O1 La1 58.7(2) 6_446 4_656
O3 O1 La1 28.82(18) 2_646 4_656
Nb O1 La1 129.4(3) . 4_656
Ga1 O1 La1 129.4(3) . 4_656
Nb O1 La1 79.75(14) 1_655 4_656
Ga1 O1 La1 79.75(14) 1_655 4_656
Ga1 O1 La1 91.39(17) 1_545 4_656
Nb O1 La1 91.39(17) 1_545 4_656
La1 O1 La1 51.0(2) 1_556 4_656
La1 O1 La1 51.0(2) 2_546 4_656
Ga2 O1 O2 81.3(3) 1_545 .
La1 O1 O2 29.4(3) . .
La1 O1 O2 115.41(16) 2_545 .
La1 O1 O2 126.72(16) 4_655 .
O2 O1 O2 83.5(4) 6 .
O2 O1 O2 80.0(3) 5_655 .
O2 O1 O2 131.8(5) 2_545 .
O2 O1 O2 68.8(4) 6_556 .
O2 O1 O2 65.2(3) 5_656 .
O2 O1 O2 113.4(5) 2_546 .
O3 O1 O2 34.6(2) 3_545 .
O3 O1 O2 150.7(4) 4_655 .
O3 O1 O2 84.3(3) . .
Ga2 O1 O2 98.7(3) 1_544 .
O2 O1 O2 82.5(3) 4 .
O2 O1 O2 35.5(3) 3_655 .
O2 O1 O2 148.5(5) 1_545 .
Ga3 O1 O2 57.30(15) 2_546 .
Ga3 O1 O2 61.65(17) . .
Ga3 O1 O2 143.6(5) 4_655 .
O3 O1 O2 43.3(3) 5_665 .
O3 O1 O2 139.4(3) 6_445 .
O3 O1 O2 100.8(2) 2_645 .
Ga3 O1 O2 75.49(19) 2_545 .
Ga3 O1 O2 78.44(18) 1_554 .
Ga3 O1 O2 141.5(4) 4_654 .
O3 O1 O2 35.3(2) 5_666 .
O3 O1 O2 121.9(4) 6_446 .
O3 O1 O2 90.6(3) 2_646 .
Nb O1 O2 44.40(14) . .
Ga1 O1 O2 44.40(14) . .
Nb O1 O2 81.75(14) 1_655 .
Ga1 O1 O2 81.75(14) 1_655 .
Ga1 O1 O2 160.35(15) 1_545 .
Nb O1 O2 160.35(15) 1_545 .
La1 O1 O2 51.7(2) 1_556 .
La1 O1 O2 93.9(3) 2_546 .
La1 O1 O2 99.1(3) 4_656 .
Ga2 O1 O2 81.3(3) 1_545 3_545
La1 O1 O2 126.72(17) . 3_545
La1 O1 O2 29.4(3) 2_545 3_545
La1 O1 O2 115.41(16) 4_655 3_545
O2 O1 O2 80.0(3) 6 3_545
O2 O1 O2 131.8(5) 5_655 3_545
O2 O1 O2 83.5(4) 2_545 3_545
O2 O1 O2 65.2(3) 6_556 3_545
O2 O1 O2 113.4(5) 5_656 3_545
O2 O1 O2 68.8(4) 2_546 3_545
O3 O1 O2 84.3(3) 3_545 3_545
O3 O1 O2 34.6(2) 4_655 3_545
O3 O1 O2 150.7(4) . 3_545
Ga2 O1 O2 98.7(3) 1_544 3_545
O2 O1 O2 35.5(3) 4 3_545
O2 O1 O2 148.5(5) 3_655 3_545
O2 O1 O2 82.5(3) 1_545 3_545
Ga3 O1 O2 61.65(17) 2_546 3_545
Ga3 O1 O2 143.6(5) . 3_545
Ga3 O1 O2 57.30(15) 4_655 3_545
O3 O1 O2 100.8(2) 5_665 3_545
O3 O1 O2 43.3(3) 6_445 3_545
O3 O1 O2 139.4(3) 2_645 3_545
Ga3 O1 O2 78.44(18) 2_545 3_545
Ga3 O1 O2 141.5(4) 1_554 3_545
Ga3 O1 O2 75.49(19) 4_654 3_545
O3 O1 O2 90.6(3) 5_666 3_545
O3 O1 O2 35.3(2) 6_446 3_545
O3 O1 O2 121.9(4) 2_646 3_545
Nb O1 O2 81.75(14) . 3_545
Ga1 O1 O2 81.75(14) . 3_545
Nb O1 O2 160.35(15) 1_655 3_545
Ga1 O1 O2 160.35(15) 1_655 3_545
Ga1 O1 O2 44.40(14) 1_545 3_545
Nb O1 O2 44.40(14) 1_545 3_545
La1 O1 O2 99.1(3) 1_556 3_545
La1 O1 O2 51.7(2) 2_546 3_545
La1 O1 O2 93.9(3) 4_656 3_545
O2 O1 O2 117.76(14) . 3_545
Ga2 O1 O2 81.3(3) 1_545 4_655
La1 O1 O2 115.41(16) . 4_655
La1 O1 O2 126.72(17) 2_545 4_655
La1 O1 O2 29.4(3) 4_655 4_655
O2 O1 O2 131.8(5) 6 4_655
O2 O1 O2 83.5(4) 5_655 4_655
O2 O1 O2 80.0(3) 2_545 4_655
O2 O1 O2 113.4(5) 6_556 4_655
O2 O1 O2 68.8(4) 5_656 4_655
O2 O1 O2 65.2(3) 2_546 4_655
O3 O1 O2 150.7(4) 3_545 4_655
O3 O1 O2 84.3(3) 4_655 4_655
O3 O1 O2 34.6(2) . 4_655
Ga2 O1 O2 98.7(3) 1_544 4_655
O2 O1 O2 148.5(5) 4 4_655
O2 O1 O2 82.5(3) 3_655 4_655
O2 O1 O2 35.5(3) 1_545 4_655
Ga3 O1 O2 143.6(5) 2_546 4_655
Ga3 O1 O2 57.30(15) . 4_655
Ga3 O1 O2 61.65(17) 4_655 4_655
O3 O1 O2 139.4(3) 5_665 4_655
O3 O1 O2 100.8(2) 6_445 4_655
O3 O1 O2 43.3(3) 2_645 4_655
Ga3 O1 O2 141.5(4) 2_545 4_655
Ga3 O1 O2 75.49(19) 1_554 4_655
Ga3 O1 O2 78.44(18) 4_654 4_655
O3 O1 O2 121.9(4) 5_666 4_655
O3 O1 O2 90.6(3) 6_446 4_655
O3 O1 O2 35.3(2) 2_646 4_655
Nb O1 O2 160.35(15) . 4_655
Ga1 O1 O2 160.35(15) . 4_655
Nb O1 O2 44.40(14) 1_655 4_655
Ga1 O1 O2 44.40(14) 1_655 4_655
Ga1 O1 O2 81.75(14) 1_545 4_655
Nb O1 O2 81.75(14) 1_545 4_655
La1 O1 O2 93.9(3) 1_556 4_655
La1 O1 O2 99.1(3) 2_546 4_655
La1 O1 O2 51.7(2) 4_656 4_655
O2 O1 O2 117.76(14) . 4_655
O2 O1 O2 117.76(14) 3_545 4_655
Ga2 O1 Ga2 72.1(2) 1_545 2_556
La1 O1 Ga2 40.33(19) . 2_556
La1 O1 Ga2 136.41(2) 2_545 2_556
La1 O1 Ga2 110.77(4) 4_655 2_556
O2 O1 Ga2 101.4(3) 6 2_556
O2 O1 Ga2 80.7(2) 5_655 2_556
O2 O1 Ga2 137.3(5) 2_545 2_556
O2 O1 Ga2 71.5(3) 6_556 2_556
O2 O1 Ga2 48.1(3) 5_656 2_556
O2 O1 Ga2 101.8(5) 2_546 2_556
O3 O1 Ga2 54.5(2) 3_545 2_556
O3 O1 Ga2 155.1(6) 4_655 2_556
O3 O1 Ga2 64.6(2) . 2_556
Ga2 O1 Ga2 107.9(2) 1_544 2_556
O2 O1 Ga2 99.3(2) 4 2_556
O2 O1 Ga2 16.7(2) 3_655 2_556
O2 O1 Ga2 127.5(4) 1_545 2_556
Ga3 O1 Ga2 70.92(15) 2_546 2_556
Ga3 O1 Ga2 40.28(7) . 2_556
Ga3 O1 Ga2 131.5(5) 4_655 2_556
O3 O1 Ga2 62.06(18) 5_665 2_556
O3 O1 Ga2 160.4(3) 6_445 2_556
O3 O1 Ga2 88.36(15) 2_645 2_556
Ga3 O1 Ga2 94.80(11) 2_545 2_556
Ga3 O1 Ga2 75.45(8) 1_554 2_556
Ga3 O1 Ga2 147.5(4) 4_654 2_556
O3 O1 Ga2 41.80(17) 5_666 2_556
O3 O1 Ga2 122.0(4) 6_446 2_556
O3 O1 Ga2 69.65(19) 2_646 2_556
Nb O1 Ga2 65.75(3) . 2_556
Ga1 O1 Ga2 65.75(3) . 2_556
Nb O1 Ga2 65.75(3) 1_655 2_556
Ga1 O1 Ga2 65.75(3) 1_655 2_556
Ga1 O1 Ga2 172.7(5) 1_545 2_556
Nb O1 Ga2 172.7(5) 1_545 2_556
La1 O1 Ga2 43.42(11) 1_556 2_556
La1 O1 Ga2 93.5(3) 2_546 2_556
La1 O1 Ga2 82.2(2) 4_656 2_556
O2 O1 Ga2 21.37(15) . 2_556
O2 O1 Ga2 132.3(3) 3_545 2_556
O2 O1 Ga2 96.87(17) 4_655 2_556
Ga2 O1 Ga2 72.1(2) 1_545 2_446
La1 O1 Ga2 110.77(4) . 2_446
La1 O1 Ga2 40.33(19) 2_545 2_446
La1 O1 Ga2 136.41(2) 4_655 2_446
O2 O1 Ga2 80.7(2) 6 2_446
O2 O1 Ga2 137.3(5) 5_655 2_446
O2 O1 Ga2 101.4(3) 2_545 2_446
O2 O1 Ga2 48.1(3) 6_556 2_446
O2 O1 Ga2 101.8(5) 5_656 2_446
O2 O1 Ga2 71.5(3) 2_546 2_446
O3 O1 Ga2 64.6(2) 3_545 2_446
O3 O1 Ga2 54.5(2) 4_655 2_446
O3 O1 Ga2 155.1(6) . 2_446
Ga2 O1 Ga2 107.9(2) 1_544 2_446
O2 O1 Ga2 16.7(2) 4 2_446
O2 O1 Ga2 127.5(4) 3_655 2_446
O2 O1 Ga2 99.3(2) 1_545 2_446
Ga3 O1 Ga2 40.28(7) 2_546 2_446
Ga3 O1 Ga2 131.5(5) . 2_446
Ga3 O1 Ga2 70.92(15) 4_655 2_446
O3 O1 Ga2 88.36(15) 5_665 2_446
O3 O1 Ga2 62.06(18) 6_445 2_446
O3 O1 Ga2 160.4(3) 2_645 2_446
Ga3 O1 Ga2 75.45(8) 2_545 2_446
Ga3 O1 Ga2 147.5(4) 1_554 2_446
Ga3 O1 Ga2 94.80(11) 4_654 2_446
O3 O1 Ga2 69.64(19) 5_666 2_446
O3 O1 Ga2 41.80(17) 6_446 2_446
O3 O1 Ga2 122.0(4) 2_646 2_446
Nb O1 Ga2 65.75(3) . 2_446
Ga1 O1 Ga2 65.75(3) . 2_446
Nb O1 Ga2 172.7(5) 1_655 2_446
Ga1 O1 Ga2 172.7(5) 1_655 2_446
Ga1 O1 Ga2 65.75(3) 1_545 2_446
Nb O1 Ga2 65.75(3) 1_545 2_446
La1 O1 Ga2 82.2(2) 1_556 2_446
La1 O1 Ga2 43.42(11) 2_546 2_446
La1 O1 Ga2 93.5(3) 4_656 2_446
O2 O1 Ga2 96.87(17) . 2_446
O2 O1 Ga2 21.37(15) 3_545 2_446
O2 O1 Ga2 132.3(3) 4_655 2_446
Ga2 O1 Ga2 111.0(2) 2_556 2_446
Ga2 O1 Ga2 72.1(2) 1_545 2_546
La1 O1 Ga2 136.41(2) . 2_546
La1 O1 Ga2 110.77(4) 2_545 2_546
La1 O1 Ga2 40.33(19) 4_655 2_546
O2 O1 Ga2 137.3(5) 6 2_546
O2 O1 Ga2 101.4(3) 5_655 2_546
O2 O1 Ga2 80.7(2) 2_545 2_546
O2 O1 Ga2 101.8(5) 6_556 2_546
O2 O1 Ga2 71.5(3) 5_656 2_546
O2 O1 Ga2 48.1(3) 2_546 2_546
O3 O1 Ga2 155.1(6) 3_545 2_546
O3 O1 Ga2 64.6(2) 4_655 2_546
O3 O1 Ga2 54.5(2) . 2_546
Ga2 O1 Ga2 107.9(2) 1_544 2_546
O2 O1 Ga2 127.5(4) 4 2_546
O2 O1 Ga2 99.3(2) 3_655 2_546
O2 O1 Ga2 16.7(2) 1_545 2_546
Ga3 O1 Ga2 131.5(5) 2_546 2_546
Ga3 O1 Ga2 70.92(15) . 2_546
Ga3 O1 Ga2 40.28(7) 4_655 2_546
O3 O1 Ga2 160.4(3) 5_665 2_546
O3 O1 Ga2 88.36(15) 6_445 2_546
O3 O1 Ga2 62.06(18) 2_645 2_546
Ga3 O1 Ga2 147.5(4) 2_545 2_546
Ga3 O1 Ga2 94.80(11) 1_554 2_546
Ga3 O1 Ga2 75.45(8) 4_654 2_546
O3 O1 Ga2 122.0(4) 5_666 2_546
O3 O1 Ga2 69.64(19) 6_446 2_546
O3 O1 Ga2 41.80(17) 2_646 2_546
Nb O1 Ga2 172.7(5) . 2_546
Ga1 O1 Ga2 172.7(5) . 2_546
Nb O1 Ga2 65.75(3) 1_655 2_546
Ga1 O1 Ga2 65.75(3) 1_655 2_546
Ga1 O1 Ga2 65.75(3) 1_545 2_546
Nb O1 Ga2 65.75(3) 1_545 2_546
La1 O1 Ga2 93.5(3) 1_556 2_546
La1 O1 Ga2 82.2(2) 2_546 2_546
La1 O1 Ga2 43.42(11) 4_656 2_546
O2 O1 Ga2 132.3(3) . 2_546
O2 O1 Ga2 96.86(17) 3_545 2_546
O2 O1 Ga2 21.37(15) 4_655 2_546
Ga2 O1 Ga2 111.0(2) 2_556 2_546
Ga2 O1 Ga2 111.0(2) 2_446 2_546
Ga2 O1 O3 115.6(3) 1_545 2_545
La1 O1 O3 60.1(2) . 2_545
La1 O1 O3 50.15(18) 2_545 2_545
La1 O1 O3 134.0(7) 4_655 2_545
O2 O1 O3 31.3(3) 6 2_545
O2 O1 O3 81.6(4) 5_655 2_545
O2 O1 O3 85.2(4) 2_545 2_545
O2 O1 O3 83.5(3) 6_556 2_545
O2 O1 O3 125.1(4) 5_656 2_545
O2 O1 O3 129.4(4) 2_546 2_545
O3 O1 O3 40.0(3) 3_545 2_545
O3 O1 O3 97.5(3) 4_655 2_545
O3 O1 O3 141.2(4) . 2_545
Ga2 O1 O3 64.4(3) 1_544 2_545
O2 O1 O3 44.3(3) 4 2_545
O2 O1 O3 99.9(2) 3_655 2_545
O2 O1 O3 143.8(3) 1_545 2_545
Ga3 O1 O3 53.21(15) 2_546 2_545
Ga3 O1 O3 128.57(13) . 2_545
Ga3 O1 O3 125.13(12) 4_655 2_545
O3 O1 O3 33.0(3) 5_665 2_545
O3 O1 O3 72.2(3) 6_445 2_545
O3 O1 O3 121.3(6) 2_645 2_545
Ga3 O1 O3 21.58(16) 2_545 2_545
Ga3 O1 O3 90.5(3) 1_554 2_545
Ga3 O1 O3 88.4(3) 4_654 2_545
O3 O1 O3 72.20(15) 5_666 2_545
O3 O1 O3 100.1(2) 6_446 2_545
O3 O1 O3 157.2(3) 2_646 2_545
Nb O1 O3 23.64(14) . 2_545
Ga1 O1 O3 23.64(14) . 2_545
Nb O1 O3 126.4(3) 1_655 2_545
Ga1 O1 O3 126.4(3) 1_655 2_545
Ga1 O1 O3 94.81(19) 1_545 2_545
Nb O1 O3 94.81(19) 1_545 2_545
La1 O1 O3 100.89(19) 1_556 2_545
La1 O1 O3 96.5(2) 2_546 2_545
La1 O1 O3 145.2(4) 4_656 2_545
O2 O1 O3 67.2(2) . 2_545
O2 O1 O3 68.0(2) 3_545 2_545
O2 O1 O3 163.1(5) 4_655 2_545
Ga2 O1 O3 88.53(13) 2_556 2_545
Ga2 O1 O3 58.77(13) 2_446 2_545
Ga2 O1 O3 160.5(2) 2_546 2_545
Ga2 O1 O3 115.6(3) 1_545 6
La1 O1 O3 50.15(18) . 6
La1 O1 O3 134.0(7) 2_545 6
La1 O1 O3 60.1(2) 4_655 6
O2 O1 O3 85.2(4) 6 6
O2 O1 O3 31.3(3) 5_655 6
O2 O1 O3 81.6(4) 2_545 6
O2 O1 O3 129.4(4) 6_556 6
O2 O1 O3 83.5(3) 5_656 6
O2 O1 O3 125.1(4) 2_546 6
O3 O1 O3 97.5(3) 3_545 6
O3 O1 O3 141.2(4) 4_655 6
O3 O1 O3 40.0(3) . 6
Ga2 O1 O3 64.4(3) 1_544 6
O2 O1 O3 143.8(3) 4 6
O2 O1 O3 44.3(3) 3_655 6
O2 O1 O3 99.9(2) 1_545 6
Ga3 O1 O3 125.13(12) 2_546 6
Ga3 O1 O3 53.21(15) . 6
Ga3 O1 O3 128.57(13) 4_655 6
O3 O1 O3 72.2(3) 5_665 6
O3 O1 O3 121.3(6) 6_445 6
O3 O1 O3 33.0(3) 2_645 6
Ga3 O1 O3 88.4(3) 2_545 6
Ga3 O1 O3 21.58(16) 1_554 6
Ga3 O1 O3 90.5(3) 4_654 6
O3 O1 O3 100.1(2) 5_666 6
O3 O1 O3 157.2(3) 6_446 6
O3 O1 O3 72.20(15) 2_646 6
Nb O1 O3 94.81(19) . 6
Ga1 O1 O3 94.81(19) . 6
Nb O1 O3 23.64(14) 1_655 6
Ga1 O1 O3 23.64(14) 1_655 6
Ga1 O1 O3 126.4(3) 1_545 6
Nb O1 O3 126.4(3) 1_545 6
La1 O1 O3 96.5(2) 1_556 6
La1 O1 O3 145.2(4) 2_546 6
La1 O1 O3 100.89(19) 4_656 6
O2 O1 O3 68.0(2) . 6
O2 O1 O3 163.1(5) 3_545 6
O2 O1 O3 67.2(2) 4_655 6
Ga2 O1 O3 58.77(13) 2_556 6
Ga2 O1 O3 160.5(2) 2_446 6
Ga2 O1 O3 88.53(13) 2_546 6
O3 O1 O3 102.7(3) 2_545 6
Ga2 O1 O3 115.6(3) 1_545 5_655
La1 O1 O3 134.0(7) . 5_655
La1 O1 O3 60.1(2) 2_545 5_655
La1 O1 O3 50.15(18) 4_655 5_655
O2 O1 O3 81.6(4) 6 5_655
O2 O1 O3 85.2(4) 5_655 5_655
O2 O1 O3 31.3(3) 2_545 5_655
O2 O1 O3 125.1(4) 6_556 5_655
O2 O1 O3 129.4(4) 5_656 5_655
O2 O1 O3 83.5(3) 2_546 5_655
O3 O1 O3 141.2(4) 3_545 5_655
O3 O1 O3 40.0(3) 4_655 5_655
O3 O1 O3 97.5(3) . 5_655
Ga2 O1 O3 64.4(3) 1_544 5_655
O2 O1 O3 99.9(2) 4 5_655
O2 O1 O3 143.8(3) 3_655 5_655
O2 O1 O3 44.3(3) 1_545 5_655
Ga3 O1 O3 128.57(13) 2_546 5_655
Ga3 O1 O3 125.13(12) . 5_655
Ga3 O1 O3 53.21(15) 4_655 5_655
O3 O1 O3 121.3(6) 5_665 5_655
O3 O1 O3 33.0(3) 6_445 5_655
O3 O1 O3 72.2(3) 2_645 5_655
Ga3 O1 O3 90.5(3) 2_545 5_655
Ga3 O1 O3 88.4(3) 1_554 5_655
Ga3 O1 O3 21.58(16) 4_654 5_655
O3 O1 O3 157.2(3) 5_666 5_655
O3 O1 O3 72.20(15) 6_446 5_655
O3 O1 O3 100.1(2) 2_646 5_655
Nb O1 O3 126.4(3) . 5_655
Ga1 O1 O3 126.4(3) . 5_655
Nb O1 O3 94.81(19) 1_655 5_655
Ga1 O1 O3 94.81(19) 1_655 5_655
Ga1 O1 O3 23.64(14) 1_545 5_655
Nb O1 O3 23.64(14) 1_545 5_655
La1 O1 O3 145.2(4) 1_556 5_655
La1 O1 O3 100.89(19) 2_546 5_655
La1 O1 O3 96.5(2) 4_656 5_655
O2 O1 O3 163.1(5) . 5_655
O2 O1 O3 67.2(2) 3_545 5_655
O2 O1 O3 68.0(2) 4_655 5_655
Ga2 O1 O3 160.5(2) 2_556 5_655
Ga2 O1 O3 88.53(13) 2_446 5_655
Ga2 O1 O3 58.77(13) 2_546 5_655
O3 O1 O3 102.7(3) 2_545 5_655
O3 O1 O3 102.7(3) 6 5_655
Ga2 O1 O1 110.6(4) 1_545 2_655
La1 O1 O1 12.96(4) . 2_655
La1 O1 O1 119.2(5) 2_545 2_655
La1 O1 O1 97.1(4) 4_655 2_655
O2 O1 O1 69.4(5) 6 2_655
O2 O1 O1 45.0(3) 5_655 2_655
O2 O1 O1 100.1(7) 2_545 2_655
O2 O1 O1 104.0(4) 6_556 2_655
O2 O1 O1 84.1(3) 5_656 2_655
O2 O1 O1 139.0(7) 2_546 2_655
O3 O1 O1 60.1(2) 3_545 2_655
O3 O1 O1 164.9(7) 4_655 2_655
O3 O1 O1 69.6(2) . 2_655
Ga2 O1 O1 69.4(4) 1_544 2_655
O2 O1 O1 107.0(2) 4 2_655
O2 O1 O1 36.0(3) 3_655 2_655
O2 O1 O1 137.0(2) 1_545 2_655
Ga3 O1 O1 88.95(11) 2_546 2_655
Ga3 O1 O1 63.44(12) . 2_655
Ga3 O1 O1 162.7(3) 4_655 2_655
O3 O1 O1 39.05(19) 5_665 2_655
O3 O1 O1 127.7(7) 6_445 2_655
O3 O1 O1 69.9(3) 2_645 2_655
Ga3 O1 O1 66.6(3) 2_545 2_655
Ga3 O1 O1 43.4(3) 1_554 2_655
Ga3 O1 O1 110.5(6) 4_654 2_655
O3 O1 O1 70.5(3) 5_666 2_655
O3 O1 O1 157.1(5) 6_446 2_655
O3 O1 O1 93.3(2) 2_646 2_655
Nb O1 O1 58.33(7) . 2_655
Ga1 O1 O1 58.33(7) . 2_655
Nb O1 O1 58.33(7) 1_655 2_655
Ga1 O1 O1 58.33(7) 1_655 2_655
Ga1 O1 O1 148.7(7) 1_545 2_655
Nb O1 O1 148.7(7) 1_545 2_655
La1 O1 O1 81.6(3) 1_556 2_655
La1 O1 O1 128.9(4) 2_546 2_655
La1 O1 O1 115.8(4) 4_656 2_655
O2 O1 O1 35.2(3) . 2_655
O2 O1 O1 139.5(2) 3_545 2_655
O2 O1 O1 102.50(15) 4_655 2_655
Ga2 O1 O1 38.5(2) 2_556 2_655
Ga2 O1 O1 123.614(14) 2_446 2_655
Ga2 O1 O1 123.614(14) 2_546 2_655
O3 O1 O1 72.1(3) 2_545 2_655
O3 O1 O1 37.56(16) 6 2_655
O3 O1 O1 130.1(6) 5_655 2_655
Ga2 O1 O1 110.6(4) 1_545 2_545
La1 O1 O1 97.1(4) . 2_545
La1 O1 O1 12.96(4) 2_545 2_545
La1 O1 O1 119.2(5) 4_655 2_545
O2 O1 O1 45.0(3) 6 2_545
O2 O1 O1 100.1(7) 5_655 2_545
O2 O1 O1 69.4(5) 2_545 2_545
O2 O1 O1 84.1(3) 6_556 2_545
O2 O1 O1 139.0(7) 5_656 2_545
O2 O1 O1 104.0(4) 2_546 2_545
O3 O1 O1 69.6(2) 3_545 2_545
O3 O1 O1 60.1(2) 4_655 2_545
O3 O1 O1 164.9(7) . 2_545
Ga2 O1 O1 69.4(4) 1_544 2_545
O2 O1 O1 36.0(3) 4 2_545
O2 O1 O1 137.0(2) 3_655 2_545
O2 O1 O1 107.0(2) 1_545 2_545
Ga3 O1 O1 63.44(12) 2_546 2_545
Ga3 O1 O1 162.7(3) . 2_545
Ga3 O1 O1 88.95(11) 4_655 2_545
O3 O1 O1 69.9(3) 5_665 2_545
O3 O1 O1 39.04(19) 6_445 2_545
O3 O1 O1 127.7(7) 2_645 2_545
Ga3 O1 O1 43.4(3) 2_545 2_545
Ga3 O1 O1 110.5(6) 1_554 2_545
Ga3 O1 O1 66.6(3) 4_654 2_545
O3 O1 O1 93.3(2) 5_666 2_545
O3 O1 O1 70.5(3) 6_446 2_545
O3 O1 O1 157.1(5) 2_646 2_545
Nb O1 O1 58.33(7) . 2_545
Ga1 O1 O1 58.33(7) . 2_545
Nb O1 O1 148.7(7) 1_655 2_545
Ga1 O1 O1 148.7(7) 1_655 2_545
Ga1 O1 O1 58.33(7) 1_545 2_545
Nb O1 O1 58.33(7) 1_545 2_545
La1 O1 O1 115.8(4) 1_556 2_545
La1 O1 O1 81.6(3) 2_546 2_545
La1 O1 O1 128.9(4) 4_656 2_545
O2 O1 O1 102.50(15) . 2_545
O2 O1 O1 35.2(3) 3_545 2_545
O2 O1 O1 139.5(2) 4_655 2_545
Ga2 O1 O1 123.614(14) 2_556 2_545
Ga2 O1 O1 38.5(2) 2_446 2_545
Ga2 O1 O1 123.613(14) 2_546 2_545
O3 O1 O1 37.56(16) 2_545 2_545
O3 O1 O1 130.1(6) 6 2_545
O3 O1 O1 72.1(3) 5_655 2_545
O1 O1 O1 108.3(4) 2_655 2_545
Ga2 O1 O1 110.6(4) 1_545 2_645
La1 O1 O1 119.2(5) . 2_645
La1 O1 O1 97.1(4) 2_545 2_645
La1 O1 O1 12.96(4) 4_655 2_645
O2 O1 O1 100.1(7) 6 2_645
O2 O1 O1 69.4(5) 5_655 2_645
O2 O1 O1 45.0(3) 2_545 2_645
O2 O1 O1 139.0(7) 6_556 2_645
O2 O1 O1 104.0(4) 5_656 2_645
O2 O1 O1 84.1(3) 2_546 2_645
O3 O1 O1 164.9(7) 3_545 2_645
O3 O1 O1 69.6(2) 4_655 2_645
O3 O1 O1 60.1(2) . 2_645
Ga2 O1 O1 69.4(4) 1_544 2_645
O2 O1 O1 137.0(2) 4 2_645
O2 O1 O1 107.0(2) 3_655 2_645
O2 O1 O1 36.0(3) 1_545 2_645
Ga3 O1 O1 162.7(3) 2_546 2_645
Ga3 O1 O1 88.95(11) . 2_645
Ga3 O1 O1 63.44(12) 4_655 2_645
O3 O1 O1 127.7(7) 5_665 2_645
O3 O1 O1 69.9(3) 6_445 2_645
O3 O1 O1 39.04(19) 2_645 2_645
Ga3 O1 O1 110.5(6) 2_545 2_645
Ga3 O1 O1 66.6(3) 1_554 2_645
Ga3 O1 O1 43.4(3) 4_654 2_645
O3 O1 O1 157.1(5) 5_666 2_645
O3 O1 O1 93.3(2) 6_446 2_645
O3 O1 O1 70.5(3) 2_646 2_645
Nb O1 O1 148.7(7) . 2_645
Ga1 O1 O1 148.7(7) . 2_645
Nb O1 O1 58.33(7) 1_655 2_645
Ga1 O1 O1 58.33(7) 1_655 2_645
Ga1 O1 O1 58.33(7) 1_545 2_645
Nb O1 O1 58.33(7) 1_545 2_645
La1 O1 O1 128.9(4) 1_556 2_645
La1 O1 O1 115.8(4) 2_546 2_645
La1 O1 O1 81.6(3) 4_656 2_645
O2 O1 O1 139.5(2) . 2_645
O2 O1 O1 102.50(15) 3_545 2_645
O2 O1 O1 35.2(3) 4_655 2_645
Ga2 O1 O1 123.614(14) 2_556 2_645
Ga2 O1 O1 123.614(14) 2_446 2_645
Ga2 O1 O1 38.5(2) 2_546 2_645
O3 O1 O1 130.1(6) 2_545 2_645
O3 O1 O1 72.1(3) 6 2_645
O3 O1 O1 37.56(16) 5_655 2_645
O1 O1 O1 108.3(4) 2_655 2_645
O1 O1 O1 108.3(4) 2_545 2_645
Ga2 O1 O1 0.002(1) 1_545 1_556
La1 O1 O1 110.1(4) . 1_556
La1 O1 O1 110.1(4) 2_545 1_556
La1 O1 O1 110.1(4) 4_655 1_556
O2 O1 O1 146.8(3) 6 1_556
O2 O1 O1 146.8(3) 5_655 1_556
O2 O1 O1 146.8(3) 2_545 1_556
O2 O1 O1 32.2(3) 6_556 1_556
O2 O1 O1 32.2(3) 5_656 1_556
O2 O1 O1 32.2(3) 2_546 1_556
O3 O1 O1 83.6(4) 3_545 1_556
O3 O1 O1 83.6(4) 4_655 1_556
O3 O1 O1 83.6(4) . 1_556
Ga2 O1 O1 179.999(1) 1_544 1_556
O2 O1 O1 78.2(4) 4 1_556
O2 O1 O1 78.2(4) 3_655 1_556
O2 O1 O1 78.2(4) 1_545 1_556
Ga3 O1 O1 62.4(3) 2_546 1_556
Ga3 O1 O1 62.4(3) . 1_556
Ga3 O1 O1 62.4(3) 4_655 1_556
O3 O1 O1 118.8(3) 5_665 1_556
O3 O1 O1 118.8(3) 6_445 1_556
O3 O1 O1 118.8(3) 2_645 1_556
Ga3 O1 O1 137.10(17) 2_545 1_556
Ga3 O1 O1 137.10(17) 1_554 1_556
Ga3 O1 O1 137.10(17) 4_654 1_556
O3 O1 O1 52.3(2) 5_666 1_556
O3 O1 O1 52.3(2) 6_446 1_556
O3 O1 O1 52.3(2) 2_646 1_556
Nb O1 O1 100.7(2) . 1_556
Ga1 O1 O1 100.7(2) . 1_556
Nb O1 O1 100.7(2) 1_655 1_556
Ga1 O1 O1 100.7(2) 1_655 1_556
Ga1 O1 O1 100.7(2) 1_545 1_556
Nb O1 O1 100.7(2) 1_545 1_556
La1 O1 O1 29.82(12) 1_556 1_556
La1 O1 O1 29.82(12) 2_546 1_556
La1 O1 O1 29.82(12) 4_656 1_556
O2 O1 O1 81.3(3) . 1_556
O2 O1 O1 81.3(3) 3_545 1_556
O2 O1 O1 81.3(3) 4_655 1_556
Ga2 O1 O1 72.1(2) 2_556 1_556
Ga2 O1 O1 72.1(2) 2_446 1_556
Ga2 O1 O1 72.1(2) 2_546 1_556
O3 O1 O1 115.6(3) 2_545 1_556
O3 O1 O1 115.6(3) 6 1_556
O3 O1 O1 115.6(3) 5_655 1_556
O1 O1 O1 110.6(4) 2_655 1_556
O1 O1 O1 110.6(4) 2_545 1_556
O1 O1 O1 110.6(4) 2_645 1_556
Ga2 O1 O1 179.998(1) 1_545 1_554
La1 O1 O1 69.9(4) . 1_554
La1 O1 O1 69.9(4) 2_545 1_554
La1 O1 O1 69.9(4) 4_655 1_554
O2 O1 O1 33.2(3) 6 1_554
O2 O1 O1 33.2(3) 5_655 1_554
O2 O1 O1 33.2(3) 2_545 1_554
O2 O1 O1 147.8(3) 6_556 1_554
O2 O1 O1 147.8(3) 5_656 1_554
O2 O1 O1 147.8(3) 2_546 1_554
O3 O1 O1 96.4(4) 3_545 1_554
O3 O1 O1 96.4(4) 4_655 1_554
O3 O1 O1 96.4(4) . 1_554
Ga2 O1 O1 0.0 1_544 1_554
O2 O1 O1 101.8(4) 4 1_554
O2 O1 O1 101.8(4) 3_655 1_554
O2 O1 O1 101.8(4) 1_545 1_554
Ga3 O1 O1 117.6(3) 2_546 1_554
Ga3 O1 O1 117.6(3) . 1_554
Ga3 O1 O1 117.6(3) 4_655 1_554
O3 O1 O1 61.2(3) 5_665 1_554
O3 O1 O1 61.2(3) 6_445 1_554
O3 O1 O1 61.2(3) 2_645 1_554
Ga3 O1 O1 42.90(17) 2_545 1_554
Ga3 O1 O1 42.90(17) 1_554 1_554
Ga3 O1 O1 42.90(17) 4_654 1_554
O3 O1 O1 127.7(2) 5_666 1_554
O3 O1 O1 127.7(2) 6_446 1_554
O3 O1 O1 127.7(2) 2_646 1_554
Nb O1 O1 79.3(2) . 1_554
Ga1 O1 O1 79.3(2) . 1_554
Nb O1 O1 79.3(2) 1_655 1_554
Ga1 O1 O1 79.3(2) 1_655 1_554
Ga1 O1 O1 79.3(2) 1_545 1_554
Nb O1 O1 79.3(2) 1_545 1_554
La1 O1 O1 150.18(12) 1_556 1_554
La1 O1 O1 150.18(12) 2_546 1_554
La1 O1 O1 150.18(12) 4_656 1_554
O2 O1 O1 98.7(3) . 1_554
O2 O1 O1 98.7(3) 3_545 1_554
O2 O1 O1 98.7(3) 4_655 1_554
Ga2 O1 O1 107.9(2) 2_556 1_554
Ga2 O1 O1 107.9(2) 2_446 1_554
Ga2 O1 O1 107.9(2) 2_546 1_554
O3 O1 O1 64.4(3) 2_545 1_554
O3 O1 O1 64.4(3) 6 1_554
O3 O1 O1 64.4(3) 5_655 1_554
O1 O1 O1 69.4(4) 2_655 1_554
O1 O1 O1 69.4(4) 2_545 1_554
O1 O1 O1 69.4(4) 2_645 1_554
O1 O1 O1 180.000(1) 1_556 1_554
Ga2 O1 Ga3 71.8(2) 1_545 4_665
La1 O1 Ga3 45.00(18) . 4_665
La1 O1 Ga3 101.48(6) 2_545 4_665
La1 O1 Ga3 146.10(4) 4_655 4_665
O2 O1 Ga3 84.1(3) 6 4_665
O2 O1 Ga3 97.0(3) 5_655 4_665
O2 O1 Ga3 140.0(5) 2_545 4_665
O2 O1 Ga3 51.8(3) 6_556 4_665
O2 O1 Ga3 66.4(3) 5_656 4_665
O2 O1 Ga3 103.0(5) 2_546 4_665
O3 O1 Ga3 20.1(2) 3_545 4_665
O3 O1 Ga3 130.7(3) 4_655 4_665
O3 O1 Ga3 100.4(3) . 4_665
Ga2 O1 Ga3 108.2(2) 1_544 4_665
O2 O1 Ga3 63.8(2) 4 4_665
O2 O1 Ga3 52.4(2) 3_655 4_665
O2 O1 Ga3 149.4(5) 1_545 4_665
Ga3 O1 Ga3 37.37(7) 2_546 4_665
Ga3 O1 Ga3 73.55(15) . 4_665
Ga3 O1 Ga3 130.1(4) 4_655 4_665
O3 O1 Ga3 47.24(19) 5_665 4_665
O3 O1 Ga3 128.33(16) 6_445 4_665
O3 O1 Ga3 120.73(17) 2_645 4_665
Ga3 O1 Ga3 74.33(6) 2_545 4_665
Ga3 O1 Ga3 97.05(10) 1_554 4_665
Ga3 O1 Ga3 146.6(3) 4_654 4_665
O3 O1 Ga3 19.81(14) 5_666 4_665
O3 O1 Ga3 103.5(3) 6_446 4_665
O3 O1 Ga3 97.7(3) 2_646 4_665
Nb O1 Ga3 36.18(3) . 4_665
Ga1 O1 Ga3 36.18(3) . 4_665
Nb O1 Ga3 100.74(5) 1_655 4_665
Ga1 O1 Ga3 100.74(5) 1_655 4_665
Ga1 O1 Ga3 142.59(9) 1_545 4_665
Nb O1 Ga3 142.59(9) 1_545 4_665
La1 O1 Ga3 45.38(10) 1_556 4_665
La1 O1 Ga3 77.1(2) 2_546 4_665
La1 O1 Ga3 96.4(3) 4_656 4_665
O2 O1 Ga3 19.98(15) . 4_665
O2 O1 Ga3 98.44(19) 3_545 4_665
O2 O1 Ga3 130.7(2) 4_655 4_665
Ga2 O1 Ga3 35.98(5) 2_556 4_665
Ga2 O1 Ga3 77.26(12) 2_446 4_665
Ga2 O1 Ga3 137.8(4) 2_546 4_665
O3 O1 Ga3 59.52(14) 2_545 4_665
O3 O1 Ga3 87.99(13) 6 4_665
O3 O1 Ga3 161.3(2) 5_655 4_665
O1 O1 Ga3 53.75(15) 2_655 4_665
O1 O1 Ga3 89.29(7) 2_545 4_665
O1 O1 Ga3 159.05(7) 2_645 4_665
O1 O1 Ga3 71.8(2) 1_556 4_665
O1 O1 Ga3 108.2(2) 1_554 4_665
Ga2 O1 Ga3 71.8(2) 1_545 1_445
La1 O1 Ga3 146.10(4) . 1_445
La1 O1 Ga3 45.00(18) 2_545 1_445
La1 O1 Ga3 101.48(6) 4_655 1_445
O2 O1 Ga3 97.0(3) 6 1_445
O2 O1 Ga3 140.0(5) 5_655 1_445
O2 O1 Ga3 84.1(3) 2_545 1_445
O2 O1 Ga3 66.4(3) 6_556 1_445
O2 O1 Ga3 103.0(5) 5_656 1_445
O2 O1 Ga3 51.8(2) 2_546 1_445
O3 O1 Ga3 100.4(3) 3_545 1_445
O3 O1 Ga3 20.1(2) 4_655 1_445
O3 O1 Ga3 130.7(3) . 1_445
Ga2 O1 Ga3 108.2(2) 1_544 1_445
O2 O1 Ga3 52.4(2) 4 1_445
O2 O1 Ga3 149.4(5) 3_655 1_445
O2 O1 Ga3 63.8(2) 1_545 1_445
Ga3 O1 Ga3 73.55(15) 2_546 1_445
Ga3 O1 Ga3 130.1(4) . 1_445
Ga3 O1 Ga3 37.37(7) 4_655 1_445
O3 O1 Ga3 120.73(17) 5_665 1_445
O3 O1 Ga3 47.24(19) 6_445 1_445
O3 O1 Ga3 128.33(16) 2_645 1_445
Ga3 O1 Ga3 97.05(10) 2_545 1_445
Ga3 O1 Ga3 146.6(3) 1_554 1_445
Ga3 O1 Ga3 74.32(6) 4_654 1_445
O3 O1 Ga3 97.7(3) 5_666 1_445
O3 O1 Ga3 19.80(14) 6_446 1_445
O3 O1 Ga3 103.5(3) 2_646 1_445
Nb O1 Ga3 100.74(5) . 1_445
Ga1 O1 Ga3 100.74(5) . 1_445
Nb O1 Ga3 142.59(9) 1_655 1_445
Ga1 O1 Ga3 142.59(9) 1_655 1_445
Ga1 O1 Ga3 36.18(3) 1_545 1_445
Nb O1 Ga3 36.18(3) 1_545 1_445
La1 O1 Ga3 96.4(3) 1_556 1_445
La1 O1 Ga3 45.38(10) 2_546 1_445
La1 O1 Ga3 77.1(2) 4_656 1_445
O2 O1 Ga3 130.7(2) . 1_445
O2 O1 Ga3 19.97(15) 3_545 1_445
O2 O1 Ga3 98.44(19) 4_655 1_445
Ga2 O1 Ga3 137.8(4) 2_556 1_445
Ga2 O1 Ga3 35.98(5) 2_446 1_445
Ga2 O1 Ga3 77.26(12) 2_546 1_445
O3 O1 Ga3 87.99(13) 2_545 1_445
O3 O1 Ga3 161.3(2) 6 1_445
O3 O1 Ga3 59.52(14) 5_655 1_445
O1 O1 Ga3 159.05(6) 2_655 1_445
O1 O1 Ga3 53.75(15) 2_545 1_445
O1 O1 Ga3 89.29(7) 2_645 1_445
O1 O1 Ga3 71.8(2) 1_556 1_445
O1 O1 Ga3 108.2(2) 1_554 1_445
Ga3 O1 Ga3 110.7(2) 4_665 1_445
Ga2 O1 Ga3 71.8(2) 1_545 2_646
La1 O1 Ga3 101.48(6) . 2_646
La1 O1 Ga3 146.10(4) 2_545 2_646
La1 O1 Ga3 45.00(18) 4_655 2_646
O2 O1 Ga3 140.0(5) 6 2_646
O2 O1 Ga3 84.1(3) 5_655 2_646
O2 O1 Ga3 97.0(3) 2_545 2_646
O2 O1 Ga3 103.0(5) 6_556 2_646
O2 O1 Ga3 51.8(3) 5_656 2_646
O2 O1 Ga3 66.4(3) 2_546 2_646
O3 O1 Ga3 130.7(3) 3_545 2_646
O3 O1 Ga3 100.4(3) 4_655 2_646
O3 O1 Ga3 20.1(2) . 2_646
Ga2 O1 Ga3 108.2(2) 1_544 2_646
O2 O1 Ga3 149.4(5) 4 2_646
O2 O1 Ga3 63.8(2) 3_655 2_646
O2 O1 Ga3 52.4(2) 1_545 2_646
Ga3 O1 Ga3 130.1(4) 2_546 2_646
Ga3 O1 Ga3 37.37(7) . 2_646
Ga3 O1 Ga3 73.55(15) 4_655 2_646
O3 O1 Ga3 128.33(16) 5_665 2_646
O3 O1 Ga3 120.73(17) 6_445 2_646
O3 O1 Ga3 47.24(19) 2_645 2_646
Ga3 O1 Ga3 146.6(3) 2_545 2_646
Ga3 O1 Ga3 74.32(6) 1_554 2_646
Ga3 O1 Ga3 97.05(10) 4_654 2_646
O3 O1 Ga3 103.5(3) 5_666 2_646
O3 O1 Ga3 97.7(3) 6_446 2_646
O3 O1 Ga3 19.80(14) 2_646 2_646
Nb O1 Ga3 142.59(9) . 2_646
Ga1 O1 Ga3 142.59(9) . 2_646
Nb O1 Ga3 36.18(3) 1_655 2_646
Ga1 O1 Ga3 36.18(3) 1_655 2_646
Ga1 O1 Ga3 100.74(5) 1_545 2_646
Nb O1 Ga3 100.74(5) 1_545 2_646
La1 O1 Ga3 77.1(2) 1_556 2_646
La1 O1 Ga3 96.4(3) 2_546 2_646
La1 O1 Ga3 45.38(10) 4_656 2_646
O2 O1 Ga3 98.44(19) . 2_646
O2 O1 Ga3 130.7(2) 3_545 2_646
O2 O1 Ga3 19.97(15) 4_655 2_646
Ga2 O1 Ga3 77.26(12) 2_556 2_646
Ga2 O1 Ga3 137.8(4) 2_446 2_646
Ga2 O1 Ga3 35.98(5) 2_546 2_646
O3 O1 Ga3 161.3(2) 2_545 2_646
O3 O1 Ga3 59.52(14) 6 2_646
O3 O1 Ga3 87.99(13) 5_655 2_646
O1 O1 Ga3 89.29(7) 2_655 2_646
O1 O1 Ga3 159.05(6) 2_545 2_646
O1 O1 Ga3 53.75(15) 2_645 2_646
O1 O1 Ga3 71.8(2) 1_556 2_646
O1 O1 Ga3 108.2(2) 1_554 2_646
Ga3 O1 Ga3 110.7(2) 4_665 2_646
Ga3 O1 Ga3 110.7(2) 1_445 2_646
Ga2 O1 O3 56.1(3) 1_545 2_546
La1 O1 O3 82.4(2) . 2_546
La1 O1 O3 74.8(2) 2_545 2_546
La1 O1 O3 165.4(6) 4_655 2_546
O2 O1 O3 90.7(3) 6 2_546
O2 O1 O3 131.6(3) 5_655 2_546
O2 O1 O3 136.2(3) 2_545 2_546
O2 O1 O3 24.1(3) 6_556 2_546
O2 O1 O3 73.8(4) 5_656 2_546
O2 O1 O3 77.1(5) 2_546 2_546
O3 O1 O3 35.7(3) 3_545 2_546
O3 O1 O3 90.8(3) 4_655 2_546
O3 O1 O3 127.7(5) . 2_546
Ga2 O1 O3 123.9(3) 1_544 2_546
O2 O1 O3 31.5(3) 4 2_546
O2 O1 O3 87.9(3) 3_655 2_546
O2 O1 O3 123.3(5) 1_545 2_546
Ga3 O1 O3 6.49(17) 2_546 2_546
Ga3 O1 O3 97.6(4) . 2_546
Ga3 O1 O3 95.0(4) 4_655 2_546
O3 O1 O3 71.85(16) 5_665 2_546
O3 O1 O3 100.3(2) 6_445 2_546
O3 O1 O3 159.9(3) 2_645 2_546
Ga3 O1 O3 80.98(16) 2_545 2_546
Ga3 O1 O3 135.04(18) 1_554 2_546
Ga3 O1 O3 132.34(15) 4_654 2_546
O3 O1 O3 30.2(2) 5_666 2_546
O3 O1 O3 65.1(3) 6_446 2_546
O3 O1 O3 105.4(4) 2_646 2_546
Nb O1 O3 48.16(15) . 2_546
Ga1 O1 O3 48.16(15) . 2_546
Nb O1 O3 136.2(2) 1_655 2_546
Ga1 O1 O3 136.2(2) 1_655 2_546
Ga1 O1 O3 104.69(17) 1_545 2_546
Nb O1 O3 104.69(17) 1_545 2_546
La1 O1 O3 49.1(2) 1_556 2_546
La1 O1 O3 43.7(2) 2_546 2_546
La1 O1 O3 85.9(4) 4_656 2_546
O2 O1 O3 60.0(2) . 2_546
O2 O1 O3 60.7(2) 3_545 2_546
O2 O1 O3 137.5(5) 4_655 2_546
Ga2 O1 O3 71.51(17) 2_556 2_546
Ga2 O1 O3 39.56(14) 2_446 2_546
Ga2 O1 O3 125.0(4) 2_546 2_546
O3 O1 O3 59.43(13) 2_545 2_546
O3 O1 O3 127.96(8) 6 2_546
O3 O1 O3 127.96(8) 5_655 2_546
O1 O1 O3 93.0(2) 2_655 2_546
O1 O1 O3 66.8(2) 2_545 2_546
O1 O1 O3 158.4(4) 2_645 2_546
O1 O1 O3 56.1(3) 1_556 2_546
O1 O1 O3 123.9(3) 1_554 2_546
Ga3 O1 O3 40.06(13) 4_665 2_546
Ga3 O1 O3 70.69(19) 1_445 2_546
Ga3 O1 O3 125.0(4) 2_646 2_546
Ga2 O1 O3 56.1(3) 1_545 6_556
La1 O1 O3 74.8(2) . 6_556
La1 O1 O3 165.4(6) 2_545 6_556
La1 O1 O3 82.4(2) 4_655 6_556
O2 O1 O3 136.2(3) 6 6_556
O2 O1 O3 90.7(3) 5_655 6_556
O2 O1 O3 131.6(3) 2_545 6_556
O2 O1 O3 77.1(5) 6_556 6_556
O2 O1 O3 24.1(3) 5_656 6_556
O2 O1 O3 73.8(4) 2_546 6_556
O3 O1 O3 90.8(3) 3_545 6_556
O3 O1 O3 127.7(5) 4_655 6_556
O3 O1 O3 35.7(3) . 6_556
Ga2 O1 O3 123.9(3) 1_544 6_556
O2 O1 O3 123.3(5) 4 6_556
O2 O1 O3 31.5(3) 3_655 6_556
O2 O1 O3 87.9(3) 1_545 6_556
Ga3 O1 O3 95.0(4) 2_546 6_556
Ga3 O1 O3 6.49(17) . 6_556
Ga3 O1 O3 97.6(4) 4_655 6_556
O3 O1 O3 100.3(2) 5_665 6_556
O3 O1 O3 159.9(3) 6_445 6_556
O3 O1 O3 71.85(16) 2_645 6_556
Ga3 O1 O3 132.34(15) 2_545 6_556
Ga3 O1 O3 80.98(16) 1_554 6_556
Ga3 O1 O3 135.04(18) 4_654 6_556
O3 O1 O3 65.1(3) 5_666 6_556
O3 O1 O3 105.4(4) 6_446 6_556
O3 O1 O3 30.2(2) 2_646 6_556
Nb O1 O3 104.69(17) . 6_556
Ga1 O1 O3 104.69(17) . 6_556
Nb O1 O3 48.16(15) 1_655 6_556
Ga1 O1 O3 48.16(15) 1_655 6_556
Ga1 O1 O3 136.2(2) 1_545 6_556
Nb O1 O3 136.2(2) 1_545 6_556
La1 O1 O3 43.7(2) 1_556 6_556
La1 O1 O3 85.9(4) 2_546 6_556
La1 O1 O3 49.1(2) 4_656 6_556
O2 O1 O3 60.7(2) . 6_556
O2 O1 O3 137.5(5) 3_545 6_556
O2 O1 O3 60.0(2) 4_655 6_556
Ga2 O1 O3 39.56(14) 2_556 6_556
Ga2 O1 O3 125.0(4) 2_446 6_556
Ga2 O1 O3 71.51(17) 2_546 6_556
O3 O1 O3 127.96(8) 2_545 6_556
O3 O1 O3 59.43(13) 6 6_556
O3 O1 O3 127.96(8) 5_655 6_556
O1 O1 O3 66.8(2) 2_655 6_556
O1 O1 O3 158.4(4) 2_545 6_556
O1 O1 O3 93.0(2) 2_645 6_556
O1 O1 O3 56.1(3) 1_556 6_556
O1 O1 O3 123.9(3) 1_554 6_556
Ga3 O1 O3 70.69(19) 4_665 6_556
Ga3 O1 O3 125.0(4) 1_445 6_556
Ga3 O1 O3 40.06(13) 2_646 6_556
O3 O1 O3 92.0(4) 2_546 6_556
Ga2 O1 O3 56.1(3) 1_545 5_656
La1 O1 O3 165.4(6) . 5_656
La1 O1 O3 82.4(2) 2_545 5_656
La1 O1 O3 74.8(2) 4_655 5_656
O2 O1 O3 131.6(3) 6 5_656
O2 O1 O3 136.2(3) 5_655 5_656
O2 O1 O3 90.7(3) 2_545 5_656
O2 O1 O3 73.8(4) 6_556 5_656
O2 O1 O3 77.1(5) 5_656 5_656
O2 O1 O3 24.1(3) 2_546 5_656
O3 O1 O3 127.7(5) 3_545 5_656
O3 O1 O3 35.7(3) 4_655 5_656
O3 O1 O3 90.8(3) . 5_656
Ga2 O1 O3 123.9(3) 1_544 5_656
O2 O1 O3 87.9(3) 4 5_656
O2 O1 O3 123.3(5) 3_655 5_656
O2 O1 O3 31.5(3) 1_545 5_656
Ga3 O1 O3 97.6(4) 2_546 5_656
Ga3 O1 O3 95.0(4) . 5_656
Ga3 O1 O3 6.49(17) 4_655 5_656
O3 O1 O3 159.9(3) 5_665 5_656
O3 O1 O3 71.85(16) 6_445 5_656
O3 O1 O3 100.3(2) 2_645 5_656
Ga3 O1 O3 135.04(18) 2_545 5_656
Ga3 O1 O3 132.34(15) 1_554 5_656
Ga3 O1 O3 80.98(16) 4_654 5_656
O3 O1 O3 105.4(4) 5_666 5_656
O3 O1 O3 30.2(2) 6_446 5_656
O3 O1 O3 65.1(3) 2_646 5_656
Nb O1 O3 136.2(2) . 5_656
Ga1 O1 O3 136.2(2) . 5_656
Nb O1 O3 104.69(17) 1_655 5_656
Ga1 O1 O3 104.69(17) 1_655 5_656
Ga1 O1 O3 48.16(15) 1_545 5_656
Nb O1 O3 48.16(15) 1_545 5_656
La1 O1 O3 85.9(4) 1_556 5_656
La1 O1 O3 49.1(2) 2_546 5_656
La1 O1 O3 43.7(2) 4_656 5_656
O2 O1 O3 137.5(5) . 5_656
O2 O1 O3 60.0(2) 3_545 5_656
O2 O1 O3 60.7(2) 4_655 5_656
Ga2 O1 O3 125.0(4) 2_556 5_656
Ga2 O1 O3 71.51(17) 2_446 5_656
Ga2 O1 O3 39.56(14) 2_546 5_656
O3 O1 O3 127.96(8) 2_545 5_656
O3 O1 O3 127.96(8) 6 5_656
O3 O1 O3 59.43(13) 5_655 5_656
O1 O1 O3 158.4(4) 2_655 5_656
O1 O1 O3 93.0(2) 2_545 5_656
O1 O1 O3 66.8(2) 2_645 5_656
O1 O1 O3 56.1(3) 1_556 5_656
O1 O1 O3 123.9(3) 1_554 5_656
Ga3 O1 O3 125.0(4) 4_665 5_656
Ga3 O1 O3 40.06(13) 1_445 5_656
Ga3 O1 O3 70.69(19) 2_646 5_656
O3 O1 O3 92.0(4) 2_546 5_656
O3 O1 O3 92.0(4) 6_556 5_656
Ga2 O1 O3 86.2(2) 1_545 1_455
La1 O1 O3 65.31(12) . 1_455
La1 O1 O3 61.73(12) 2_545 1_455
La1 O1 O3 163.6(6) 4_655 1_455
O2 O1 O3 60.9(3) 6 1_455
O2 O1 O3 105.2(4) 5_655 1_455
O2 O1 O3 113.0(4) 2_545 1_455
O2 O1 O3 54.4(3) 6_556 1_455
O2 O1 O3 98.4(4) 5_656 1_455
O2 O1 O3 105.6(4) 2_546 1_455
O3 O1 O3 21.2(3) 3_545 1_455
O3 O1 O3 98.4(3) 4_655 1_455
O3 O1 O3 139.9(3) . 1_455
Ga2 O1 O3 93.8(2) 1_544 1_455
O2 O1 O3 29.0(2) 4 1_455
O2 O1 O3 91.1(2) 3_655 1_455
O2 O1 O3 144.7(3) 1_545 1_455
Ga3 O1 O3 23.85(18) 2_546 1_455
Ga3 O1 O3 113.0(2) . 1_455
Ga3 O1 O3 115.6(2) 4_655 1_455
O3 O1 O3 45.8(3) 5_665 1_455
O3 O1 O3 88.7(2) 6_445 1_455
O3 O1 O3 144.5(4) 2_645 1_455
Ga3 O1 O3 50.91(15) 2_545 1_455
Ga3 O1 O3 111.8(2) 1_554 1_455
Ga3 O1 O3 113.8(2) 4_654 1_455
O3 O1 O3 45.7(3) 5_666 1_455
O3 O1 O3 84.9(2) 6_446 1_455
O3 O1 O3 131.8(3) 2_646 1_455
Nb O1 O3 21.35(13) . 1_455
Ga1 O1 O3 21.35(13) . 1_455
Nb O1 O3 135.65(12) 1_655 1_455
Ga1 O1 O3 135.65(12) 1_655 1_455
Ga1 O1 O3 104.65(11) 1_545 1_455
Nb O1 O3 104.65(11) 1_545 1_455
La1 O1 O3 73.12(18) 1_556 1_455
La1 O1 O3 71.33(18) 2_546 1_455
La1 O1 O3 116.0(3) 4_656 1_455
O2 O1 O3 55.79(17) . 1_455
O2 O1 O3 63.79(18) 3_545 1_455
O2 O1 O3 166.9(4) 4_655 1_455
Ga2 O1 O3 75.32(12) 2_556 1_455
Ga2 O1 O3 45.50(11) 2_446 1_455
Ga2 O1 O3 153.3(4) 2_546 1_455
O3 O1 O3 29.6(3) 2_545 1_455
O3 O1 O3 115.41(15) 6 1_455
O3 O1 O3 121.75(17) 5_655 1_455
O1 O1 O3 78.12(11) 2_655 1_455
O1 O1 O3 49.75(14) 2_545 1_455
O1 O1 O3 157.2(5) 2_645 1_455
O1 O1 O3 86.2(2) 1_556 1_455
O1 O1 O3 93.8(2) 1_554 1_455
Ga3 O1 O3 39.76(11) 4_665 1_455
Ga3 O1 O3 81.34(13) 1_445 1_455
Ga3 O1 O3 149.0(3) 2_646 1_455
O3 O1 O3 30.2(3) 2_546 1_455
O3 O1 O3 109.4(2) 6_556 1_455
O3 O1 O3 114.9(2) 5_656 1_455
Ga2 O1 O3 86.2(2) 1_545 4_765
La1 O1 O3 61.73(12) . 4_765
La1 O1 O3 163.6(6) 2_545 4_765
La1 O1 O3 65.31(12) 4_655 4_765
O2 O1 O3 113.0(4) 6 4_765
O2 O1 O3 60.9(3) 5_655 4_765
O2 O1 O3 105.2(4) 2_545 4_765
O2 O1 O3 105.6(4) 6_556 4_765
O2 O1 O3 54.4(3) 5_656 4_765
O2 O1 O3 98.4(4) 2_546 4_765
O3 O1 O3 98.4(3) 3_545 4_765
O3 O1 O3 139.9(3) 4_655 4_765
O3 O1 O3 21.2(3) . 4_765
Ga2 O1 O3 93.8(2) 1_544 4_765
O2 O1 O3 144.7(3) 4 4_765
O2 O1 O3 29.0(2) 3_655 4_765
O2 O1 O3 91.1(2) 1_545 4_765
Ga3 O1 O3 115.6(2) 2_546 4_765
Ga3 O1 O3 23.85(18) . 4_765
Ga3 O1 O3 113.0(2) 4_655 4_765
O3 O1 O3 88.7(2) 5_665 4_765
O3 O1 O3 144.5(4) 6_445 4_765
O3 O1 O3 45.8(3) 2_645 4_765
Ga3 O1 O3 113.8(2) 2_545 4_765
Ga3 O1 O3 50.91(15) 1_554 4_765
Ga3 O1 O3 111.8(2) 4_654 4_765
O3 O1 O3 84.9(2) 5_666 4_765
O3 O1 O3 131.8(3) 6_446 4_765
O3 O1 O3 45.7(3) 2_646 4_765
Nb O1 O3 104.65(10) . 4_765
Ga1 O1 O3 104.65(10) . 4_765
Nb O1 O3 21.35(13) 1_655 4_765
Ga1 O1 O3 21.35(13) 1_655 4_765
Ga1 O1 O3 135.65(12) 1_545 4_765
Nb O1 O3 135.65(12) 1_545 4_765
La1 O1 O3 71.33(18) 1_556 4_765
La1 O1 O3 116.0(3) 2_546 4_765
La1 O1 O3 73.12(18) 4_656 4_765
O2 O1 O3 63.79(18) . 4_765
O2 O1 O3 166.9(4) 3_545 4_765
O2 O1 O3 55.79(17) 4_655 4_765
Ga2 O1 O3 45.50(11) 2_556 4_765
Ga2 O1 O3 153.3(4) 2_446 4_765
Ga2 O1 O3 75.32(12) 2_546 4_765
O3 O1 O3 121.75(17) 2_545 4_765
O3 O1 O3 29.6(3) 6 4_765
O3 O1 O3 115.41(15) 5_655 4_765
O1 O1 O3 49.75(14) 2_655 4_765
O1 O1 O3 157.2(5) 2_545 4_765
O1 O1 O3 78.11(11) 2_645 4_765
O1 O1 O3 86.2(2) 1_556 4_765
O1 O1 O3 93.8(2) 1_554 4_765
Ga3 O1 O3 81.34(13) 4_665 4_765
Ga3 O1 O3 149.0(3) 1_445 4_765
Ga3 O1 O3 39.76(11) 2_646 4_765
O3 O1 O3 114.9(2) 2_546 4_765
O3 O1 O3 30.2(3) 6_556 4_765
O3 O1 O3 109.4(2) 5_656 4_765
O3 O1 O3 119.57(5) 1_455 4_765
Ga2 O1 O3 86.2(2) 1_545 3_535
La1 O1 O3 163.6(6) . 3_535
La1 O1 O3 65.31(12) 2_545 3_535
La1 O1 O3 61.73(12) 4_655 3_535
O2 O1 O3 105.2(4) 6 3_535
O2 O1 O3 113.0(4) 5_655 3_535
O2 O1 O3 60.9(3) 2_545 3_535
O2 O1 O3 98.4(4) 6_556 3_535
O2 O1 O3 105.6(4) 5_656 3_535
O2 O1 O3 54.4(3) 2_546 3_535
O3 O1 O3 139.9(3) 3_545 3_535
O3 O1 O3 21.2(3) 4_655 3_535
O3 O1 O3 98.4(3) . 3_535
Ga2 O1 O3 93.8(2) 1_544 3_535
O2 O1 O3 91.1(2) 4 3_535
O2 O1 O3 144.7(3) 3_655 3_535
O2 O1 O3 29.0(2) 1_545 3_535
Ga3 O1 O3 113.0(2) 2_546 3_535
Ga3 O1 O3 115.6(2) . 3_535
Ga3 O1 O3 23.85(18) 4_655 3_535
O3 O1 O3 144.5(4) 5_665 3_535
O3 O1 O3 45.8(3) 6_445 3_535
O3 O1 O3 88.7(2) 2_645 3_535
Ga3 O1 O3 111.8(2) 2_545 3_535
Ga3 O1 O3 113.8(2) 1_554 3_535
Ga3 O1 O3 50.91(15) 4_654 3_535
O3 O1 O3 131.8(3) 5_666 3_535
O3 O1 O3 45.7(2) 6_446 3_535
O3 O1 O3 84.9(2) 2_646 3_535
Nb O1 O3 135.65(12) . 3_535
Ga1 O1 O3 135.65(12) . 3_535
Nb O1 O3 104.65(10) 1_655 3_535
Ga1 O1 O3 104.65(10) 1_655 3_535
Ga1 O1 O3 21.35(13) 1_545 3_535
Nb O1 O3 21.35(13) 1_545 3_535
La1 O1 O3 116.0(3) 1_556 3_535
La1 O1 O3 73.12(18) 2_546 3_535
La1 O1 O3 71.33(18) 4_656 3_535
O2 O1 O3 166.9(4) . 3_535
O2 O1 O3 55.79(17) 3_545 3_535
O2 O1 O3 63.79(18) 4_655 3_535
Ga2 O1 O3 153.3(4) 2_556 3_535
Ga2 O1 O3 75.32(12) 2_446 3_535
Ga2 O1 O3 45.50(11) 2_546 3_535
O3 O1 O3 115.41(15) 2_545 3_535
O3 O1 O3 121.75(17) 6 3_535
O3 O1 O3 29.6(3) 5_655 3_535
O1 O1 O3 157.2(5) 2_655 3_535
O1 O1 O3 78.11(11) 2_545 3_535
O1 O1 O3 49.75(14) 2_645 3_535
O1 O1 O3 86.2(2) 1_556 3_535
O1 O1 O3 93.8(2) 1_554 3_535
Ga3 O1 O3 149.0(3) 4_665 3_535
Ga3 O1 O3 39.76(11) 1_445 3_535
Ga3 O1 O3 81.34(13) 2_646 3_535
O3 O1 O3 109.4(2) 2_546 3_535
O3 O1 O3 114.9(2) 6_556 3_535
O3 O1 O3 30.2(3) 5_656 3_535
O3 O1 O3 119.57(5) 1_455 3_535
O3 O1 O3 119.57(5) 4_765 3_535
Ga2 O1 O1 54.6(3) 1_545 2_656
La1 O1 O1 56.98(10) . 2_656
La1 O1 O1 136.8(3) 2_545 2_656
La1 O1 O1 114.34(17) 4_655 2_656
O2 O1 O1 115.7(3) 6 2_656
O2 O1 O1 97.2(3) 5_655 2_656
O2 O1 O1 153.4(5) 2_545 2_656
O2 O1 O1 57.4(4) 6_556 2_656
O2 O1 O1 32.9(3) 5_656 2_656
O2 O1 O1 84.7(6) 2_546 2_656
O3 O1 O1 57.8(2) 3_545 2_656
O3 O1 O1 137.9(7) 4_655 2_656
O3 O1 O1 66.2(3) . 2_656
Ga2 O1 O1 125.4(3) 1_544 2_656
O2 O1 O1 94.2(3) 4 2_656
O2 O1 O1 27.8(2) 3_655 2_656
O2 O1 O1 117.2(5) 1_545 2_656
Ga3 O1 O1 64.8(2) 2_546 2_656
Ga3 O1 O1 36.88(11) . 2_656
Ga3 O1 O1 114.9(6) 4_655 2_656
O3 O1 O1 75.57(18) 5_665 2_656
O3 O1 O1 163.6(3) 6_445 2_656
O3 O1 O1 97.34(15) 2_645 2_656
Ga3 O1 O1 107.63(14) 2_545 2_656
Ga3 O1 O1 90.92(15) 1_554 2_656
Ga3 O1 O1 162.5(3) 4_654 2_656
O3 O1 O1 33.7(2) 5_666 2_656
O3 O1 O1 105.1(5) 6_446 2_656
O3 O1 O1 60.6(3) 2_646 2_656
Nb O1 O1 72.931(11) . 2_656
Ga1 O1 O1 72.931(11) . 2_656
Nb O1 O1 72.930(11) 1_655 2_656
Ga1 O1 O1 72.930(11) 1_655 2_656
Ga1 O1 O1 155.3(6) 1_545 2_656
Nb O1 O1 155.3(6) 1_545 2_656
La1 O1 O1 26.4(2) 1_556 2_656
La1 O1 O1 77.2(4) 2_546 2_656
La1 O1 O1 67.1(3) 4_656 2_656
O2 O1 O1 32.27(18) . 2_656
O2 O1 O1 121.9(4) 3_545 2_656
O2 O1 O1 93.1(2) 4_655 2_656
Ga2 O1 O1 17.48(11) 2_556 2_656
Ga2 O1 O1 102.1(3) 2_446 2_656
Ga2 O1 O1 102.1(3) 2_546 2_656
O3 O1 O1 96.57(14) 2_545 2_656
O3 O1 O1 72.06(15) 6 2_656
O3 O1 O1 160.7(3) 5_655 2_656
O1 O1 O1 56.01(10) 2_655 2_656
O1 O1 O1 125.8(2) 2_545 2_656
O1 O1 O1 125.8(2) 2_645 2_656
O1 O1 O1 54.6(3) 1_556 2_656
O1 O1 O1 125.4(3) 1_554 2_656
Ga3 O1 O1 37.63(3) 4_665 2_656
Ga3 O1 O1 122.4(5) 1_445 2_656
Ga3 O1 O1 73.28(17) 2_646 2_656
O3 O1 O1 63.4(2) 2_546 2_656
O3 O1 O1 33.24(17) 6_556 2_656
O3 O1 O1 108.4(5) 5_656 2_656
O3 O1 O1 76.24(14) 1_455 2_656
O3 O1 O1 51.58(13) 4_765 2_656
O3 O1 O1 138.1(5) 3_535 2_656
Ga2 O1 O1 54.6(3) 1_545 2_546
La1 O1 O1 114.34(17) . 2_546
La1 O1 O1 56.98(10) 2_545 2_546
La1 O1 O1 136.8(3) 4_655 2_546
O2 O1 O1 97.2(3) 6 2_546
O2 O1 O1 153.4(5) 5_655 2_546
O2 O1 O1 115.7(3) 2_545 2_546
O2 O1 O1 32.9(3) 6_556 2_546
O2 O1 O1 84.7(6) 5_656 2_546
O2 O1 O1 57.4(4) 2_546 2_546
O3 O1 O1 66.2(3) 3_545 2_546
O3 O1 O1 57.8(2) 4_655 2_546
O3 O1 O1 137.9(7) . 2_546
Ga2 O1 O1 125.4(3) 1_544 2_546
O2 O1 O1 27.8(2) 4 2_546
O2 O1 O1 117.2(5) 3_655 2_546
O2 O1 O1 94.2(3) 1_545 2_546
Ga3 O1 O1 36.89(12) 2_546 2_546
Ga3 O1 O1 114.9(6) . 2_546
Ga3 O1 O1 64.8(2) 4_655 2_546
O3 O1 O1 97.34(15) 5_665 2_546
O3 O1 O1 75.57(18) 6_445 2_546
O3 O1 O1 163.6(3) 2_645 2_546
Ga3 O1 O1 90.92(15) 2_545 2_546
Ga3 O1 O1 162.5(3) 1_554 2_546
Ga3 O1 O1 107.63(14) 4_654 2_546
O3 O1 O1 60.6(3) 5_666 2_546
O3 O1 O1 33.7(2) 6_446 2_546
O3 O1 O1 105.1(5) 2_646 2_546
Nb O1 O1 72.931(11) . 2_546
Ga1 O1 O1 72.931(11) . 2_546
Nb O1 O1 155.3(6) 1_655 2_546
Ga1 O1 O1 155.3(6) 1_655 2_546
Ga1 O1 O1 72.930(11) 1_545 2_546
Nb O1 O1 72.930(11) 1_545 2_546
La1 O1 O1 67.1(3) 1_556 2_546
La1 O1 O1 26.4(2) 2_546 2_546
La1 O1 O1 77.2(4) 4_656 2_546
O2 O1 O1 93.1(2) . 2_546
O2 O1 O1 32.27(18) 3_545 2_546
O2 O1 O1 121.9(4) 4_655 2_546
Ga2 O1 O1 102.1(3) 2_556 2_546
Ga2 O1 O1 17.48(11) 2_446 2_546
Ga2 O1 O1 102.1(3) 2_546 2_546
O3 O1 O1 72.06(15) 2_545 2_546
O3 O1 O1 160.7(3) 6 2_546
O3 O1 O1 96.57(14) 5_655 2_546
O1 O1 O1 125.8(2) 2_655 2_546
O1 O1 O1 56.01(10) 2_545 2_546
O1 O1 O1 125.8(2) 2_645 2_546
O1 O1 O1 54.6(3) 1_556 2_546
O1 O1 O1 125.4(3) 1_554 2_546
Ga3 O1 O1 73.28(17) 4_665 2_546
Ga3 O1 O1 37.63(3) 1_445 2_546
Ga3 O1 O1 122.4(5) 2_646 2_546
O3 O1 O1 33.24(17) 2_546 2_546
O3 O1 O1 108.4(5) 6_556 2_546
O3 O1 O1 63.4(2) 5_656 2_546
O3 O1 O1 51.58(13) 1_455 2_546
O3 O1 O1 138.1(5) 4_765 2_546
O3 O1 O1 76.23(14) 3_535 2_546
O1 O1 O1 89.8(5) 2_656 2_546
Ga2 O1 O1 54.6(3) 1_545 2_646
La1 O1 O1 136.8(3) . 2_646
La1 O1 O1 114.34(17) 2_545 2_646
La1 O1 O1 56.98(10) 4_655 2_646
O2 O1 O1 153.4(5) 6 2_646
O2 O1 O1 115.7(3) 5_655 2_646
O2 O1 O1 97.2(3) 2_545 2_646
O2 O1 O1 84.7(6) 6_556 2_646
O2 O1 O1 57.4(4) 5_656 2_646
O2 O1 O1 32.9(3) 2_546 2_646
O3 O1 O1 137.9(7) 3_545 2_646
O3 O1 O1 66.2(3) 4_655 2_646
O3 O1 O1 57.8(2) . 2_646
Ga2 O1 O1 125.4(3) 1_544 2_646
O2 O1 O1 117.2(5) 4 2_646
O2 O1 O1 94.2(3) 3_655 2_646
O2 O1 O1 27.7(2) 1_545 2_646
Ga3 O1 O1 114.9(6) 2_546 2_646
Ga3 O1 O1 64.8(2) . 2_646
Ga3 O1 O1 36.88(11) 4_655 2_646
O3 O1 O1 163.6(3) 5_665 2_646
O3 O1 O1 97.34(15) 6_445 2_646
O3 O1 O1 75.57(18) 2_645 2_646
Ga3 O1 O1 162.5(3) 2_545 2_646
Ga3 O1 O1 107.63(14) 1_554 2_646
Ga3 O1 O1 90.92(15) 4_654 2_646
O3 O1 O1 105.1(5) 5_666 2_646
O3 O1 O1 60.6(3) 6_446 2_646
O3 O1 O1 33.7(2) 2_646 2_646
Nb O1 O1 155.3(6) . 2_646
Ga1 O1 O1 155.3(6) . 2_646
Nb O1 O1 72.930(11) 1_655 2_646
Ga1 O1 O1 72.930(11) 1_655 2_646
Ga1 O1 O1 72.930(12) 1_545 2_646
Nb O1 O1 72.930(12) 1_545 2_646
La1 O1 O1 77.2(4) 1_556 2_646
La1 O1 O1 67.1(3) 2_546 2_646
La1 O1 O1 26.4(2) 4_656 2_646
O2 O1 O1 121.9(4) . 2_646
O2 O1 O1 93.1(2) 3_545 2_646
O2 O1 O1 32.27(18) 4_655 2_646
Ga2 O1 O1 102.1(3) 2_556 2_646
Ga2 O1 O1 102.1(3) 2_446 2_646
Ga2 O1 O1 17.48(11) 2_546 2_646
O3 O1 O1 160.7(3) 2_545 2_646
O3 O1 O1 96.57(14) 6 2_646
O3 O1 O1 72.06(15) 5_655 2_646
O1 O1 O1 125.8(2) 2_655 2_646
O1 O1 O1 125.8(2) 2_545 2_646
O1 O1 O1 56.01(10) 2_645 2_646
O1 O1 O1 54.6(3) 1_556 2_646
O1 O1 O1 125.4(3) 1_554 2_646
Ga3 O1 O1 122.4(5) 4_665 2_646
Ga3 O1 O1 73.28(17) 1_445 2_646
Ga3 O1 O1 37.63(3) 2_646 2_646
O3 O1 O1 108.4(5) 2_546 2_646
O3 O1 O1 63.4(2) 6_556 2_646
O3 O1 O1 33.24(17) 5_656 2_646
O3 O1 O1 138.1(5) 1_455 2_646
O3 O1 O1 76.23(14) 4_765 2_646
O3 O1 O1 51.58(13) 3_535 2_646
O1 O1 O1 89.8(5) 2_656 2_646
O1 O1 O1 89.8(5) 2_546 2_646
Ga2 O1 O2 141.18(17) 1_545 4_554
La1 O1 O2 74.6(4) . 4_554
La1 O1 O2 38.9(3) 2_545 4_554
La1 O1 O2 104.0(5) 4_655 4_554
O2 O1 O2 13.2(3) 6 4_554
O2 O1 O2 67.2(4) 5_655 4_554
O2 O1 O2 53.5(3) 2_545 4_554
O2 O1 O2 110.3(3) 6_556 4_554
O2 O1 O2 156.45(17) 5_656 4_554
O2 O1 O2 135.7(2) 2_546 4_554
O3 O1 O2 71.4(3) 3_545 4_554
O3 O1 O2 83.2(3) 4_655 4_554
O3 O1 O2 134.4(5) . 4_554
Ga2 O1 O2 38.82(17) 1_544 4_554
O2 O1 O2 62.9(3) 4 4_554
O2 O1 O2 117.8(3) 3_655 4_554
O2 O1 O2 117.8(3) 1_545 4_554
Ga3 O1 O2 82.2(2) 2_546 4_554
Ga3 O1 O2 145.5(3) . 4_554
Ga3 O1 O2 113.2(2) 4_655 4_554
O3 O1 O2 50.5(3) 5_665 4_554
O3 O1 O2 48.4(2) 6_445 4_554
O3 O1 O2 100.0(4) 2_645 4_554
Ga3 O1 O2 17.74(15) 2_545 4_554
Ga3 O1 O2 77.6(3) 1_554 4_554
Ga3 O1 O2 57.0(2) 4_654 4_554
O3 O1 O2 103.9(2) 5_666 4_554
O3 O1 O2 102.44(19) 6_446 4_554
O3 O1 O2 166.4(4) 2_646 4_554
Nb O1 O2 54.0(2) . 4_554
Ga1 O1 O2 54.0(2) . 4_554
Nb O1 O2 116.6(4) 1_655 4_554
Ga1 O1 O2 116.6(4) 1_655 4_554
Ga1 O1 O2 73.0(2) 1_545 4_554
Nb O1 O2 73.0(2) 1_545 4_554
La1 O1 O2 132.58(14) 1_556 4_554
La1 O1 O2 113.94(13) 2_546 4_554
La1 O1 O2 161.02(17) 4_656 4_554
O2 O1 O2 93.1(3) . 4_554
O2 O1 O2 67.40(19) 3_545 4_554
O2 O1 O2 133.1(4) 4_655 4_554
Ga2 O1 O2 112.5(2) 2_556 4_554
Ga2 O1 O2 70.51(17) 2_446 4_554
Ga2 O1 O2 132.0(3) 2_546 4_554
O3 O1 O2 31.7(2) 2_545 4_554
O3 O1 O2 97.1(4) 6 4_554
O3 O1 O2 73.6(3) 5_655 4_554
O1 O1 O2 82.3(4) 2_655 4_554
O1 O1 O2 33.1(3) 2_545 4_554
O1 O1 O2 98.5(5) 2_645 4_554
O1 O1 O2 141.18(17) 1_556 4_554
O1 O1 O2 38.82(17) 1_554 4_554
Ga3 O1 O2 90.08(18) 4_665 4_554
Ga3 O1 O2 83.88(16) 1_445 4_554
Ga3 O1 O2 146.7(3) 2_646 4_554
O3 O1 O2 87.7(2) 2_546 4_554
O3 O1 O2 149.1(3) 6_556 4_554
O3 O1 O2 118.9(2) 5_656 4_554
O3 O1 O2 60.0(2) 1_455 4_554
O3 O1 O2 125.6(3) 4_765 4_554
O3 O1 O2 94.1(2) 3_535 4_554
O1 O1 O2 125.0(2) 2_656 4_554
O1 O1 O2 87.7(2) 2_546 4_554
O1 O1 O2 145.0(3) 2_646 4_554
Ga2 O1 O2 141.18(17) 1_545 3_654
La1 O1 O2 38.9(3) . 3_654
La1 O1 O2 104.0(5) 2_545 3_654
La1 O1 O2 74.6(4) 4_655 3_654
O2 O1 O2 53.5(3) 6 3_654
O2 O1 O2 13.2(3) 5_655 3_654
O2 O1 O2 67.2(4) 2_545 3_654
O2 O1 O2 135.7(2) 6_556 3_654
O2 O1 O2 110.3(3) 5_656 3_654
O2 O1 O2 156.45(17) 2_546 3_654
O3 O1 O2 83.2(3) 3_545 3_654
O3 O1 O2 134.4(5) 4_655 3_654
O3 O1 O2 71.4(3) . 3_654
Ga2 O1 O2 38.82(17) 1_544 3_654
O2 O1 O2 117.8(3) 4 3_654
O2 O1 O2 62.9(3) 3_655 3_654
O2 O1 O2 117.8(3) 1_545 3_654
Ga3 O1 O2 113.2(2) 2_546 3_654
Ga3 O1 O2 82.2(2) . 3_654
Ga3 O1 O2 145.5(3) 4_655 3_654
O3 O1 O2 48.4(2) 5_665 3_654
O3 O1 O2 100.0(4) 6_445 3_654
O3 O1 O2 50.5(3) 2_645 3_654
Ga3 O1 O2 57.0(2) 2_545 3_654
Ga3 O1 O2 17.74(15) 1_554 3_654
Ga3 O1 O2 77.6(3) 4_654 3_654
O3 O1 O2 102.44(19) 5_666 3_654
O3 O1 O2 166.4(4) 6_446 3_654
O3 O1 O2 103.9(2) 2_646 3_654
Nb O1 O2 73.0(2) . 3_654
Ga1 O1 O2 73.0(2) . 3_654
Nb O1 O2 54.0(2) 1_655 3_654
Ga1 O1 O2 54.0(2) 1_655 3_654
Ga1 O1 O2 116.6(4) 1_545 3_654
Nb O1 O2 116.6(4) 1_545 3_654
La1 O1 O2 113.94(13) 1_556 3_654
La1 O1 O2 161.02(17) 2_546 3_654
La1 O1 O2 132.58(14) 4_656 3_654
O2 O1 O2 67.40(19) . 3_654
O2 O1 O2 133.1(4) 3_545 3_654
O2 O1 O2 93.1(3) 4_655 3_654
Ga2 O1 O2 70.52(17) 2_556 3_654
Ga2 O1 O2 132.0(3) 2_446 3_654
Ga2 O1 O2 112.5(2) 2_546 3_654
O3 O1 O2 73.6(3) 2_545 3_654
O3 O1 O2 31.7(2) 6 3_654
O3 O1 O2 97.1(4) 5_655 3_654
O1 O1 O2 33.1(3) 2_655 3_654
O1 O1 O2 98.5(5) 2_545 3_654
O1 O1 O2 82.3(4) 2_645 3_654
O1 O1 O2 141.18(17) 1_556 3_654
O1 O1 O2 38.82(17) 1_554 3_654
Ga3 O1 O2 83.88(16) 4_665 3_654
Ga3 O1 O2 146.7(3) 1_445 3_654
Ga3 O1 O2 90.08(18) 2_646 3_654
O3 O1 O2 118.9(2) 2_546 3_654
O3 O1 O2 87.7(2) 6_556 3_654
O3 O1 O2 149.1(3) 5_656 3_654
O3 O1 O2 94.1(2) 1_455 3_654
O3 O1 O2 60.0(2) 4_765 3_654
O3 O1 O2 125.6(3) 3_535 3_654
O1 O1 O2 87.7(2) 2_656 3_654
O1 O1 O2 145.0(3) 2_546 3_654
O1 O1 O2 125.0(2) 2_646 3_654
O2 O1 O2 65.8(3) 4_554 3_654
Ga2 O1 O2 141.18(17) 1_545 1_544
La1 O1 O2 104.0(5) . 1_544
La1 O1 O2 74.6(4) 2_545 1_544
La1 O1 O2 38.9(3) 4_655 1_544
O2 O1 O2 67.2(4) 6 1_544
O2 O1 O2 53.5(3) 5_655 1_544
O2 O1 O2 13.2(3) 2_545 1_544
O2 O1 O2 156.45(17) 6_556 1_544
O2 O1 O2 135.7(2) 5_656 1_544
O2 O1 O2 110.3(3) 2_546 1_544
O3 O1 O2 134.4(5) 3_545 1_544
O3 O1 O2 71.4(3) 4_655 1_544
O3 O1 O2 83.2(3) . 1_544
Ga2 O1 O2 38.82(17) 1_544 1_544
O2 O1 O2 117.8(3) 4 1_544
O2 O1 O2 117.8(3) 3_655 1_544
O2 O1 O2 62.9(3) 1_545 1_544
Ga3 O1 O2 145.5(3) 2_546 1_544
Ga3 O1 O2 113.2(2) . 1_544
Ga3 O1 O2 82.2(2) 4_655 1_544
O3 O1 O2 100.0(4) 5_665 1_544
O3 O1 O2 50.5(3) 6_445 1_544
O3 O1 O2 48.4(2) 2_645 1_544
Ga3 O1 O2 77.6(3) 2_545 1_544
Ga3 O1 O2 57.0(2) 1_554 1_544
Ga3 O1 O2 17.74(15) 4_654 1_544
O3 O1 O2 166.4(4) 5_666 1_544
O3 O1 O2 103.9(2) 6_446 1_544
O3 O1 O2 102.44(19) 2_646 1_544
Nb O1 O2 116.6(4) . 1_544
Ga1 O1 O2 116.6(4) . 1_544
Nb O1 O2 73.0(2) 1_655 1_544
Ga1 O1 O2 73.0(2) 1_655 1_544
Ga1 O1 O2 54.0(2) 1_545 1_544
Nb O1 O2 54.0(2) 1_545 1_544
La1 O1 O2 161.02(17) 1_556 1_544
La1 O1 O2 132.57(14) 2_546 1_544
La1 O1 O2 113.94(13) 4_656 1_544
O2 O1 O2 133.1(4) . 1_544
O2 O1 O2 93.1(3) 3_545 1_544
O2 O1 O2 67.40(19) 4_655 1_544
Ga2 O1 O2 132.0(3) 2_556 1_544
Ga2 O1 O2 112.5(2) 2_446 1_544
Ga2 O1 O2 70.51(17) 2_546 1_544
O3 O1 O2 97.1(4) 2_545 1_544
O3 O1 O2 73.6(3) 6 1_544
O3 O1 O2 31.7(2) 5_655 1_544
O1 O1 O2 98.5(5) 2_655 1_544
O1 O1 O2 82.3(4) 2_545 1_544
O1 O1 O2 33.1(3) 2_645 1_544
O1 O1 O2 141.18(17) 1_556 1_544
O1 O1 O2 38.82(17) 1_554 1_544
Ga3 O1 O2 146.7(3) 4_665 1_544
Ga3 O1 O2 90.08(18) 1_445 1_544
Ga3 O1 O2 83.88(16) 2_646 1_544
O3 O1 O2 149.1(3) 2_546 1_544
O3 O1 O2 118.9(2) 6_556 1_544
O3 O1 O2 87.7(2) 5_656 1_544
O3 O1 O2 125.6(3) 1_455 1_544
O3 O1 O2 94.1(2) 4_765 1_544
O3 O1 O2 60.0(2) 3_535 1_544
O1 O1 O2 145.0(3) 2_656 1_544
O1 O1 O2 125.0(2) 2_546 1_544
O1 O1 O2 87.7(2) 2_646 1_544
O2 O1 O2 65.8(3) 4_554 1_544
O2 O1 O2 65.8(3) 3_654 1_544
Ga2 O1 O3 146.16(15) 1_545 3_544
La1 O1 O3 47.1(4) . 3_544
La1 O1 O3 67.5(3) 2_545 3_544
La1 O1 O3 102.1(5) 4_655 3_544
O2 O1 O3 15.8(3) 6 3_544
O2 O1 O3 46.5(4) 5_655 3_544
O2 O1 O3 64.3(4) 2_545 3_544
O2 O1 O3 116.3(3) 6_556 3_544
O2 O1 O3 135.1(3) 5_656 3_544
O2 O1 O3 163.1(3) 2_546 3_544
O3 O1 O3 62.6(3) 3_545 3_544
O3 O1 O3 111.7(4) 4_655 3_544
O3 O1 O3 111.7(4) . 3_544
Ga2 O1 O3 33.84(15) 1_544 3_544
O2 O1 O3 79.3(3) 4 3_544
O2 O1 O3 89.4(3) 3_655 3_544
O2 O1 O3 134.8(4) 1_545 3_544
Ga3 O1 O3 86.0(2) 2_546 3_544
Ga3 O1 O3 116.6(3) . 3_544
Ga3 O1 O3 141.0(3) 4_655 3_544
O3 O1 O3 28.7(4) 5_665 3_544
O3 O1 O3 75.3(3) 6_445 3_544
O3 O1 O3 85.9(4) 2_645 3_544
Ga3 O1 O3 16.63(12) 2_545 3_544
Ga3 O1 O3 55.9(2) 1_554 3_544
Ga3 O1 O3 72.1(3) 4_654 3_544
O3 O1 O3 94.4(3) 5_666 3_544
O3 O1 O3 129.8(2) 6_446 3_544
O3 O1 O3 143.6(2) 2_646 3_544
Nb O1 O3 45.7(2) . 3_544
Ga1 O1 O3 45.7(2) . 3_544
Nb O1 O3 94.3(3) 1_655 3_544
Ga1 O1 O3 94.3(3) 1_655 3_544
Ga1 O1 O3 99.4(3) 1_545 3_544
Nb O1 O3 99.4(3) 1_545 3_544
La1 O1 O3 120.74(14) 1_556 3_544
La1 O1 O3 131.95(10) 2_546 3_544
La1 O1 O3 169.18(14) 4_656 3_544
O2 O1 O3 70.9(3) . 3_544
O2 O1 O3 94.5(2) 3_545 3_544
O2 O1 O3 128.6(3) 4_655 3_544
Ga2 O1 O3 87.1(2) 2_556 3_544
Ga2 O1 O3 91.97(17) 2_446 3_544
Ga2 O1 O3 141.5(3) 2_546 3_544
O3 O1 O3 35.4(3) 2_545 3_544
O3 O1 O3 71.8(3) 6 3_544
O3 O1 O3 92.9(3) 5_655 3_544
O1 O1 O3 53.6(4) 2_655 3_544
O1 O1 O3 59.3(3) 2_545 3_544
O1 O1 O3 103.1(5) 2_645 3_544
O1 O1 O3 146.16(15) 1_556 3_544
O1 O1 O3 33.84(15) 1_554 3_544
Ga3 O1 O3 75.71(18) 4_665 3_544
Ga3 O1 O3 112.39(19) 1_445 3_544
Ga3 O1 O3 130.2(3) 2_646 3_544
O3 O1 O3 92.4(3) 2_546 3_544
O3 O1 O3 120.4(3) 6_556 3_544
O3 O1 O3 147.2(2) 5_656 3_544
O3 O1 O3 62.39(16) 1_455 3_544
O3 O1 O3 98.1(3) 4_765 3_544
O3 O1 O3 119.2(3) 3_535 3_544
O1 O1 O3 102.6(3) 2_656 3_544
O1 O1 O3 107.0(2) 2_546 3_544
O1 O1 O3 158.9(4) 2_646 3_544
O2 O1 O3 28.96(19) 4_554 3_544
O2 O1 O3 40.3(2) 3_654 3_544
O2 O1 O3 72.3(3) 1_544 3_544
Ga2 O1 O3 146.16(15) 1_545 4_654
La1 O1 O3 102.1(5) . 4_654
La1 O1 O3 47.1(4) 2_545 4_654
La1 O1 O3 67.5(3) 4_655 4_654
O2 O1 O3 46.5(4) 6 4_654
O2 O1 O3 64.3(4) 5_655 4_654
O2 O1 O3 15.8(3) 2_545 4_654
O2 O1 O3 135.1(3) 6_556 4_654
O2 O1 O3 163.1(3) 5_656 4_654
O2 O1 O3 116.3(3) 2_546 4_654
O3 O1 O3 111.7(4) 3_545 4_654
O3 O1 O3 62.6(3) 4_655 4_654
O3 O1 O3 111.7(4) . 4_654
Ga2 O1 O3 33.84(15) 1_544 4_654
O2 O1 O3 89.4(3) 4 4_654
O2 O1 O3 134.8(4) 3_655 4_654
O2 O1 O3 79.3(3) 1_545 4_654
Ga3 O1 O3 116.6(3) 2_546 4_654
Ga3 O1 O3 141.0(3) . 4_654
Ga3 O1 O3 86.0(2) 4_655 4_654
O3 O1 O3 85.9(4) 5_665 4_654
O3 O1 O3 28.7(4) 6_445 4_654
O3 O1 O3 75.3(3) 2_645 4_654
Ga3 O1 O3 55.9(2) 2_545 4_654
Ga3 O1 O3 72.1(3) 1_554 4_654
Ga3 O1 O3 16.63(12) 4_654 4_654
O3 O1 O3 143.6(2) 5_666 4_654
O3 O1 O3 94.4(3) 6_446 4_654
O3 O1 O3 129.8(2) 2_646 4_654
Nb O1 O3 94.3(3) . 4_654
Ga1 O1 O3 94.3(3) . 4_654
Nb O1 O3 99.4(3) 1_655 4_654
Ga1 O1 O3 99.4(3) 1_655 4_654
Ga1 O1 O3 45.7(2) 1_545 4_654
Nb O1 O3 45.7(2) 1_545 4_654
La1 O1 O3 169.18(14) 1_556 4_654
La1 O1 O3 120.74(14) 2_546 4_654
La1 O1 O3 131.95(10) 4_656 4_654
O2 O1 O3 128.6(3) . 4_654
O2 O1 O3 70.9(3) 3_545 4_654
O2 O1 O3 94.5(2) 4_655 4_654
Ga2 O1 O3 141.5(3) 2_556 4_654
Ga2 O1 O3 87.1(2) 2_446 4_654
Ga2 O1 O3 91.97(17) 2_546 4_654
O3 O1 O3 71.8(3) 2_545 4_654
O3 O1 O3 92.9(3) 6 4_654
O3 O1 O3 35.4(3) 5_655 4_654
O1 O1 O3 103.1(5) 2_655 4_654
O1 O1 O3 53.6(4) 2_545 4_654
O1 O1 O3 59.3(3) 2_645 4_654
O1 O1 O3 146.16(15) 1_556 4_654
O1 O1 O3 33.84(15) 1_554 4_654
Ga3 O1 O3 130.2(3) 4_665 4_654
Ga3 O1 O3 75.71(18) 1_445 4_654
Ga3 O1 O3 112.39(19) 2_646 4_654
O3 O1 O3 120.4(3) 2_546 4_654
O3 O1 O3 147.2(2) 6_556 4_654
O3 O1 O3 92.4(3) 5_656 4_654
O3 O1 O3 98.1(3) 1_455 4_654
O3 O1 O3 119.2(3) 4_765 4_654
O3 O1 O3 62.39(16) 3_535 4_654
O1 O1 O3 158.9(4) 2_656 4_654
O1 O1 O3 102.6(3) 2_546 4_654
O1 O1 O3 107.0(2) 2_646 4_654
O2 O1 O3 40.3(2) 4_554 4_654
O2 O1 O3 72.3(3) 3_654 4_654
O2 O1 O3 28.96(19) 1_544 4_654
O3 O1 O3 57.7(2) 3_544 4_654
Ga2 O1 O3 146.16(15) 1_545 1_554
La1 O1 O3 67.5(3) . 1_554
La1 O1 O3 102.1(5) 2_545 1_554
La1 O1 O3 47.1(4) 4_655 1_554
O2 O1 O3 64.3(4) 6 1_554
O2 O1 O3 15.8(3) 5_655 1_554
O2 O1 O3 46.5(4) 2_545 1_554
O2 O1 O3 163.1(3) 6_556 1_554
O2 O1 O3 116.3(3) 5_656 1_554
O2 O1 O3 135.1(3) 2_546 1_554
O3 O1 O3 111.7(4) 3_545 1_554
O3 O1 O3 111.7(4) 4_655 1_554
O3 O1 O3 62.6(3) . 1_554
Ga2 O1 O3 33.84(15) 1_544 1_554
O2 O1 O3 134.8(4) 4 1_554
O2 O1 O3 79.3(3) 3_655 1_554
O2 O1 O3 89.4(3) 1_545 1_554
Ga3 O1 O3 141.0(3) 2_546 1_554
Ga3 O1 O3 86.0(2) . 1_554
Ga3 O1 O3 116.6(3) 4_655 1_554
O3 O1 O3 75.3(3) 5_665 1_554
O3 O1 O3 85.9(4) 6_445 1_554
O3 O1 O3 28.7(4) 2_645 1_554
Ga3 O1 O3 72.1(3) 2_545 1_554
Ga3 O1 O3 16.63(12) 1_554 1_554
Ga3 O1 O3 55.9(2) 4_654 1_554
O3 O1 O3 129.8(2) 5_666 1_554
O3 O1 O3 143.6(2) 6_446 1_554
O3 O1 O3 94.4(3) 2_646 1_554
Nb O1 O3 99.4(3) . 1_554
Ga1 O1 O3 99.4(3) . 1_554
Nb O1 O3 45.7(2) 1_655 1_554
Ga1 O1 O3 45.7(2) 1_655 1_554
Ga1 O1 O3 94.3(3) 1_545 1_554
Nb O1 O3 94.3(3) 1_545 1_554
La1 O1 O3 131.95(10) 1_556 1_554
La1 O1 O3 169.18(14) 2_546 1_554
La1 O1 O3 120.74(14) 4_656 1_554
O2 O1 O3 94.5(2) . 1_554
O2 O1 O3 128.6(3) 3_545 1_554
O2 O1 O3 70.9(3) 4_655 1_554
Ga2 O1 O3 91.97(17) 2_556 1_554
Ga2 O1 O3 141.5(3) 2_446 1_554
Ga2 O1 O3 87.1(2) 2_546 1_554
O3 O1 O3 92.9(3) 2_545 1_554
O3 O1 O3 35.4(3) 6 1_554
O3 O1 O3 71.8(3) 5_655 1_554
O1 O1 O3 59.3(3) 2_655 1_554
O1 O1 O3 103.1(5) 2_545 1_554
O1 O1 O3 53.6(4) 2_645 1_554
O1 O1 O3 146.16(15) 1_556 1_554
O1 O1 O3 33.84(15) 1_554 1_554
Ga3 O1 O3 112.39(19) 4_665 1_554
Ga3 O1 O3 130.2(3) 1_445 1_554
Ga3 O1 O3 75.71(19) 2_646 1_554
O3 O1 O3 147.2(2) 2_546 1_554
O3 O1 O3 92.4(3) 6_556 1_554
O3 O1 O3 120.4(3) 5_656 1_554
O3 O1 O3 119.2(3) 1_455 1_554
O3 O1 O3 62.39(16) 4_765 1_554
O3 O1 O3 98.1(3) 3_535 1_554
O1 O1 O3 107.0(2) 2_656 1_554
O1 O1 O3 158.9(4) 2_546 1_554
O1 O1 O3 102.6(3) 2_646 1_554
O2 O1 O3 72.3(3) 4_554 1_554
O2 O1 O3 28.96(19) 3_654 1_554
O2 O1 O3 40.3(2) 1_544 1_554
O3 O1 O3 57.7(2) 3_544 1_554
O3 O1 O3 57.7(2) 4_654 1_554
Ga2 O1 O3 86.5(2) 1_545 4_665
La1 O1 O3 41.32(19) . 4_665
La1 O1 O3 86.93(13) 2_545 4_665
La1 O1 O3 150.2(3) 4_655 4_665
O2 O1 O3 66.7(3) 6 4_665
O2 O1 O3 90.1(3) 5_655 4_665
O2 O1 O3 123.2(5) 2_545 4_665
O2 O1 O3 60.9(3) 6_556 4_665
O2 O1 O3 84.3(3) 5_656 4_665
O2 O1 O3 115.5(5) 2_546 4_665
O3 O1 O3 6.9(3) 3_545 4_665
O3 O1 O3 125.5(3) 4_655 4_665
O3 O1 O3 113.1(3) . 4_665
Ga2 O1 O3 93.5(2) 1_544 4_665
O2 O1 O3 55.6(2) 4 4_665
O2 O1 O3 64.3(2) 3_655 4_665
O2 O1 O3 164.1(5) 1_545 4_665
Ga3 O1 O3 36.67(15) 2_546 4_665
Ga3 O1 O3 89.26(17) . 4_665
Ga3 O1 O3 136.9(3) 4_655 4_665
O3 O1 O3 32.9(3) 5_665 4_665
O3 O1 O3 112.55(15) 6_445 4_665
O3 O1 O3 123.02(18) 2_645 4_665
Ga3 O1 O3 56.68(13) 2_545 4_665
Ga3 O1 O3 93.26(17) 1_554 4_665
Ga3 O1 O3 128.8(3) 4_654 4_665
O3 O1 O3 34.6(3) 5_666 4_665
O3 O1 O3 106.4(2) 6_446 4_665
O3 O1 O3 115.4(2) 2_646 4_665
Nb O1 O3 18.29(12) . 4_665
Ga1 O1 O3 18.29(12) . 4_665
Nb O1 O3 108.70(13) 1_655 4_665
Ga1 O1 O3 108.70(13) 1_655 4_665
Ga1 O1 O3 131.52(14) 1_545 4_665
Nb O1 O3 131.52(14) 1_545 4_665
La1 O1 O3 62.49(15) 1_556 4_665
La1 O1 O3 84.69(19) 2_546 4_665
La1 O1 O3 113.3(3) 4_656 4_665
O2 O1 O3 28.83(19) . 4_665
O2 O1 O3 90.91(19) 3_545 4_665
O2 O1 O3 146.3(2) 4_655 4_665
Ga2 O1 O3 49.48(13) 2_556 4_665
Ga2 O1 O3 71.44(13) 2_446 4_665
Ga2 O1 O3 155.7(4) 2_546 4_665
O3 O1 O3 41.8(2) 2_545 4_665
O3 O1 O3 90.6(2) 6 4_665
O3 O1 O3 144.5(3) 5_655 4_665
O1 O1 O3 53.21(16) 2_655 4_665
O1 O1 O3 74.16(12) 2_545 4_665
O1 O1 O3 159.5(5) 2_645 4_665
O1 O1 O3 86.5(2) 1_556 4_665
O1 O1 O3 93.5(2) 1_554 4_665
Ga3 O1 O3 17.92(12) 4_665 4_665
Ga3 O1 O3 107.33(15) 1_445 4_665
Ga3 O1 O3 126.6(2) 2_646 4_665
O3 O1 O3 41.9(3) 2_546 4_665
O3 O1 O3 87.2(2) 6_556 4_665
O3 O1 O3 133.7(3) 5_656 4_665
O3 O1 O3 27.36(16) 1_455 4_665
O3 O1 O3 92.34(16) 4_765 4_665
O3 O1 O3 146.63(18) 3_535 4_665
O1 O1 O3 54.83(12) 2_656 4_665
O1 O1 O3 73.02(14) 2_546 4_665
O1 O1 O3 139.6(5) 2_646 4_665
O2 O1 O3 72.2(2) 4_554 4_665
O2 O1 O3 77.17(19) 3_654 4_665
O2 O1 O3 132.2(3) 1_544 4_665
O3 O1 O3 59.89(15) 3_544 4_665
O3 O1 O3 112.3(3) 4_654 4_665
O3 O1 O3 105.9(3) 1_554 4_665
Ga2 O1 O3 86.5(2) 1_545 1_445
La1 O1 O3 150.2(3) . 1_445
La1 O1 O3 41.32(19) 2_545 1_445
La1 O1 O3 86.93(13) 4_655 1_445
O2 O1 O3 90.1(3) 6 1_445
O2 O1 O3 123.2(5) 5_655 1_445
O2 O1 O3 66.7(3) 2_545 1_445
O2 O1 O3 84.3(3) 6_556 1_445
O2 O1 O3 115.5(5) 5_656 1_445
O2 O1 O3 60.9(3) 2_546 1_445
O3 O1 O3 113.1(3) 3_545 1_445
O3 O1 O3 6.9(3) 4_655 1_445
O3 O1 O3 125.5(3) . 1_445
Ga2 O1 O3 93.5(2) 1_544 1_445
O2 O1 O3 64.3(2) 4 1_445
O2 O1 O3 164.1(5) 3_655 1_445
O2 O1 O3 55.6(2) 1_545 1_445
Ga3 O1 O3 89.26(17) 2_546 1_445
Ga3 O1 O3 136.9(3) . 1_445
Ga3 O1 O3 36.67(15) 4_655 1_445
O3 O1 O3 123.02(18) 5_665 1_445
O3 O1 O3 32.9(3) 6_445 1_445
O3 O1 O3 112.55(15) 2_645 1_445
Ga3 O1 O3 93.26(17) 2_545 1_445
Ga3 O1 O3 128.8(3) 1_554 1_445
Ga3 O1 O3 56.68(13) 4_654 1_445
O3 O1 O3 115.4(2) 5_666 1_445
O3 O1 O3 34.6(3) 6_446 1_445
O3 O1 O3 106.4(2) 2_646 1_445
Nb O1 O3 108.70(13) . 1_445
Ga1 O1 O3 108.70(13) . 1_445
Nb O1 O3 131.52(14) 1_655 1_445
Ga1 O1 O3 131.52(14) 1_655 1_445
Ga1 O1 O3 18.29(12) 1_545 1_445
Nb O1 O3 18.29(12) 1_545 1_445
La1 O1 O3 113.3(3) 1_556 1_445
La1 O1 O3 62.49(15) 2_546 1_445
La1 O1 O3 84.68(19) 4_656 1_445
O2 O1 O3 146.3(2) . 1_445
O2 O1 O3 28.83(19) 3_545 1_445
O2 O1 O3 90.91(19) 4_655 1_445
Ga2 O1 O3 155.7(4) 2_556 1_445
Ga2 O1 O3 49.48(12) 2_446 1_445
Ga2 O1 O3 71.44(13) 2_546 1_445
O3 O1 O3 90.6(2) 2_545 1_445
O3 O1 O3 144.5(3) 6 1_445
O3 O1 O3 41.8(2) 5_655 1_445
O1 O1 O3 159.5(5) 2_655 1_445
O1 O1 O3 53.20(16) 2_545 1_445
O1 O1 O3 74.16(12) 2_645 1_445
O1 O1 O3 86.5(2) 1_556 1_445
O1 O1 O3 93.5(2) 1_554 1_445
Ga3 O1 O3 126.6(2) 4_665 1_445
Ga3 O1 O3 17.92(12) 1_445 1_445
Ga3 O1 O3 107.33(15) 2_646 1_445
O3 O1 O3 87.2(2) 2_546 1_445
O3 O1 O3 133.7(3) 6_556 1_445
O3 O1 O3 41.9(3) 5_656 1_445
O3 O1 O3 92.34(16) 1_455 1_445
O3 O1 O3 146.63(18) 4_765 1_445
O3 O1 O3 27.36(16) 3_535 1_445
O1 O1 O3 139.6(5) 2_656 1_445
O1 O1 O3 54.83(12) 2_546 1_445
O1 O1 O3 73.02(14) 2_646 1_445
O2 O1 O3 77.17(19) 4_554 1_445
O2 O1 O3 132.2(3) 3_654 1_445
O2 O1 O3 72.2(2) 1_544 1_445
O3 O1 O3 105.9(3) 3_544 1_445
O3 O1 O3 59.89(15) 4_654 1_445
O3 O1 O3 112.3(3) 1_554 1_445
O3 O1 O3 119.63(5) 4_665 1_445
Ga2 O1 O3 86.5(2) 1_545 3_645
La1 O1 O3 86.93(13) . 3_645
La1 O1 O3 150.2(3) 2_545 3_645
La1 O1 O3 41.32(19) 4_655 3_645
O2 O1 O3 123.2(5) 6 3_645
O2 O1 O3 66.7(3) 5_655 3_645
O2 O1 O3 90.1(3) 2_545 3_645
O2 O1 O3 115.5(5) 6_556 3_645
O2 O1 O3 60.9(3) 5_656 3_645
O2 O1 O3 84.3(3) 2_546 3_645
O3 O1 O3 125.5(3) 3_545 3_645
O3 O1 O3 113.1(3) 4_655 3_645
O3 O1 O3 6.9(3) . 3_645
Ga2 O1 O3 93.5(2) 1_544 3_645
O2 O1 O3 164.1(5) 4 3_645
O2 O1 O3 55.6(2) 3_655 3_645
O2 O1 O3 64.3(2) 1_545 3_645
Ga3 O1 O3 136.9(3) 2_546 3_645
Ga3 O1 O3 36.67(15) . 3_645
Ga3 O1 O3 89.26(17) 4_655 3_645
O3 O1 O3 112.55(15) 5_665 3_645
O3 O1 O3 123.02(18) 6_445 3_645
O3 O1 O3 32.9(3) 2_645 3_645
Ga3 O1 O3 128.8(3) 2_545 3_645
Ga3 O1 O3 56.68(13) 1_554 3_645
Ga3 O1 O3 93.26(17) 4_654 3_645
O3 O1 O3 106.4(2) 5_666 3_645
O3 O1 O3 115.4(2) 6_446 3_645
O3 O1 O3 34.6(3) 2_646 3_645
Nb O1 O3 131.52(14) . 3_645
Ga1 O1 O3 131.52(14) . 3_645
Nb O1 O3 18.29(12) 1_655 3_645
Ga1 O1 O3 18.29(12) 1_655 3_645
Ga1 O1 O3 108.70(13) 1_545 3_645
Nb O1 O3 108.70(13) 1_545 3_645
La1 O1 O3 84.68(19) 1_556 3_645
La1 O1 O3 113.3(3) 2_546 3_645
La1 O1 O3 62.49(15) 4_656 3_645
O2 O1 O3 90.91(19) . 3_645
O2 O1 O3 146.3(2) 3_545 3_645
O2 O1 O3 28.83(19) 4_655 3_645
Ga2 O1 O3 71.44(13) 2_556 3_645
Ga2 O1 O3 155.7(4) 2_446 3_645
Ga2 O1 O3 49.48(12) 2_546 3_645
O3 O1 O3 144.5(3) 2_545 3_645
O3 O1 O3 41.8(2) 6 3_645
O3 O1 O3 90.6(2) 5_655 3_645
O1 O1 O3 74.16(12) 2_655 3_645
O1 O1 O3 159.5(5) 2_545 3_645
O1 O1 O3 53.20(16) 2_645 3_645
O1 O1 O3 86.5(2) 1_556 3_645
O1 O1 O3 93.5(2) 1_554 3_645
Ga3 O1 O3 107.33(15) 4_665 3_645
Ga3 O1 O3 126.6(2) 1_445 3_645
Ga3 O1 O3 17.92(12) 2_646 3_645
O3 O1 O3 133.7(3) 2_546 3_645
O3 O1 O3 41.9(3) 6_556 3_645
O3 O1 O3 87.2(2) 5_656 3_645
O3 O1 O3 146.63(18) 1_455 3_645
O3 O1 O3 27.36(16) 4_765 3_645
O3 O1 O3 92.34(16) 3_535 3_645
O1 O1 O3 73.02(14) 2_656 3_645
O1 O1 O3 139.6(5) 2_546 3_645
O1 O1 O3 54.83(12) 2_646 3_645
O2 O1 O3 132.2(3) 4_554 3_645
O2 O1 O3 72.2(2) 3_654 3_645
O2 O1 O3 77.17(19) 1_544 3_645
O3 O1 O3 112.3(3) 3_544 3_645
O3 O1 O3 105.9(3) 4_654 3_645
O3 O1 O3 59.89(15) 1_554 3_645
O3 O1 O3 119.63(5) 4_665 3_645
O3 O1 O3 119.63(5) 1_445 3_645
Ga2 O1 La1 98.59(19) 1_545 4
La1 O1 La1 80.35(11) . 4
La1 O1 La1 37.72(4) 2_545 4
La1 O1 La1 143.6(5) 4_655 4
O2 O1 La1 49.2(2) 6 4
O2 O1 La1 104.2(4) 5_655 4
O2 O1 La1 91.9(3) 2_545 4
O2 O1 La1 67.3(2) 6_556 4
O2 O1 La1 119.1(4) 5_656 4
O2 O1 La1 106.2(3) 2_546 4
O3 O1 La1 44.4(2) 3_545 4
O3 O1 La1 79.2(2) 4_655 4
O3 O1 La1 162.0(2) . 4
Ga2 O1 La1 81.41(19) 1_544 4
O2 O1 La1 21.6(3) 4 4
O2 O1 La1 113.8(2) 3_655 4
O2 O1 La1 128.1(2) 1_545 4
Ga3 O1 La1 40.69(7) 2_546 4
Ga3 O1 La1 137.14(19) . 4
Ga3 O1 La1 103.46(8) 4_655 4
O3 O1 La1 54.78(16) 5_665 4
O3 O1 La1 64.58(16) 6_445 4
O3 O1 La1 142.2(5) 2_645 4
Ga3 O1 La1 41.86(4) 2_545 4
Ga3 O1 La1 113.6(3) 1_554 4
Ga3 O1 La1 90.93(18) 4_654 4
O3 O1 La1 68.59(13) 5_666 4
O3 O1 La1 76.60(16) 6_446 4
O3 O1 La1 150.5(4) 2_646 4
Nb O1 La1 36.14(2) . 4
Ga1 O1 La1 36.14(2) . 4
Nb O1 La1 149.8(3) 1_655 4
Ga1 O1 La1 149.8(3) 1_655 4
Ga1 O1 La1 81.98(6) 1_545 4
Nb O1 La1 81.98(6) 1_545 4
La1 O1 La1 93.89(14) 1_556 4
La1 O1 La1 74.81(9) 2_546 4
La1 O1 La1 125.6(3) 4_656 4
O2 O1 La1 78.40(14) . 4
O2 O1 La1 46.39(14) 3_545 4
O2 O1 La1 163.41(14) 4_655 4
Ga2 O1 La1 98.88(3) 2_556 4
Ga2 O1 La1 35.15(3) 2_446 4
Ga2 O1 La1 143.24(10) 2_546 4
O3 O1 La1 23.62(13) 2_545 4
O3 O1 La1 126.2(3) 6 4
O3 O1 La1 97.6(2) 5_655 4
O1 O1 La1 93.10(15) 2_655 4
O1 O1 La1 25.58(8) 2_545 4
O1 O1 La1 133.7(4) 2_645 4
O1 O1 La1 98.59(19) 1_556 4
O1 O1 La1 81.41(19) 1_554 4
Ga3 O1 La1 63.82(3) 4_665 4
Ga3 O1 La1 66.15(3) 1_445 4
Ga3 O1 La1 170.3(4) 2_646 4
O3 O1 La1 45.49(14) 2_546 4
O3 O1 La1 133.3(3) 6_556 4
O3 O1 La1 105.33(14) 5_656 4
O3 O1 La1 24.17(11) 1_455 4
O3 O1 La1 140.78(11) 4_765 4
O3 O1 La1 99.63(11) 3_535 4
O1 O1 La1 100.33(9) 2_656 4
O1 O1 La1 49.20(10) 2_546 4
O1 O1 La1 137.2(3) 2_646 4
O2 O1 La1 43.02(16) 4_554 4
O2 O1 La1 97.1(2) 3_654 4
O2 O1 La1 105.0(3) 1_544 4
O3 O1 La1 57.76(15) 3_544 4
O3 O1 La1 76.2(2) 4_654 4
O3 O1 La1 113.6(3) 1_554 4
O3 O1 La1 49.60(12) 4_665 4
O3 O1 La1 72.56(13) 1_445 4
O3 O1 La1 167.3(2) 3_645 4
Ga2 O1 La1 98.59(19) 1_545 2_655
La1 O1 La1 37.72(4) . 2_655
La1 O1 La1 143.6(5) 2_545 2_655
La1 O1 La1 80.35(11) 4_655 2_655
O2 O1 La1 91.9(3) 6 2_655
O2 O1 La1 49.2(2) 5_655 2_655
O2 O1 La1 104.2(4) 2_545 2_655
O2 O1 La1 106.2(3) 6_556 2_655
O2 O1 La1 67.3(2) 5_656 2_655
O2 O1 La1 119.1(4) 2_546 2_655
O3 O1 La1 79.2(2) 3_545 2_655
O3 O1 La1 162.0(2) 4_655 2_655
O3 O1 La1 44.4(2) . 2_655
Ga2 O1 La1 81.41(19) 1_544 2_655
O2 O1 La1 128.1(2) 4 2_655
O2 O1 La1 21.6(3) 3_655 2_655
O2 O1 La1 113.8(2) 1_545 2_655
Ga3 O1 La1 103.46(8) 2_546 2_655
Ga3 O1 La1 40.69(7) . 2_655
Ga3 O1 La1 137.14(19) 4_655 2_655
O3 O1 La1 64.58(16) 5_665 2_655
O3 O1 La1 142.2(5) 6_445 2_655
O3 O1 La1 54.78(16) 2_645 2_655
Ga3 O1 La1 90.93(18) 2_545 2_655
Ga3 O1 La1 41.86(4) 1_554 2_655
Ga3 O1 La1 113.6(3) 4_654 2_655
O3 O1 La1 76.60(16) 5_666 2_655
O3 O1 La1 150.5(4) 6_446 2_655
O3 O1 La1 68.59(13) 2_646 2_655
Nb O1 La1 81.98(6) . 2_655
Ga1 O1 La1 81.98(6) . 2_655
Nb O1 La1 36.14(2) 1_655 2_655
Ga1 O1 La1 36.14(2) 1_655 2_655
Ga1 O1 La1 149.8(3) 1_545 2_655
Nb O1 La1 149.8(3) 1_545 2_655
La1 O1 La1 74.81(9) 1_556 2_655
La1 O1 La1 125.6(3) 2_546 2_655
La1 O1 La1 93.89(15) 4_656 2_655
O2 O1 La1 46.39(14) . 2_655
O2 O1 La1 163.41(14) 3_545 2_655
O2 O1 La1 78.40(14) 4_655 2_655
Ga2 O1 La1 35.15(3) 2_556 2_655
Ga2 O1 La1 143.24(10) 2_446 2_655
Ga2 O1 La1 98.88(3) 2_546 2_655
O3 O1 La1 97.6(2) 2_545 2_655
O3 O1 La1 23.62(13) 6 2_655
O3 O1 La1 126.2(3) 5_655 2_655
O1 O1 La1 25.58(8) 2_655 2_655
O1 O1 La1 133.7(4) 2_545 2_655
O1 O1 La1 93.10(15) 2_645 2_655
O1 O1 La1 98.59(19) 1_556 2_655
O1 O1 La1 81.41(19) 1_554 2_655
Ga3 O1 La1 66.15(3) 4_665 2_655
Ga3 O1 La1 170.3(4) 1_445 2_655
Ga3 O1 La1 63.82(3) 2_646 2_655
O3 O1 La1 105.33(14) 2_546 2_655
O3 O1 La1 45.49(14) 6_556 2_655
O3 O1 La1 133.3(3) 5_656 2_655
O3 O1 La1 99.63(11) 1_455 2_655
O3 O1 La1 24.17(11) 4_765 2_655
O3 O1 La1 140.78(11) 3_535 2_655
O1 O1 La1 49.20(10) 2_656 2_655
O1 O1 La1 137.2(3) 2_546 2_655
O1 O1 La1 100.33(9) 2_646 2_655
O2 O1 La1 105.0(3) 4_554 2_655
O2 O1 La1 43.02(16) 3_654 2_655
O2 O1 La1 97.1(2) 1_544 2_655
O3 O1 La1 76.2(2) 3_544 2_655
O3 O1 La1 113.6(3) 4_654 2_655
O3 O1 La1 57.76(15) 1_554 2_655
O3 O1 La1 72.56(13) 4_665 2_655
O3 O1 La1 167.3(2) 1_445 2_655
O3 O1 La1 49.60(12) 3_645 2_655
La1 O1 La1 117.81(10) 4 2_655
Ga2 O1 La1 98.58(19) 1_545 1_545
La1 O1 La1 143.6(5) . 1_545
La1 O1 La1 80.35(11) 2_545 1_545
La1 O1 La1 37.72(4) 4_655 1_545
O2 O1 La1 104.2(4) 6 1_545
O2 O1 La1 91.9(3) 5_655 1_545
O2 O1 La1 49.2(2) 2_545 1_545
O2 O1 La1 119.1(4) 6_556 1_545
O2 O1 La1 106.2(3) 5_656 1_545
O2 O1 La1 67.3(2) 2_546 1_545
O3 O1 La1 162.0(2) 3_545 1_545
O3 O1 La1 44.4(2) 4_655 1_545
O3 O1 La1 79.2(2) . 1_545
Ga2 O1 La1 81.41(19) 1_544 1_545
O2 O1 La1 113.8(2) 4 1_545
O2 O1 La1 128.1(2) 3_655 1_545
O2 O1 La1 21.6(3) 1_545 1_545
Ga3 O1 La1 137.14(19) 2_546 1_545
Ga3 O1 La1 103.46(8) . 1_545
Ga3 O1 La1 40.69(7) 4_655 1_545
O3 O1 La1 142.2(5) 5_665 1_545
O3 O1 La1 54.78(16) 6_445 1_545
O3 O1 La1 64.58(16) 2_645 1_545
Ga3 O1 La1 113.6(3) 2_545 1_545
Ga3 O1 La1 90.93(18) 1_554 1_545
Ga3 O1 La1 41.86(4) 4_654 1_545
O3 O1 La1 150.5(4) 5_666 1_545
O3 O1 La1 68.59(13) 6_446 1_545
O3 O1 La1 76.60(16) 2_646 1_545
Nb O1 La1 149.8(3) . 1_545
Ga1 O1 La1 149.8(3) . 1_545
Nb O1 La1 81.98(6) 1_655 1_545
Ga1 O1 La1 81.98(6) 1_655 1_545
Ga1 O1 La1 36.14(2) 1_545 1_545
Nb O1 La1 36.14(2) 1_545 1_545
La1 O1 La1 125.6(3) 1_556 1_545
La1 O1 La1 93.89(15) 2_546 1_545
La1 O1 La1 74.81(9) 4_656 1_545
O2 O1 La1 163.41(14) . 1_545
O2 O1 La1 78.40(14) 3_545 1_545
O2 O1 La1 46.39(14) 4_655 1_545
Ga2 O1 La1 143.24(10) 2_556 1_545
Ga2 O1 La1 98.88(3) 2_446 1_545
Ga2 O1 La1 35.15(3) 2_546 1_545
O3 O1 La1 126.2(3) 2_545 1_545
O3 O1 La1 97.6(2) 6 1_545
O3 O1 La1 23.62(13) 5_655 1_545
O1 O1 La1 133.7(4) 2_655 1_545
O1 O1 La1 93.10(15) 2_545 1_545
O1 O1 La1 25.58(8) 2_645 1_545
O1 O1 La1 98.59(19) 1_556 1_545
O1 O1 La1 81.41(19) 1_554 1_545
Ga3 O1 La1 170.3(4) 4_665 1_545
Ga3 O1 La1 63.82(3) 1_445 1_545
Ga3 O1 La1 66.15(3) 2_646 1_545
O3 O1 La1 133.3(3) 2_546 1_545
O3 O1 La1 105.33(14) 6_556 1_545
O3 O1 La1 45.49(14) 5_656 1_545
O3 O1 La1 140.78(11) 1_455 1_545
O3 O1 La1 99.63(11) 4_765 1_545
O3 O1 La1 24.17(11) 3_535 1_545
O1 O1 La1 137.2(3) 2_656 1_545
O1 O1 La1 100.33(9) 2_546 1_545
O1 O1 La1 49.20(10) 2_646 1_545
O2 O1 La1 97.1(2) 4_554 1_545
O2 O1 La1 105.0(3) 3_654 1_545
O2 O1 La1 43.02(16) 1_544 1_545
O3 O1 La1 113.6(3) 3_544 1_545
O3 O1 La1 57.76(15) 4_654 1_545
O3 O1 La1 76.2(2) 1_554 1_545
O3 O1 La1 167.3(2) 4_665 1_545
O3 O1 La1 49.60(12) 1_445 1_545
O3 O1 La1 72.56(13) 3_645 1_545
La1 O1 La1 117.81(10) 4 1_545
La1 O1 La1 117.81(10) 2_655 1_545
Ga2 O1 O2 83.3(2) 1_545 1_445
La1 O1 O2 101.81(12) . 1_445
La1 O1 O2 33.1(2) 2_545 1_445
La1 O1 O2 138.8(2) 4_655 1_445
O2 O1 O2 68.2(3) 6 1_445
O2 O1 O2 124.8(4) 5_655 1_445
O2 O1 O2 95.4(4) 2_545 1_445
O2 O1 O2 56.3(4) 6_556 1_445
O2 O1 O2 111.2(4) 5_656 1_445
O2 O1 O2 84.1(3) 2_546 1_445
O3 O1 O2 58.9(2) 3_545 1_445
O3 O1 O2 60.2(2) 4_655 1_445
O3 O1 O2 166.9(6) . 1_445
Ga2 O1 O2 96.7(2) 1_544 1_445
O2 O1 O2 11.1(2) 4 1_445
O2 O1 O2 127.0(3) 3_655 1_445
O2 O1 O2 107.9(3) 1_545 1_445
Ga3 O1 O2 40.48(14) 2_546 1_445
Ga3 O1 O2 138.9(4) . 1_445
Ga3 O1 O2 81.06(14) 4_655 1_445
O3 O1 O2 77.49(18) 5_665 1_445
O3 O1 O2 58.5(2) 6_445 1_445
O3 O1 O2 155.3(4) 2_645 1_445
Ga3 O1 O2 62.80(13) 2_545 1_445
Ga3 O1 O2 134.9(3) 1_554 1_445
Ga3 O1 O2 90.44(17) 4_654 1_445
O3 O1 O2 71.46(19) 5_666 1_445
O3 O1 O2 53.52(19) 6_446 1_445
O3 O1 O2 134.3(4) 2_646 1_445
Nb O1 O2 56.47(12) . 1_445
Ga1 O1 O2 56.47(12) . 1_445
Nb O1 O2 172.9(2) 1_655 1_445
Ga1 O1 O2 172.9(2) 1_655 1_445
Ga1 O1 O2 67.97(13) 1_545 1_445
Nb O1 O2 67.97(13) 1_545 1_445
La1 O1 O2 89.2(2) 1_556 1_445
La1 O1 O2 55.54(14) 2_546 1_445
La1 O1 O2 106.0(3) 4_656 1_445
O2 O1 O2 93.06(18) . 1_445
O2 O1 O2 25.70(17) 3_545 1_445
O2 O1 O2 142.6(3) 4_655 1_445
Ga2 O1 O2 110.38(17) 2_556 1_445
Ga2 O1 O2 12.65(14) 2_446 1_445
Ga2 O1 O2 121.32(18) 2_546 1_445
O3 O1 O2 46.62(19) 2_545 1_445
O3 O1 O2 149.3(3) 6 1_445
O3 O1 O2 88.76(19) 5_655 1_445
O1 O1 O2 114.76(13) 2_655 1_445
O1 O1 O2 28.0(3) 2_545 1_445
O1 O1 O2 126.00(17) 2_645 1_445
O1 O1 O2 83.3(2) 1_556 1_445
O1 O1 O2 96.7(2) 1_554 1_445
Ga3 O1 O2 74.71(14) 4_665 1_445
Ga3 O1 O2 44.29(12) 1_445 1_445
Ga3 O1 O2 150.5(3) 2_646 1_445
O3 O1 O2 41.94(19) 2_546 1_445
O3 O1 O2 132.9(4) 6_556 1_445
O3 O1 O2 82.45(19) 5_656 1_445
O3 O1 O2 38.13(16) 1_455 1_445
O3 O1 O2 155.8(2) 4_765 1_445
O3 O1 O2 81.44(16) 3_535 1_445
O1 O1 O2 105.2(3) 2_656 1_445
O1 O1 O2 29.2(2) 2_546 1_445
O1 O1 O2 114.1(3) 2_646 1_445
O2 O1 O2 58.52(10) 4_554 1_445
O2 O1 O2 119.4(3) 3_654 1_445
O2 O1 O2 107.7(3) 1_544 1_445
O3 O1 O2 79.32(18) 3_544 1_445
O3 O1 O2 80.0(2) 4_654 1_445
O3 O1 O2 130.5(3) 1_554 1_445
O3 O1 O2 65.38(17) 4_665 1_445
O3 O1 O2 54.25(17) 1_445 1_445
O3 O1 O2 168.4(4) 3_645 1_445
La1 O1 O2 23.10(12) 4 1_445
La1 O1 O2 137.72(12) 2_655 1_445
La1 O1 O2 103.43(12) 1_545 1_445
Ga2 O1 O2 83.3(2) 1_545 4_665
La1 O1 O2 33.1(2) . 4_665
La1 O1 O2 138.8(2) 2_545 4_665
La1 O1 O2 101.81(12) 4_655 4_665
O2 O1 O2 95.4(4) 6 4_665
O2 O1 O2 68.2(3) 5_655 4_665
O2 O1 O2 124.8(4) 2_545 4_665
O2 O1 O2 84.1(3) 6_556 4_665
O2 O1 O2 56.3(4) 5_656 4_665
O2 O1 O2 111.2(4) 2_546 4_665
O3 O1 O2 60.2(2) 3_545 4_665
O3 O1 O2 166.9(6) 4_655 4_665
O3 O1 O2 58.9(2) . 4_665
Ga2 O1 O2 96.7(2) 1_544 4_665
O2 O1 O2 107.9(3) 4 4_665
O2 O1 O2 11.1(2) 3_655 4_665
O2 O1 O2 127.0(3) 1_545 4_665
Ga3 O1 O2 81.06(14) 2_546 4_665
Ga3 O1 O2 40.48(14) . 4_665
Ga3 O1 O2 138.9(4) 4_655 4_665
O3 O1 O2 58.5(2) 5_665 4_665
O3 O1 O2 155.3(4) 6_445 4_665
O3 O1 O2 77.49(18) 2_645 4_665
Ga3 O1 O2 90.44(17) 2_545 4_665
Ga3 O1 O2 62.80(13) 1_554 4_665
Ga3 O1 O2 134.9(3) 4_654 4_665
O3 O1 O2 53.52(19) 5_666 4_665
O3 O1 O2 134.3(4) 6_446 4_665
O3 O1 O2 71.46(19) 2_646 4_665
Nb O1 O2 67.97(13) . 4_665
Ga1 O1 O2 67.97(13) . 4_665
Nb O1 O2 56.47(12) 1_655 4_665
Ga1 O1 O2 56.47(12) 1_655 4_665
Ga1 O1 O2 172.9(2) 1_545 4_665
Nb O1 O2 172.9(2) 1_545 4_665
La1 O1 O2 55.54(14) 1_556 4_665
La1 O1 O2 106.0(3) 2_546 4_665
La1 O1 O2 89.2(2) 4_656 4_665
O2 O1 O2 25.70(17) . 4_665
O2 O1 O2 142.6(3) 3_545 4_665
O2 O1 O2 93.06(18) 4_655 4_665
Ga2 O1 O2 12.66(14) 2_556 4_665
Ga2 O1 O2 121.32(18) 2_446 4_665
Ga2 O1 O2 110.38(17) 2_546 4_665
O3 O1 O2 88.76(19) 2_545 4_665
O3 O1 O2 46.62(19) 6 4_665
O3 O1 O2 149.3(3) 5_655 4_665
O1 O1 O2 28.0(3) 2_655 4_665
O1 O1 O2 126.00(17) 2_545 4_665
O1 O1 O2 114.76(13) 2_645 4_665
O1 O1 O2 83.3(2) 1_556 4_665
O1 O1 O2 96.7(2) 1_554 4_665
Ga3 O1 O2 44.29(12) 4_665 4_665
Ga3 O1 O2 150.5(3) 1_445 4_665
Ga3 O1 O2 74.71(14) 2_646 4_665
O3 O1 O2 82.45(19) 2_546 4_665
O3 O1 O2 41.94(19) 6_556 4_665
O3 O1 O2 132.9(4) 5_656 4_665
O3 O1 O2 81.44(16) 1_455 4_665
O3 O1 O2 38.13(16) 4_765 4_665
O3 O1 O2 155.8(2) 3_535 4_665
O1 O1 O2 29.2(2) 2_656 4_665
O1 O1 O2 114.1(3) 2_546 4_665
O1 O1 O2 105.2(3) 2_646 4_665
O2 O1 O2 107.7(3) 4_554 4_665
O2 O1 O2 58.53(10) 3_654 4_665
O2 O1 O2 119.4(3) 1_544 4_665
O3 O1 O2 80.0(2) 3_544 4_665
O3 O1 O2 130.5(3) 4_654 4_665
O3 O1 O2 79.32(18) 1_554 4_665
O3 O1 O2 54.25(17) 4_665 4_665
O3 O1 O2 168.4(3) 1_445 4_665
O3 O1 O2 65.38(17) 3_645 4_665
La1 O1 O2 103.43(12) 4 4_665
La1 O1 O2 23.10(12) 2_655 4_665
La1 O1 O2 137.72(12) 1_545 4_665
O2 O1 O2 118.66(8) 1_445 4_665
Ga2 O1 O2 83.3(2) 1_545 3_645
La1 O1 O2 138.8(2) . 3_645
La1 O1 O2 101.81(12) 2_545 3_645
La1 O1 O2 33.1(2) 4_655 3_645
O2 O1 O2 124.8(4) 6 3_645
O2 O1 O2 95.4(4) 5_655 3_645
O2 O1 O2 68.2(3) 2_545 3_645
O2 O1 O2 111.2(4) 6_556 3_645
O2 O1 O2 84.1(3) 5_656 3_645
O2 O1 O2 56.3(4) 2_546 3_645
O3 O1 O2 166.9(6) 3_545 3_645
O3 O1 O2 58.9(2) 4_655 3_645
O3 O1 O2 60.2(2) . 3_645
Ga2 O1 O2 96.7(2) 1_544 3_645
O2 O1 O2 127.0(3) 4 3_645
O2 O1 O2 107.9(3) 3_655 3_645
O2 O1 O2 11.1(2) 1_545 3_645
Ga3 O1 O2 138.9(4) 2_546 3_645
Ga3 O1 O2 81.06(14) . 3_645
Ga3 O1 O2 40.48(14) 4_655 3_645
O3 O1 O2 155.3(4) 5_665 3_645
O3 O1 O2 77.49(18) 6_445 3_645
O3 O1 O2 58.5(2) 2_645 3_645
Ga3 O1 O2 134.9(3) 2_545 3_645
Ga3 O1 O2 90.44(17) 1_554 3_645
Ga3 O1 O2 62.80(13) 4_654 3_645
O3 O1 O2 134.3(4) 5_666 3_645
O3 O1 O2 71.46(19) 6_446 3_645
O3 O1 O2 53.52(19) 2_646 3_645
Nb O1 O2 172.9(2) . 3_645
Ga1 O1 O2 172.9(2) . 3_645
Nb O1 O2 67.97(13) 1_655 3_645
Ga1 O1 O2 67.97(13) 1_655 3_645
Ga1 O1 O2 56.47(12) 1_545 3_645
Nb O1 O2 56.47(12) 1_545 3_645
La1 O1 O2 106.0(3) 1_556 3_645
La1 O1 O2 89.2(2) 2_546 3_645
La1 O1 O2 55.54(14) 4_656 3_645
O2 O1 O2 142.6(3) . 3_645
O2 O1 O2 93.06(18) 3_545 3_645
O2 O1 O2 25.70(17) 4_655 3_645
Ga2 O1 O2 121.32(18) 2_556 3_645
Ga2 O1 O2 110.38(17) 2_446 3_645
Ga2 O1 O2 12.65(14) 2_546 3_645
O3 O1 O2 149.3(3) 2_545 3_645
O3 O1 O2 88.76(19) 6 3_645
O3 O1 O2 46.62(19) 5_655 3_645
O1 O1 O2 126.00(17) 2_655 3_645
O1 O1 O2 114.76(13) 2_545 3_645
O1 O1 O2 28.0(3) 2_645 3_645
O1 O1 O2 83.3(2) 1_556 3_645
O1 O1 O2 96.7(2) 1_554 3_645
Ga3 O1 O2 150.5(3) 4_665 3_645
Ga3 O1 O2 74.71(14) 1_445 3_645
Ga3 O1 O2 44.29(12) 2_646 3_645
O3 O1 O2 132.9(4) 2_546 3_645
O3 O1 O2 82.45(19) 6_556 3_645
O3 O1 O2 41.94(19) 5_656 3_645
O3 O1 O2 155.8(2) 1_455 3_645
O3 O1 O2 81.44(16) 4_765 3_645
O3 O1 O2 38.13(16) 3_535 3_645
O1 O1 O2 114.1(3) 2_656 3_645
O1 O1 O2 105.2(3) 2_546 3_645
O1 O1 O2 29.2(2) 2_646 3_645
O2 O1 O2 119.4(3) 4_554 3_645
O2 O1 O2 107.7(3) 3_654 3_645
O2 O1 O2 58.52(10) 1_544 3_645
O3 O1 O2 130.5(3) 3_544 3_645
O3 O1 O2 79.32(18) 4_654 3_645
O3 O1 O2 80.0(2) 1_554 3_645
O3 O1 O2 168.4(4) 4_665 3_645
O3 O1 O2 65.38(17) 1_445 3_645
O3 O1 O2 54.25(17) 3_645 3_645
La1 O1 O2 137.72(12) 4 3_645
La1 O1 O2 103.43(12) 2_655 3_645
La1 O1 O2 23.10(12) 1_545 3_645
O2 O1 O2 118.66(8) 1_445 3_645
O2 O1 O2 118.66(8) 4_665 3_645
Ga2 O1 O3 30.22(14) 1_545 3_546
La1 O1 O3 86.5(3) . 3_546
La1 O1 O3 102.0(4) 2_545 3_546
La1 O1 O3 138.0(5) 4_655 3_546
O2 O1 O3 118.8(3) 6 3_546
O2 O1 O3 136.7(3) 5_655 3_546
O2 O1 O3 163.5(3) 2_545 3_546
O2 O1 O3 15.0(3) 6_556 3_546
O2 O1 O3 43.4(3) 5_656 3_546
O2 O1 O3 59.9(4) 2_546 3_546
O3 O1 O3 53.4(3) 3_545 3_546
O3 O1 O3 98.8(4) 4_655 3_546
O3 O1 O3 98.8(4) . 3_546
Ga2 O1 O3 149.78(14) 1_544 3_546
O2 O1 O3 60.1(3) 4 3_546
O2 O1 O3 70.2(3) 3_655 3_546
O2 O1 O3 107.9(5) 1_545 3_546
Ga3 O1 O3 35.7(2) 2_546 3_546
Ga3 O1 O3 69.9(3) . 3_546
Ga3 O1 O3 87.4(4) 4_655 3_546
O3 O1 O3 89.2(3) 5_665 3_546
O3 O1 O3 123.4(4) 6_445 3_546
O3 O1 O3 135.6(3) 2_645 3_546
Ga3 O1 O3 108.48(13) 2_545 3_546
Ga3 O1 O3 132.57(13) 1_554 3_546
Ga3 O1 O3 154.90(19) 4_654 3_546
O3 O1 O3 23.5(3) 5_666 3_546
O3 O1 O3 66.0(3) 6_446 3_546
O3 O1 O3 75.0(3) 2_646 3_546
Nb O1 O3 70.56(18) . 3_546
Ga1 O1 O3 70.56(18) . 3_546
Nb O1 O3 111.5(2) 1_655 3_546
Ga1 O1 O3 111.5(2) 1_655 3_546
Ga1 O1 O3 116.5(3) 1_545 3_546
Nb O1 O3 116.5(3) 1_545 3_546
La1 O1 O3 20.11(11) 1_556 3_546
La1 O1 O3 37.17(18) 2_546 3_546
La1 O1 O3 59.1(2) 4_656 3_546
O2 O1 O3 57.4(2) . 3_546
O2 O1 O3 80.1(3) 3_545 3_546
O2 O1 O3 108.7(3) 4_655 3_546
Ga2 O1 O3 57.13(18) 2_556 3_546
Ga2 O1 O3 62.2(2) 2_446 3_546
Ga2 O1 O3 102.2(3) 2_546 3_546
O3 O1 O3 87.7(3) 2_545 3_546
O3 O1 O3 114.5(3) 6 3_546
O3 O1 O3 138.0(3) 5_655 3_546
O1 O1 O3 91.8(3) 2_655 3_546
O1 O1 O3 96.2(4) 2_545 3_546
O1 O1 O3 140.7(5) 2_645 3_546
O1 O1 O3 30.22(14) 1_556 3_546
O1 O1 O3 149.78(14) 1_554 3_546
Ga3 O1 O3 43.28(15) 4_665 3_546
Ga3 O1 O3 80.8(2) 1_445 3_546
Ga3 O1 O3 94.5(3) 2_646 3_546
O3 O1 O3 30.6(3) 2_546 3_546
O3 O1 O3 63.7(3) 6_556 3_546
O3 O1 O3 81.9(3) 5_656 3_546
O3 O1 O3 58.29(16) 1_455 3_546
O3 O1 O3 91.2(3) 4_765 3_546
O3 O1 O3 109.5(3) 3_535 3_546
O1 O1 O3 42.5(3) 2_656 3_546
O1 O1 O3 47.8(3) 2_546 3_546
O1 O1 O3 84.7(4) 2_646 3_546
O2 O1 O3 117.86(17) 4_554 3_546
O2 O1 O3 124.69(17) 3_654 3_546
O2 O1 O3 169.5(2) 1_544 3_546
O3 O1 O3 115.94(18) 3_544 3_546
O3 O1 O3 149.08(8) 4_654 3_546
O3 O1 O3 149.08(9) 1_554 3_546
O3 O1 O3 56.47(15) 4_665 3_546
O3 O1 O3 98.6(3) 1_445 3_546
O3 O1 O3 104.1(3) 3_645 3_546
La1 O1 O3 76.05(15) 4 3_546
La1 O1 O3 91.49(17) 2_655 3_546
La1 O1 O3 127.0(3) 1_545 3_546
O2 O1 O3 69.1(2) 1_445 3_546
O2 O1 O3 69.78(19) 4_665 3_546
O2 O1 O3 113.5(3) 3_645 3_546
Ga2 O2 Ga3 122.4(8) 2_556 4_665
Ga2 O2 La1 104.4(6) 2_556 4_665
Ga3 O2 La1 120.5(6) 4_665 4_665
Ga2 O2 O3 117.0(6) 2_556 3_545
Ga3 O2 O3 62.0(4) 4_665 3_545
La1 O2 O3 126.9(6) 4_665 3_545
Ga2 O2 O2 38.7(3) 2_556 4_665
Ga3 O2 O2 145.1(6) 4_665 4_665
La1 O2 O2 65.8(5) 4_665 4_665
O3 O2 O2 145.7(7) 3_545 4_665
Ga2 O2 O2 38.7(3) 2_556 3_655
Ga3 O2 O2 129.3(7) 4_665 3_655
La1 O2 O2 110.2(4) 4_665 3_655
O3 O2 O2 86.4(7) 3_545 3_655
O2 O2 O2 60.000(2) 4_665 3_655
Ga2 O2 La1 89.6(5) 2_556 .
Ga3 O2 La1 111.7(6) 4_665 .
La1 O2 La1 102.4(5) 4_665 .
O3 O2 La1 49.7(3) 3_545 .
O2 O2 La1 98.8(3) 4_665 .
O2 O2 La1 50.9(4) 3_655 .
Ga2 O2 O2 104.3(8) 2_556 2_556
Ga3 O2 O2 40.5(5) 4_665 2_556
La1 O2 O2 97.5(5) 4_665 2_556
O3 O2 O2 102.5(4) 3_545 2_556
O2 O2 O2 107.2(3) 4_665 2_556
O2 O2 O2 137.4(5) 3_655 2_556
La1 O2 O2 152.1(3) . 2_556
Ga2 O2 O3 160.9(8) 2_556 4_665
Ga3 O2 O3 38.8(4) 4_665 4_665
La1 O2 O3 92.1(4) 4_665 4_665
O3 O2 O3 56.5(5) 3_545 4_665
O2 O2 O3 155.4(7) 4_665 4_665
O2 O2 O3 142.7(7) 3_655 4_665
La1 O2 O3 96.3(5) . 4_665
O2 O2 O3 63.4(4) 2_556 4_665
Ga2 O2 O1 82.4(4) 2_556 2_655
Ga3 O2 O1 152.6(7) 4_665 2_655
La1 O2 O1 55.3(3) 4_665 2_655
O3 O2 O1 97.6(5) 3_545 2_655
O2 O2 O1 61.7(3) 4_665 2_655
O2 O2 O1 61.7(3) 3_655 2_655
La1 O2 O1 51.9(3) . 2_655
O2 O2 O1 152.7(6) 2_556 2_655
O3 O2 O1 115.4(6) 4_665 2_655
Ga2 O2 O3 91.2(6) 2_556 5_666
Ga3 O2 O3 35.7(3) 4_665 5_666
La1 O2 O3 154.9(5) 4_665 5_666
O3 O2 O3 57.7(5) 3_545 5_666
O2 O2 O3 126.6(4) 4_665 5_666
O2 O2 O3 94.4(5) 3_655 5_666
La1 O2 O3 97.1(5) . 5_666
O2 O2 O3 59.1(5) 2_556 5_666
O3 O2 O3 70.0(5) 4_665 5_666
O1 O2 O3 148.1(5) 2_655 5_666
Ga2 O2 O1 32.2(3) 2_556 2_656
Ga3 O2 O1 90.8(6) 4_665 2_656
La1 O2 O1 122.3(5) 4_665 2_656
O3 O2 O1 110.2(5) 3_545 2_656
O2 O2 O1 62.5(3) 4_665 2_656
O2 O2 O1 62.5(3) 3_655 2_656
La1 O2 O1 109.0(4) . 2_656
O2 O2 O1 75.4(6) 2_556 2_656
O3 O2 O1 129.5(6) 4_665 2_656
O1 O2 O1 114.6(4) 2_655 2_656
O3 O2 O1 64.1(5) 5_666 2_656
Ga2 O2 O3 131.3(6) 2_556 5_665
Ga3 O2 O3 93.5(5) 4_665 5_665
La1 O2 O3 78.8(4) 4_665 5_665
O3 O2 O3 49.3(5) 3_545 5_665
O2 O2 O3 120.8(3) 4_665 5_665
O2 O2 O3 93.8(4) 3_655 5_665
La1 O2 O3 43.9(3) . 5_665
O2 O2 O3 123.8(5) 2_556 5_665
O3 O2 O3 60.7(5) 4_665 5_665
O1 O2 O3 59.2(4) 2_655 5_665
O3 O2 O3 105.6(5) 5_666 5_665
O1 O2 O3 151.7(5) 2_656 5_665
Ga2 O2 O1 128.7(6) 2_556 1_565
Ga3 O2 O1 75.5(4) 4_665 1_565
La1 O2 O1 45.8(3) 4_665 1_565
O3 O2 O1 113.7(4) 3_545 1_565
O2 O2 O1 97.3(6) 4_665 1_565
O2 O2 O1 154.7(6) 3_655 1_565
La1 O2 O1 131.2(5) . 1_565
O2 O2 O1 56.0(5) 2_556 1_565
O3 O2 O1 58.3(3) 4_665 1_565
O1 O2 O1 99.0(4) 2_655 1_565
O3 O2 O1 109.1(4) 5_666 1_565
O1 O2 O1 119.3(5) 2_656 1_565
O3 O2 O1 88.8(4) 5_665 1_565
Ga2 O2 Ga1 148.6(6) 2_556 .
Ga3 O2 Ga1 61.0(4) 4_665 .
La1 O2 Ga1 97.2(4) 4_665 .
O3 O2 Ga1 33.0(3) 3_545 .
O2 O2 Ga1 153.2(2) 4_665 .
O2 O2 Ga1 112.2(6) 3_655 .
La1 O2 Ga1 63.3(3) . .
O2 O2 Ga1 95.1(3) 2_556 .
O3 O2 Ga1 33.0(3) 4_665 .
O1 O2 Ga1 91.7(5) 2_655 .
O3 O2 Ga1 77.6(4) 5_666 .
O1 O2 Ga1 140.0(5) 2_656 .
O3 O2 Ga1 32.5(2) 5_665 .
O1 O2 Ga1 82.7(3) 1_565 .
Ga2 O2 Nb 148.6(6) 2_556 .
Ga3 O2 Nb 61.0(4) 4_665 .
La1 O2 Nb 97.2(4) 4_665 .
O3 O2 Nb 33.0(3) 3_545 .
O2 O2 Nb 153.2(2) 4_665 .
O2 O2 Nb 112.2(6) 3_655 .
La1 O2 Nb 63.3(3) . .
O2 O2 Nb 95.1(3) 2_556 .
O3 O2 Nb 33.0(3) 4_665 .
O1 O2 Nb 91.7(5) 2_655 .
O3 O2 Nb 77.6(4) 5_666 .
O1 O2 Nb 140.0(5) 2_656 .
O3 O2 Nb 32.5(2) 5_665 .
O1 O2 Nb 82.7(3) 1_565 .
Ga1 O2 Nb 0.0 . .
Ga2 O2 O2 139.0(6) 2_556 2
Ga3 O2 O2 97.3(5) 4_665 2
La1 O2 O2 39.0(3) 4_665 2
O3 O2 O2 89.0(4) 3_545 2
O2 O2 O2 102.4(2) 4_665 2
O2 O2 O2 122.3(4) 3_655 2
La1 O2 O2 84.2(5) . 2
O2 O2 O2 99.7(6) 2_556 2
O3 O2 O2 59.9(4) 4_665 2
O1 O2 O2 62.1(5) 2_655 2
O3 O2 O2 129.7(4) 5_666 2
O1 O2 O2 160.7(3) 2_656 2
O3 O2 O2 45.4(3) 5_665 2
O1 O2 O2 47.3(4) 1_565 2
Ga1 O2 O2 58.2(2) . 2
Nb O2 O2 58.2(2) . 2
Ga2 O2 Ga2 113.3(6) 2_556 .
Ga3 O2 Ga2 60.2(4) 4_665 .
La1 O2 Ga2 69.1(3) 4_665 .
O3 O2 Ga2 117.1(4) 3_545 .
O2 O2 Ga2 97.1(6) 4_665 .
O2 O2 Ga2 151.9(5) 3_655 .
La1 O2 Ga2 156.7(5) . .
O2 O2 Ga2 28.6(3) 2_556 .
O3 O2 Ga2 63.5(3) 4_665 .
O1 O2 Ga2 124.4(4) 2_655 .
O3 O2 Ga2 86.8(4) 5_666 .
O1 O2 Ga2 93.4(4) 2_656 .
O3 O2 Ga2 112.9(4) 5_665 .
O1 O2 Ga2 28.9(3) 1_565 .
Ga1 O2 Ga2 95.5(3) . .
Nb O2 Ga2 95.5(3) . .
O2 O2 Ga2 75.8(3) 2 .
Ga2 O2 O3 80.6(5) 2_556 1_565
Ga3 O2 O3 114.8(6) 4_665 1_565
La1 O2 O3 36.6(3) 4_665 1_565
O3 O2 O3 161.5(5) 3_545 1_565
O2 O2 O3 47.1(5) 4_665 1_565
O2 O2 O3 106.8(5) 3_655 1_565
La1 O2 O3 130.0(5) . 1_565
O2 O2 O3 76.8(3) 2_556 1_565
O3 O2 O3 108.7(5) 4_665 1_565
O1 O2 O3 78.2(3) 2_655 1_565
O3 O2 O3 131.7(5) 5_666 1_565
O1 O2 O3 87.7(4) 2_656 1_565
O3 O2 O3 115.4(4) 5_665 1_565
O1 O2 O3 50.3(2) 1_565 1_565
Ga1 O2 O3 128.5(4) . 1_565
Nb O2 O3 128.5(4) . 1_565
O2 O2 O3 73.0(3) 2 1_565
Ga2 O2 O3 54.9(2) . 1_565
Ga2 O2 La1 66.3(5) 2_556 4_666
Ga3 O2 La1 69.9(5) 4_665 4_666
La1 O2 La1 102.8(4) 4_665 4_666
O3 O2 La1 122.9(5) 3_545 4_666
O2 O2 La1 75.2(3) 4_665 4_666
O2 O2 La1 102.4(2) 3_655 4_666
La1 O2 La1 148.6(4) . 4_666
O2 O2 La1 38.2(4) 2_556 4_666
O3 O2 La1 101.1(4) 4_665 4_666
O1 O2 La1 136.5(4) 2_655 4_666
O3 O2 La1 65.4(4) 5_666 4_666
O1 O2 La1 40.6(3) 2_656 4_666
O3 O2 La1 161.9(4) 5_665 4_666
O1 O2 La1 80.1(4) 1_565 4_666
Ga1 O2 La1 130.6(4) . 4_666
Nb O2 La1 130.6(4) . 4_666
O2 O2 La1 127.1(4) 2 4_666
Ga2 O2 La1 52.9(2) . 4_666
O3 O2 La1 67.9(3) 1_565 4_666
Ga2 O2 Ga3 108.3(5) 2_556 2_546
Ga3 O2 Ga3 49.0(3) 4_665 2_546
La1 O2 Ga3 144.5(5) 4_665 2_546
O3 O2 Ga3 20.4(3) 3_545 2_546
O2 O2 Ga3 145.6(5) 4_665 2_546
O2 O2 Ga3 87.8(6) 3_655 2_546
La1 O2 Ga3 64.8(3) . 2_546
O2 O2 Ga3 87.7(3) 2_556 2_546
O3 O2 Ga3 58.9(3) 4_665 2_546
O1 O2 Ga3 115.8(4) 2_655 2_546
O3 O2 Ga3 37.4(3) 5_666 2_546
O1 O2 Ga3 93.1(4) 2_656 2_546
O3 O2 Ga3 69.4(3) 5_665 2_546
O1 O2 Ga3 116.4(3) 1_565 2_546
Ga1 O2 Ga3 47.28(16) . 2_546
Nb O2 Ga3 47.28(16) . 2_546
O2 O2 Ga3 105.50(19) 2 2_546
Ga2 O2 Ga3 108.9(3) . 2_546
O3 O2 Ga3 163.8(4) 1_565 2_546
La1 O2 Ga3 102.7(3) 4_666 2_546
Ga2 O2 O3 53.9(4) 2_556 2_656
Ga3 O2 O3 101.9(6) 4_665 2_656
La1 O2 O3 76.5(4) 4_665 2_656
O3 O2 O3 155.5(5) 3_545 2_656
O2 O2 O3 43.9(4) 4_665 2_656
O2 O2 O3 91.6(4) 3_655 2_656
La1 O2 O3 140.4(4) . 2_656
O2 O2 O3 63.5(3) 2_556 2_656
O3 O2 O3 123.3(5) 4_665 2_656
O1 O2 O3 102.9(4) 2_655 2_656
O3 O2 O3 98.2(6) 5_666 2_656
O1 O2 O3 48.7(3) 2_656 2_656
O3 O2 O3 155.0(5) 5_665 2_656
O1 O2 O3 76.4(4) 1_565 2_656
Ga1 O2 O3 156.0(4) . 2_656
Nb O2 O3 156.0(4) . 2_656
O2 O2 O3 112.3(3) 2 2_656
Ga2 O2 O3 60.6(3) . 2_656
O3 O2 O3 40.0(4) 1_565 2_656
La1 O2 O3 34.1(2) 4_666 2_656
Ga3 O2 O3 135.2(4) 2_546 2_656
Ga2 O2 Ga3 44.1(3) 2_556 2_656
Ga3 O2 Ga3 126.5(6) 4_665 2_656
La1 O2 Ga3 66.4(3) 4_665 2_656
O3 O2 Ga3 160.9(4) 3_545 2_656
O2 O2 Ga3 19.5(3) 4_665 2_656
O2 O2 Ga3 75.3(4) 3_655 2_656
La1 O2 Ga3 118.1(3) . 2_656
O2 O2 Ga3 87.7(3) 2_556 2_656
O3 O2 Ga3 142.0(5) 4_665 2_656
O1 O2 Ga3 78.8(3) 2_655 2_656
O3 O2 Ga3 117.3(5) 5_666 2_656
O1 O2 Ga3 56.3(2) 2_656 2_656
O3 O2 Ga3 136.1(5) 5_665 2_656
O1 O2 Ga3 85.5(3) 1_565 2_656
Ga1 O2 Ga3 163.6(4) . 2_656
Nb O2 Ga3 163.6(4) . 2_656
O2 O2 Ga3 105.35(19) 2 2_656
Ga2 O2 Ga3 79.3(3) . 2_656
O3 O2 Ga3 36.6(2) 1_565 2_656
La1 O2 Ga3 57.7(2) 4_666 2_656
Ga3 O2 Ga3 149.2(4) 2_546 2_656
O3 O2 Ga3 24.67(17) 2_656 2_656
Ga2 O2 La1 58.3(4) 2_556 1_556
Ga3 O2 La1 68.7(4) 4_665 1_556
La1 O2 La1 159.4(5) 4_665 1_556
O3 O2 La1 73.4(4) 3_545 1_556
O2 O2 La1 96.0(2) 4_665 1_556
O2 O2 La1 64.5(3) 3_655 1_556
La1 O2 La1 89.3(3) . 1_556
O2 O2 La1 78.2(6) 2_556 1_556
O3 O2 La1 103.5(4) 4_665 1_556
O1 O2 La1 125.8(4) 2_655 1_556
O3 O2 La1 33.8(3) 5_666 1_556
O1 O2 La1 37.1(2) 2_656 1_556
O3 O2 La1 120.5(4) 5_665 1_556
O1 O2 La1 134.1(5) 1_565 1_556
Ga1 O2 La1 103.2(3) . 1_556
Nb O2 La1 103.2(3) . 1_556
O2 O2 La1 161.23(18) 2 1_556
Ga2 O2 La1 105.8(4) . 1_556
O3 O2 La1 123.7(4) 1_565 1_556
La1 O2 La1 61.4(2) 4_666 1_556
Ga3 O2 La1 55.98(17) 2_546 1_556
O3 O2 La1 83.7(4) 2_656 1_556
Ga3 O2 La1 93.2(3) 2_656 1_556
Ga2 O2 La1 47.7(3) 2_556 2_655
Ga3 O2 La1 169.2(6) 4_665 2_655
La1 O2 La1 69.6(3) 4_665 2_655
O3 O2 La1 116.2(4) 3_545 2_655
O2 O2 La1 32.1(2) 4_665 2_655
O2 O2 La1 41.1(3) 3_655 2_655
La1 O2 La1 67.1(2) . 2_655
O2 O2 La1 139.3(3) 2_556 2_655
O3 O2 La1 150.6(5) 4_665 2_655
O1 O2 La1 35.2(2) 2_655 2_655
O3 O2 La1 133.7(4) 5_666 2_655
O1 O2 La1 79.8(3) 2_656 2_655
O3 O2 La1 92.4(4) 5_665 2_655
O1 O2 La1 113.7(3) 1_565 2_655
Ga1 O2 La1 124.1(4) . 2_655
Nb O2 La1 124.1(4) . 2_655
O2 O2 La1 93.3(4) 2 2_655
Ga2 O2 La1 125.1(3) . 2_655
O3 O2 La1 70.4(3) 1_565 2_655
La1 O2 La1 105.2(3) 4_666 2_655
Ga3 O2 La1 125.7(3) 2_546 2_655
O3 O2 La1 75.9(3) 2_656 2_655
Ga3 O2 La1 51.63(14) 2_656 2_655
La1 O2 La1 100.5(2) 1_556 2_655
Ga2 O2 Ga3 135.7(6) 2_556 4_664
Ga3 O2 Ga3 100.1(5) 4_665 4_664
La1 O2 Ga3 57.2(3) 4_665 4_664
O3 O2 Ga3 70.0(4) 3_545 4_664
O2 O2 Ga3 109.7(2) 4_665 4_664
O2 O2 Ga3 105.1(2) 3_655 4_664
La1 O2 Ga3 60.9(3) . 4_664
O2 O2 Ga3 117.2(6) 2_556 4_664
O3 O2 Ga3 61.9(4) 4_665 4_664
O1 O2 Ga3 53.6(3) 2_655 4_664
O3 O2 Ga3 122.5(5) 5_666 4_664
O1 O2 Ga3 167.3(5) 2_656 4_664
O3 O2 Ga3 22.2(2) 5_665 4_664
O1 O2 Ga3 70.4(3) 1_565 4_664
Ga1 O2 Ga3 44.95(17) . 4_664
Nb O2 Ga3 44.95(17) . 4_664
O2 O2 Ga3 24.0(2) 2 4_664
Ga2 O2 Ga3 97.7(3) . 4_664
O3 O2 Ga3 93.6(3) 1_565 4_664
La1 O2 Ga3 150.4(3) 4_666 4_664
Ga3 O2 Ga3 89.2(3) 2_546 4_664
O3 O2 Ga3 133.6(4) 2_656 4_664
Ga3 O2 Ga3 119.8(3) 2_656 4_664
La1 O2 Ga3 142.6(3) 1_556 4_664
La1 O2 Ga3 88.8(3) 2_655 4_664
Ga2 O2 O3 122.8(7) 2_556 6_456
Ga3 O2 O3 1.3(3) 4_665 6_456
La1 O2 O3 119.4(4) 4_665 6_456
O3 O2 O3 63.1(4) 3_545 6_456
O2 O2 O3 144.5(4) 4_665 6_456
O2 O2 O3 130.5(5) 3_655 6_456
La1 O2 O3 112.8(4) . 6_456
O2 O2 O3 39.4(2) 2_556 6_456
O3 O2 O3 38.5(4) 4_665 6_456
O1 O2 O3 152.8(5) 2_655 6_456
O3 O2 O3 36.7(3) 5_666 6_456
O1 O2 O3 91.1(5) 2_656 6_456
O3 O2 O3 93.9(3) 5_665 6_456
O1 O2 O3 74.3(3) 1_565 6_456
Ga1 O2 O3 61.4(2) . 6_456
Nb O2 O3 61.4(2) . 6_456
O2 O2 O3 96.7(3) 2 6_456
Ga2 O2 O3 59.0(2) . 6_456
O3 O2 O3 113.6(4) 1_565 6_456
La1 O2 O3 69.4(3) 4_666 6_456
Ga3 O2 O3 50.24(19) 2_546 6_456
O3 O2 O3 101.1(4) 2_656 6_456
Ga3 O2 O3 125.8(4) 2_656 6_456
La1 O2 O3 69.6(3) 1_556 6_456
La1 O2 O3 170.0(4) 2_655 6_456
Ga3 O2 O3 100.0(3) 4_664 6_456
Ga2 O2 Ga3 36.7(3) 2_556 .
Ga3 O2 Ga3 116.5(5) 4_665 .
La1 O2 Ga3 122.9(4) 4_665 .
O3 O2 Ga3 82.1(4) 3_545 .
O2 O2 Ga3 66.8(3) 4_665 .
O2 O2 Ga3 13.6(3) 3_655 .
La1 O2 Ga3 56.44(19) . .
O2 O2 Ga3 125.7(7) 2_556 .
O3 O2 Ga3 137.6(5) 4_665 .
O1 O2 Ga3 75.1(3) 2_655 .
O3 O2 Ga3 81.2(3) 5_666 .
O1 O2 Ga3 53.3(2) 2_656 .
O3 O2 Ga3 100.4(4) 5_665 .
O1 O2 Ga3 164.0(4) 1_565 .
Ga1 O2 Ga3 112.0(3) . .
Nb O2 Ga3 112.0(3) . .
O2 O2 Ga3 134.6(6) 2 .
Ga2 O2 Ga3 146.6(4) . .
O3 O2 Ga3 113.7(3) 1_565 .
La1 O2 Ga3 93.9(3) 4_666 .
Ga3 O2 Ga3 79.3(2) 2_546 .
O3 O2 Ga3 90.3(3) 2_656 .
Ga3 O2 Ga3 78.83(19) 2_656 .
La1 O2 Ga3 50.90(14) 1_556 .
La1 O2 Ga3 53.35(13) 2_655 .
Ga3 O2 Ga3 115.1(3) 4_664 .
O3 O2 Ga3 117.7(3) 6_456 .
Ga2 O2 La1 162.7(6) 2_556 2
Ga3 O2 La1 59.3(3) 4_665 2
La1 O2 La1 65.3(2) 4_665 2
O3 O2 La1 79.6(3) 3_545 2
O2 O2 La1 128.7(6) 4_665 2
O2 O2 La1 156.2(4) 3_655 2
La1 O2 La1 106.0(4) . 2
O2 O2 La1 65.2(4) 2_556 2
O3 O2 La1 27.2(3) 4_665 2
O1 O2 La1 101.0(4) 2_655 2
O3 O2 La1 94.3(3) 5_666 2
O1 O2 La1 140.6(5) 2_656 2
O3 O2 La1 62.5(2) 5_665 2
O1 O2 La1 34.21(15) 1_565 2
Ga1 O2 La1 48.74(14) . 2
Nb O2 La1 48.74(14) . 2
O2 O2 La1 39.1(2) 2 2
Ga2 O2 La1 50.77(14) . 2
O3 O2 La1 83.5(3) 1_565 2
La1 O2 La1 101.3(3) 4_666 2
Ga3 O2 La1 85.7(2) 2_546 2
O3 O2 La1 109.0(3) 2_656 2
Ga3 O2 La1 119.5(3) 2_656 2
La1 O2 La1 127.9(3) 1_556 2
La1 O2 La1 131.5(3) 2_655 2
Ga3 O2 La1 52.04(15) 4_664 2
O3 O2 La1 58.5(2) 6_456 2
Ga3 O2 La1 160.6(4) . 2
Ga2 O2 O3 86.3(5) 2_556 2_655
Ga3 O2 O3 139.2(6) 4_665 2_655
La1 O2 O3 19.6(2) 4_665 2_655
O3 O2 O3 134.1(5) 3_545 2_655
O2 O2 O3 48.3(4) 4_665 2_655
O2 O2 O3 91.5(4) 3_655 2_655
La1 O2 O3 95.3(4) . 2_655
O2 O2 O3 109.5(4) 2_556 2_655
O3 O2 O3 111.1(4) 4_665 2_655
O1 O2 O3 43.8(2) 2_655 2_655
O3 O2 O3 167.3(6) 5_666 2_655
O1 O2 O3 109.2(4) 2_656 2_655
O3 O2 O3 85.2(5) 5_665 2_655
O1 O2 O3 63.7(3) 1_565 2_655
Ga1 O2 O3 110.6(4) . 2_655
Nb O2 O3 110.6(4) . 2_655
O2 O2 O3 54.2(3) 2 2_655
Ga2 O2 O3 82.7(3) . 2_655
O3 O2 O3 35.6(3) 1_565 2_655
La1 O2 O3 102.3(3) 4_666 2_655
Ga3 O2 O3 154.5(4) 2_546 2_655
O3 O2 O3 70.3(3) 2_656 2_655
Ga3 O2 O3 53.5(2) 2_656 2_655
La1 O2 O3 144.2(4) 1_556 2_655
La1 O2 O3 50.4(2) 2_655 2_655
Ga3 O2 O3 66.4(3) 4_664 2_655
O3 O2 O3 138.0(4) 6_456 2_655
Ga3 O2 O3 103.7(3) . 2_655
La1 O2 O3 84.7(3) 2 2_655
Ga2 O2 Ga2 94.8(5) 2_556 2
Ga3 O2 Ga2 140.9(6) 4_665 2
La1 O2 Ga2 51.2(3) 4_665 2
O3 O2 Ga2 92.0(4) 3_545 2
O2 O2 Ga2 72.11(12) 4_665 2
O2 O2 Ga2 72.11(12) 3_655 2
La1 O2 Ga2 51.7(2) . 2
O2 O2 Ga2 147.1(6) 2_556 2
O3 O2 Ga2 103.1(5) 4_665 2
O1 O2 Ga2 12.5(2) 2_655 2
O3 O2 Ga2 148.1(5) 5_666 2
O1 O2 Ga2 127.0(4) 2_656 2
O3 O2 Ga2 48.8(3) 5_665 2
O1 O2 Ga2 91.2(4) 1_565 2
Ga1 O2 Ga2 81.1(3) . 2
Nb O2 Ga2 81.1(3) . 2
O2 O2 Ga2 50.6(4) 2 2
Ga2 O2 Ga2 118.8(3) . 2
O3 O2 Ga2 80.2(3) 1_565 2
La1 O2 Ga2 144.7(3) 4_666 2
Ga3 O2 Ga2 111.7(3) 2_546 2
O3 O2 Ga2 110.6(3) 2_656 2
Ga3 O2 Ga2 87.8(2) 2_656 2
La1 O2 Ga2 134.6(3) 1_556 2
La1 O2 Ga2 47.56(15) 2_655 2
Ga3 O2 Ga2 41.19(14) 4_664 2
O3 O2 Ga2 140.9(4) 6_456 2
Ga3 O2 Ga2 85.2(2) . 2
La1 O2 Ga2 89.1(3) 2 2
O3 O2 Ga2 44.6(2) 2_655 2
Ga2 O2 O2 91.4(7) 2_556 5_666
Ga3 O2 O2 76.3(5) 4_665 5_666
La1 O2 O2 67.3(3) 4_665 5_666
O3 O2 O2 137.5(5) 3_545 5_666
O2 O2 O2 75.8(6) 4_665 5_666
O2 O2 O2 129.5(6) 3_655 5_666
La1 O2 O2 169.6(6) . 5_666
O2 O2 O2 36.8(3) 2_556 5_666
O3 O2 O2 86.1(4) 4_665 5_666
O1 O2 O2 118.0(5) 2_655 5_666
O3 O2 O2 93.2(6) 5_666 5_666
O1 O2 O2 76.7(5) 2_656 5_666
O3 O2 O2 131.4(4) 5_665 5_666
O1 O2 O2 42.6(3) 1_565 5_666
Ga1 O2 O2 118.2(4) . 5_666
Nb O2 O2 118.2(4) . 5_666
O2 O2 O2 88.2(3) 2 5_666
Ga2 O2 O2 22.73(11) . 5_666
O3 O2 O2 40.2(3) 1_565 5_666
La1 O2 O2 39.2(3) 4_666 5_666
Ga3 O2 O2 124.5(5) 2_546 5_666
O3 O2 O2 38.0(3) 2_656 5_666
Ga3 O2 O2 57.1(3) 2_656 5_666
La1 O2 O2 100.0(5) 1_556 5_666
La1 O2 O2 106.2(4) 2_655 5_666
Ga3 O2 O2 112.1(4) 4_664 5_666
O3 O2 O2 75.2(4) 6_456 5_666
Ga3 O2 O2 126.9(5) . 5_666
La1 O2 O2 71.9(2) 2 5_666
O3 O2 O2 74.4(3) 2_655 5_666
Ga2 O2 O2 117.8(4) 2 5_666
Ga2 O2 O2 51.5(4) 2_556 5_656
Ga3 O2 O2 93.3(6) 4_665 5_656
La1 O2 O2 146.2(6) 4_665 5_656
O3 O2 O2 65.8(3) 3_545 5_656
O2 O2 O2 87.6(4) 4_665 5_656
O2 O2 O2 36.0(4) 3_655 5_656
La1 O2 O2 59.67(18) . 5_656
O2 O2 O2 110.6(8) 2_556 5_656
O3 O2 O2 116.8(5) 4_665 5_656
O1 O2 O2 94.4(4) 2_655 5_656
O3 O2 O2 58.5(4) 5_666 5_656
O1 O2 O2 52.3(3) 2_656 5_656
O3 O2 O2 99.5(4) 5_665 5_656
O1 O2 O2 166.6(6) 1_565 5_656
Ga1 O2 O2 98.6(4) . 5_656
Nb O2 O2 98.6(4) . 5_656
O2 O2 O2 143.7(6) 2 5_656
Ga2 O2 O2 138.2(6) . 5_656
O3 O2 O2 132.2(5) 1_565 5_656
La1 O2 O2 89.1(5) 4_666 5_656
Ga3 O2 O2 58.0(3) 2_546 5_656
O3 O2 O2 99.1(5) 2_656 5_656
Ga3 O2 O2 95.6(4) 2_656 5_656
La1 O2 O2 32.5(3) 1_556 5_656
La1 O2 O2 76.8(3) 2_655 5_656
Ga3 O2 O2 119.8(4) 4_664 5_656
O3 O2 O2 94.5(4) 6_456 5_656
Ga3 O2 O2 23.49(16) . 5_656
La1 O2 O2 143.7(4) 2 5_656
O3 O2 O2 127.2(4) 2_655 5_656
Ga2 O2 O2 102.3(4) 2 5_656
O2 O2 O2 128.0(7) 5_666 5_656
Ga2 O2 O3 165.2(7) 2_556 6_455
Ga3 O2 O3 67.8(4) 4_665 6_455
La1 O2 O3 75.6(4) 4_665 6_455
O3 O2 O3 55.9(4) 3_545 6_455
O2 O2 O3 139.1(4) 4_665 6_455
O2 O2 O3 127.0(5) 3_655 6_455
La1 O2 O3 76.2(3) . 6_455
O2 O2 O3 90.3(4) 2_556 6_455
O3 O2 O3 29.7(4) 4_665 6_455
O1 O2 O3 85.8(5) 2_655 6_455
O3 O2 O3 94.2(3) 5_666 6_455
O1 O2 O3 157.9(5) 2_656 6_455
O3 O2 O3 33.9(3) 5_665 6_455
O1 O2 O3 62.0(3) 1_565 6_455
Ga1 O2 O3 22.96(15) . 6_455
Nb O2 O3 22.96(15) . 6_455
O2 O2 O3 37.1(2) 2 6_455
Ga2 O2 O3 80.7(2) . 6_455
O3 O2 O3 105.6(3) 1_565 6_455
La1 O2 O3 128.4(3) 4_666 6_455
Ga3 O2 O3 69.3(2) 2_546 6_455
O3 O2 O3 138.3(4) 2_656 6_455
Ga3 O2 O3 141.2(4) 2_656 6_455
La1 O2 O3 124.1(3) 1_556 6_455
La1 O2 O3 121.0(4) 2_655 6_455
Ga3 O2 O3 32.3(2) 4_664 6_455
O3 O2 O3 67.6(2) 6_456 6_455
Ga3 O2 O3 131.0(3) . 6_455
La1 O2 O3 30.08(15) 2 6_455
O3 O2 O3 91.3(4) 2_655 6_455
Ga2 O2 O3 73.5(3) 2 6_455
O2 O2 O3 101.9(3) 5_666 6_455
O2 O2 O3 121.1(4) 5_656 6_455
Ga2 O2 O2 85.5(5) 2_556 6_556
Ga3 O2 O2 62.6(4) 4_665 6_556
La1 O2 O2 162.2(7) 4_665 6_556
O3 O2 O2 36.5(3) 3_545 6_556
O2 O2 O2 123.1(4) 4_665 6_556
O2 O2 O2 68.5(5) 3_655 6_556
La1 O2 O2 62.4(3) . 6_556
O2 O2 O2 94.2(6) 2_556 6_556
O3 O2 O2 81.2(3) 4_665 6_556
O1 O2 O2 112.9(5) 2_655 6_556
O3 O2 O2 35.3(3) 5_666 6_556
O1 O2 O2 73.7(4) 2_656 6_556
O3 O2 O2 83.6(4) 5_665 6_556
O1 O2 O2 136.7(2) 1_565 6_556
Ga1 O2 O2 68.3(3) . 6_556
Nb O2 O2 68.3(3) . 6_556
O2 O2 O2 125.6(4) 2 6_556
Ga2 O2 O2 121.0(4) . 6_556
O3 O2 O2 161.0(6) 1_565 6_556
La1 O2 O2 94.7(5) 4_666 6_556
Ga3 O2 O2 22.76(16) 2_546 6_556
O3 O2 O2 121.0(5) 2_656 6_556
Ga3 O2 O2 127.7(4) 2_656 6_556
La1 O2 O2 37.3(2) 1_556 6_556
La1 O2 O2 109.2(2) 2_655 6_556
Ga3 O2 O2 105.4(4) 4_664 6_556
O3 O2 O2 63.9(2) 6_456 6_556
Ga3 O2 O2 58.12(17) . 6_556
La1 O2 O2 108.2(2) 2 6_556
O3 O2 O2 156.2(4) 2_655 6_556
Ga2 O2 O2 114.1(4) 2 6_556
O2 O2 O2 128.1(7) 5_666 6_556
O2 O2 O2 35.7(3) 5_656 6_556
O3 O2 O2 91.0(3) 6_455 6_556
Ga2 O2 Nb 100.8(5) 2_556 1_556
Ga3 O2 Nb 23.7(3) 4_665 1_556
La1 O2 Nb 142.7(4) 4_665 1_556
O3 O2 Nb 60.0(3) 3_545 1_556
O2 O2 Nb 132.87(16) 4_665 1_556
O2 O2 Nb 106.7(4) 3_655 1_556
La1 O2 Nb 104.7(3) . 1_556
O2 O2 Nb 49.4(3) 2_556 1_556
O3 O2 Nb 60.1(3) 4_665 1_556
O1 O2 Nb 156.5(4) 2_655 1_556
O3 O2 Nb 12.3(2) 5_666 1_556
O1 O2 Nb 71.3(4) 2_656 1_556
O3 O2 Nb 104.2(4) 5_665 1_556
O1 O2 Nb 97.0(3) 1_565 1_556
Ga1 O2 Nb 73.3(2) . 1_556
Nb O2 Nb 73.3(2) . 1_556
O2 O2 Nb 120.0(3) 2 1_556
Ga2 O2 Nb 76.0(2) . 1_556
O3 O2 Nb 125.2(4) 1_565 1_556
La1 O2 Nb 63.5(2) 4_666 1_556
Ga3 O2 Nb 40.95(13) 2_546 1_556
O3 O2 Nb 97.6(4) 2_656 1_556
Ga3 O2 Nb 119.7(3) 2_656 1_556
La1 O2 Nb 45.09(14) 1_556 1_556
La1 O2 Nb 145.5(3) 2_655 1_556
Ga3 O2 Nb 117.4(3) 4_664 1_556
O3 O2 Nb 24.64(17) 6_456 1_556
Ga3 O2 Nb 93.5(2) . 1_556
La1 O2 Nb 82.84(19) 2 1_556
O3 O2 Nb 158.7(4) 2_655 1_556
Ga2 O2 Nb 151.8(3) 2 1_556
O2 O2 Nb 85.3(4) 5_666 1_556
O2 O2 Nb 70.8(4) 5_656 1_556
O3 O2 Nb 86.6(3) 6_455 1_556
O2 O2 Nb 45.1(2) 6_556 1_556
Ga2 O2 Ga1 100.8(5) 2_556 1_556
Ga3 O2 Ga1 23.7(3) 4_665 1_556
La1 O2 Ga1 142.7(4) 4_665 1_556
O3 O2 Ga1 60.0(3) 3_545 1_556
O2 O2 Ga1 132.87(16) 4_665 1_556
O2 O2 Ga1 106.7(4) 3_655 1_556
La1 O2 Ga1 104.7(3) . 1_556
O2 O2 Ga1 49.4(3) 2_556 1_556
O3 O2 Ga1 60.1(3) 4_665 1_556
O1 O2 Ga1 156.5(4) 2_655 1_556
O3 O2 Ga1 12.3(2) 5_666 1_556
O1 O2 Ga1 71.3(4) 2_656 1_556
O3 O2 Ga1 104.2(4) 5_665 1_556
O1 O2 Ga1 97.0(3) 1_565 1_556
Ga1 O2 Ga1 73.3(2) . 1_556
Nb O2 Ga1 73.3(2) . 1_556
O2 O2 Ga1 120.0(3) 2 1_556
Ga2 O2 Ga1 76.0(2) . 1_556
O3 O2 Ga1 125.2(4) 1_565 1_556
La1 O2 Ga1 63.5(2) 4_666 1_556
Ga3 O2 Ga1 40.95(13) 2_546 1_556
O3 O2 Ga1 97.6(4) 2_656 1_556
Ga3 O2 Ga1 119.7(3) 2_656 1_556
La1 O2 Ga1 45.09(14) 1_556 1_556
La1 O2 Ga1 145.5(3) 2_655 1_556
Ga3 O2 Ga1 117.4(3) 4_664 1_556
O3 O2 Ga1 24.64(17) 6_456 1_556
Ga3 O2 Ga1 93.5(2) . 1_556
La1 O2 Ga1 82.84(19) 2 1_556
O3 O2 Ga1 158.7(4) 2_655 1_556
Ga2 O2 Ga1 151.8(3) 2 1_556
O2 O2 Ga1 85.3(4) 5_666 1_556
O2 O2 Ga1 70.8(4) 5_656 1_556
O3 O2 Ga1 86.6(3) 6_455 1_556
O2 O2 Ga1 45.1(2) 6_556 1_556
Nb O2 Ga1 0.0 1_556 1_556
Ga2 O2 O1 81.9(4) 2_556 .
Ga3 O2 O1 95.1(5) 4_665 .
La1 O2 O1 128.2(5) 4_665 .
O3 O2 O1 39.4(3) 3_545 .
O2 O2 O1 106.4(4) 4_665 .
O2 O2 O1 47.3(4) 3_655 .
La1 O2 O1 25.8(3) . .
O2 O2 O1 131.4(4) 2_556 .
O3 O2 O1 95.5(4) 4_665 .
O1 O2 O1 75.4(3) 2_655 .
O3 O2 O1 72.8(4) 5_666 .
O1 O2 O1 90.4(4) 2_656 .
O3 O2 O1 61.4(3) 5_665 .
O1 O2 O1 148.5(5) 1_565 .
Ga1 O2 O1 66.7(2) . .
Nb O2 O1 66.7(2) . .
O2 O2 O1 106.2(4) 2 .
Ga2 O2 O1 155.1(3) . .
O3 O2 O1 150.0(3) 1_565 .
La1 O2 O1 125.5(4) 4_666 .
Ga3 O2 O1 46.20(17) 2_546 .
O3 O2 O1 135.1(4) 2_656 .
Ga3 O2 O1 122.5(2) 2_656 .
La1 O2 O1 64.3(3) 1_556 .
La1 O2 O1 79.8(2) 2_655 .
Ga3 O2 O1 82.2(3) 4_664 .
O3 O2 O1 96.4(3) 6_456 .
Ga3 O2 O1 45.25(16) . .
La1 O2 O1 115.4(3) 2 .
O3 O2 O1 119.1(4) 2_655 .
Ga2 O2 O1 77.2(3) 2 .
O2 O2 O1 164.2(5) 5_666 .
O2 O2 O1 38.1(3) 5_656 .
O3 O2 O1 86.6(3) 6_455 .
O2 O2 O1 37.5(3) 6_556 .
Nb O2 O1 82.0(3) 1_556 .
Ga1 O2 O1 82.0(3) 1_556 .
Ga2 O2 O3 140.4(6) 2_556 1_455
Ga3 O2 O3 41.1(4) 4_665 1_455
La1 O2 O3 114.2(4) 4_665 1_455
O3 O2 O3 28.7(3) 3_545 1_455
O2 O2 O3 173.4(5) 4_665 1_455
O2 O2 O3 115.0(6) 3_655 1_455
La1 O2 O3 74.7(3) . 1_455
O2 O2 O3 79.4(2) 2_556 1_455
O3 O2 O3 28.3(3) 4_665 1_455
O1 O2 O3 112.6(5) 2_655 1_455
O3 O2 O3 56.2(4) 5_666 1_455
O1 O2 O3 120.1(4) 2_656 1_455
O3 O2 O3 53.7(4) 5_665 1_455
O1 O2 O3 86.6(3) 1_565 1_455
Ga1 O2 O3 21.92(19) . 1_455
Nb O2 O3 21.92(19) . 1_455
O2 O2 O3 76.3(2) 2 1_455
Ga2 O2 O3 88.9(2) . 1_455
O3 O2 O3 136.9(4) 1_565 1_455
La1 O2 O3 110.8(3) 4_666 1_455
Ga3 O2 O3 32.20(19) 2_546 1_455
O3 O2 O3 142.7(3) 2_656 1_455
Ga3 O2 O3 167.1(4) 2_656 1_455
La1 O2 O3 85.0(3) 1_556 1_455
La1 O2 O3 141.3(4) 2_655 1_455
Ga3 O2 O3 66.5(2) 4_664 1_455
O3 O2 O3 41.8(3) 6_456 1_455
Ga3 O2 O3 109.4(3) . 1_455
La1 O2 O3 53.9(2) 2 1_455
O3 O2 O3 130.4(3) 2_655 1_455
Ga2 O2 O3 102.6(3) 2 1_455
O2 O2 O3 110.5(4) 5_666 1_455
O2 O2 O3 89.8(4) 5_656 1_455
O3 O2 O3 39.2(3) 6_455 1_455
O2 O2 O3 55.0(2) 6_556 1_455
Nb O2 O3 51.4(2) 1_556 1_455
Ga1 O2 O3 51.4(2) 1_556 1_455
O1 O2 O3 68.1(2) . 1_455
Ga2 O2 Ga2 72.6(4) 2_556 1_545
Ga3 O2 Ga2 84.2(4) 4_665 1_545
La1 O2 Ga2 148.4(5) 4_665 1_545
O3 O2 Ga2 44.4(3) 3_545 1_545
O2 O2 Ga2 106.2(4) 4_665 1_545
O2 O2 Ga2 48.0(4) 3_655 1_545
La1 O2 Ga2 47.01(19) . 1_545
O2 O2 Ga2 113.8(5) 2_556 1_545
O3 O2 Ga2 98.2(4) 4_665 1_545
O1 O2 Ga2 93.5(3) 2_655 1_545
O3 O2 Ga2 55.0(3) 5_666 1_545
O1 O2 Ga2 72.1(2) 2_656 1_545
O3 O2 Ga2 80.5(3) 5_665 1_545
O1 O2 Ga2 156.4(3) 1_565 1_545
Ga1 O2 Ga2 77.0(2) . 1_545
Nb O2 Ga2 77.0(2) . 1_545
O2 O2 Ga2 125.9(4) 2 1_545
Ga2 O2 Ga2 141.8(4) . 1_545
O3 O2 Ga2 152.9(3) 1_565 1_545
La1 O2 Ga2 104.3(3) 4_666 1_545
Ga3 O2 Ga2 40.07(12) 2_546 1_545
O3 O2 Ga2 120.2(4) 2_656 1_545
Ga3 O2 Ga2 116.7(2) 2_656 1_545
La1 O2 Ga2 42.92(13) 1_556 1_545
La1 O2 Ga2 87.9(2) 2_655 1_545
Ga3 O2 Ga2 102.2(3) 4_664 1_545
O3 O2 Ga2 85.5(3) 6_456 1_545
Ga3 O2 Ga2 39.46(10) . 1_545
La1 O2 Ga2 123.6(3) 2 1_545
O3 O2 Ga2 135.2(3) 2_655 1_545
Ga2 O2 Ga2 97.3(3) 2 1_545
O2 O2 Ga2 142.8(5) 5_666 1_545
O2 O2 Ga2 21.67(16) 5_656 1_545
O3 O2 Ga2 99.4(3) 6_455 1_545
O2 O2 Ga2 21.61(15) 6_556 1_545
Nb O2 Ga2 65.93(18) 1_556 1_545
Ga1 O2 Ga2 65.93(18) 1_556 1_545
O1 O2 Ga2 21.4(2) . 1_545
O3 O2 Ga2 70.1(2) 1_455 1_545
Ga2 O2 Ga3 138.6(6) 2_556 1_455
Ga3 O2 Ga3 21.0(3) 4_665 1_455
La1 O2 Ga3 114.3(3) 4_665 1_455
O3 O2 Ga3 47.2(3) 3_545 1_455
O2 O2 Ga3 165.2(5) 4_665 1_455
O2 O2 Ga3 129.1(6) 3_655 1_455
La1 O2 Ga3 95.6(3) . 1_455
O2 O2 Ga3 58.07(19) 2_556 1_455
O3 O2 Ga3 22.8(3) 4_665 1_455
O1 O2 Ga3 131.6(5) 2_655 1_455
O3 O2 Ga3 47.4(3) 5_666 1_455
O1 O2 Ga3 109.3(4) 2_656 1_455
O3 O2 Ga3 72.5(3) 5_665 1_455
O1 O2 Ga3 75.5(2) 1_565 1_455
Ga1 O2 Ga3 40.06(12) . 1_455
Nb O2 Ga3 40.06(12) . 1_455
O2 O2 Ga3 82.4(2) 2 1_455
Ga2 O2 Ga3 70.29(19) . 1_455
O3 O2 Ga3 123.5(3) 1_565 1_455
La1 O2 Ga3 90.7(3) 4_666 1_455
Ga3 O2 Ga3 41.33(12) 2_546 1_455
O3 O2 Ga3 121.4(4) 2_656 1_455
Ga3 O2 Ga3 145.8(4) 2_656 1_455
La1 O2 Ga3 80.7(2) 1_556 1_455
La1 O2 Ga3 162.6(4) 2_655 1_455
Ga3 O2 Ga3 80.4(2) 4_664 1_455
O3 O2 Ga3 21.39(16) 6_456 1_455
Ga3 O2 Ga3 119.6(3) . 1_455
La1 O2 Ga3 49.00(12) 2 1_455
O3 O2 Ga3 133.7(3) 2_655 1_455
Ga2 O2 Ga3 120.3(3) 2 1_455
O2 O2 Ga3 90.5(3) 5_666 1_455
O2 O2 Ga3 96.8(4) 5_656 1_455
O3 O2 Ga3 48.6(2) 6_455 1_455
O2 O2 Ga3 61.52(15) 6_556 1_455
Nb O2 Ga3 38.21(10) 1_556 1_455
Ga1 O2 Ga3 38.21(10) 1_556 1_455
O1 O2 Ga3 85.2(2) . 1_455
O3 O2 Ga3 21.34(15) 1_455 1_455
Ga2 O2 Ga3 81.2(2) 1_545 1_455
Ga2 O2 Ga3 82.5(5) 2_556 1_565
Ga3 O2 Ga3 97.7(5) 4_665 1_565
La1 O2 Ga3 51.8(3) 4_665 1_565
O3 O2 Ga3 156.9(4) 3_545 1_565
O2 O2 Ga3 57.4(5) 4_665 1_565
O2 O2 Ga3 116.3(5) 3_655 1_565
La1 O2 Ga3 149.0(4) . 1_565
O2 O2 Ga3 58.32(17) 2_556 1_565
O3 O2 Ga3 101.0(4) 4_665 1_565
O1 O2 Ga3 97.3(3) 2_655 1_565
O3 O2 Ga3 112.9(5) 5_666 1_565
O1 O2 Ga3 79.1(3) 2_656 1_565
O3 O2 Ga3 127.7(4) 5_665 1_565
O1 O2 Ga3 46.3(2) 1_565 1_565
Ga1 O2 Ga3 129.0(3) . 1_565
Nb O2 Ga3 129.0(3) . 1_565
O2 O2 Ga3 82.5(2) 2 1_565
Ga2 O2 Ga3 39.88(14) . 1_565
O3 O2 Ga3 19.09(19) 1_565 1_565
La1 O2 Ga3 51.06(17) 4_666 1_565
Ga3 O2 Ga3 146.0(3) 2_546 1_565
O3 O2 Ga3 31.2(2) 2_656 1_565
Ga3 O2 Ga3 40.99(14) 2_656 1_565
La1 O2 Ga3 111.1(3) 1_556 1_565
La1 O2 Ga3 85.8(2) 2_655 1_565
Ga3 O2 Ga3 105.7(3) 4_664 1_565
O3 O2 Ga3 96.5(3) 6_456 1_565
Ga3 O2 Ga3 118.9(3) . 1_565
La1 O2 Ga3 80.3(2) 2 1_565
O3 O2 Ga3 54.4(2) 2_655 1_565
Ga2 O2 Ga3 99.0(2) 2 1_565
O2 O2 Ga3 21.53(19) 5_666 1_565
O2 O2 Ga3 130.3(5) 5_656 1_565
O3 O2 Ga3 107.9(3) 6_455 1_565
O2 O2 Ga3 145.6(5) 6_556 1_565
Nb O2 Ga3 106.2(3) 1_556 1_565
Ga1 O2 Ga3 106.2(3) 1_556 1_565
O1 O2 Ga3 163.5(3) . 1_565
O3 O2 Ga3 128.2(3) 1_455 1_565
Ga2 O2 Ga3 151.2(3) 1_545 1_565
Ga3 O2 Ga3 110.1(2) 1_455 1_565
Ga2 O2 O2 115.6(5) 2_556 1_554
Ga3 O2 O2 120.7(5) 4_665 1_554
La1 O2 O2 49.1(4) 4_665 1_554
O3 O2 O2 82.5(4) 3_545 1_554
O2 O2 O2 90.000(1) 4_665 1_554
O2 O2 O2 90.0 3_655 1_554
La1 O2 O2 56.1(3) . 1_554
O2 O2 O2 132.2(5) 2_556 1_554
O3 O2 O2 82.4(4) 4_665 1_554
O1 O2 O2 33.2(3) 2_655 1_554
O3 O2 O2 139.5(4) 5_666 1_554
O1 O2 O2 147.8(3) 2_656 1_554
O3 O2 O2 33.9(3) 5_665 1_554
O1 O2 O2 78.2(4) 1_565 1_554
Ga1 O2 O2 63.6(2) . 1_554
Nb O2 O2 63.6(2) . 1_554
O2 O2 O2 32.5(4) 2 1_554
Ga2 O2 O2 107.2(2) . 1_554
O3 O2 O2 84.5(3) 1_565 1_554
La1 O2 O2 151.9(2) 4_666 1_554
Ga3 O2 O2 102.9(2) 2_546 1_554
O3 O2 O2 121.9(3) 2_656 1_554
Ga3 O2 O2 102.8(2) 2_656 1_554
La1 O2 O2 145.4(2) 1_556 1_554
La1 O2 O2 68.2(2) 2_655 1_554
Ga3 O2 O2 20.68(16) 4_664 1_554
O3 O2 O2 120.6(3) 6_456 1_554
Ga3 O2 O2 102.1(2) . 1_554
La1 O2 O2 69.28(19) 2 1_554
O3 O2 O2 51.6(3) 2_655 1_554
Ga2 O2 O2 20.78(15) 2 1_554
O2 O2 O2 114.4(4) 5_666 1_554
O2 O2 O2 114.4(4) 5_656 1_554
O3 O2 O2 53.0(3) 6_455 1_554
O2 O2 O2 113.4(4) 6_556 1_554
Nb O2 O2 136.92(17) 1_556 1_554
Ga1 O2 O2 136.92(17) 1_556 1_554
O1 O2 O2 81.3(3) . 1_554
O3 O2 O2 85.6(2) 1_455 1_554
Ga2 O2 O2 102.75(19) 1_545 1_554
Ga3 O2 O2 100.91(18) 1_455 1_554
Ga3 O2 O2 100.83(18) 1_565 1_554
Ga2 O2 O2 64.4(5) 2_556 1_556
Ga3 O2 O2 59.3(5) 4_665 1_556
La1 O2 O2 130.9(4) 4_665 1_556
O3 O2 O2 97.5(4) 3_545 1_556
O2 O2 O2 90.000(1) 4_665 1_556
O2 O2 O2 90.0 3_655 1_556
La1 O2 O2 123.9(3) . 1_556
O2 O2 O2 47.8(5) 2_556 1_556
O3 O2 O2 97.6(4) 4_665 1_556
O1 O2 O2 146.8(3) 2_655 1_556
O3 O2 O2 40.5(4) 5_666 1_556
O1 O2 O2 32.2(3) 2_656 1_556
O3 O2 O2 146.1(3) 5_665 1_556
O1 O2 O2 101.8(4) 1_565 1_556
Ga1 O2 O2 116.4(2) . 1_556
Nb O2 O2 116.4(2) . 1_556
O2 O2 O2 147.5(4) 2 1_556
Ga2 O2 O2 72.8(2) . 1_556
O3 O2 O2 95.5(3) 1_565 1_556
La1 O2 O2 28.1(2) 4_666 1_556
Ga3 O2 O2 77.1(2) 2_546 1_556
O3 O2 O2 58.1(3) 2_656 1_556
Ga3 O2 O2 77.3(2) 2_656 1_556
La1 O2 O2 34.6(2) 1_556 1_556
La1 O2 O2 111.8(2) 2_655 1_556
Ga3 O2 O2 159.32(16) 4_664 1_556
O3 O2 O2 59.4(3) 6_456 1_556
Ga3 O2 O2 77.9(2) . 1_556
La1 O2 O2 110.72(19) 2 1_556
O3 O2 O2 128.4(3) 2_655 1_556
Ga2 O2 O2 159.22(15) 2 1_556
O2 O2 O2 65.6(4) 5_666 1_556
O2 O2 O2 65.6(4) 5_656 1_556
O3 O2 O2 127.0(3) 6_455 1_556
O2 O2 O2 66.6(4) 6_556 1_556
Nb O2 O2 43.08(17) 1_556 1_556
Ga1 O2 O2 43.08(17) 1_556 1_556
O1 O2 O2 98.7(3) . 1_556
O3 O2 O2 94.4(2) 1_455 1_556
Ga2 O2 O2 77.25(19) 1_545 1_556
Ga3 O2 O2 79.09(18) 1_455 1_556
Ga3 O2 O2 79.17(18) 1_565 1_556
O2 O2 O2 179.999(3) 1_554 1_556
Ga2 O2 O2 116.3(6) 2_556 5_665
Ga3 O2 O2 107.1(4) 4_665 5_665
La1 O2 O2 13.56(15) 4_665 5_665
O3 O2 O2 120.7(6) 3_545 5_665
O2 O2 O2 77.8(6) 4_665 5_665
O2 O2 O2 123.4(5) 3_655 5_665
La1 O2 O2 107.8(5) . 5_665
O2 O2 O2 87.9(4) 2_556 5_665
O3 O2 O2 79.2(4) 4_665 5_665
O1 O2 O2 65.8(4) 2_655 5_665
O3 O2 O2 142.2(4) 5_666 5_665
O1 O2 O2 128.8(4) 2_656 5_665
O3 O2 O2 76.3(4) 5_665 5_665
O1 O2 O2 33.4(3) 1_565 5_665
Ga1 O2 O2 88.6(4) . 5_665
Nb O2 O2 88.6(4) . 5_665
O2 O2 O2 32.0(3) 2 5_665
Ga2 O2 O2 59.37(9) . 5_665
O3 O2 O2 41.1(2) 1_565 5_665
La1 O2 O2 101.0(3) 4_666 5_665
Ga3 O2 O2 134.9(4) 2_546 5_665
O3 O2 O2 80.4(3) 2_656 5_665
Ga3 O2 O2 75.3(3) 2_656 5_665
La1 O2 O2 162.4(4) 1_556 5_665
La1 O2 O2 83.1(4) 2_655 5_665
Ga3 O2 O2 54.1(3) 4_664 5_665
O3 O2 O2 106.0(3) 6_456 5_665
Ga3 O2 O2 136.4(4) . 5_665
La1 O2 O2 52.18(18) 2 5_665
O3 O2 O2 33.1(3) 2_655 5_665
Ga2 O2 O2 59.5(3) 2 5_665
O2 O2 O2 62.54(10) 5_666 5_665
O2 O2 O2 159.3(6) 5_656 5_665
O3 O2 O2 65.9(3) 6_455 5_665
O2 O2 O2 156.9(5) 6_556 5_665
Nb O2 O2 129.9(3) 1_556 5_665
Ga1 O2 O2 129.9(3) 1_556 5_665
O1 O2 O2 133.2(5) . 5_665
O3 O2 O2 103.1(4) 1_455 5_665
Ga2 O2 O2 154.6(5) 1_545 5_665
Ga3 O2 O2 101.1(3) 1_455 5_665
Ga3 O2 O2 51.64(14) 1_565 5_665
O2 O2 O2 51.9(3) 1_554 5_665
O2 O2 O2 128.1(3) 1_556 5_665
Ga2 O2 O2 83.3(4) 2_556 5_655
Ga3 O2 O2 123.2(6) 4_665 5_655
La1 O2 O2 94.5(6) 4_665 5_655
O3 O2 O2 61.2(3) 3_545 5_655
O2 O2 O2 87.9(3) 4_665 5_655
O2 O2 O2 45.7(3) 3_655 5_655
La1 O2 O2 11.51(5) . 5_655
O2 O2 O2 163.6(3) 2_556 5_655
O3 O2 O2 105.2(5) 4_665 5_655
O1 O2 O2 41.5(3) 2_655 5_655
O3 O2 O2 106.9(4) 5_666 5_655
O1 O2 O2 107.2(3) 2_656 5_655
O3 O2 O2 48.2(4) 5_665 5_655
O1 O2 O2 129.9(6) 1_565 5_655
Ga1 O2 O2 72.3(3) . 5_655
Nb O2 O2 72.3(3) . 5_655
O2 O2 O2 82.8(6) 2 5_655
Ga2 O2 O2 158.6(5) . 5_655
O3 O2 O2 119.1(4) 1_565 5_655
La1 O2 O2 147.8(4) 4_666 5_655
Ga3 O2 O2 76.1(2) 2_546 5_655
O3 O2 O2 130.7(4) 2_656 5_655
Ga3 O2 O2 107.4(3) 2_656 5_655
La1 O2 O2 94.21(19) 1_556 5_655
La1 O2 O2 56.0(2) 2_655 5_655
Ga3 O2 O2 61.2(4) 4_664 5_655
O3 O2 O2 124.3(4) 6_456 5_655
Ga3 O2 O2 53.97(12) . 5_655
La1 O2 O2 110.6(4) 2 5_655
O3 O2 O2 85.3(4) 2_655 5_655
Ga2 O2 O2 43.3(3) 2 5_655
O2 O2 O2 159.3(6) 5_666 5_655
O2 O2 O2 62.54(10) 5_656 5_655
O3 O2 O2 82.0(4) 6_455 5_655
O2 O2 O2 71.6(2) 6_556 5_655
Nb O2 O2 115.4(3) 1_556 5_655
Ga1 O2 O2 115.4(3) 1_556 5_655
O1 O2 O2 34.2(2) . 5_655
O3 O2 O2 85.5(3) 1_455 5_655
Ga2 O2 O2 53.99(10) 1_545 5_655
Ga3 O2 O2 106.7(3) 1_455 5_655
Ga3 O2 O2 137.9(4) 1_565 5_655
O2 O2 O2 51.9(3) 1_554 5_655
O2 O2 O2 128.1(3) 1_556 5_655
O2 O2 O2 101.9(5) 5_665 5_655
Ga2 O2 O3 111.3(6) 2_556 2_546
Ga3 O2 O3 30.5(3) 4_665 2_546
La1 O2 O3 143.8(4) 4_665 2_546
O3 O2 O3 37.2(4) 3_545 2_546
O2 O2 O3 149.2(3) 4_665 2_546
O2 O2 O3 101.7(6) 3_655 2_546
La1 O2 O3 84.2(3) . 2_546
O2 O2 O3 68.2(3) 2_556 2_546
O3 O2 O3 51.7(4) 4_665 2_546
O1 O2 O3 134.7(5) 2_655 2_546
O3 O2 O3 24.0(2) 5_666 2_546
O1 O2 O3 87.4(4) 2_656 2_546
O3 O2 O3 82.4(3) 5_665 2_546
O1 O2 O3 103.6(3) 1_565 2_546
Ga1 O2 O3 53.6(2) . 2_546
Nb O2 O3 53.6(2) . 2_546
O2 O2 O3 108.4(2) 2 2_546
Ga2 O2 O3 90.7(3) . 2_546
O3 O2 O3 144.8(3) 1_565 2_546
La1 O2 O3 86.3(3) 4_666 2_546
Ga3 O2 O3 19.45(15) 2_546 2_546
O3 O2 O3 120.3(5) 2_656 2_546
Ga3 O2 O3 141.2(4) 2_656 2_546
La1 O2 O3 53.3(2) 1_556 2_546
La1 O2 O3 142.3(3) 2_655 2_546
Ga3 O2 O3 98.6(3) 4_664 2_546
O3 O2 O3 31.8(2) 6_456 2_546
Ga3 O2 O3 90.7(3) . 2_546
La1 O2 O3 78.5(2) 2 2_546
O3 O2 O3 162.4(5) 2_655 2_546
Ga2 O2 O3 128.9(4) 2 2_546
O2 O2 O3 105.0(5) 5_666 2_546
O2 O2 O3 67.4(4) 5_656 2_546
O3 O2 O3 71.53(17) 6_455 2_546
O2 O2 O3 33.2(2) 6_556 2_546
Nb O2 O3 22.91(16) 1_556 2_546
Ga1 O2 O3 22.91(16) 1_556 2_546
O1 O2 O3 64.8(2) . 2_546
O3 O2 O3 32.7(3) 1_455 2_546
Ga2 O2 O3 54.4(2) 1_545 2_546
Ga3 O2 O3 29.64(17) 1_455 2_546
Ga3 O2 O3 126.5(3) 1_565 2_546
O2 O2 O3 116.0(2) 1_554 2_546
O2 O2 O3 64.0(2) 1_556 2_546
O2 O2 O3 130.7(4) 5_665 2_546
O2 O2 O3 95.5(3) 5_655 2_546
Ga2 O2 O3 18.6(3) 2_556 6_556
Ga3 O2 O3 115.2(6) 4_665 6_556
La1 O2 O3 119.5(4) 4_665 6_556
O3 O2 O3 98.4(4) 3_545 6_556
O2 O2 O3 55.2(3) 4_665 6_556
O2 O2 O3 27.3(2) 3_655 6_556
La1 O2 O3 76.1(3) . 6_556
O2 O2 O3 110.5(7) 2_556 6_556
O3 O2 O3 148.3(4) 4_665 6_556
O1 O2 O3 84.3(3) 2_655 6_556
O3 O2 O3 80.4(4) 5_666 6_556
O1 O2 O3 35.3(2) 2_656 6_556
O3 O2 O3 120.0(4) 5_665 6_556
O1 O2 O3 146.9(4) 1_565 6_556
Ga1 O2 O3 130.3(3) . 6_556
Nb O2 O3 130.3(3) . 6_556
O2 O2 O3 146.3(5) 2 6_556
Ga2 O2 O3 127.1(4) . 6_556
O3 O2 O3 99.1(4) 1_565 6_556
La1 O2 O3 75.3(3) 4_666 6_556
Ga3 O2 O3 90.7(3) 2_546 6_556
O3 O2 O3 70.8(3) 2_656 6_556
Ga3 O2 O3 62.67(19) 2_656 6_556
La1 O2 O3 46.6(2) 1_556 6_556
La1 O2 O3 54.0(2) 2_655 6_556
Ga3 O2 O3 132.2(3) 4_664 6_556
O3 O2 O3 116.0(4) 6_456 6_556
Ga3 O2 O3 20.00(13) . 6_556
La1 O2 O3 174.5(4) 2 6_556
O3 O2 O3 100.2(2) 2_655 6_556
Ga2 O2 O3 96.1(3) 2 6_556
O2 O2 O3 106.9(5) 5_666 6_556
O2 O2 O3 33.1(3) 5_656 6_556
O3 O2 O3 150.8(4) 6_455 6_556
O2 O2 O3 68.0(2) 6_556 6_556
Nb O2 O3 91.7(3) 1_556 6_556
Ga1 O2 O3 91.7(3) 1_556 6_556
O1 O2 O3 64.4(2) . 6_556
O3 O2 O3 122.8(3) 1_455 6_556
Ga2 O2 O3 54.02(18) 1_545 6_556
Ga3 O2 O3 126.1(3) 1_455 6_556
Ga3 O2 O3 100.6(3) 1_565 6_556
O2 O2 O3 115.7(2) 1_554 6_556
O2 O2 O3 64.3(2) 1_556 6_556
O2 O2 O3 132.4(4) 5_665 6_556
O2 O2 O3 72.5(2) 5_655 6_556
O3 O2 O3 96.7(4) 2_546 6_556
Ga2 O2 Ga2 133.4(5) 2_556 1_554
Ga3 O2 Ga2 98.4(4) 4_665 1_554
La1 O2 Ga2 29.25(19) 4_665 1_554
O3 O2 Ga2 100.9(4) 3_545 1_554
O2 O2 Ga2 94.9(4) 4_665 1_554
O2 O2 Ga2 127.47(18) 3_655 1_554
La1 O2 Ga2 95.8(4) . 1_554
O2 O2 Ga2 92.1(5) 2_556 1_554
O3 O2 Ga2 64.3(3) 4_665 1_554
O1 O2 Ga2 65.8(3) 2_655 1_554
O3 O2 Ga2 133.5(4) 5_666 1_554
O1 O2 Ga2 148.2(4) 2_656 1_554
O3 O2 Ga2 58.3(3) 5_665 1_554
O1 O2 Ga2 37.0(3) 1_565 1_554
Ga1 O2 Ga2 69.0(2) . 1_554
Nb O2 Ga2 69.0(2) . 1_554
O2 O2 Ga2 12.90(17) 2 1_554
Ga2 O2 Ga2 65.96(19) . 1_554
O3 O2 Ga2 60.8(3) 1_565 1_554
La1 O2 Ga2 115.3(3) 4_666 1_554
Ga3 O2 Ga2 115.9(3) 2_546 1_554
O3 O2 Ga2 99.6(3) 2_656 1_554
Ga3 O2 Ga2 94.7(2) 2_656 1_554
La1 O2 Ga2 167.2(3) 1_556 1_554
La1 O2 Ga2 92.4(3) 2_655 1_554
Ga3 O2 Ga2 36.69(11) 4_664 1_554
O3 O2 Ga2 97.6(2) 6_456 1_554
Ga3 O2 Ga2 140.9(3) . 1_554
La1 O2 Ga2 39.28(11) 2 1_554
O3 O2 Ga2 47.1(2) 2_655 1_554
Ga2 O2 Ga2 55.84(16) 2 1_554
O2 O2 Ga2 76.1(3) 5_666 1_554
O2 O2 Ga2 155.3(5) 5_656 1_554
O3 O2 Ga2 46.6(2) 6_455 1_554
O2 O2 Ga2 137.2(4) 6_556 1_554
Nb O2 Ga2 122.1(2) 1_556 1_554
Ga1 O2 Ga2 122.1(2) 1_556 1_554
O1 O2 Ga2 118.7(4) . 1_554
O3 O2 Ga2 85.0(2) 1_455 1_554
Ga2 O2 Ga2 138.8(3) 1_545 1_554
Ga3 O2 Ga2 87.04(18) 1_455 1_554
Ga3 O2 Ga2 69.55(17) 1_565 1_554
O2 O2 Ga2 41.20(16) 1_554 1_554
O2 O2 Ga2 138.80(16) 1_556 1_554
O2 O2 Ga2 19.75(17) 5_665 1_554
O2 O2 Ga2 93.0(4) 5_655 1_554
O3 O2 Ga2 115.4(3) 2_546 1_554
O3 O2 Ga2 146.1(3) 6_556 1_554
Ga2 O2 O2 109.9(5) 2_556 6
Ga3 O2 O2 94.7(5) 4_665 6
La1 O2 O2 102.2(5) 4_665 6
O3 O2 O2 34.4(3) 3_545 6
O2 O2 O2 118.4(3) 4_665 6
O2 O2 O2 71.4(4) 3_655 6
La1 O2 O2 21.3(2) . 6
O2 O2 O2 134.33(7) 2_556 6
O3 O2 O2 75.0(4) 4_665 6
O1 O2 O2 63.2(3) 2_655 6
O3 O2 O2 90.3(5) 5_666 6
O1 O2 O2 123.7(4) 2_656 6
O3 O2 O2 28.1(2) 5_665 6
O1 O2 O2 116.3(4) 1_565 6
Ga1 O2 O2 42.1(2) . 6
Nb O2 O2 42.1(2) . 6
O2 O2 O2 73.2(4) 2 6
Ga2 O2 O2 136.7(2) . 6
O3 O2 O2 137.3(5) 1_565 6
La1 O2 O2 154.8(5) 4_666 6
Ga3 O2 O2 53.5(2) 2_546 6
O3 O2 O2 161.5(2) 2_656 6
Ga3 O2 O2 138.0(3) 2_656 6
La1 O2 O2 94.8(3) 1_556 6
La1 O2 O2 86.3(2) 2_655 6
Ga3 O2 O2 49.3(2) 4_664 6
O3 O2 O2 95.6(3) 6_456 6
Ga3 O2 O2 74.8(2) . 6
La1 O2 O2 86.5(2) 2 6
O3 O2 O2 102.2(4) 2_655 6
Ga2 O2 O2 58.2(3) 2 6
O2 O2 O2 158.3(4) 5_666 6
O2 O2 O2 71.4(3) 5_656 6
O3 O2 O2 56.4(2) 6_455 6
O2 O2 O2 60.1(3) 6_556 6
Nb O2 O2 94.2(3) 1_556 6
Ga1 O2 O2 94.2(3) 1_556 6
O1 O2 O2 33.3(3) . 6
O3 O2 O2 55.0(2) 1_455 6
Ga2 O2 O2 52.9(2) 1_545 6
Ga3 O2 O2 76.27(19) 1_455 6
Ga3 O2 O2 153.9(5) 1_565 6
O2 O2 O2 53.2(3) 1_554 6
O2 O2 O2 126.8(3) 1_556 6
O2 O2 O2 102.7(5) 5_665 6
O2 O2 O2 30.9(3) 5_655 6
O3 O2 O2 71.6(3) 2_546 6
O3 O2 O2 94.7(2) 6_556 6
Ga2 O2 O2 86.0(3) 1_554 6
Ga2 O2 O2 119.2(7) 2_556 6_566
Ga3 O2 O2 48.1(2) 4_665 6_566
La1 O2 O2 78.8(4) 4_665 6_566
O3 O2 O2 105.6(3) 3_545 6_566
O2 O2 O2 108.4(7) 4_665 6_566
O2 O2 O2 156.8(4) 3_655 6_566
La1 O2 O2 150.3(4) . 6_566
O2 O2 O2 21.5(3) 2_556 6_566
O3 O2 O2 54.1(2) 4_665 6_566
O1 O2 O2 133.6(5) 2_655 6_566
O3 O2 O2 76.4(4) 5_666 6_566
O1 O2 O2 94.4(5) 2_656 6_566
O3 O2 O2 109.1(3) 5_665 6_566
O1 O2 O2 34.9(3) 1_565 6_566
Ga1 O2 O2 86.94(16) . 6_566
Nb O2 O2 86.94(16) . 6_566
O2 O2 O2 78.5(3) 2 6_566
Ga2 O2 O2 12.24(14) . 6_566
O3 O2 O2 67.1(3) 1_565 6_566
La1 O2 O2 54.4(3) 4_666 6_566
Ga3 O2 O2 96.7(3) 2_546 6_566
O3 O2 O2 69.2(4) 2_656 6_566
Ga3 O2 O2 89.9(4) 2_656 6_566
La1 O2 O2 99.4(4) 1_556 6_566
La1 O2 O2 137.3(4) 2_655 6_566
Ga3 O2 O2 97.7(3) 4_664 6_566
O3 O2 O2 46.8(2) 6_456 6_566
Ga3 O2 O2 146.7(5) . 6_566
La1 O2 O2 46.95(12) 2 6_566
O3 O2 O2 93.9(4) 2_655 6_566
Ga2 O2 O2 125.9(4) 2 6_566
O2 O2 O2 32.8(3) 5_666 6_566
O2 O2 O2 131.7(7) 5_656 6_566
O3 O2 O2 75.4(2) 6_455 6_566
O2 O2 O2 109.5(4) 6_556 6_566
Nb O2 O2 65.0(3) 1_556 6_566
Ga1 O2 O2 65.0(3) 1_556 6_566
O1 O2 O2 142.8(4) . 6_566
O3 O2 O2 77.8(2) 1_455 6_566
Ga2 O2 O2 130.9(4) 1_545 6_566
Ga3 O2 O2 58.46(13) 1_455 6_566
Ga3 O2 O2 51.7(3) 1_565 6_566
O2 O2 O2 110.9(3) 1_554 6_566
O2 O2 O2 69.1(3) 1_556 6_566
O2 O2 O2 67.76(15) 5_665 6_566
O2 O2 O2 157.4(5) 5_655 6_566
O3 O2 O2 78.6(3) 2_546 6_566
O3 O2 O2 129.6(5) 6_556 6_566
Ga2 O2 O2 70.6(3) 1_554 6_566
O2 O2 O2 129.0(3) 6 6_566
Ga2 O2 O2 25.44(19) 2_556 6_666
Ga3 O2 O2 126.4(8) 4_665 6_666
La1 O2 O2 83.1(4) 4_665 6_666
O3 O2 O2 142.4(5) 3_545 6_666
O2 O2 O2 21.1(3) 4_665 6_666
O2 O2 O2 59.7(2) 3_655 6_666
La1 O2 O2 107.8(3) . 6_666
O2 O2 O2 93.8(5) 2_556 6_666
O3 O2 O2 156.0(6) 4_665 6_666
O1 O2 O2 81.0(3) 2_655 6_666
O3 O2 O2 105.9(6) 5_666 6_666
O1 O2 O2 41.9(3) 2_656 6_666
O3 O2 O2 139.9(5) 5_665 6_666
O1 O2 O2 103.6(4) 1_565 6_666
Ga1 O2 O2 171.0(5) . 6_666
Nb O2 O2 171.0(5) . 6_666
O2 O2 O2 121.6(3) 2 6_666
Ga2 O2 O2 93.0(4) . 6_666
O3 O2 O2 55.3(4) 1_565 6_666
La1 O2 O2 57.6(3) 4_666 6_666
Ga3 O2 O2 131.8(4) 2_546 6_666
O3 O2 O2 32.7(3) 2_656 6_666
Ga3 O2 O2 18.73(17) 2_656 6_666
La1 O2 O2 77.2(3) 1_556 6_666
La1 O2 O2 47.59(12) 2_655 6_666
Ga3 O2 O2 130.8(4) 4_664 6_666
O3 O2 O2 126.1(5) 6_456 6_666
Ga3 O2 O2 61.14(13) . 6_666
La1 O2 O2 137.8(4) 2 6_666
O3 O2 O2 67.6(3) 2_655 6_666
Ga2 O2 O2 92.3(3) 2 6_666
O2 O2 O2 70.3(5) 5_666 6_666
O2 O2 O2 76.8(3) 5_656 6_666
O3 O2 O2 158.6(5) 6_455 6_666
O2 O2 O2 109.5(4) 6_556 6_666
Nb O2 O2 111.8(4) 1_556 6_666
Ga1 O2 O2 111.8(4) 1_556 6_666
O1 O2 O2 106.0(2) . 6_666
O3 O2 O2 161.9(5) 1_455 6_666
Ga2 O2 O2 98.1(3) 1_545 6_666
Ga3 O2 O2 147.4(5) 1_455 6_666
Ga3 O2 O2 57.8(3) 1_565 6_666
O2 O2 O2 110.9(3) 1_554 6_666
O2 O2 O2 69.1(3) 1_556 6_666
O2 O2 O2 93.2(4) 5_665 6_666
O2 O2 O2 98.7(2) 5_655 6_666
O3 O2 O2 129.3(5) 2_546 6_666
O3 O2 O2 44.05(18) 6_556 6_666
Ga2 O2 O2 112.2(4) 1_554 6_666
O2 O2 O2 129.0(3) 6 6_666
O2 O2 O2 101.9(5) 6_566 6_666
Ga2 O2 O3 32.2(4) 2_556 4_765
Ga3 O2 O3 143.8(5) 4_665 4_765
La1 O2 O3 95.2(3) 4_665 4_765
O3 O2 O3 102.5(3) 3_545 4_765
O2 O2 O3 43.3(4) 4_665 4_765
O2 O2 O3 17.3(4) 3_655 4_765
La1 O2 O3 61.0(2) . 4_765
O2 O2 O3 136.4(6) 2_556 4_765
O3 O2 O3 157.2(5) 4_665 4_765
O1 O2 O3 53.9(3) 2_655 4_765
O3 O2 O3 108.2(3) 5_666 4_765
O1 O2 O3 62.7(3) 2_656 4_765
O3 O2 O3 99.5(3) 5_665 4_765
O1 O2 O3 137.8(3) 1_565 4_765
Ga1 O2 O3 124.4(3) . 4_765
Nb O2 O3 124.4(3) . 4_765
O2 O2 O3 115.8(5) 2 4_765
Ga2 O2 O3 139.2(4) . 4_765
O3 O2 O3 89.7(2) 1_565 4_765
La1 O2 O3 98.3(3) 4_666 4_765
Ga3 O2 O3 105.1(3) 2_546 4_765
O3 O2 O3 79.5(3) 2_656 4_765
Ga3 O2 O3 60.05(19) 2_656 4_765
La1 O2 O3 75.6(2) 1_556 4_765
La1 O2 O3 25.64(16) 2_655 4_765
Ga3 O2 O3 104.7(3) 4_664 4_765
O3 O2 O3 144.9(3) 6_456 4_765
Ga3 O2 O3 27.95(15) . 4_765
La1 O2 O3 154.9(4) 2 4_765
O3 O2 O3 75.8(3) 2_655 4_765
Ga2 O2 O3 65.9(2) 2 4_765
O2 O2 O3 116.6(4) 5_666 4_765
O2 O2 O3 51.4(3) 5_656 4_765
O3 O2 O3 133.2(4) 6_455 4_765
O2 O2 O3 85.43(19) 6_556 4_765
Nb O2 O3 120.2(3) 1_556 4_765
Ga1 O2 O3 120.2(3) 1_556 4_765
O1 O2 O3 63.19(17) . 4_765
O3 O2 O3 131.2(3) 1_455 4_765
Ga2 O2 O3 65.19(18) 1_545 4_765
Ga3 O2 O3 146.4(3) 1_455 4_765
Ga3 O2 O3 100.5(2) 1_565 4_765
O2 O2 O3 86.1(2) 1_554 4_765
O2 O2 O3 93.9(2) 1_556 4_765
O2 O2 O3 108.7(4) 5_665 4_765
O2 O2 O3 52.7(2) 5_655 4_765
O3 O2 O3 118.4(3) 2_546 4_765
O3 O2 O3 30.5(3) 6_556 4_765
Ga2 O2 O3 117.1(3) 1_554 4_765
O2 O2 O3 82.28(19) 6 4_765
O2 O2 O3 148.7(4) 6_566 4_765
O2 O2 O3 46.81(16) 6_666 4_765
Ga2 O2 Nb 76.5(4) 2_556 1_665
Ga3 O2 Nb 130.7(5) 4_665 1_665
La1 O2 Nb 30.2(2) 4_665 1_665
O3 O2 Nb 155.0(5) 3_545 1_665
O2 O2 Nb 38.7(4) 4_665 1_665
O2 O2 Nb 94.8(4) 3_655 1_665
La1 O2 Nb 113.5(4) . 1_665
O2 O2 Nb 93.4(2) 2_556 1_665
O3 O2 Nb 117.0(4) 4_665 1_665
O1 O2 Nb 61.9(2) 2_655 1_665
O3 O2 Nb 146.5(5) 5_666 1_665
O1 O2 Nb 92.3(3) 2_656 1_665
O3 O2 Nb 105.7(4) 5_665 1_665
O1 O2 Nb 60.37(19) 1_565 1_665
Ga1 O2 Nb 127.4(3) . 1_665
Nb O2 Nb 127.4(3) . 1_665
O2 O2 Nb 69.18(15) 2 1_665
Ga2 O2 Nb 70.5(2) . 1_665
O3 O2 Nb 16.58(19) 1_565 1_665
La1 O2 Nb 81.2(2) 4_666 1_665
Ga3 O2 Nb 174.7(3) 2_546 1_665
O3 O2 Nb 49.4(2) 2_656 1_665
Ga3 O2 Nb 36.17(11) 2_656 1_665
La1 O2 Nb 129.4(3) 1_556 1_665
La1 O2 Nb 55.69(15) 2_655 1_665
Ga3 O2 Nb 85.7(2) 4_664 1_665
O3 O2 Nb 129.4(3) 6_456 1_665
Ga3 O2 Nb 104.2(2) . 1_665
La1 O2 Nb 90.0(2) 2 1_665
O3 O2 Nb 21.14(16) 2_655 1_665
Ga2 O2 Nb 64.99(17) 2 1_665
O2 O2 Nb 56.7(3) 5_666 1_665
O2 O2 Nb 126.1(4) 5_656 1_665
O3 O2 Nb 105.5(3) 6_455 1_665
O2 O2 Nb 161.74(19) 6_556 1_665
Nb O2 Nb 141.6(3) 1_556 1_665
Ga1 O2 Nb 141.6(3) 1_556 1_665
O1 O2 Nb 134.0(3) . 1_665
O3 O2 Nb 143.0(3) 1_455 1_665
Ga2 O2 Nb 142.8(2) 1_545 1_665
Ga3 O2 Nb 135.9(2) 1_455 1_665
Ga3 O2 Nb 35.48(9) 1_565 1_665
O2 O2 Nb 72.57(17) 1_554 1_665
O2 O2 Nb 107.44(17) 1_556 1_665
O2 O2 Nb 40.01(19) 5_665 1_665
O2 O2 Nb 102.6(4) 5_655 1_665
O3 O2 Nb 161.1(3) 2_546 1_665
O3 O2 Nb 93.8(2) 6_556 1_665
Ga2 O2 Nb 58.87(14) 1_554 1_665
O2 O2 Nb 123.1(4) 6 1_665
O2 O2 Nb 82.6(3) 6_566 1_665
O2 O2 Nb 53.3(3) 6_666 1_665
O3 O2 Nb 77.6(2) 4_765 1_665
Ga2 O2 Ga1 76.5(4) 2_556 1_665
Ga3 O2 Ga1 130.7(5) 4_665 1_665
La1 O2 Ga1 30.2(2) 4_665 1_665
O3 O2 Ga1 155.0(5) 3_545 1_665
O2 O2 Ga1 38.7(4) 4_665 1_665
O2 O2 Ga1 94.8(4) 3_655 1_665
La1 O2 Ga1 113.5(4) . 1_665
O2 O2 Ga1 93.4(2) 2_556 1_665
O3 O2 Ga1 117.0(4) 4_665 1_665
O1 O2 Ga1 61.9(2) 2_655 1_665
O3 O2 Ga1 146.5(5) 5_666 1_665
O1 O2 Ga1 92.3(3) 2_656 1_665
O3 O2 Ga1 105.7(4) 5_665 1_665
O1 O2 Ga1 60.37(19) 1_565 1_665
Ga1 O2 Ga1 127.4(3) . 1_665
Nb O2 Ga1 127.4(3) . 1_665
O2 O2 Ga1 69.18(15) 2 1_665
Ga2 O2 Ga1 70.5(2) . 1_665
O3 O2 Ga1 16.58(19) 1_565 1_665
La1 O2 Ga1 81.2(2) 4_666 1_665
Ga3 O2 Ga1 174.7(3) 2_546 1_665
O3 O2 Ga1 49.4(2) 2_656 1_665
Ga3 O2 Ga1 36.17(11) 2_656 1_665
La1 O2 Ga1 129.4(3) 1_556 1_665
La1 O2 Ga1 55.69(15) 2_655 1_665
Ga3 O2 Ga1 85.7(2) 4_664 1_665
O3 O2 Ga1 129.4(3) 6_456 1_665
Ga3 O2 Ga1 104.2(2) . 1_665
La1 O2 Ga1 90.0(2) 2 1_665
O3 O2 Ga1 21.14(16) 2_655 1_665
Ga2 O2 Ga1 64.99(17) 2 1_665
O2 O2 Ga1 56.7(3) 5_666 1_665
O2 O2 Ga1 126.1(4) 5_656 1_665
O3 O2 Ga1 105.5(3) 6_455 1_665
O2 O2 Ga1 161.74(19) 6_556 1_665
Nb O2 Ga1 141.6(3) 1_556 1_665
Ga1 O2 Ga1 141.6(3) 1_556 1_665
O1 O2 Ga1 134.0(3) . 1_665
O3 O2 Ga1 143.0(3) 1_455 1_665
Ga2 O2 Ga1 142.8(2) 1_545 1_665
Ga3 O2 Ga1 135.9(2) 1_455 1_665
Ga3 O2 Ga1 35.48(9) 1_565 1_665
O2 O2 Ga1 72.57(17) 1_554 1_665
O2 O2 Ga1 107.44(17) 1_556 1_665
O2 O2 Ga1 40.01(19) 5_665 1_665
O2 O2 Ga1 102.6(4) 5_655 1_665
O3 O2 Ga1 161.1(3) 2_546 1_665
O3 O2 Ga1 93.8(2) 6_556 1_665
Ga2 O2 Ga1 58.87(14) 1_554 1_665
O2 O2 Ga1 123.1(4) 6 1_665
O2 O2 Ga1 82.6(3) 6_566 1_665
O2 O2 Ga1 53.3(3) 6_666 1_665
O3 O2 Ga1 77.6(2) 4_765 1_665
Nb O2 Ga1 0.0 1_665 1_665
Ga2 O2 La1 15.9(3) 2_556 2_656
Ga3 O2 La1 108.2(5) 4_665 2_656
La1 O2 La1 110.0(4) 4_665 2_656
O3 O2 La1 119.0(4) 3_545 2_656
O2 O2 La1 46.32(17) 4_665 2_656
O2 O2 La1 52.11(19) 3_655 2_656
La1 O2 La1 102.5(3) . 2_656
O2 O2 La1 88.6(5) 2_556 2_656
O3 O2 La1 146.8(5) 4_665 2_656
O1 O2 La1 97.7(3) 2_655 2_656
O3 O2 La1 80.6(4) 5_666 2_656
O1 O2 La1 17.4(2) 2_656 2_656
O3 O2 La1 145.9(4) 5_665 2_656
O1 O2 La1 121.5(4) 1_565 2_656
Ga1 O2 La1 151.8(3) . 2_656
Nb O2 La1 151.8(3) . 2_656
O2 O2 La1 148.44(19) 2 2_656
Ga2 O2 La1 100.8(3) . 2_656
O3 O2 La1 79.5(3) 1_565 2_656
La1 O2 La1 50.96(16) 4_666 2_656
Ga3 O2 La1 105.2(3) 2_546 2_656
O3 O2 La1 45.2(2) 2_656 2_656
Ga3 O2 La1 44.18(12) 2_656 2_656
La1 O2 La1 50.28(14) 1_556 2_656
La1 O2 La1 62.57(15) 2_655 2_656
Ga3 O2 La1 151.2(3) 4_664 2_656
O3 O2 La1 108.4(4) 6_456 2_656
Ga3 O2 La1 46.59(12) . 2_656
La1 O2 La1 151.5(3) 2 2_656
O3 O2 La1 94.3(3) 2_655 2_656
Ga2 O2 La1 110.1(2) 2 2_656
O2 O2 La1 80.4(4) 5_666 2_656
O2 O2 La1 54.4(3) 5_656 2_656
O3 O2 La1 174.4(4) 6_455 2_656
O2 O2 La1 83.6(3) 6_556 2_656
Nb O2 La1 88.5(2) 1_556 2_656
Ga1 O2 La1 88.5(2) 1_556 2_656
O1 O2 La1 90.0(2) . 2_656
O3 O2 La1 135.3(3) 1_455 2_656
Ga2 O2 La1 76.03(17) 1_545 2_656
Ga3 O2 La1 126.7(3) 1_455 2_656
Ga3 O2 La1 76.2(2) 1_565 2_656
O2 O2 La1 130.78(15) 1_554 2_656
O2 O2 La1 49.22(15) 1_556 2_656
O2 O2 La1 119.5(4) 5_665 2_656
O2 O2 La1 97.7(3) 5_655 2_656
O3 O2 La1 103.0(3) 2_546 2_656
O3 O2 La1 26.60(14) 6_556 2_656
Ga2 O2 La1 138.9(3) 1_554 2_656
O2 O2 La1 121.3(2) 6 2_656
O2 O2 La1 104.9(4) 6_566 2_656
O2 O2 La1 26.95(18) 6_666 2_656
O3 O2 La1 47.97(17) 4_765 2_656
Nb O2 La1 80.03(18) 1_665 2_656
Ga1 O2 La1 80.03(18) 1_665 2_656
Ga2 O2 O3 138.7(6) 2_556 2_545
Ga3 O2 O3 70.6(4) 4_665 2_545
La1 O2 O3 98.3(4) 4_665 2_545
O3 O2 O3 28.9(4) 3_545 2_545
O2 O2 O3 144.3(3) 4_665 2_545
O2 O2 O3 101.0(5) 3_655 2_545
La1 O2 O3 51.6(2) . 2_545
O2 O2 O3 106.5(3) 2_556 2_545
O3 O2 O3 44.7(4) 4_665 2_545
O1 O2 O3 82.9(4) 2_655 2_545
O3 O2 O3 81.6(3) 5_666 2_545
O1 O2 O3 139.1(4) 2_656 2_545
O3 O2 O3 24.6(2) 5_665 2_545
O1 O2 O3 91.7(3) 1_565 2_545
Ga1 O2 O3 11.76(15) . 2_545
Nb O2 O3 11.76(15) . 2_545
O2 O2 O3 60.2(2) 2 2_545
Ga2 O2 O3 106.9(3) . 2_545
O3 O2 O3 133.0(3) 1_565 2_545
La1 O2 O3 140.5(3) 4_666 2_545
Ga3 O2 O3 47.1(2) 2_546 2_545
O3 O2 O3 167.4(4) 2_656 2_545
Ga3 O2 O3 160.8(4) 2_656 2_545
La1 O2 O3 102.2(3) 1_556 2_545
La1 O2 O3 113.4(3) 2_655 2_545
Ga3 O2 O3 42.15(19) 4_664 2_545
O3 O2 O3 71.18(17) 6_456 2_545
Ga3 O2 O3 102.1(3) . 2_545
La1 O2 O3 58.6(2) 2 2_545
O3 O2 O3 108.4(4) 2_655 2_545
Ga2 O2 O3 73.2(3) 2 2_545
O2 O2 O3 129.4(4) 5_666 2_545
O2 O2 O3 91.6(3) 5_656 2_545
O3 O2 O3 29.9(2) 6_455 2_545
O2 O2 O3 65.4(3) 6_556 2_545
Nb O2 O3 79.5(2) 1_556 2_545
Ga1 O2 O3 79.5(2) 1_556 2_545
O1 O2 O3 57.0(3) . 2_545
O3 O2 O3 29.7(3) 1_455 2_545
Ga2 O2 O3 70.0(2) 1_545 2_545
Ga3 O2 O3 49.98(17) 1_455 2_545
Ga3 O2 O3 137.7(3) 1_565 2_545
O2 O2 O3 58.1(2) 1_554 2_545
O2 O2 O3 121.9(2) 1_556 2_545
O2 O2 O3 92.0(4) 5_665 2_545
O2 O2 O3 60.6(3) 5_655 2_545
O3 O2 O3 57.92(18) 2_546 2_545
O3 O2 O3 121.3(3) 6_556 2_545
Ga2 O2 O3 72.3(2) 1_554 2_545
O2 O2 O3 30.38(19) 6 2_545
O2 O2 O3 98.6(2) 6_566 2_545
O2 O2 O3 159.3(4) 6_666 2_545
O3 O2 O3 112.7(3) 4_765 2_545
Nb O2 O3 127.7(3) 1_665 2_545
Ga1 O2 O3 127.7(3) 1_665 2_545
La1 O2 O3 146.0(3) 2_656 2_545
Ga2 O2 O3 60.5(4) 2_556 6
Ga3 O2 O3 151.7(6) 4_665 6
La1 O2 O3 81.6(4) 4_665 6
O3 O2 O3 90.9(4) 3_545 6
O2 O2 O3 57.3(3) 4_665 6
O2 O2 O3 32.7(2) 3_655 6
La1 O2 O3 41.7(2) . 6
O2 O2 O3 163.5(4) 2_556 6
O3 O2 O3 133.0(5) 4_665 6
O1 O2 O3 29.0(2) 2_655 6
O3 O2 O3 123.4(3) 5_666 6
O1 O2 O3 91.0(3) 2_656 6
O3 O2 O3 72.4(4) 5_665 6
O1 O2 O3 127.0(4) 1_565 6
Ga1 O2 O3 101.4(3) . 6
Nb O2 O3 101.4(3) . 6
O2 O2 O3 90.0(5) 2 6
Ga2 O2 O3 147.8(4) . 6
O3 O2 O3 93.5(3) 1_565 6
La1 O2 O3 125.7(3) 4_666 6
Ga3 O2 O3 102.7(3) 2_546 6
O3 O2 O3 100.5(2) 2_656 6
Ga3 O2 O3 76.8(2) 2_656 6
La1 O2 O3 96.8(2) 1_556 6
La1 O2 O3 25.48(14) 2_655 6
Ga3 O2 O3 76.3(3) 4_664 6
O3 O2 O3 152.9(4) 6_456 6
Ga3 O2 O3 46.09(16) . 6
La1 O2 O3 127.7(4) 2 6
O3 O2 O3 65.7(3) 2_655 6
Ga2 O2 O3 39.50(18) 2 6
O2 O2 O3 131.4(4) 5_666 6
O2 O2 O3 66.0(3) 5_656 6
O3 O2 O3 105.3(4) 6_455 6
O2 O2 O3 90.9(3) 6_556 6
Nb O2 O3 135.2(3) 1_556 6
Ga1 O2 O3 135.2(3) 1_556 6
O1 O2 O3 56.6(2) . 6
O3 O2 O3 116.1(3) 1_455 6
Ga2 O2 O3 69.5(2) 1_545 6
Ga3 O2 O3 137.2(3) 1_455 6
Ga3 O2 O3 110.4(3) 1_565 6
O2 O2 O3 58.5(2) 1_554 6
O2 O2 O3 121.5(2) 1_556 6
O2 O2 O3 93.6(4) 5_665 6
O2 O2 O3 30.6(2) 5_655 6
O3 O2 O3 121.4(3) 2_546 6
O3 O2 O3 57.23(17) 6_556 6
Ga2 O2 O3 94.8(3) 1_554 6
O2 O2 O3 61.3(2) 6 6
O2 O2 O3 159.6(4) 6_566 6
O2 O2 O3 69.72(19) 6_666 6
O3 O2 O3 28.5(3) 4_765 6
Nb O2 O3 77.5(2) 1_665 6
Ga1 O2 O3 77.5(2) 1_665 6
La1 O2 O3 76.32(18) 2_656 6
O3 O2 O3 90.0(3) 2_545 6
Ga2 O2 O3 55.3(4) 2_556 3_655
Ga3 O2 O3 137.1(6) 4_665 3_655
La1 O2 O3 50.8(3) 4_665 3_655
O3 O2 O3 160.8(5) 3_545 3_655
O2 O2 O3 18.6(4) 4_665 3_655
O2 O2 O3 78.2(4) 3_655 3_655
La1 O2 O3 111.1(3) . 3_655
O2 O2 O3 96.6(2) 2_556 3_655
O3 O2 O3 136.9(4) 4_665 3_655
O1 O2 O3 65.0(3) 2_655 3_655
O3 O2 O3 134.3(5) 5_666 3_655
O1 O2 O3 72.8(3) 2_656 3_655
O3 O2 O3 119.7(4) 5_665 3_655
O1 O2 O3 78.7(3) 1_565 3_655
Ga1 O2 O3 147.1(4) . 3_655
Nb O2 O3 147.1(4) . 3_655
O2 O2 O3 89.5(2) 2 3_655
Ga2 O2 O3 81.0(3) . 3_655
O3 O2 O3 28.6(3) 1_565 3_655
La1 O2 O3 72.3(3) 4_666 3_655
Ga3 O2 O3 163.5(3) 2_546 3_655
O3 O2 O3 38.2(3) 2_656 3_655
Ga3 O2 O3 17.06(16) 2_656 3_655
La1 O2 O3 109.3(3) 1_556 3_655
La1 O2 O3 44.78(18) 2_655 3_655
Ga3 O2 O3 102.8(3) 4_664 3_655
O3 O2 O3 136.0(4) 6_456 3_655
Ga3 O2 O3 85.4(2) . 3_655
La1 O2 O3 110.5(3) 2 3_655
O3 O2 O3 36.6(3) 2_655 3_655
Ga2 O2 O3 72.5(2) 2 3_655
O2 O2 O3 61.5(3) 5_666 3_655
O2 O2 O3 105.8(4) 5_656 3_655
O3 O2 O3 126.4(3) 6_455 3_655
O2 O2 O3 140.8(3) 6_556 3_655
Nb O2 O3 135.6(3) 1_556 3_655
Ga1 O2 O3 135.6(3) 1_556 3_655
O1 O2 O3 123.6(3) . 3_655
O3 O2 O3 164.3(3) 1_455 3_655
Ga2 O2 O3 124.8(3) 1_545 3_655
Ga3 O2 O3 151.2(3) 1_455 3_655
Ga3 O2 O3 41.17(18) 1_565 3_655
O2 O2 O3 86.0(2) 1_554 3_655
O2 O2 O3 94.0(2) 1_556 3_655
O2 O2 O3 61.3(3) 5_665 3_655
O2 O2 O3 99.6(3) 5_655 3_655
O3 O2 O3 157.9(3) 2_546 3_655
O3 O2 O3 72.9(2) 6_556 3_655
Ga2 O2 O3 79.9(2) 1_554 3_655
O2 O2 O3 127.6(3) 6 3_655
O2 O2 O3 92.9(4) 6_566 3_655
O2 O2 O3 32.3(2) 6_666 3_655
O3 O2 O3 61.2(3) 4_765 3_655
Nb O2 O3 21.32(13) 1_665 3_655
Ga1 O2 O3 21.32(13) 1_665 3_655
La1 O2 O3 59.19(19) 2_656 3_655
O3 O2 O3 144.1(3) 2_545 3_655
O3 O2 O3 69.9(2) 6 3_655
Ga2 O2 La1 113.0(6) 2_556 2_556
Ga3 O2 La1 26.3(3) 4_665 2_556
La1 O2 La1 105.1(3) 4_665 2_556
O3 O2 La1 88.4(4) 3_545 2_556
O2 O2 La1 121.2(4) 4_665 2_556
O2 O2 La1 139.3(2) 3_655 2_556
La1 O2 La1 138.1(4) . 2_556
O2 O2 La1 14.23(15) 2_556 2_556
O3 O2 La1 52.1(3) 4_665 2_556
O1 O2 La1 158.8(4) 2_655 2_556
O3 O2 La1 50.0(3) 5_666 2_556
O1 O2 La1 81.8(4) 2_656 2_556
O3 O2 La1 112.7(3) 5_665 2_556
O1 O2 La1 60.2(3) 1_565 2_556
Ga1 O2 La1 82.2(2) . 2_556
Nb O2 La1 82.2(2) . 2_556
O2 O2 La1 97.9(4) 2 2_556
Ga2 O2 La1 37.18(14) . 2_556
O3 O2 La1 89.7(3) 1_565 2_556
La1 O2 La1 49.19(15) 4_666 2_556
Ga3 O2 La1 74.4(2) 2_546 2_556
O3 O2 La1 77.3(3) 2_656 2_556
Ga3 O2 La1 101.7(3) 2_656 2_556
La1 O2 La1 75.4(2) 1_556 2_556
La1 O2 La1 153.2(3) 2_655 2_556
Ga3 O2 La1 110.9(2) 4_664 2_556
O3 O2 La1 25.26(16) 6_456 2_556
Ga3 O2 La1 126.0(3) . 2_556
La1 O2 La1 59.95(14) 2 2_556
O3 O2 La1 119.9(3) 2_655 2_556
Ga2 O2 La1 148.5(3) 2 2_556
O2 O2 La1 50.2(3) 5_666 2_556
O2 O2 La1 106.5(5) 5_656 2_556
O3 O2 La1 80.8(2) 6_455 2_556
O2 O2 La1 83.8(3) 6_556 2_556
Nb O2 La1 38.82(10) 1_556 2_556
Ga1 O2 La1 38.82(10) 1_556 2_556
O1 O2 La1 119.7(3) . 2_556
O3 O2 La1 65.40(19) 1_455 2_556
Ga2 O2 La1 104.7(2) 1_545 2_556
Ga3 O2 La1 44.06(11) 1_455 2_556
Ga3 O2 La1 71.70(18) 1_565 2_556
O2 O2 La1 129.23(14) 1_554 2_556
O2 O2 La1 50.77(14) 1_556 2_556
O2 O2 La1 93.6(2) 5_665 2_556
O2 O2 La1 149.6(4) 5_655 2_556
O3 O2 La1 55.2(2) 2_546 2_556
O3 O2 La1 115.0(3) 6_556 2_556
Ga2 O2 La1 93.16(18) 1_554 2_556
O2 O2 La1 120.2(2) 6 2_556
O2 O2 La1 26.36(18) 6_566 2_556
O2 O2 La1 106.4(4) 6_666 2_556
O3 O2 La1 144.4(3) 4_765 2_556
Nb O2 La1 106.1(2) 1_665 2_556
Ga1 O2 La1 106.1(2) 1_665 2_556
La1 O2 La1 97.1(3) 2_656 2_556
O3 O2 La1 93.2(2) 2_545 2_556
O3 O2 La1 172.0(3) 6 2_556
O3 O2 La1 110.8(3) 3_655 2_556
Ga2 O2 O3 80.5(5) 2_556 3_546
Ga3 O2 O3 44.2(4) 4_665 3_546
La1 O2 O3 156.7(5) 4_665 3_546
O3 O2 O3 66.5(3) 3_545 3_546
O2 O2 O3 115.40(18) 4_665 3_546
O2 O2 O3 88.1(3) 3_655 3_546
La1 O2 O3 100.4(4) . 3_546
O2 O2 O3 59.4(4) 2_556 3_546
O3 O2 O3 80.5(4) 4_665 3_546
O1 O2 O3 147.4(4) 2_655 3_546
O3 O2 O3 11.2(3) 5_666 3_546
O1 O2 O3 52.9(3) 2_656 3_546
O3 O2 O3 115.4(4) 5_665 3_546
O1 O2 O3 113.4(4) 1_565 3_546
Ga1 O2 O3 88.6(3) . 3_546
Nb O2 O3 88.6(3) . 3_546
O2 O2 O3 140.5(3) 2 3_546
Ga2 O2 O3 87.9(3) . 3_546
O3 O2 O3 125.5(4) 1_565 3_546
La1 O2 O3 57.8(2) 4_666 3_546
Ga3 O2 O3 46.1(2) 2_546 3_546
O3 O2 O3 89.1(3) 2_656 3_546
Ga3 O2 O3 106.7(3) 2_656 3_546
La1 O2 O3 24.57(13) 1_556 3_546
La1 O2 O3 125.0(3) 2_655 3_546
Ga3 O2 O3 133.4(3) 4_664 3_546
O3 O2 O3 45.1(3) 6_456 3_546
Ga3 O2 O3 74.6(2) . 3_546
La1 O2 O3 103.5(3) 2 3_546
O3 O2 O3 159.4(4) 2_655 3_546
Ga2 O2 O3 152.0(3) 2 3_546
O2 O2 O3 90.0(5) 5_666 3_546
O2 O2 O3 53.5(4) 5_656 3_546
O3 O2 O3 105.4(4) 6_455 3_546
O2 O2 O3 38.3(3) 6_556 3_546
Nb O2 O3 20.74(12) 1_556 3_546
Ga1 O2 O3 20.74(12) 1_556 3_546
O1 O2 O3 74.8(3) . 3_546
O3 O2 O3 67.42(19) 1_455 3_546
Ga2 O2 O3 54.9(2) 1_545 3_546
Ga3 O2 O3 58.11(19) 1_455 3_546
Ga3 O2 O3 107.7(3) 1_565 3_546
O2 O2 O3 149.0(2) 1_554 3_546
O2 O2 O3 31.0(2) 1_556 3_546
O2 O2 O3 146.7(3) 5_665 3_546
O2 O2 O3 108.7(3) 5_655 3_546
O3 O2 O3 34.9(3) 2_546 3_546
O3 O2 O3 71.0(3) 6_556 3_546
Ga2 O2 O3 142.6(3) 1_554 3_546
O2 O2 O3 97.2(4) 6 3_546
O2 O2 O3 79.0(3) 6_566 3_546
O2 O2 O3 94.7(4) 6_666 3_546
O3 O2 O3 100.2(2) 4_765 3_546
Nb O2 O3 138.4(3) 1_665 3_546
Ga1 O2 O3 138.4(3) 1_665 3_546
La1 O2 O3 69.4(2) 2_656 3_546
O3 O2 O3 91.9(3) 2_545 3_546
O3 O2 O3 119.5(3) 6 3_546
O3 O2 O3 123.7(4) 3_655 3_546
La1 O2 O3 53.15(18) 2_556 3_546
Ga2 O2 O3 50.0(4) 2_556 .
Ga3 O2 O3 122.4(5) 4_665 .
La1 O2 O3 115.3(4) 4_665 .
O3 O2 O3 74.4(4) 3_545 .
O2 O2 O3 71.7(4) 4_665 .
O2 O2 O3 12.3(4) 3_655 .
La1 O2 O3 40.3(2) . .
O2 O2 O3 141.4(7) 2_556 .
O3 O2 O3 130.5(4) 4_665 .
O1 O2 O3 62.3(3) 2_655 .
O3 O2 O3 89.8(4) 5_666 .
O1 O2 O3 70.1(3) 2_656 .
O3 O2 O3 84.1(3) 5_665 .
O1 O2 O3 161.0(4) 1_565 .
Ga1 O2 O3 100.1(3) . .
Nb O2 O3 100.1(3) . .
O2 O2 O3 118.5(5) 2 .
Ga2 O2 O3 162.9(4) . .
O3 O2 O3 117.9(3) 1_565 .
La1 O2 O3 110.7(3) 4_666 .
Ga3 O2 O3 77.4(2) 2_546 .
O3 O2 O3 103.5(3) 2_656 .
Ga3 O2 O3 87.5(2) 2_656 .
La1 O2 O3 63.9(2) 1_556 .
La1 O2 O3 49.33(16) 2_655 .
Ga3 O2 O3 98.2(3) 4_664 .
O3 O2 O3 123.7(3) 6_456 .
Ga3 O2 O3 16.87(16) . .
La1 O2 O3 146.2(4) 2 .
O3 O2 O3 98.1(3) 2_655 .
Ga2 O2 O3 70.9(2) 2 .
O2 O2 O3 141.4(5) 5_666 .
O2 O2 O3 32.1(3) 5_656 .
O3 O2 O3 116.2(3) 6_455 .
O2 O2 O3 60.0(2) 6_556 .
Nb O2 O3 101.9(3) 1_556 .
Ga1 O2 O3 101.9(3) 1_556 .
O1 O2 O3 35.10(14) . .
O3 O2 O3 103.1(3) 1_455 .
Ga2 O2 O3 38.53(15) 1_545 .
Ga3 O2 O3 118.6(3) 1_455 .
Ga3 O2 O3 128.4(3) 1_565 .
O2 O2 O3 86.1(2) 1_554 .
O2 O2 O3 93.9(2) 1_556 .
O2 O2 O3 127.5(4) 5_665 .
O2 O2 O3 37.1(2) 5_655 .
O3 O2 O3 92.9(3) 2_546 .
O3 O2 O3 35.9(3) 6_556 .
Ga2 O2 O3 126.5(3) 1_554 .
O2 O2 O3 59.9(2) 6 .
O2 O2 O3 162.9(5) 6_566 .
O2 O2 O3 71.88(17) 6_666 .
O3 O2 O3 28.4(2) 4_765 .
Nb O2 O3 104.7(2) 1_665 .
Ga1 O2 O3 104.7(2) 1_665 .
La1 O2 O3 62.17(18) 2_656 .
O3 O2 O3 89.1(3) 2_545 .
O3 O2 O3 34.0(3) 6 .
O3 O2 O3 89.57(19) 3_655 .
La1 O2 O3 138.7(3) 2_556 .
O3 O2 O3 85.6(3) 3_546 .
Ga2 O2 O3 94.9(5) 2_556 4_666
Ga3 O2 O3 28.8(4) 4_665 4_666
La1 O2 O3 128.8(4) 4_665 4_666
O3 O2 O3 80.6(4) 3_545 4_666
O2 O2 O3 117.9(3) 4_665 4_666
O2 O2 O3 114.2(3) 3_655 4_666
La1 O2 O3 125.0(4) . 4_666
O2 O2 O3 31.3(4) 2_556 4_666
O3 O2 O3 66.9(4) 4_665 4_666
O1 O2 O3 175.7(4) 2_655 4_666
O3 O2 O3 28.2(3) 5_666 4_666
O1 O2 O3 62.8(4) 2_656 4_666
O3 O2 O3 121.2(4) 5_665 4_666
O1 O2 O3 85.3(4) 1_565 4_666
Ga1 O2 O3 88.8(3) . 4_666
Nb O2 O3 88.8(3) . 4_666
O2 O2 O3 121.6(4) 2 4_666
Ga2 O2 O3 59.7(2) . 4_666
O3 O2 O3 104.7(4) 1_565 4_666
La1 O2 O3 44.03(19) 4_666 4_666
Ga3 O2 O3 61.8(2) 2_546 4_666
O3 O2 O3 78.0(3) 2_656 4_666
Ga3 O2 O3 101.6(3) 2_656 4_666
La1 O2 O3 49.95(18) 1_556 4_666
La1 O2 O3 142.5(3) 2_655 4_666
Ga3 O2 O3 128.7(3) 4_664 4_666
O3 O2 O3 28.8(3) 6_456 4_666
Ga3 O2 O3 100.7(3) . 4_666
La1 O2 O3 82.5(2) 2 4_666
O3 O2 O3 139.6(3) 2_655 4_666
Ga2 O2 O3 169.7(3) 2 4_666
O2 O2 O3 65.3(4) 5_666 4_666
O2 O2 O3 81.3(4) 5_656 4_666
O3 O2 O3 96.4(3) 6_455 4_666
O2 O2 O3 63.4(3) 6_556 4_666
Nb O2 O3 20.85(14) 1_556 4_666
Ga1 O2 O3 20.85(14) 1_556 4_666
O1 O2 O3 100.9(3) . 4_666
O3 O2 O3 67.6(2) 1_455 4_666
Ga2 O2 O3 82.5(2) 1_545 4_666
Ga3 O2 O3 49.43(18) 1_455 4_666
Ga3 O2 O3 85.6(2) 1_565 4_666
O2 O2 O3 149.30(18) 1_554 4_666
O2 O2 O3 30.70(18) 1_556 4_666
O2 O2 O3 118.4(3) 5_665 4_666
O2 O2 O3 135.0(3) 5_655 4_666
O3 O2 O3 43.4(3) 2_546 4_666
O3 O2 O3 92.0(3) 6_556 4_666
Ga2 O2 O3 118.3(2) 1_554 4_666
O2 O2 O3 115.0(3) 6 4_666
O2 O2 O3 50.7(3) 6_566 4_666
O2 O2 O3 98.0(4) 6_666 4_666
O3 O2 O3 122.6(3) 4_765 4_666
Nb O2 O3 120.8(3) 1_665 4_666
Ga1 O2 O3 120.8(3) 1_665 4_666
La1 O2 O3 79.9(2) 2_656 4_666
O3 O2 O3 97.1(3) 2_545 4_666
O3 O2 O3 146.8(3) 6 4_666
O3 O2 O3 116.1(3) 3_655 4_666
La1 O2 O3 25.42(12) 2_556 4_666
O3 O2 O3 28.3(2) 3_546 4_666
O3 O2 O3 113.4(3) . 4_666
Ga2 O2 O2 153.9(5) 2_556 3
Ga3 O2 O2 31.6(4) 4_665 3
La1 O2 O2 96.0(4) 4_665 3
O3 O2 O2 58.8(2) 3_545 3
O2 O2 O2 155.1(7) 4_665 3
O2 O2 O2 144.9(7) 3_655 3
La1 O2 O2 101.9(3) . 3
O2 O2 O2 56.4(4) 2_556 3
O3 O2 O2 7.7(4) 4_665 3
O1 O2 O2 123.1(3) 2_655 3
O3 O2 O2 64.3(3) 5_666 3
O1 O2 O2 122.0(3) 2_656 3
O3 O2 O2 68.2(2) 5_665 3
O1 O2 O2 58.4(3) 1_565 3
Ga1 O2 O2 39.11(14) . 3
Nb O2 O2 39.11(14) . 3
O2 O2 O2 66.3(3) 2 3
Ga2 O2 O2 59.2(3) . 3
O3 O2 O2 108.1(4) 1_565 3
La1 O2 O2 93.7(2) 4_666 3
Ga3 O2 O2 58.06(12) 2_546 3
O3 O2 O2 117.7(4) 2_656 3
Ga3 O2 O2 138.5(4) 2_656 3
La1 O2 O2 98.08(17) 1_556 3
La1 O2 O2 158.2(2) 2_655 3
Ga3 O2 O2 69.51(15) 4_664 3
O3 O2 O2 31.2(3) 6_456 3
Ga3 O2 O2 137.3(3) . 3
La1 O2 O2 30.69(19) 2 3
O3 O2 O2 115.4(3) 2_655 3
Ga2 O2 O2 110.69(15) 2 3
O2 O2 O2 81.6(4) 5_666 3
O2 O2 O2 114.9(4) 5_656 3
O3 O2 O2 37.4(3) 6_455 3
O2 O2 O2 79.4(2) 6_556 3
Nb O2 O2 53.74(13) 1_556 3
Ga1 O2 O2 53.74(13) 1_556 3
O1 O2 O2 98.2(2) . 3
O3 O2 O2 30.10(16) 1_455 3
Ga2 O2 O2 98.1(2) 1_545 3
Ga3 O2 O2 18.40(12) 1_455 3
Ga3 O2 O2 98.2(3) 1_565 3
O2 O2 O2 90.000(2) 1_554 3
O2 O2 O2 90.000(1) 1_556 3
O2 O2 O2 82.7(3) 5_665 3
O2 O2 O2 111.4(3) 5_655 3
O3 O2 O2 48.0(2) 2_546 3
O3 O2 O2 144.2(3) 6_556 3
Ga2 O2 O2 69.4(2) 1_554 3
O2 O2 O2 80.76(19) 6 3
O2 O2 O2 48.95(17) 6_566 3
O2 O2 O2 149.9(4) 6_666 3
O3 O2 O2 161.3(3) 4_765 3
Nb O2 O2 118.5(3) 1_665 3
Ga1 O2 O2 118.5(3) 1_665 3
La1 O2 O2 139.21(15) 2_656 3
O3 O2 O2 50.80(16) 2_545 3
O3 O2 O2 140.2(3) 6 3
O3 O2 O2 136.7(4) 3_655 3
La1 O2 O2 44.58(16) 2_556 3
O3 O2 O2 74.40(15) 3_546 3
O3 O2 O2 133.1(3) . 3
O3 O2 O2 59.31(18) 4_666 3
Ga2 O2 O2 112.3(6) 2_556 4
Ga3 O2 O2 58.5(3) 4_665 4
La1 O2 O2 134.4(3) 4_665 4
O3 O2 O2 7.6(4) 3_545 4
O2 O2 O2 144.9(7) 4_665 4
O2 O2 O2 84.9(7) 3_655 4
La1 O2 O2 53.6(3) . 4
O2 O2 O2 98.54(14) 2_556 4
O3 O2 O2 58.8(2) 4_665 4
O1 O2 O2 103.4(4) 2_655 4
O3 O2 O2 50.5(4) 5_666 4
O1 O2 O2 103.0(3) 2_656 4
O3 O2 O2 57.0(3) 5_665 4
O1 O2 O2 117.0(3) 1_565 4
Ga1 O2 O2 39.11(14) . 4
Nb O2 O2 39.11(14) . 4
O2 O2 O2 96.19(8) 2 4
Ga2 O2 O2 116.3(2) . 4
O3 O2 O2 167.0(4) 1_565 4
La1 O2 O2 115.89(18) 4_666 4
Ga3 O2 O2 13.2(2) 2_546 4
O3 O2 O2 148.0(3) 2_656 4
Ga3 O2 O2 156.3(3) 2_656 4
La1 O2 O2 66.0(2) 1_556 4
La1 O2 O2 118.3(4) 2_655 4
Ga3 O2 O2 77.60(15) 4_664 4
O3 O2 O2 59.64(17) 6_456 4
Ga3 O2 O2 79.0(3) . 4
La1 O2 O2 83.61(15) 2 4
O3 O2 O2 141.5(3) 2_655 4
Ga2 O2 O2 98.6(2) 2 4
O2 O2 O2 134.8(4) 5_666 4
O2 O2 O2 60.8(4) 5_656 4
O3 O2 O2 62.02(18) 6_455 4
O2 O2 O2 29.5(4) 6_556 4
Nb O2 O2 53.74(13) 1_556 4
Ga1 O2 O2 53.74(13) 1_556 4
O1 O2 O2 39.1(2) . 4
O3 O2 O2 30.49(17) 1_455 4
Ga2 O2 O2 40.0(2) 1_545 4
Ga3 O2 O2 46.12(8) 1_455 4
Ga3 O2 O2 155.9(3) 1_565 4
O2 O2 O2 90.000(2) 1_554 4
O2 O2 O2 90.000(1) 1_556 4
O2 O2 O2 127.5(3) 5_665 4
O2 O2 O2 65.1(3) 5_655 4
O3 O2 O2 31.35(19) 2_546 4
O3 O2 O2 93.8(3) 6_556 4
Ga2 O2 O2 107.79(14) 1_554 4
O2 O2 O2 40.5(3) 6 4
O2 O2 O2 104.28(15) 6_566 4
O2 O2 O2 137.6(4) 6_666 4
O3 O2 O2 101.7(3) 4_765 4
Nb O2 O2 162.57(17) 1_665 4
Ga1 O2 O2 162.57(17) 1_665 4
La1 O2 O2 112.7(3) 2_656 4
O3 O2 O2 36.2(2) 2_545 4
O3 O2 O2 93.6(3) 6 4
O3 O2 O2 162.7(4) 3_655 4
La1 O2 O2 84.71(13) 2_556 4
O3 O2 O2 59.0(2) 3_546 4
O3 O2 O2 73.3(3) . 4
O3 O2 O2 74.53(16) 4_666 4
O2 O2 O2 60.000(2) 3 4
Ga2 O2 O1 90.4(5) 2_556 1_566
Ga3 O2 O1 51.3(4) 4_665 1_566
La1 O2 O1 98.6(4) 4_665 1_566
O3 O2 O1 112.1(4) 3_545 1_566
O2 O2 O1 94.7(4) 4_665 1_566
O2 O2 O1 125.4(2) 3_655 1_566
La1 O2 O1 158.3(4) . 1_566
O2 O2 O1 14.2(3) 2_556 1_566
O3 O2 O1 77.5(4) 4_665 1_566
O1 O2 O1 149.4(4) 2_655 1_566
O3 O2 O1 61.2(4) 5_666 1_566
O1 O2 O1 62.8(3) 2_656 1_566
O3 O2 O1 137.9(3) 5_665 1_566
O1 O2 O1 62.9(3) 1_565 1_566
Ga1 O2 O1 108.8(3) . 1_566
Nb O2 O1 108.8(3) . 1_566
O2 O2 O1 109.4(5) 2 1_566
Ga2 O2 O1 34.0(2) . 1_566
O3 O2 O1 71.2(3) 1_565 1_566
La1 O2 O1 24.16(11) 4_666 1_566
Ga3 O2 O1 94.7(2) 2_546 1_566
O3 O2 O1 50.8(2) 2_656 1_566
Ga3 O2 O1 75.4(2) 2_656 1_566
La1 O2 O1 72.4(2) 1_556 1_566
La1 O2 O1 126.5(3) 2_655 1_566
Ga3 O2 O1 129.5(3) 4_664 1_566
O3 O2 O1 50.5(2) 6_456 1_566
Ga3 O2 O1 115.1(3) . 1_566
La1 O2 O1 78.0(2) 2 1_566
O3 O2 O1 106.3(3) 2_655 1_566
Ga2 O2 O1 149.7(3) 2 1_566
O2 O2 O1 32.1(3) 5_666 1_566
O2 O2 O1 104.3(5) 5_656 1_566
O3 O2 O1 104.3(3) 6_455 1_566
O2 O2 O1 96.0(4) 6_556 1_566
Nb O2 O1 54.08(15) 1_556 1_566
Ga1 O2 O1 54.08(15) 1_556 1_566
O1 O2 O1 133.1(4) . 1_566
O3 O2 O1 91.9(2) 1_455 1_566
Ga2 O2 O1 112.7(3) 1_545 1_566
Ga3 O2 O1 70.60(17) 1_455 1_566
Ga3 O2 O1 52.16(17) 1_565 1_566
O2 O2 O1 141.18(17) 1_554 1_566
O2 O2 O1 38.82(17) 1_556 1_566
O2 O2 O1 91.6(3) 5_665 1_566
O2 O2 O1 166.5(4) 5_655 1_566
O3 O2 O1 75.6(2) 2_546 1_566
O3 O2 O1 98.1(3) 6_556 1_566
Ga2 O2 O1 100.0(2) 1_554 1_566
O2 O2 O1 145.9(3) 6 1_566
O2 O2 O1 31.7(3) 6_566 1_566
O2 O2 O1 79.9(4) 6_666 1_566
O3 O2 O1 122.5(3) 4_765 1_566
Nb O2 O1 87.5(2) 1_665 1_566
Ga1 O2 O1 87.5(2) 1_665 1_566
La1 O2 O1 74.9(2) 2_656 1_566
O3 O2 O1 120.0(3) 2_545 1_566
O3 O2 O1 149.4(3) 6 1_566
O3 O2 O1 86.4(3) 3_655 1_566
La1 O2 O1 26.74(8) 2_556 1_566
O3 O2 O1 58.3(2) 3_546 1_566
O3 O2 O1 131.8(3) . 1_566
O3 O2 O1 33.48(15) 4_666 1_566
O2 O2 O1 70.39(19) 3 1_566
O2 O2 O1 106.91(14) 4 1_566
Ga2 O2 O2 144.4(6) 2_556 6_565
Ga3 O2 O2 81.3(3) 4_665 6_565
La1 O2 O2 42.0(3) 4_665 6_565
O3 O2 O2 97.2(4) 3_545 6_565
O2 O2 O2 106.4(6) 4_665 6_565
O2 O2 O2 145.2(3) 3_655 6_565
La1 O2 O2 106.9(5) . 6_565
O2 O2 O2 75.7(4) 2_556 6_565
O3 O2 O2 50.3(3) 4_665 6_565
O1 O2 O2 83.6(5) 2_655 6_565
O3 O2 O2 116.9(3) 5_666 6_565
O1 O2 O2 143.7(5) 2_656 6_565
O3 O2 O2 64.5(3) 5_665 6_565
O1 O2 O2 24.4(3) 1_565 6_565
Ga1 O2 O2 64.3(2) . 6_565
Nb O2 O2 64.3(2) . 6_565
O2 O2 O2 24.1(2) 2 6_565
Ga2 O2 O2 51.96(16) . 6_565
O3 O2 O2 64.5(3) 1_565 6_565
La1 O2 O2 104.3(4) 4_666 6_565
Ga3 O2 O2 107.4(2) 2_546 6_565
O3 O2 O2 98.2(4) 2_656 6_565
Ga3 O2 O2 101.0(3) 2_656 6_565
La1 O2 O2 149.6(3) 1_556 6_565
La1 O2 O2 109.5(4) 2_655 6_565
Ga3 O2 O2 46.1(2) 4_664 6_565
O3 O2 O2 80.32(17) 6_456 6_565
Ga3 O2 O2 158.3(5) . 6_565
La1 O2 O2 23.39(6) 2 6_565
O3 O2 O2 61.4(3) 2_655 6_565
Ga2 O2 O2 73.2(3) 2 6_565
O2 O2 O2 66.97(18) 5_666 6_565
O2 O2 O2 162.6(5) 5_656 6_565
O3 O2 O2 41.5(2) 6_455 6_565
O2 O2 O2 130.1(3) 6_556 6_565
Nb O2 O2 104.96(17) 1_556 6_565
Ga1 O2 O2 104.96(17) 1_556 6_565
O1 O2 O2 125.5(4) . 6_565
O3 O2 O2 75.1(2) 1_455 6_565
Ga2 O2 O2 141.0(4) 1_545 6_565
Ga3 O2 O2 72.39(9) 1_455 6_565
Ga3 O2 O2 67.1(3) 1_565 6_565
O2 O2 O2 56.5(3) 1_554 6_565
O2 O2 O2 123.5(3) 1_556 6_565
O2 O2 O2 28.9(2) 5_665 6_565
O2 O2 O2 106.7(6) 5_655 6_565
O3 O2 O2 101.9(2) 2_546 6_565
O3 O2 O2 161.4(4) 6_556 6_565
Ga2 O2 O2 17.89(17) 1_554 6_565
O2 O2 O2 92.4(4) 6 6_565
O2 O2 O2 54.38(15) 6_566 6_565
O2 O2 O2 119.7(5) 6_666 6_565
O3 O2 O2 134.7(4) 4_765 6_565
Nb O2 O2 68.0(3) 1_665 6_565
Ga1 O2 O2 68.0(3) 1_665 6_565
La1 O2 O2 143.0(4) 2_656 6_565
O3 O2 O2 71.0(3) 2_545 6_565
O3 O2 O2 112.5(4) 6 6_565
O3 O2 O2 89.1(3) 3_655 6_565
La1 O2 O2 75.52(16) 2_556 6_565
O3 O2 O2 125.1(2) 3_546 6_565
O3 O2 O2 142.7(4) . 6_565
O3 O2 O2 100.5(2) 4_666 6_565
O2 O2 O2 54.08(16) 3 6_565
O2 O2 O2 102.73(14) 4 6_565
O1 O2 O2 85.3(3) 1_566 6_565
Ga2 O2 O2 64.5(3) 2_556 6_665
Ga3 O2 O2 167.3(6) 4_665 6_665
La1 O2 O2 47.3(3) 4_665 6_665
O3 O2 O2 126.5(6) 3_545 6_665
O2 O2 O2 33.5(3) 4_665 6_665
O2 O2 O2 63.2(2) 3_655 6_665
La1 O2 O2 77.7(3) . 6_665
O2 O2 O2 130.1(3) 2_556 6_665
O3 O2 O2 134.5(5) 4_665 6_665
O1 O2 O2 29.83(18) 2_655 6_665
O3 O2 O2 155.0(4) 5_666 6_665
O1 O2 O2 94.1(3) 2_656 6_665
O3 O2 O2 87.7(5) 5_665 6_665
O1 O2 O2 91.8(4) 1_565 6_665
Ga1 O2 O2 119.7(5) . 6_665
Nb O2 O2 119.7(5) . 6_665
O2 O2 O2 74.6(4) 2 6_665
Ga2 O2 O2 107.7(4) . 6_665
O3 O2 O2 53.7(3) 1_565 6_665
La1 O2 O2 106.8(4) 4_666 6_665
Ga3 O2 O2 142.1(4) 2_546 6_665
O3 O2 O2 73.0(3) 2_656 6_665
Ga3 O2 O2 49.16(17) 2_656 6_665
La1 O2 O2 121.2(2) 1_556 6_665
La1 O2 O2 22.25(7) 2_655 6_665
Ga3 O2 O2 76.7(3) 4_664 6_665
O3 O2 O2 166.0(4) 6_456 6_665
Ga3 O2 O2 75.60(10) . 6_665
La1 O2 O2 110.7(4) 2 6_665
O3 O2 O2 28.3(2) 2_655 6_665
Ga2 O2 O2 38.9(2) 2 6_665
O2 O2 O2 93.3(4) 5_666 6_665
O2 O2 O2 99.0(2) 5_656 6_665
O3 O2 O2 107.9(5) 6_455 6_665
O2 O2 O2 130.1(3) 6_556 6_665
Nb O2 O2 165.3(4) 1_556 6_665
Ga1 O2 O2 165.3(4) 1_556 6_665
O1 O2 O2 96.6(3) . 6_665
O3 O2 O2 141.4(5) 1_455 6_665
Ga2 O2 O2 108.5(2) 1_545 6_665
Ga3 O2 O2 156.5(4) 1_455 6_665
Ga3 O2 O2 71.8(3) 1_565 6_665
O2 O2 O2 56.5(3) 1_554 6_665
O2 O2 O2 123.5(3) 1_556 6_665
O2 O2 O2 60.9(4) 5_665 6_665
O2 O2 O2 66.3(3) 5_655 6_665
O3 O2 O2 161.4(4) 2_546 6_665
O3 O2 O2 74.68(17) 6_556 6_665
Ga2 O2 O2 71.5(3) 1_554 6_665
O2 O2 O2 92.4(4) 6 6_665
O2 O2 O2 119.7(5) 6_566 6_665
O2 O2 O2 54.38(15) 6_666 6_665
O3 O2 O2 47.84(15) 4_765 6_665
Nb O2 O2 37.4(2) 1_665 6_665
Ga1 O2 O2 37.4(2) 1_665 6_665
La1 O2 O2 76.83(17) 2_656 6_665
O3 O2 O2 112.1(4) 2_545 6_665
O3 O2 O2 40.13(18) 6 6_665
O3 O2 O2 35.3(2) 3_655 6_665
La1 O2 O2 143.4(4) 2_556 6_665
O3 O2 O2 145.0(3) 3_546 6_665
O3 O2 O2 70.33(17) . 6_665
O3 O2 O2 150.7(4) 4_666 6_665
O2 O2 O2 140.6(2) 3 6_665
O2 O2 O2 131.2(4) 4 6_665
O1 O2 O2 121.5(4) 1_566 6_665
O2 O2 O2 87.9(4) 6_565 6_665
Ga2 O2 Ga3 127.1(5) 2_556 2_545
Ga3 O2 Ga3 88.6(5) 4_665 2_545
La1 O2 Ga3 90.7(4) 4_665 2_545
O3 O2 Ga3 38.0(3) 3_545 2_545
O2 O2 Ga3 126.4(2) 4_665 2_545
O2 O2 Ga3 88.4(4) 3_655 2_545
La1 O2 Ga3 37.52(19) . 2_545
O2 O2 Ga3 123.9(3) 2_556 2_545
O3 O2 Ga3 60.9(3) 4_665 2_545
O1 O2 Ga3 65.3(3) 2_655 2_545
O3 O2 Ga3 95.3(4) 5_666 2_545
O1 O2 Ga3 141.1(3) 2_656 2_545
O3 O2 Ga3 12.0(2) 5_665 2_545
O1 O2 Ga3 98.2(3) 1_565 2_545
Ga1 O2 Ga3 28.89(13) . 2_545
Nb O2 Ga3 28.89(13) . 2_545
O2 O2 Ga3 57.0(2) 2 2_545
Ga2 O2 Ga3 119.4(3) . 2_545
O3 O2 Ga3 127.3(4) 1_565 2_545
La1 O2 Ga3 158.2(3) 4_666 2_545
Ga3 O2 Ga3 58.39(18) 2_546 2_545
O3 O2 Ga3 166.4(4) 2_656 2_545
Ga3 O2 Ga3 144.1(3) 2_656 2_545
La1 O2 Ga3 108.5(3) 1_556 2_545
La1 O2 Ga3 95.4(3) 2_655 2_545
Ga3 O2 Ga3 34.15(12) 4_664 2_545
O3 O2 Ga3 89.2(3) 6_456 2_545
Ga3 O2 Ga3 92.8(2) . 2_545
La1 O2 Ga3 68.73(18) 2 2_545
O3 O2 Ga3 96.1(3) 2_655 2_545
Ga2 O2 Ga3 56.55(17) 2 2_545
O2 O2 Ga3 140.2(4) 5_666 2_545
O2 O2 Ga3 88.9(3) 5_656 2_545
O3 O2 Ga3 38.71(17) 6_455 2_545
O2 O2 Ga3 71.6(3) 6_556 2_545
Nb O2 Ga3 95.5(2) 1_556 2_545
Ga1 O2 Ga3 95.5(2) 1_556 2_545
O1 O2 Ga3 51.0(2) . 2_545
O3 O2 Ga3 47.48(19) 1_455 2_545
Ga2 O2 Ga3 69.07(18) 1_545 2_545
Ga3 O2 Ga3 68.01(16) 1_455 2_545
Ga3 O2 Ga3 139.5(3) 1_565 2_545
O2 O2 Ga3 44.49(14) 1_554 2_545
O2 O2 Ga3 135.51(14) 1_556 2_545
O2 O2 Ga3 88.2(3) 5_665 2_545
O2 O2 Ga3 44.6(3) 5_655 2_545
O3 O2 Ga3 72.9(2) 2_546 2_545
O3 O2 Ga3 112.8(3) 6_556 2_545
Ga2 O2 Ga3 69.92(17) 1_554 2_545
O2 O2 Ga3 18.19(15) 6 2_545
O2 O2 Ga3 113.3(3) 6_566 2_545
O2 O2 Ga3 142.3(3) 6_666 2_545
O3 O2 Ga3 97.3(2) 4_765 2_545
Nb O2 Ga3 117.0(3) 1_665 2_545
Ga1 O2 Ga3 117.0(3) 1_665 2_545
La1 O2 Ga3 139.4(2) 2_656 2_545
O3 O2 Ga3 18.03(13) 2_545 2_545
O3 O2 Ga3 72.6(2) 6 2_545
O3 O2 Ga3 128.9(3) 3_655 2_545
La1 O2 Ga3 111.1(2) 2_556 2_545
O3 O2 Ga3 104.5(3) 3_546 2_545
O3 O2 Ga3 77.5(2) . 2_545
O3 O2 Ga3 114.3(3) 4_666 2_545
O2 O2 Ga3 67.65(12) 3 2_545
O2 O2 Ga3 45.58(13) 4 2_545
O1 O2 Ga3 137.7(2) 1_566 2_545
O2 O2 Ga3 74.5(3) 6_565 2_545
O2 O2 Ga3 94.9(4) 6_665 2_545
Ga2 O2 O2 89.9(5) 2_556 4_664
Ga3 O2 O2 147.7(5) 4_665 4_664
La1 O2 O2 39.5(3) 4_665 4_664
O3 O2 O2 106.7(4) 3_545 4_664
O2 O2 O2 60.93(17) 4_665 4_664
O2 O2 O2 75.94(7) 3_655 4_664
La1 O2 O2 65.6(2) . 4_664
O2 O2 O2 137.0(5) 2_556 4_664
O3 O2 O2 109.1(4) 4_665 4_664
O1 O2 O2 15.92(15) 2_655 4_664
O3 O2 O2 162.7(5) 5_666 4_664
O1 O2 O2 121.0(4) 2_656 4_664
O3 O2 O2 61.5(2) 5_665 4_664
O1 O2 O2 83.3(4) 1_565 4_664
Ga1 O2 O2 92.6(2) . 4_664
Nb O2 O2 92.6(2) . 4_664
O2 O2 O2 50.8(2) 2 4_664
Ga2 O2 O2 108.5(4) . 4_664
O3 O2 O2 65.5(3) 1_565 4_664
La1 O2 O2 130.3(4) 4_666 4_664
Ga3 O2 O2 126.5(3) 2_546 4_664
O3 O2 O2 96.4(4) 2_656 4_664
Ga3 O2 O2 74.6(3) 2_656 4_664
La1 O2 O2 140.4(3) 1_556 4_664
La1 O2 O2 42.6(2) 2_655 4_664
Ga3 O2 O2 49.15(13) 4_664 4_664
O3 O2 O2 147.2(3) 6_456 4_664
Ga3 O2 O2 89.5(3) . 4_664
La1 O2 O2 89.7(3) 2 4_664
O3 O2 O2 30.0(3) 2_655 4_664
Ga2 O2 O2 14.89(8) 2 4_664
O2 O2 O2 104.0(5) 5_666 4_664
O2 O2 O2 109.9(4) 5_656 4_664
O3 O2 O2 80.9(3) 6_455 4_664
O2 O2 O2 127.7(5) 6_556 4_664
Nb O2 O2 165.7(3) 1_556 4_664
Ga1 O2 O2 165.7(3) 1_556 4_664
O1 O2 O2 90.3(3) . 4_664
O3 O2 O2 114.5(3) 1_455 4_664
Ga2 O2 O2 109.2(3) 1_545 4_664
Ga3 O2 O2 129.4(3) 1_455 4_664
Ga3 O2 O2 84.4(3) 1_565 4_664
O2 O2 O2 29.07(17) 1_554 4_664
O2 O2 O2 150.93(17) 1_556 4_664
O2 O2 O2 50.0(4) 5_665 4_664
O2 O2 O2 56.1(3) 5_655 4_664
O3 O2 O2 143.2(3) 2_546 4_664
O3 O2 O2 95.8(3) 6_556 4_664
Ga2 O2 O2 51.96(19) 1_554 4_664
O2 O2 O2 73.0(3) 6 4_664
O2 O2 O2 117.8(5) 6_566 4_664
O2 O2 O2 81.9(4) 6_666 4_664
O3 O2 O2 65.6(3) 4_765 4_664
Nb O2 O2 50.1(2) 1_665 4_664
Ga1 O2 O2 50.1(2) 1_665 4_664
La1 O2 O2 103.6(3) 2_656 4_664
O3 O2 O2 86.2(2) 2_545 4_664
O3 O2 O2 44.0(2) 6 4_664
O3 O2 O2 58.6(3) 3_655 4_664
La1 O2 O2 143.5(3) 2_556 4_664
O3 O2 O2 163.3(4) 3_546 4_664
O3 O2 O2 77.8(3) . 4_664
O3 O2 O2 168.3(4) 4_666 4_664
O2 O2 O2 116.1(2) 3 4_664
O2 O2 O2 113.4(2) 4 4_664
O1 O2 O2 136.1(4) 1_566 4_664
O2 O2 O2 69.8(3) 6_565 4_664
O2 O2 O2 27.5(3) 6_665 4_664
Ga3 O2 O2 70.40(14) 2_545 4_664
Ga2 O2 O2 40.8(4) 2_556 4_666
Ga3 O2 O2 87.2(5) 4_665 4_666
La1 O2 O2 111.9(5) 4_665 4_666
O3 O2 O2 121.0(4) 3_545 4_666
O2 O2 O2 60.93(16) 4_665 4_666
O2 O2 O2 75.94(7) 3_655 4_666
La1 O2 O2 124.2(4) . 4_666
O2 O2 O2 63.7(4) 2_556 4_666
O3 O2 O2 123.9(5) 4_665 4_666
O1 O2 O2 120.0(4) 2_655 4_666
O3 O2 O2 68.0(4) 5_666 4_666
O1 O2 O2 15.45(14) 2_656 4_666
O3 O2 O2 167.1(5) 5_665 4_666
O1 O2 O2 103.9(5) 1_565 4_666
Ga1 O2 O2 145.3(3) . 4_666
Nb O2 O2 145.3(3) . 4_666
O2 O2 O2 147.3(4) 2 4_666
Ga2 O2 O2 78.6(3) . 4_666
O3 O2 O2 75.7(4) 1_565 4_666
La1 O2 O2 26.47(16) 4_666 4_666
Ga3 O2 O2 101.9(2) 2_546 4_666
O3 O2 O2 35.7(3) 2_656 4_666
Ga3 O2 O2 49.4(3) 2_656 4_666
La1 O2 O2 48.02(11) 1_556 4_666
La1 O2 O2 85.0(3) 2_655 4_666
Ga3 O2 O2 168.9(4) 4_664 4_666
O3 O2 O2 87.1(3) 6_456 4_666
Ga3 O2 O2 68.0(2) . 4_666
La1 O2 O2 127.8(4) 2 4_666
O3 O2 O2 102.7(4) 2_655 4_666
Ga2 O2 O2 131.9(3) 2 4_666
O2 O2 O2 61.3(5) 5_666 4_666
O2 O2 O2 67.5(3) 5_656 4_666
O3 O2 O2 153.3(4) 6_455 4_666
O2 O2 O2 85.3(3) 6_556 4_666
Nb O2 O2 72.07(16) 1_556 4_666
Ga1 O2 O2 72.07(16) 1_556 4_666
O1 O2 O2 105.6(3) . 4_666
O3 O2 O2 123.4(3) 1_455 4_666
Ga2 O2 O2 86.7(2) 1_545 4_666
Ga3 O2 O2 107.7(2) 1_455 4_666
Ga3 O2 O2 64.8(3) 1_565 4_666
O2 O2 O2 150.93(17) 1_554 4_666
O2 O2 O2 29.07(17) 1_556 4_666
O2 O2 O2 115.9(4) 5_665 4_666
O2 O2 O2 121.4(3) 5_655 4_666
O3 O2 O2 91.9(3) 2_546 4_666
O3 O2 O2 48.9(2) 6_556 4_666
Ga2 O2 O2 134.4(4) 1_554 4_666
O2 O2 O2 139.0(4) 6 4_666
O2 O2 O2 80.9(4) 6_566 4_666
O2 O2 O2 40.0(4) 6_666 4_666
O3 O2 O2 72.9(3) 4_765 4_666
Nb O2 O2 83.3(3) 1_665 4_666
Ga1 O2 O2 83.3(3) 1_665 4_666
La1 O2 O2 24.98(15) 2_656 4_666
O3 O2 O2 148.9(3) 2_545 4_666
O3 O2 O2 101.2(3) 6 4_666
O3 O2 O2 66.4(3) 3_655 4_666
La1 O2 O2 72.5(2) 2_556 4_666
O3 O2 O2 57.27(17) 3_546 4_666
O3 O2 O2 84.6(3) . 4_666
O3 O2 O2 58.41(18) 4_666 4_666
O2 O2 O2 116.1(2) 3 4_666
O2 O2 O2 113.4(2) 4 4_666
O1 O2 O2 50.1(2) 1_566 4_666
O2 O2 O2 128.2(5) 6_565 4_666
O2 O2 O2 94.4(3) 6_665 4_666
Ga3 O2 O2 155.7(3) 2_545 4_666
O2 O2 O2 121.9(3) 4_664 4_666
Ga2 O2 O2 89.9(5) 2_556 3_654
Ga3 O2 O2 139.0(6) 4_665 3_654
La1 O2 O2 66.1(2) 4_665 3_654
O3 O2 O2 81.7(5) 3_545 3_654
O2 O2 O2 75.94(7) 4_665 3_654
O2 O2 O2 60.93(17) 3_655 3_654
La1 O2 O2 37.5(3) . 3_654
O2 O2 O2 160.9(6) 2_556 3_654
O3 O2 O2 105.7(5) 4_665 3_654
O1 O2 O2 15.91(15) 2_655 3_654
O3 O2 O2 134.6(5) 5_666 3_654
O1 O2 O2 121.0(4) 2_656 3_654
O3 O2 O2 46.1(3) 5_665 3_654
O1 O2 O2 105.1(4) 1_565 3_654
Ga1 O2 O2 78.2(3) . 3_654
Nb O2 O2 78.2(3) . 3_654
O2 O2 O2 61.5(3) 2 3_654
Ga2 O2 O2 133.4(3) . 3_654
O3 O2 O2 93.2(3) 1_565 3_654
La1 O2 O2 151.1(4) 4_666 3_654
Ga3 O2 O2 100.2(4) 2_546 3_654
O3 O2 O2 118.4(4) 2_656 3_654
Ga3 O2 O2 94.0(3) 2_656 3_654
La1 O2 O2 120.7(3) 1_556 3_654
La1 O2 O2 46.3(2) 2_655 3_654
Ga3 O2 O2 46.27(15) 4_664 3_654
O3 O2 O2 139.5(4) 6_456 3_654
Ga3 O2 O2 73.2(3) . 3_654
La1 O2 O2 97.8(2) 2 3_654
O3 O2 O2 58.0(2) 2_655 3_654
Ga2 O2 O2 14.89(8) 2 3_654
O2 O2 O2 132.1(4) 5_666 3_654
O2 O2 O2 88.2(4) 5_656 3_654
O3 O2 O2 76.5(3) 6_455 3_654
O2 O2 O2 99.7(5) 6_556 3_654
Nb O2 O2 141.1(4) 1_556 3_654
Ga1 O2 O2 141.1(4) 1_556 3_654
O1 O2 O2 62.5(3) . 3_654
O3 O2 O2 97.9(3) 1_455 3_654
Ga2 O2 O2 82.4(3) 1_545 3_654
Ga3 O2 O2 118.2(3) 1_455 3_654
Ga3 O2 O2 112.3(3) 1_565 3_654
O2 O2 O2 29.07(17) 1_554 3_654
O2 O2 O2 150.93(17) 1_556 3_654
O2 O2 O2 74.2(3) 5_665 3_654
O2 O2 O2 28.5(3) 5_655 3_654
O3 O2 O2 118.8(4) 2_546 3_654
O3 O2 O2 87.0(3) 6_556 3_654
Ga2 O2 O2 68.77(14) 1_554 3_654
O2 O2 O2 47.3(2) 6 3_654
O2 O2 O2 139.4(4) 6_566 3_654
O2 O2 O2 93.8(3) 6_666 3_654
O3 O2 O2 58.4(2) 4_765 3_654
Nb O2 O2 77.2(2) 1_665 3_654
Ga1 O2 O2 77.2(2) 1_665 3_654
La1 O2 O2 105.8(3) 2_656 3_654
O3 O2 O2 68.4(3) 2_545 3_654
O3 O2 O2 30.0(2) 6 3_654
O3 O2 O2 80.8(3) 3_655 3_654
La1 O2 O2 157.1(3) 2_556 3_654
O3 O2 O2 137.2(4) 3_546 3_654
O3 O2 O2 57.7(3) . 3_654
O3 O2 O2 161.9(4) 4_666 3_654
O2 O2 O2 113.4(2) 3 3_654
O2 O2 O2 87.5(3) 4 3_654
O1 O2 O2 164.2(3) 1_566 3_654
O2 O2 O2 85.3(3) 6_565 3_654
O2 O2 O2 45.5(2) 6_665 3_654
Ga3 O2 O2 50.5(2) 2_545 3_654
O2 O2 O2 28.12(15) 4_664 3_654
O2 O2 O2 130.2(3) 4_666 3_654
Ga2 O2 O2 40.8(4) 2_556 3_656
Ga3 O2 O2 82.0(4) 4_665 3_656
La1 O2 O2 137.7(5) 4_665 3_656
O3 O2 O2 94.8(5) 3_545 3_656
O2 O2 O2 75.94(7) 4_665 3_656
O2 O2 O2 60.93(17) 3_655 3_656
La1 O2 O2 100.4(4) . 3_656
O2 O2 O2 76.7(5) 2_556 3_656
O3 O2 O2 120.1(5) 4_665 3_656
O1 O2 O2 120.0(4) 2_655 3_656
O3 O2 O2 51.1(3) 5_666 3_656
O1 O2 O2 15.45(14) 2_656 3_656
O3 O2 O2 139.3(4) 5_665 3_656
O1 O2 O2 128.1(4) 1_565 3_656
Ga1 O2 O2 124.9(4) . 3_656
Nb O2 O2 124.9(4) . 3_656
O2 O2 O2 175.2(5) 2 3_656
Ga2 O2 O2 99.8(3) . 3_656
O3 O2 O2 102.9(4) 1_565 3_656
La1 O2 O2 48.20(10) 4_666 3_656
Ga3 O2 O2 77.7(3) 2_546 3_656
O3 O2 O2 63.4(3) 2_656 3_656
Ga3 O2 O2 71.6(2) 2_656 3_656
La1 O2 O2 21.72(14) 1_556 3_656
La1 O2 O2 87.6(3) 2_655 3_656
Ga3 O2 O2 160.8(4) 4_664 3_656
O3 O2 O2 82.5(3) 6_456 3_656
Ga3 O2 O2 49.0(2) . 3_656
La1 O2 O2 138.9(3) 2 3_656
O3 O2 O2 123.7(4) 2_655 3_656
Ga2 O2 O2 131.9(3) 2 3_656
O2 O2 O2 87.0(4) 5_666 3_656
O2 O2 O2 41.0(4) 5_656 3_656
O3 O2 O2 144.9(4) 6_455 3_656
O2 O2 O2 58.3(3) 6_556 3_656
Nb O2 O2 60.1(2) 1_556 3_656
Ga1 O2 O2 60.1(2) 1_556 3_656
O1 O2 O2 78.6(3) . 3_656
O3 O2 O2 105.9(3) 1_455 3_656
Ga2 O2 O2 58.8(2) 1_545 3_656
Ga3 O2 O2 98.1(3) 1_455 3_656
Ga3 O2 O2 92.9(2) 1_565 3_656
O2 O2 O2 150.93(17) 1_554 3_656
O2 O2 O2 29.07(17) 1_556 3_656
O2 O2 O2 143.8(4) 5_665 3_656
O2 O2 O2 101.5(3) 5_655 3_656
O3 O2 O2 73.4(3) 2_546 3_656
O3 O2 O2 35.8(3) 6_556 3_656
Ga2 O2 O2 162.4(3) 1_554 3_656
O2 O2 O2 111.6(4) 6 3_656
O2 O2 O2 97.7(4) 6_566 3_656
O2 O2 O2 56.1(3) 6_666 3_656
O3 O2 O2 66.2(3) 4_765 3_656
Nb O2 O2 107.6(3) 1_665 3_656
Ga1 O2 O2 107.6(3) 1_665 3_656
La1 O2 O2 29.62(16) 2_656 3_656
O3 O2 O2 123.7(4) 2_545 3_656
O3 O2 O2 92.8(3) 6 3_656
O3 O2 O2 87.8(3) 3_655 3_656
La1 O2 O2 79.37(18) 2_556 3_656
O3 O2 O2 40.1(2) 3_546 3_656
O3 O2 O2 65.4(3) . 3_656
O3 O2 O2 56.48(18) 4_666 3_656
O2 O2 O2 113.4(2) 3 3_656
O2 O2 O2 87.5(3) 4 3_656
O1 O2 O2 66.45(16) 1_566 3_656
O2 O2 O2 151.7(4) 6_565 3_656
O2 O2 O2 105.2(3) 6_665 3_656
Ga3 O2 O2 127.6(3) 2_545 3_656
O2 O2 O2 130.2(3) 4_664 3_656
O2 O2 O2 28.12(15) 4_666 3_656
O2 O2 O2 121.9(3) 3_654 3_656
Ga2 O2 La1 119.2(5) 2_556 1_565
Ga3 O2 La1 87.5(4) 4_665 1_565
La1 O2 La1 35.0(2) 4_665 1_565
O3 O2 La1 123.8(4) 3_545 1_565
O2 O2 La1 85.4(5) 4_665 1_565
O2 O2 La1 142.3(5) 3_655 1_565
La1 O2 La1 130.1(4) . 1_565
O2 O2 La1 63.5(4) 2_556 1_565
O3 O2 La1 70.1(3) 4_665 1_565
O1 O2 La1 89.9(3) 2_655 1_565
O3 O2 La1 120.0(4) 5_666 1_565
O1 O2 La1 116.6(4) 2_656 1_565
O3 O2 La1 91.5(3) 5_665 1_565
O1 O2 La1 12.50(13) 1_565 1_565
Ga1 O2 La1 91.6(2) . 1_565
Nb O2 La1 91.6(2) . 1_565
O2 O2 La1 46.8(2) 2 1_565
Ga2 O2 La1 35.01(13) . 1_565
O3 O2 La1 39.0(2) 1_565 1_565
La1 O2 La1 80.7(2) 4_666 1_565
Ga3 O2 La1 128.7(2) 2_546 1_565
O3 O2 La1 69.9(3) 2_656 1_565
Ga3 O2 La1 75.16(19) 2_656 1_565
La1 O2 La1 140.1(3) 1_556 1_565
La1 O2 La1 101.4(2) 2_655 1_565
Ga3 O2 La1 70.84(18) 4_664 1_565
O3 O2 La1 86.3(2) 6_456 1_565
Ga3 O2 La1 152.1(3) . 1_565
La1 O2 La1 44.47(11) 2 1_565
O3 O2 La1 51.8(2) 2_655 1_565
Ga2 O2 La1 83.8(2) 2 1_565
O2 O2 La1 41.5(2) 5_666 1_565
O2 O2 La1 168.8(5) 5_656 1_565
O3 O2 La1 69.42(19) 6_455 1_565
O2 O2 La1 149.22(14) 6_556 1_565
Nb O2 La1 108.1(2) 1_556 1_565
Ga1 O2 La1 108.1(2) 1_556 1_565
O1 O2 La1 152.9(4) . 1_565
O3 O2 La1 98.0(2) 1_455 1_565
Ga2 O2 La1 168.1(3) 1_545 1_565
Ga3 O2 La1 87.98(17) 1_455 1_565
Ga3 O2 La1 38.72(10) 1_565 1_565
O2 O2 La1 74.27(15) 1_554 1_565
O2 O2 La1 105.73(15) 1_556 1_565
O2 O2 La1 24.35(12) 5_665 1_565
O2 O2 La1 125.7(4) 5_655 1_565
O3 O2 La1 116.1(3) 2_546 1_565
O3 O2 La1 137.8(3) 6_556 1_565
Ga2 O2 La1 34.55(8) 1_554 1_565
O2 O2 La1 119.6(3) 6 1_565
O2 O2 La1 43.9(2) 6_566 1_565
O2 O2 La1 93.7(3) 6_666 1_565
O3 O2 La1 125.3(3) 4_765 1_565
Nb O2 La1 47.97(11) 1_665 1_565
Ga1 O2 La1 47.97(11) 1_665 1_565
La1 O2 La1 114.8(2) 2_656 1_565
O3 O2 La1 99.2(3) 2_545 1_565
O3 O2 La1 116.6(3) 6 1_565
O3 O2 La1 66.8(2) 3_655 1_565
La1 O2 La1 70.11(14) 2_556 1_565
O3 O2 La1 122.7(3) 3_546 1_565
O3 O2 La1 149.9(3) . 1_565
O3 O2 La1 94.3(2) 4_666 1_565
O2 O2 La1 70.6(2) 3 1_565
O2 O2 La1 128.1(2) 4 1_565
O1 O2 La1 67.8(2) 1_566 1_565
O2 O2 La1 28.35(18) 6_565 1_565
O2 O2 La1 79.8(3) 6_665 1_565
Ga3 O2 La1 102.3(2) 2_545 1_565
O2 O2 La1 74.0(3) 4_664 1_565
O2 O2 La1 101.4(3) 4_666 1_565
O2 O2 La1 98.47(19) 3_654 1_565
O2 O2 La1 128.4(3) 3_656 1_565
Ga2 O2 O3 124.6(5) 2_556 3_544
Ga3 O2 O3 101.8(5) 4_665 3_544
La1 O2 O3 74.8(4) 4_665 3_544
O3 O2 O3 55.1(3) 3_545 3_544
O2 O2 O3 112.55(16) 4_665 3_544
O2 O2 O3 88.3(3) 3_655 3_544
La1 O2 O3 40.4(2) . 3_544
O2 O2 O3 131.0(5) 2_556 3_544
O3 O2 O3 68.6(4) 4_665 3_544
O1 O2 O3 50.9(3) 2_655 3_544
O3 O2 O3 112.4(4) 5_666 3_544
O1 O2 O3 149.4(4) 2_656 3_544
O3 O2 O3 8.3(2) 5_665 3_544
O1 O2 O3 91.0(4) 1_565 3_544
Ga1 O2 O3 40.83(19) . 3_544
Nb O2 O3 40.83(19) . 3_544
O2 O2 O3 45.2(3) 2 3_544
Ga2 O2 O3 117.1(3) . 3_544
O3 O2 O3 111.2(4) 1_565 3_544
La1 O2 O3 169.1(3) 4_666 3_544
Ga3 O2 O3 75.5(2) 2_546 3_544
O3 O2 O3 149.3(4) 2_656 3_544
Ga3 O2 O3 128.4(3) 2_656 3_544
La1 O2 O3 123.3(3) 1_556 3_544
La1 O2 O3 84.2(2) 2_655 3_544
Ga3 O2 O3 21.14(13) 4_664 3_544
O3 O2 O3 102.2(3) 6_456 3_544
Ga3 O2 O3 96.3(3) . 3_544
La1 O2 O3 67.9(2) 2 3_544
O3 O2 O3 79.0(3) 2_655 3_544
Ga2 O2 O3 40.77(16) 2 3_544
O2 O2 O3 133.2(4) 5_666 3_544
O2 O2 O3 98.7(4) 5_656 3_544
O3 O2 O3 40.7(3) 6_455 3_544
O2 O2 O3 87.4(4) 6_556 3_544
Nb O2 O3 111.8(3) 1_556 3_544
Ga1 O2 O3 111.8(3) 1_556 3_544
O1 O2 O3 61.1(3) . 3_544
O3 O2 O3 61.9(2) 1_455 3_544
Ga2 O2 O3 81.4(2) 1_545 3_544
Ga3 O2 O3 80.8(2) 1_455 3_544
Ga3 O2 O3 125.6(3) 1_565 3_544
O2 O2 O3 27.42(16) 1_554 3_544
O2 O2 O3 152.58(16) 1_556 3_544
O2 O2 O3 74.1(3) 5_665 3_544
O2 O2 O3 42.8(3) 5_655 3_544
O3 O2 O3 89.6(3) 2_546 3_544
O3 O2 O3 115.3(3) 6_556 3_544
Ga2 O2 O3 57.71(19) 1_554 3_544
O2 O2 O3 28.6(2) 6 3_544
O2 O2 O3 114.8(3) 6_566 3_544
O2 O2 O3 131.6(4) 6_666 3_544
O3 O2 O3 92.5(2) 4_765 3_544
Nb O2 O3 100.0(3) 1_665 3_544
Ga1 O2 O3 100.0(3) 1_665 3_544
La1 O2 O3 140.0(3) 2_656 3_544
O3 O2 O3 32.5(2) 2_545 3_544
O3 O2 O3 64.9(2) 6 3_544
O3 O2 O3 112.4(3) 3_655 3_544
La1 O2 O3 120.6(2) 2_556 3_544
O3 O2 O3 121.6(3) 3_546 3_544
O3 O2 O3 79.6(3) . 3_544
O3 O2 O3 129.4(2) 4_666 3_544
O2 O2 O3 76.09(13) 3 3_544
O2 O2 O3 62.59(16) 4 3_544
O1 O2 O3 145.0(2) 1_566 3_544
O2 O2 O3 66.6(3) 6_565 3_544
O2 O2 O3 79.6(3) 6_665 3_544
Ga3 O2 O3 17.09(12) 2_545 3_544
O2 O2 O3 53.88(15) 4_664 3_544
O2 O2 O3 164.2(3) 4_666 3_544
O2 O2 O3 37.82(19) 3_654 3_544
O2 O2 O3 139.6(3) 3_656 3_544
La1 O2 O3 92.0(2) 1_565 3_544
Ga2 O2 O2 96.7(6) 2_556 3_665
Ga3 O2 O2 94.4(4) 4_665 3_665
La1 O2 O2 42.0(4) 4_665 3_665
O3 O2 O2 145.4(4) 3_545 3_665
O2 O2 O2 67.4(6) 4_665 3_665
O2 O2 O2 127.4(6) 3_655 3_665
La1 O2 O2 144.3(3) . 3_665
O2 O2 O2 59.1(3) 2_556 3_665
O3 O2 O2 89.1(3) 4_665 3_665
O1 O2 O2 94.1(3) 2_655 3_665
O3 O2 O2 117.7(4) 5_666 3_665
O1 O2 O2 94.0(3) 2_656 3_665
O3 O2 O2 113.5(3) 5_665 3_665
O1 O2 O2 32.02(12) 1_565 3_665
Ga1 O2 O2 114.6(2) . 3_665
Nb O2 O2 114.6(2) . 3_665
O2 O2 O2 68.1(3) 2 3_665
Ga2 O2 O2 34.16(11) . 3_665
O3 O2 O2 21.3(3) 1_565 3_665
La1 O2 O2 62.4(2) 4_666 3_665
Ga3 O2 O2 142.8(3) 2_546 3_665
O3 O2 O2 46.3(3) 2_656 3_665
Ga3 O2 O2 53.6(3) 2_656 3_665
La1 O2 O2 123.7(2) 1_556 3_665
La1 O2 O2 91.5(3) 2_655 3_665
Ga3 O2 O2 91.80(14) 4_664 3_665
O3 O2 O2 93.1(2) 6_456 3_665
Ga3 O2 O2 132.4(4) . 3_665
La1 O2 O2 66.23(11) 2 3_665
O3 O2 O2 50.4(3) 2_655 3_665
Ga2 O2 O2 92.6(2) 2 3_665
O2 O2 O2 25.3(4) 5_666 3_665
O2 O2 O2 145.4(4) 5_656 3_665
O3 O2 O2 92.89(19) 6_455 3_665
O2 O2 O2 153.0(3) 6_556 3_665
Nb O2 O2 108.47(15) 1_556 3_665
Ga1 O2 O2 108.47(15) 1_556 3_665
O1 O2 O2 169.5(3) . 3_665
O3 O2 O2 117.4(3) 1_455 3_665
Ga2 O2 O2 166.0(2) 1_545 3_665
Ga3 O2 O2 102.31(19) 1_455 3_665
Ga3 O2 O2 15.16(17) 1_565 3_665
O2 O2 O2 90.0 1_554 3_665
O2 O2 O2 90.0 1_556 3_665
O2 O2 O2 38.6(3) 5_665 3_665
O2 O2 O2 135.4(3) 5_655 3_665
O3 O2 O2 124.9(3) 2_546 3_665
O3 O2 O2 115.1(3) 6_556 3_665
Ga2 O2 O2 55.22(13) 1_554 3_665
O2 O2 O2 141.0(3) 6 3_665
O2 O2 O2 46.33(19) 6_566 3_665
O2 O2 O2 71.5(4) 6_666 3_665
O3 O2 O2 110.6(3) 4_765 3_665
Nb O2 O2 36.3(2) 1_665 3_665
Ga1 O2 O2 36.3(2) 1_665 3_665
La1 O2 O2 91.3(3) 2_656 3_665
O3 O2 O2 122.7(2) 2_545 3_665
O3 O2 O2 113.7(3) 6 3_665
O3 O2 O2 49.4(3) 3_655 3_665
La1 O2 O2 70.50(10) 2_556 3_665
O3 O2 O2 115.33(19) 3_546 3_665
O3 O2 O2 138.9(4) . 3_665
O3 O2 O2 89.56(15) 4_666 3_665
O2 O2 O2 87.6(3) 3 3_665
O2 O2 O2 147.6(3) 4 3_665
O1 O2 O2 57.12(14) 1_566 3_665
O2 O2 O2 51.9(2) 6_565 3_665
O2 O2 O2 73.6(4) 6_665 3_665
Ga3 O2 O2 124.92(13) 2_545 3_665
O2 O2 O2 79.3(3) 4_664 3_665
O2 O2 O2 79.3(3) 4_666 3_665
O2 O2 O2 107.2(2) 3_654 3_665
O2 O2 O2 107.2(2) 3_656 3_665
La1 O2 O2 23.58(11) 1_565 3_665
O3 O2 O2 112.49(16) 3_544 3_665
Ga2 O2 O2 146.4(5) 2_556 4_565
Ga3 O2 O2 45.3(4) 4_665 4_565
La1 O2 O2 75.3(2) 4_665 4_565
O3 O2 O2 86.2(4) 3_545 4_565
O2 O2 O2 127.4(6) 4_665 4_565
O2 O2 O2 172.6(6) 3_655 4_565
La1 O2 O2 123.7(4) . 4_565
O2 O2 O2 44.0(5) 2_556 4_565
O3 O2 O2 30.0(3) 4_665 4_565
O1 O2 O2 120.4(3) 2_655 4_565
O3 O2 O2 80.8(3) 5_666 4_565
O1 O2 O2 119.5(3) 2_656 4_565
O3 O2 O2 82.1(3) 5_665 4_565
O1 O2 O2 32.02(12) 1_565 4_565
Ga1 O2 O2 61.3(2) . 4_565
Nb O2 O2 61.3(2) . 4_565
O2 O2 O2 58.5(4) 2 4_565
Ga2 O2 O2 34.16(11) . 4_565
O3 O2 O2 80.6(2) 1_565 4_565
La1 O2 O2 80.87(14) 4_666 4_565
Ga3 O2 O2 84.9(3) 2_546 4_565
O3 O2 O2 94.7(3) 2_656 4_565
Ga3 O2 O2 112.0(3) 2_656 4_565
La1 O2 O2 112.3(2) 1_556 4_565
La1 O2 O2 144.8(3) 2_655 4_565
Ga3 O2 O2 73.21(17) 4_664 4_565
O3 O2 O2 44.2(2) 6_456 4_565
Ga3 O2 O2 161.8(3) . 4_565
La1 O2 O2 21.2(2) 2 4_565
O3 O2 O2 94.4(2) 2_655 4_565
Ga2 O2 O2 109.12(14) 2 4_565
O2 O2 O2 56.85(16) 5_666 4_565
O2 O2 O2 138.4(5) 5_656 4_565
O3 O2 O2 48.3(2) 6_455 4_565
O2 O2 O2 104.72(18) 6_556 4_565
Nb O2 O2 68.6(2) 1_556 4_565
Ga1 O2 O2 68.6(2) 1_556 4_565
O1 O2 O2 125.4(3) . 4_565
O3 O2 O2 57.6(3) 1_455 4_565
Ga2 O2 O2 124.9(3) 1_545 4_565
Ga3 O2 O2 43.66(19) 1_455 4_565
Ga3 O2 O2 71.02(15) 1_565 4_565
O2 O2 O2 90.0 1_554 4_565
O2 O2 O2 90.0 1_556 4_565
O2 O2 O2 61.80(15) 5_665 4_565
O2 O2 O2 130.3(4) 5_655 4_565
O3 O2 O2 71.7(3) 2_546 4_565
O3 O2 O2 154.2(2) 6_556 4_565
Ga2 O2 O2 55.22(13) 1_554 4_565
O2 O2 O2 102.82(15) 6 4_565
O2 O2 O2 27.1(3) 6_566 4_565
O2 O2 O2 127.0(4) 6_666 4_565
O3 O2 O2 169.8(3) 4_765 4_565
Nb O2 O2 92.26(19) 1_665 4_565
Ga1 O2 O2 92.26(19) 1_665 4_565
La1 O2 O2 131.79(19) 2_656 4_565
O3 O2 O2 72.7(3) 2_545 4_565
O3 O2 O2 148.4(2) 6 4_565
O3 O2 O2 109.2(3) 3_655 4_565
La1 O2 O2 39.44(14) 2_556 4_565
O3 O2 O2 88.0(2) 3_546 4_565
O3 O2 O2 160.5(4) . 4_565
O3 O2 O2 63.51(18) 4_666 4_565
O2 O2 O2 27.6(3) 3 4_565
O2 O2 O2 87.6(3) 4 4_565
O1 O2 O2 57.12(14) 1_566 4_565
O2 O2 O2 37.3(2) 6_565 4_565
O2 O2 O2 122.6(3) 6_665 4_565
Ga3 O2 O2 86.3(2) 2_545 4_565
O2 O2 O2 107.2(2) 4_664 4_565
O2 O2 O2 107.2(2) 4_666 4_565
O2 O2 O2 118.80(18) 3_654 4_565
O2 O2 O2 118.80(18) 3_656 4_565
La1 O2 O2 44.52(10) 1_565 4_565
O3 O2 O2 88.23(19) 3_544 4_565
O2 O2 O2 60.000(1) 3_665 4_565
Ga2 O2 O3 142.5(6) 2_556 4_664
Ga3 O2 O3 93.7(5) 4_665 4_664
La1 O2 O3 58.2(3) 4_665 4_664
O3 O2 O3 68.8(4) 3_545 4_664
O2 O2 O3 114.7(2) 4_665 4_664
O2 O2 O3 111.5(2) 3_655 4_664
La1 O2 O3 65.7(3) . 4_664
O2 O2 O3 110.6(6) 2_556 4_664
O3 O2 O3 55.3(3) 4_665 4_664
O1 O2 O3 60.3(3) 2_655 4_664
O3 O2 O3 118.2(5) 5_666 4_664
O1 O2 O3 174.0(4) 2_656 4_664
O3 O2 O3 24.0(2) 5_665 4_664
O1 O2 O3 65.8(3) 1_565 4_664
Ga1 O2 O3 41.0(2) . 4_664
Nb O2 O3 41.0(2) . 4_664
O2 O2 O3 21.6(2) 2 4_664
Ga2 O2 O3 92.2(3) . 4_664
O3 O2 O3 93.9(4) 1_565 4_664
La1 O2 O3 145.1(3) 4_666 4_664
Ga3 O2 O3 87.0(3) 2_546 4_664
O3 O2 O3 133.7(3) 2_656 4_664
Ga3 O2 O3 123.1(3) 2_656 4_664
La1 O2 O3 142.2(3) 1_556 4_664
La1 O2 O3 95.4(3) 2_655 4_664
Ga3 O2 O3 6.90(13) 4_664 4_664
O3 O2 O3 93.6(3) 6_456 4_664
Ga3 O2 O3 120.9(3) . 4_664
La1 O2 O3 45.36(18) 2 4_664
O3 O2 O3 69.6(2) 2_655 4_664
Ga2 O2 O3 47.84(18) 2 4_664
O2 O2 O3 108.2(3) 5_666 4_664
O2 O2 O3 123.4(4) 5_656 4_664
O3 O2 O3 26.0(3) 6_455 4_664
O2 O2 O3 105.0(4) 6_556 4_664
Nb O2 O3 112.1(3) 1_556 4_664
Ga1 O2 O3 112.1(3) 1_556 4_664
O1 O2 O3 85.3(3) . 4_664
O3 O2 O3 62.0(2) 1_455 4_664
Ga2 O2 O3 104.4(3) 1_545 4_664
Ga3 O2 O3 74.5(2) 1_455 4_664
Ga3 O2 O3 104.1(2) 1_565 4_664
O2 O2 O3 27.14(17) 1_554 4_664
O2 O2 O3 152.86(17) 1_556 4_664
O2 O2 O3 53.3(3) 5_665 4_664
O2 O2 O3 67.0(3) 5_655 4_664
O3 O2 O3 94.5(3) 2_546 4_664
O3 O2 O3 138.7(3) 6_556 4_664
Ga2 O2 O3 34.54(13) 1_554 4_664
O2 O2 O3 52.0(3) 6 4_664
O2 O2 O3 91.5(3) 6_566 4_664
O2 O2 O3 135.8(4) 6_666 4_664
O3 O2 O3 111.5(3) 4_765 4_664
Nb O2 O3 87.8(2) 1_665 4_664
Ga1 O2 O3 87.8(2) 1_665 4_664
La1 O2 O3 157.9(3) 2_656 4_664
O3 O2 O3 40.1(3) 2_545 4_664
O3 O2 O3 83.1(3) 6 4_664
O3 O2 O3 106.2(3) 3_655 4_664
La1 O2 O3 104.0(2) 2_556 4_664
O3 O2 O3 129.4(2) 3_546 4_664
O3 O2 O3 104.1(3) . 4_664
O3 O2 O3 122.2(3) 4_666 4_664
O2 O2 O3 62.87(17) 3 4_664
O2 O2 O3 76.21(15) 4 4_664
O1 O2 O3 123.1(2) 1_566 4_664
O2 O2 O3 41.3(2) 6_565 4_664
O2 O2 O3 82.3(3) 6_665 4_664
Ga3 O2 O3 35.39(13) 2_545 4_664
O2 O2 O3 54.95(17) 4_664 4_664
O2 O2 O3 168.9(4) 4_666 4_664
O2 O2 O3 53.15(19) 3_654 4_664
O2 O2 O3 162.9(3) 3_656 4_664
La1 O2 O3 67.56(16) 1_565 4_664
O3 O2 O3 25.28(19) 3_544 4_664
O2 O2 O3 89.61(13) 3_665 4_664
O2 O2 O3 66.52(17) 4_565 4_664
Ga2 O2 O3 62.3(5) 2_556 1_566
Ga3 O2 O3 80.9(5) 4_665 1_566
La1 O2 O3 92.0(4) 4_665 1_566
O3 O2 O3 135.5(5) 3_545 1_566
O2 O2 O3 64.3(3) 4_665 1_566
O2 O2 O3 100.6(3) 3_655 1_566
La1 O2 O3 151.1(3) . 1_566
O2 O2 O3 45.1(3) 2_556 1_566
O3 O2 O3 108.3(4) 4_665 1_566
O1 O2 O3 124.5(4) 2_655 1_566
O3 O2 O3 77.9(4) 5_666 1_566
O1 O2 O3 43.0(2) 2_656 1_566
O3 O2 O3 164.9(4) 5_665 1_566
O1 O2 O3 76.3(4) 1_565 1_566
Ga1 O2 O3 140.1(3) . 1_566
Nb O2 O3 140.1(3) . 1_566
O2 O2 O3 121.1(4) 2 1_566
Ga2 O2 O3 52.2(2) . 1_566
O3 O2 O3 56.1(2) 1_565 1_566
La1 O2 O3 12.64(13) 4_666 1_566
Ga3 O2 O3 115.3(3) 2_546 1_566
O3 O2 O3 21.7(2) 2_656 1_566
Ga3 O2 O3 45.89(19) 2_656 1_566
La1 O2 O3 70.6(2) 1_556 1_566
La1 O2 O3 95.5(3) 2_655 1_566
Ga3 O2 O3 145.1(3) 4_664 1_566
O3 O2 O3 80.2(3) 6_456 1_566
Ga3 O2 O3 94.7(3) . 1_566
La1 O2 O3 102.8(3) 2 1_566
O3 O2 O3 89.9(3) 2_655 1_566
Ga2 O2 O3 132.1(3) 2 1_566
O2 O2 O3 33.7(3) 5_666 1_566
O2 O2 O3 94.8(4) 5_656 1_566
O3 O2 O3 132.3(3) 6_455 1_566
O2 O2 O3 105.8(4) 6_556 1_566
Nb O2 O3 76.1(2) 1_556 1_566
Ga1 O2 O3 76.1(2) 1_556 1_566
O1 O2 O3 132.7(3) . 1_566
O3 O2 O3 122.0(3) 1_455 1_566
Ga2 O2 O3 112.6(3) 1_545 1_566
Ga3 O2 O3 101.2(3) 1_455 1_566
Ga3 O2 O3 40.58(17) 1_565 1_566
O2 O2 O3 140.58(16) 1_554 1_566
O2 O2 O3 39.42(16) 1_556 1_566
O2 O2 O3 91.9(3) 5_665 1_566
O2 O2 O3 145.6(4) 5_655 1_566
O3 O2 O3 99.0(3) 2_546 1_566
O3 O2 O3 74.9(2) 6_556 1_566
Ga2 O2 O3 108.4(3) 1_554 1_566
O2 O2 O3 165.4(4) 6 1_566
O2 O2 O3 56.9(3) 6_566 1_566
O2 O2 O3 48.7(3) 6_666 1_566
O3 O2 O3 93.1(2) 4_765 1_566
Nb O2 O3 68.8(2) 1_665 1_566
Ga1 O2 O3 68.8(2) 1_665 1_566
La1 O2 O3 48.65(17) 2_656 1_566
O3 O2 O3 151.1(3) 2_545 1_566
O3 O2 O3 118.3(3) 6 1_566
O3 O2 O3 59.9(2) 3_655 1_566
La1 O2 O3 57.94(18) 2_556 1_566
O3 O2 O3 69.9(3) 3_546 1_566
O3 O2 O3 110.8(3) . 1_566
O3 O2 O3 56.3(3) 4_666 1_566
O2 O2 O3 101.5(2) 3 1_566
O2 O2 O3 128.44(15) 4 1_566
O1 O2 O3 31.29(13) 1_566 1_566
O2 O2 O3 100.6(4) 6_565 1_566
O2 O2 O3 94.7(3) 6_665 1_566
Ga3 O2 O3 169.0(2) 2_545 1_566
O2 O2 O3 117.7(3) 4_664 1_566
O2 O2 O3 27.6(2) 4_666 1_566
O2 O2 O3 139.9(3) 3_654 1_566
O2 O2 O3 54.14(18) 3_656 1_566
La1 O2 O3 74.4(2) 1_565 1_566
O3 O2 O3 166.0(3) 3_544 1_566
O2 O2 O3 53.53(19) 3_665 1_566
O2 O2 O3 84.04(17) 4_565 1_566
O3 O2 O3 141.7(3) 4_664 1_566
Ga2 O2 O1 36.5(4) 2_556 1_665
Ga3 O2 O1 155.5(6) 4_665 1_665
La1 O2 O1 70.3(3) 4_665 1_665
O3 O2 O1 131.9(4) 3_545 1_665
O2 O2 O1 14.2(3) 4_665 1_665
O2 O2 O1 47.9(4) 3_655 1_665
La1 O2 O1 84.7(3) . 1_665
O2 O2 O1 120.7(3) 2_556 1_665
O3 O2 O1 162.0(5) 4_665 1_665
O1 O2 O1 51.9(4) 2_655 1_665
O3 O2 O1 127.8(4) 5_666 1_665
O1 O2 O1 66.1(4) 2_656 1_665
O3 O2 O1 110.6(4) 5_665 1_665
O1 O2 O1 107.9(3) 1_565 1_665
Ga1 O2 O1 142.8(4) . 1_665
Nb O2 O1 142.8(4) . 1_665
O2 O2 O1 102.5(3) 2 1_665
Ga2 O2 O1 111.0(3) . 1_665
O3 O2 O1 59.0(2) 1_565 1_665
La1 O2 O1 86.6(3) 4_666 1_665
Ga3 O2 O1 135.6(2) 2_546 1_665
O3 O2 O1 57.2(3) 2_656 1_665
Ga3 O2 O1 33.47(15) 2_656 1_665
La1 O2 O1 94.4(2) 1_556 1_665
La1 O2 O1 18.86(17) 2_655 1_665
Ga3 O2 O1 103.9(3) 4_664 1_665
O3 O2 O1 155.3(4) 6_456 1_665
Ga3 O2 O1 56.61(15) . 1_665
La1 O2 O1 135.6(3) 2 1_665
O3 O2 O1 51.0(2) 2_655 1_665
Ga2 O2 O1 63.6(2) 2 1_665
O2 O2 O1 89.9(4) 5_666 1_665
O2 O2 O1 79.1(3) 5_656 1_665
O3 O2 O1 135.9(4) 6_455 1_665
O2 O2 O1 114.63(13) 6_556 1_665
Nb O2 O1 137.0(3) 1_556 1_665
Ga1 O2 O1 137.0(3) 1_556 1_665
O1 O2 O1 93.06(18) . 1_665
O3 O2 O1 159.4(3) 1_455 1_665
Ga2 O2 O1 95.49(18) 1_545 1_665
Ga3 O2 O1 175.1(3) 1_455 1_665
Ga3 O2 O1 71.15(17) 1_565 1_665
O2 O2 O1 83.3(2) 1_554 1_665
O2 O2 O1 96.7(2) 1_556 1_665
O2 O2 O1 83.4(3) 5_665 1_665
O2 O2 O1 73.9(3) 5_655 1_665
O3 O2 O1 145.9(3) 2_546 1_665
O3 O2 O1 49.3(2) 6_556 1_665
Ga2 O2 O1 97.8(2) 1_554 1_665
O2 O2 O1 104.7(2) 6 1_665
O2 O2 O1 122.5(4) 6_566 1_665
O2 O2 O1 29.3(3) 6_666 1_665
O3 O2 O1 30.67(14) 4_765 1_665
Nb O2 O1 47.61(11) 1_665 1_665
Ga1 O2 O1 47.61(11) 1_665 1_665
La1 O2 O1 48.7(2) 2_656 1_665
O3 O2 O1 132.3(3) 2_545 1_665
O3 O2 O1 43.39(17) 6 1_665
O3 O2 O1 30.67(14) 3_655 1_665
La1 O2 O1 134.4(3) 2_556 1_665
O3 O2 O1 117.0(3) 3_546 1_665
O3 O2 O1 58.93(15) . 1_665
O3 O2 O1 126.7(3) 4_666 1_665
O2 O2 O1 165.9(3) 3 1_665
O2 O2 O1 132.1(3) 4 1_665
O1 O2 O1 107.7(3) 1_566 1_665
O2 O2 O1 112.2(3) 6_565 1_665
O2 O2 O1 28.2(2) 6_665 1_665
Ga3 O2 O1 114.3(2) 2_545 1_665
O2 O2 O1 55.0(3) 4_664 1_665
O2 O2 O1 68.3(3) 4_666 1_665
O2 O2 O1 64.7(2) 3_654 1_665
O2 O2 O1 77.1(3) 3_656 1_665
La1 O2 O1 95.57(19) 1_565 1_665
O3 O2 O1 102.3(3) 3_544 1_665
O2 O2 O1 80.0(3) 3_665 1_665
O2 O2 O1 139.5(3) 4_565 1_665
O3 O2 O1 109.9(3) 4_664 1_665
O3 O2 O1 76.6(2) 1_566 1_665
Ga3 O3 Nb 113.5(5) . 1_655
Ga3 O3 Ga1 113.5(5) . 1_655
Nb O3 Ga1 0.0 1_655 1_655
Ga3 O3 La1 137.8(6) . 4_655
Nb O3 La1 104.0(5) 1_655 4_655
Ga1 O3 La1 104.0(5) 1_655 4_655
Ga3 O3 Ga3 95.9(6) . 2_646
Nb O3 Ga3 87.4(4) 1_655 2_646
Ga1 O3 Ga3 87.4(4) 1_655 2_646
La1 O3 Ga3 104.6(4) 4_655 2_646
Ga3 O3 O3 155.1(8) . 2_645
Nb O3 O3 47.6(3) 1_655 2_645
Ga1 O3 O3 47.6(3) 1_655 2_645
La1 O3 O3 56.4(3) 4_655 2_645
Ga3 O3 O3 98.8(6) 2_646 2_645
Ga3 O3 O3 63.5(5) . 2_646
Nb O3 O3 119.3(5) 1_655 2_646
Ga1 O3 O3 119.3(5) 1_655 2_646
La1 O3 O3 113.7(4) 4_655 2_646
Ga3 O3 O3 39.0(3) 2_646 2_646
O3 O3 O3 136.5(10) 2_645 2_646
Ga3 O3 O3 66.4(5) . 4_765
Nb O3 O3 47.4(3) 1_655 4_765
Ga1 O3 O3 47.4(3) 1_655 4_765
La1 O3 O3 149.0(3) 4_655 4_765
Ga3 O3 O3 87.8(3) 2_646 4_765
O3 O3 O3 94.13(9) 2_645 4_765
O3 O3 O3 93.94(9) 2_646 4_765
Ga3 O3 O3 106.7(3) . 3_645
Nb O3 O3 47.4(3) 1_655 3_645
Ga1 O3 O3 47.4(3) 1_655 3_645
La1 O3 O3 112.8(6) 4_655 3_645
Ga3 O3 O3 40.1(4) 2_646 3_645
O3 O3 O3 73.4(5) 2_645 3_645
O3 O3 O3 74.1(5) 2_646 3_645
O3 O3 O3 60.0 4_765 3_645
Ga3 O3 O2 126.1(7) . 4_655
Nb O3 O2 95.3(5) 1_655 4_655
Ga1 O3 O2 95.3(5) 1_655 4_655
La1 O3 O2 65.8(4) 4_655 4_655
Ga3 O3 O2 38.8(3) 2_646 4_655
O3 O3 O2 76.6(6) 2_645 4_655
O3 O3 O2 62.7(5) 2_646 4_655
O3 O3 O2 120.6(6) 4_765 4_655
O3 O3 O2 61.1(6) 3_645 4_655
Ga3 O3 O2 39.2(4) . 3_655
Nb O3 O2 96.4(5) 1_655 3_655
Ga1 O3 O2 96.4(5) 1_655 3_655
La1 O3 O2 120.5(5) 4_655 3_655
Ga3 O3 O2 132.0(5) 2_646 3_655
O3 O3 O2 118.8(8) 2_645 3_655
O3 O3 O2 102.7(6) 2_646 3_655
O3 O3 O2 62.4(5) 4_765 3_655
O3 O3 O2 121.8(5) 3_645 3_655
O2 O3 O2 164.6(8) 4_655 3_655
Ga3 O3 O2 36.1(3) . 5_656
Nb O3 O2 149.3(5) 1_655 5_656
Ga1 O3 O2 149.3(5) 1_655 5_656
La1 O3 O2 103.6(4) 4_655 5_656
Ga3 O3 O2 98.6(6) 2_646 5_656
O3 O3 O2 156.4(6) 2_645 5_656
O3 O3 O2 59.6(5) 2_646 5_656
O3 O3 O2 102.4(4) 4_765 5_656
O3 O3 O2 129.7(4) 3_645 5_656
O2 O3 O2 108.2(5) 4_655 5_656
O2 O3 O2 57.5(6) 3_655 5_656
Ga3 O3 O1 87.2(5) . .
Nb O3 O1 132.5(6) 1_655 .
Ga1 O3 O1 132.5(6) 1_655 .
La1 O3 O1 52.3(3) 4_655 .
Ga3 O3 O1 134.5(4) 2_646 .
O3 O3 O1 96.6(5) 2_645 .
O3 O3 O1 108.2(5) 2_646 .
O3 O3 O1 133.4(6) 4_765 .
O3 O3 O1 164.9(6) 3_645 .
O2 O3 O1 106.1(4) 4_655 .
O2 O3 O1 72.8(4) 3_655 .
O2 O3 O1 59.8(5) 5_656 .
Ga3 O3 O3 101.6(5) . 6
Nb O3 O3 36.2(4) 1_655 6
Ga1 O3 O3 36.2(4) 1_655 6
La1 O3 O3 97.4(6) 4_655 6
Ga3 O3 O3 123.2(2) 2_646 6
O3 O3 O3 53.5(6) 2_645 6
O3 O3 O3 146.6(3) 2_646 6
O3 O3 O3 53.1(4) 4_765 6
O3 O3 O3 83.1(3) 3_645 6
O2 O3 O3 125.6(5) 4_655 6
O2 O3 O3 69.0(4) 3_655 6
O2 O3 O3 126.1(4) 5_656 6
O1 O3 O3 100.2(4) . 6
Ga3 O3 O3 23.7(4) . 6_556
Nb O3 O3 100.2(4) 1_655 6_556
Ga1 O3 O3 100.2(4) 1_655 6_556
La1 O3 O3 155.8(6) 4_655 6_556
Ga3 O3 O3 75.5(4) 2_646 6_556
O3 O3 O3 147.8(3) 2_645 6_556
O3 O3 O3 51.4(5) 2_646 6_556
O3 O3 O3 54.5(5) 4_765 6_556
O3 O3 O3 83.3(3) 3_645 6_556
O2 O3 O3 111.3(6) 4_655 6_556
O2 O3 O3 56.7(4) 3_655 6_556
O2 O3 O3 53.3(4) 5_656 6_556
O1 O3 O3 110.1(4) . 6_556
O3 O3 O3 102.7(5) 6 6_556
Ga3 O3 O2 112.2(6) . 5_655
Nb O3 O2 79.2(5) 1_655 5_655
Ga1 O3 O2 79.2(5) 1_655 5_655
La1 O3 O2 56.0(3) 4_655 5_655
Ga3 O3 O2 151.8(5) 2_646 5_655
O3 O3 O2 54.1(6) 2_645 5_655
O3 O3 O2 161.5(4) 2_646 5_655
O3 O3 O2 100.6(4) 4_765 5_655
O3 O3 O2 123.2(3) 3_645 5_655
O2 O3 O2 117.5(5) 4_655 5_655
O2 O3 O2 74.6(5) 3_655 5_655
O2 O3 O2 105.6(5) 5_656 5_655
O1 O3 O2 53.3(4) . 5_655
O3 O3 O2 50.2(4) 6 5_655
O3 O3 O2 131.1(4) 6_556 5_655
Ga3 O3 Ga2 65.2(3) . 1_545
Nb O3 Ga2 160.4(6) 1_655 1_545
Ga1 O3 Ga2 160.4(6) 1_655 1_545
La1 O3 Ga2 72.9(3) 4_655 1_545
Ga3 O3 Ga2 112.2(4) 2_646 1_545
O3 O3 Ga2 125.8(4) 2_645 1_545
O3 O3 Ga2 78.5(4) 2_646 1_545
O3 O3 Ga2 128.9(5) 4_765 1_545
O3 O3 Ga2 152.0(4) 3_645 1_545
O2 O3 Ga2 100.7(4) 4_655 1_545
O2 O3 Ga2 70.2(4) 3_655 1_545
O2 O3 Ga2 31.3(3) 5_656 1_545
O1 O3 Ga2 31.1(4) . 1_545
O3 O3 Ga2 124.3(2) 6 1_545
O3 O3 Ga2 84.5(3) 6_556 1_545
O2 O3 Ga2 83.4(3) 5_655 1_545
Ga3 O3 Ga3 64.2(3) . 4_765
Nb O3 Ga3 60.4(3) 1_655 4_765
Ga1 O3 Ga3 60.4(3) 1_655 4_765
La1 O3 Ga3 157.4(5) 4_655 4_765
Ga3 O3 Ga3 61.0(2) 2_646 4_765
O3 O3 Ga3 106.2(2) 2_645 4_765
O3 O3 Ga3 67.4(2) 2_646 4_765
O3 O3 Ga3 28.35(19) 4_765 4_765
O3 O3 Ga3 44.8(2) 3_645 4_765
O2 O3 Ga3 97.8(4) 4_655 4_765
O2 O3 Ga3 79.5(3) 3_655 4_765
O2 O3 Ga3 96.2(4) 5_656 4_765
O1 O3 Ga3 150.3(4) . 4_765
O3 O3 Ga3 79.2(3) 6 4_765
O3 O3 Ga3 43.0(2) 6_556 4_765
O2 O3 Ga3 128.6(4) 5_655 4_765
Ga2 O3 Ga3 127.5(4) 1_545 4_765
Ga3 O3 O2 116.1(5) . 1_545
Nb O3 O2 129.4(5) 1_655 1_545
Ga1 O3 O2 129.4(5) 1_655 1_545
La1 O3 O2 37.4(3) 4_655 1_545
Ga3 O3 O2 78.8(3) 2_646 1_545
O3 O3 O2 86.5(3) 2_645 1_545
O3 O3 O2 76.6(3) 2_646 1_545
O3 O3 O2 166.5(6) 4_765 1_545
O3 O3 O2 107.5(6) 3_645 1_545
O2 O3 O2 46.5(4) 4_655 1_545
O2 O3 O2 128.7(5) 3_655 1_545
O2 O3 O2 81.3(3) 5_656 1_545
O1 O3 O2 59.8(2) . 1_545
O3 O3 O2 134.6(6) 6 1_545
O3 O3 O2 122.1(6) 6_556 1_545
O2 O3 O2 90.7(3) 5_655 1_545
Ga2 O3 O2 59.3(2) 1_545 1_545
Ga3 O3 O2 139.0(4) 4_765 1_545
Ga3 O3 La1 73.7(4) . .
Nb O3 La1 101.3(5) 1_655 .
Ga1 O3 La1 101.3(5) 1_655 .
La1 O3 La1 80.9(3) 4_655 .
Ga3 O3 La1 168.4(5) 2_646 .
O3 O3 La1 92.7(6) 2_645 .
O3 O3 La1 129.4(6) 2_646 .
O3 O3 La1 92.5(5) 4_765 .
O3 O3 La1 147.1(4) 3_645 .
O2 O3 La1 145.5(4) 4_655 .
O2 O3 La1 40.1(3) 3_655 .
O2 O3 La1 70.1(4) 5_656 .
O1 O3 La1 41.84(18) . .
O3 O3 La1 65.14(18) 6 .
O3 O3 La1 95.3(2) 6_556 .
O2 O3 La1 39.2(3) 5_655 .
Ga2 O3 La1 59.2(2) 1_545 .
Ga3 O3 La1 116.7(3) 4_765 .
O2 O3 La1 101.0(3) 1_545 .
Ga3 O3 Ga2 115.0(5) . 2_546
Nb O3 Ga2 118.3(5) 1_655 2_546
Ga1 O3 Ga2 118.3(5) 1_655 2_546
La1 O3 Ga2 57.5(2) 4_655 2_546
Ga3 O3 Ga2 52.4(2) 2_646 2_546
O3 O3 Ga2 89.9(5) 2_645 2_546
O3 O3 Ga2 58.4(3) 2_646 2_546
O3 O3 Ga2 140.1(5) 4_765 2_546
O3 O3 Ga2 83.5(5) 3_645 2_546
O2 O3 Ga2 23.7(3) 4_655 2_546
O2 O3 Ga2 145.1(5) 3_655 2_546
O2 O3 Ga2 88.1(4) 5_656 2_546
O1 O3 Ga2 85.3(2) . 2_546
O3 O3 Ga2 143.3(5) 6 2_546
O3 O3 Ga2 109.5(5) 6_556 2_546
O2 O3 Ga2 113.5(3) 5_655 2_546
Ga2 O3 Ga2 77.0(2) 1_545 2_546
Ga3 O3 Ga2 113.1(4) 4_765 2_546
O2 O3 Ga2 26.41(18) 1_545 2_546
La1 O3 Ga2 127.0(3) . 2_546
Ga3 O3 O3 120.5(4) . 5_765
Nb O3 O3 8.5(3) 1_655 5_765
Ga1 O3 O3 8.5(3) 1_655 5_765
La1 O3 O3 98.9(5) 4_655 5_765
Ga3 O3 O3 82.0(3) 2_646 5_765
O3 O3 O3 43.1(3) 2_645 5_765
O3 O3 O3 116.6(5) 2_646 5_765
O3 O3 O3 54.1(4) 4_765 5_765
O3 O3 O3 42.8(3) 3_645 5_765
O2 O3 O3 87.0(3) 4_655 5_765
O2 O3 O3 104.9(4) 3_655 5_765
O2 O3 O3 156.5(4) 5_656 5_765
O1 O3 O3 134.2(6) . 5_765
O3 O3 O3 42.8(3) 6 5_765
O3 O3 O3 105.0(3) 6_556 5_765
O2 O3 O3 81.5(5) 5_655 5_765
Ga2 O3 O3 164.9(6) 1_545 5_765
Ga3 O3 O3 63.3(3) 4_765 5_765
O2 O3 O3 121.5(3) 1_545 5_765
La1 O3 O3 107.5(4) . 5_765
Ga2 O3 O3 109.83(17) 2_546 5_765
Ga3 O3 O3 65.2(5) . 5_766
Nb O3 O3 79.8(4) 1_655 5_766
Ga1 O3 O3 79.8(4) 1_655 5_766
La1 O3 O3 143.3(3) 4_655 5_766
Ga3 O3 O3 38.6(2) 2_646 5_766
O3 O3 O3 117.3(5) 2_645 5_766
O3 O3 O3 41.9(3) 2_646 5_766
O3 O3 O3 55.0(4) 4_765 5_766
O3 O3 O3 44.1(3) 3_645 5_766
O2 O3 O3 77.5(3) 4_655 5_766
O2 O3 O3 94.8(4) 3_655 5_766
O2 O3 O3 86.2(5) 5_656 5_766
O1 O3 O3 145.5(6) . 5_766
O3 O3 O3 105.2(3) 6 5_766
O3 O3 O3 41.7(3) 6_556 5_766
O2 O3 O3 155.2(5) 5_655 5_766
Ga2 O3 O3 114.6(5) 1_545 5_766
Ga3 O3 O3 26.8(2) 4_765 5_766
O2 O3 O3 112.9(4) 1_545 5_766
La1 O3 O3 135.0(2) . 5_766
Ga2 O3 O3 88.1(2) 2_546 5_766
O3 O3 O3 79.7(4) 5_765 5_766
Ga3 O3 Ga3 117.9(5) . 1_554
Nb O3 Ga3 52.0(3) 1_655 1_554
Ga1 O3 Ga3 52.0(3) 1_655 1_554
La1 O3 Ga3 71.4(3) 4_655 1_554
Ga3 O3 Ga3 134.1(4) 2_646 1_554
O3 O3 Ga3 39.6(5) 2_645 1_554
O3 O3 Ga3 171.3(4) 2_646 1_554
O3 O3 Ga3 79.5(2) 4_765 1_554
O3 O3 Ga3 97.51(13) 3_645 1_554
O2 O3 Ga3 115.7(4) 4_655 1_554
O2 O3 Ga3 79.4(4) 3_655 1_554
O2 O3 Ga3 127.2(5) 5_656 1_554
O1 O3 Ga3 80.5(4) . 1_554
O3 O3 Ga3 26.4(3) 6 1_554
O3 O3 Ga3 126.3(5) 6_556 1_554
O2 O3 Ga3 27.2(2) 5_655 1_554
Ga2 O3 Ga3 110.0(3) 1_545 1_554
Ga3 O3 Ga3 105.1(3) 4_765 1_554
O2 O3 Ga3 108.8(3) 1_545 1_554
La1 O3 Ga3 57.2(2) . 1_554
Ga2 O3 Ga3 124.0(3) 2_546 1_554
O3 O3 Ga3 54.9(3) 5_765 1_554
O3 O3 Ga3 129.9(4) 5_766 1_554
Ga3 O3 Nb 46.0(4) . 1_656
Nb O3 Nb 106.6(4) 1_655 1_656
Ga1 O3 Nb 106.6(4) 1_655 1_656
La1 O3 Nb 138.1(4) 4_655 1_656
Ga3 O3 Nb 49.9(2) 2_646 1_656
O3 O3 Nb 144.3(6) 2_645 1_656
O3 O3 Nb 24.7(2) 2_646 1_656
O3 O3 Nb 71.10(12) 4_765 1_656
O3 O3 Nb 71.10(12) 3_645 1_656
O2 O3 Nb 83.4(4) 4_655 1_656
O2 O3 Nb 83.8(4) 3_655 1_656
O2 O3 Nb 58.6(4) 5_656 1_656
O1 O3 Nb 117.4(5) . 1_656
O3 O3 Nb 124.1(4) 6 1_656
O3 O3 Nb 28.1(3) 6_556 1_656
O2 O3 Nb 158.2(4) 5_655 1_656
Ga2 O3 Nb 86.5(3) 1_545 1_656
Ga3 O3 Nb 47.51(15) 4_765 1_656
O2 O3 Nb 100.7(3) 1_545 1_656
La1 O3 Nb 119.5(3) . 1_656
Ga2 O3 Nb 82.8(3) 2_546 1_656
O3 O3 Nb 107.4(4) 5_765 1_656
O3 O3 Nb 28.1(2) 5_766 1_656
Ga3 O3 Nb 150.4(3) 1_554 1_656
Ga3 O3 Ga1 46.0(4) . 1_656
Nb O3 Ga1 106.6(4) 1_655 1_656
Ga1 O3 Ga1 106.6(4) 1_655 1_656
La1 O3 Ga1 138.1(4) 4_655 1_656
Ga3 O3 Ga1 49.9(2) 2_646 1_656
O3 O3 Ga1 144.3(6) 2_645 1_656
O3 O3 Ga1 24.7(2) 2_646 1_656
O3 O3 Ga1 71.10(12) 4_765 1_656
O3 O3 Ga1 71.10(12) 3_645 1_656
O2 O3 Ga1 83.4(4) 4_655 1_656
O2 O3 Ga1 83.8(4) 3_655 1_656
O2 O3 Ga1 58.6(4) 5_656 1_656
O1 O3 Ga1 117.4(5) . 1_656
O3 O3 Ga1 124.1(4) 6 1_656
O3 O3 Ga1 28.1(3) 6_556 1_656
O2 O3 Ga1 158.2(4) 5_655 1_656
Ga2 O3 Ga1 86.5(3) 1_545 1_656
Ga3 O3 Ga1 47.51(15) 4_765 1_656
O2 O3 Ga1 100.7(3) 1_545 1_656
La1 O3 Ga1 119.5(3) . 1_656
Ga2 O3 Ga1 82.8(3) 2_546 1_656
O3 O3 Ga1 107.4(4) 5_765 1_656
O3 O3 Ga1 28.1(2) 5_766 1_656
Ga3 O3 Ga1 150.4(3) 1_554 1_656
Nb O3 Ga1 0.0 1_656 1_656
Ga3 O3 O2 77.4(4) . 2_546
Nb O3 O2 169.0(5) 1_655 2_546
Ga1 O3 O2 169.0(5) 1_655 2_546
La1 O3 O2 66.2(3) 4_655 2_546
Ga3 O3 O2 90.2(4) 2_646 2_546
O3 O3 O2 122.4(3) 2_645 2_546
O3 O3 O2 63.4(3) 2_646 2_546
O3 O3 O2 143.3(4) 4_765 2_546
O3 O3 O2 130.1(5) 3_645 2_546
O2 O3 O2 76.2(3) 4_655 2_546
O2 O3 O2 93.2(4) 3_655 2_546
O2 O3 O2 41.7(4) 5_656 2_546
O1 O3 O2 46.2(4) . 2_546
O3 O3 O2 146.2(3) 6 2_546
O3 O3 O2 89.6(5) 6_556 2_546
O2 O3 O2 98.2(3) 5_655 2_546
Ga2 O3 O2 24.78(18) 1_545 2_546
Ga3 O3 O2 127.1(4) 4_765 2_546
O2 O3 O2 39.7(4) 1_545 2_546
La1 O3 O2 82.6(3) . 2_546
Ga2 O3 O2 52.7(2) 2_546 2_546
O3 O3 O2 161.0(3) 5_765 2_546
O3 O3 O2 104.8(5) 5_766 2_546
Ga3 O3 O2 125.1(4) 1_554 2_546
Nb O3 O2 79.7(3) 1_656 2_546
Ga1 O3 O2 79.7(3) 1_656 2_546
Ga3 O3 La1 64.5(4) . 4_656
Nb O3 La1 149.2(6) 1_655 4_656
Ga1 O3 La1 149.2(6) 1_655 4_656
La1 O3 La1 92.5(3) 4_655 4_656
Ga3 O3 La1 63.1(3) 2_646 4_656
O3 O3 La1 140.4(5) 2_645 4_656
O3 O3 La1 30.39(19) 2_646 4_656
O3 O3 La1 118.27(13) 4_765 4_656
O3 O3 La1 102.4(3) 3_645 4_656
O2 O3 La1 67.8(4) 4_655 4_656
O2 O3 La1 97.3(4) 3_655 4_656
O2 O3 La1 40.9(3) 5_656 4_656
O1 O3 La1 78.0(4) . 4_656
O3 O3 La1 165.9(4) 6 4_656
O3 O3 La1 65.6(4) 6_556 4_656
O2 O3 La1 131.1(4) 5_655 4_656
Ga2 O3 La1 49.66(17) 1_545 4_656
Ga3 O3 La1 95.4(3) 4_765 4_656
O2 O3 La1 56.6(3) 1_545 4_656
La1 O3 La1 106.9(3) . 4_656
Ga2 O3 La1 50.82(16) 2_546 4_656
O3 O3 La1 145.0(5) 5_765 4_656
O3 O3 La1 71.7(3) 5_766 4_656
Ga3 O3 La1 158.2(3) 1_554 4_656
Nb O3 La1 48.09(15) 1_656 4_656
Ga1 O3 La1 48.09(15) 1_656 4_656
O2 O3 La1 33.1(2) 2_546 4_656
Ga3 O3 La1 67.9(3) . 2_655
Nb O3 La1 54.0(3) 1_655 2_655
Ga1 O3 La1 54.0(3) 1_655 2_655
La1 O3 La1 127.0(5) 4_655 2_655
Ga3 O3 La1 119.3(3) 2_646 2_655
O3 O3 La1 87.4(4) 2_645 2_655
O3 O3 La1 119.0(3) 2_646 2_655
O3 O3 La1 31.6(3) 4_765 2_655
O3 O3 La1 87.2(3) 3_645 2_655
O2 O3 La1 147.3(4) 4_655 2_655
O2 O3 La1 42.4(3) 3_655 2_655
O2 O3 La1 97.9(4) 5_656 2_655
O1 O3 La1 103.9(3) . 2_655
O3 O3 La1 34.3(2) 6 2_655
O3 O3 La1 69.3(3) 6_556 2_655
O2 O3 La1 71.8(3) 5_655 2_655
Ga2 O3 La1 111.8(3) 1_545 2_655
Ga3 O3 La1 59.34(14) 4_765 2_655
O2 O3 La1 161.6(4) 1_545 2_655
La1 O3 La1 62.07(19) . 2_655
Ga2 O3 La1 170.7(3) 2_546 2_655
O3 O3 La1 62.51(16) 5_765 2_655
O3 O3 La1 85.3(2) 5_766 2_655
Ga3 O3 La1 57.14(17) 1_554 2_655
Nb O3 La1 94.3(2) 1_656 2_655
Ga1 O3 La1 94.3(2) 1_656 2_655
O2 O3 La1 135.6(4) 2_546 2_655
La1 O3 La1 132.2(3) 4_656 2_655
Ga3 O3 O1 157.7(6) . 2_645
Nb O3 O1 88.2(4) 1_655 2_645
Ga1 O3 O1 88.2(4) 1_655 2_645
La1 O3 O1 29.11(17) 4_655 2_645
Ga3 O3 O1 79.7(3) 2_646 2_645
O3 O3 O1 46.2(3) 2_645 2_645
O3 O3 O1 102.4(6) 2_646 2_645
O3 O3 O1 134.5(4) 4_765 2_645
O3 O3 O1 84.1(5) 3_645 2_645
O2 O3 O1 42.2(4) 4_655 2_645
O2 O3 O1 148.1(5) 3_655 2_645
O2 O3 O1 122.5(4) 5_656 2_645
O1 O3 O1 80.9(2) . 2_645
O3 O3 O1 99.0(6) 6 2_645
O3 O3 O1 153.3(6) 6_556 2_645
O2 O3 O1 75.3(4) 5_655 2_645
Ga2 O3 O1 96.0(2) 1_545 2_645
Ga3 O3 O1 128.8(3) 4_765 2_645
O2 O3 O1 41.6(3) 1_545 2_645
La1 O3 O1 108.0(3) . 2_645
Ga2 O3 O1 45.6(3) 2_546 2_645
O3 O3 O1 80.8(3) 5_765 2_645
O3 O3 O1 117.1(3) 5_766 2_645
Ga3 O3 O1 78.7(3) 1_554 2_645
Nb O3 O1 125.2(4) 1_656 2_645
Ga1 O3 O1 125.2(4) 1_656 2_645
O2 O3 O1 80.8(3) 2_546 2_645
La1 O3 O1 94.5(3) 4_656 2_645
La1 O3 O1 133.3(4) 2_655 2_645
Ga3 O3 O2 96.2(6) . 6_656
Nb O3 O2 88.1(4) 1_655 6_656
Ga1 O3 O2 88.1(4) 1_655 6_656
La1 O3 O2 103.9(4) 4_655 6_656
Ga3 O3 O2 0.9(2) 2_646 6_656
O3 O3 O2 98.8(6) 2_645 6_656
O3 O3 O2 38.8(4) 2_646 6_656
O3 O3 O2 88.7(4) 4_765 6_656
O3 O3 O2 40.9(3) 3_645 6_656
O2 O3 O2 38.1(4) 4_655 6_656
O2 O3 O2 132.5(5) 3_655 6_656
O2 O3 O2 98.3(6) 5_656 6_656
O1 O3 O2 133.7(4) . 6_656
O3 O3 O2 123.9(2) 6 6_656
O3 O3 O2 76.0(4) 6_556 6_656
O2 O3 O2 151.6(5) 5_655 6_656
Ga2 O3 O2 111.5(4) 1_545 6_656
Ga3 O3 O2 61.9(3) 4_765 6_656
O2 O3 O2 77.9(3) 1_545 6_656
La1 O3 O2 168.3(4) . 6_656
Ga2 O3 O2 51.5(2) 2_546 6_656
O3 O3 O2 82.5(3) 5_765 6_656
O3 O3 O2 39.4(2) 5_766 6_656
Ga3 O3 O2 134.4(3) 1_554 6_656
Nb O3 O2 50.2(3) 1_656 6_656
Ga1 O3 O2 50.2(3) 1_656 6_656
O2 O3 O2 89.4(4) 2_546 6_656
La1 O3 O2 62.6(3) 4_656 6_656
La1 O3 O2 120.2(3) 2_655 6_656
O1 O3 O2 79.1(3) 2_645 6_656
Ga3 O3 Ga3 154.0(5) . 2_645
Nb O3 Ga3 41.4(3) 1_655 2_645
Ga1 O3 Ga3 41.4(3) 1_655 2_645
La1 O3 Ga3 63.5(3) 4_655 2_645
Ga3 O3 Ga3 90.2(3) 2_646 2_645
O3 O3 Ga3 10.0(3) 2_645 2_645
O3 O3 Ga3 128.8(6) 2_646 2_645
O3 O3 Ga3 88.7(2) 4_765 2_645
O3 O3 Ga3 63.4(3) 3_645 2_645
O2 O3 Ga3 72.2(4) 4_655 2_645
O2 O3 Ga3 123.1(5) 3_655 2_645
O2 O3 Ga3 166.0(5) 5_656 2_645
O1 O3 Ga3 106.3(4) . 2_645
O3 O3 Ga3 54.8(3) 6 2_645
O3 O3 Ga3 140.2(3) 6_556 2_645
O2 O3 Ga3 63.4(3) 5_655 2_645
Ga2 O3 Ga3 134.9(3) 1_545 2_645
Ga3 O3 Ga3 97.6(2) 4_765 2_645
O2 O3 Ga3 89.8(3) 1_545 2_645
La1 O3 Ga3 101.4(3) . 2_645
Ga2 O3 Ga3 88.6(2) 2_546 2_645
O3 O3 Ga3 35.5(3) 5_765 2_645
O3 O3 Ga3 107.3(4) 5_766 2_645
Ga3 O3 Ga3 46.03(15) 1_554 2_645
Nb O3 Ga3 134.3(3) 1_656 2_645
Ga1 O3 Ga3 134.3(3) 1_656 2_645
O2 O3 Ga3 128.0(3) 2_546 2_645
La1 O3 Ga3 139.2(3) 4_656 2_645
La1 O3 Ga3 87.1(2) 2_655 2_645
O1 O3 Ga3 48.3(2) 2_645 2_645
O2 O3 Ga3 90.3(3) 6_656 2_645
Ga3 O3 O2 126.8(5) . 2_545
Nb O3 O2 102.4(5) 1_655 2_545
Ga1 O3 O2 102.4(5) 1_655 2_545
La1 O3 O2 19.9(2) 4_655 2_545
Ga3 O3 O2 124.5(4) 2_646 2_545
O3 O3 O2 57.9(3) 2_645 2_545
O3 O3 O2 128.3(3) 2_646 2_545
O3 O3 O2 137.7(4) 4_765 2_545
O3 O3 O2 126.5(4) 3_645 2_545
O2 O3 O2 85.7(3) 4_655 2_545
O2 O3 O2 101.4(4) 3_655 2_545
O2 O3 O2 98.9(4) 5_656 2_545
O1 O3 O2 40.2(4) . 2_545
O3 O3 O2 84.9(5) 6 2_545
O3 O3 O2 150.2(3) 6_556 2_545
O2 O3 O2 38.0(3) 5_655 2_545
Ga2 O3 O2 67.9(3) 1_545 2_545
Ga3 O3 O2 162.6(4) 4_765 2_545
O2 O3 O2 52.8(4) 1_545 2_545
La1 O3 O2 61.4(2) . 2_545
Ga2 O3 O2 76.1(2) 2_546 2_545
O3 O3 O2 100.0(5) 5_765 2_545
O3 O3 O2 163.2(2) 5_766 2_545
Ga3 O3 O2 58.6(3) 1_554 2_545
Nb O3 O2 149.8(4) 1_656 2_545
Ga1 O3 O2 149.8(4) 1_656 2_545
O2 O3 O2 70.3(3) 2_546 2_545
La1 O3 O2 101.7(3) 4_656 2_545
La1 O3 O2 109.7(4) 2_655 2_545
O1 O3 O2 46.9(2) 2_645 2_545
O2 O3 O2 123.8(3) 6_656 2_545
Ga3 O3 O2 67.1(3) 2_645 2_545
Ga3 O3 Ga2 31.9(3) . 2_556
Nb O3 Ga2 98.8(4) 1_655 2_556
Ga1 O3 Ga2 98.8(4) 1_655 2_556
La1 O3 Ga2 126.0(4) 4_655 2_556
Ga3 O3 Ga2 124.8(4) 2_646 2_556
O3 O3 Ga2 125.4(7) 2_645 2_556
O3 O3 Ga2 95.4(5) 2_646 2_556
O3 O3 Ga2 60.8(4) 4_765 2_556
O3 O3 Ga2 118.6(4) 3_645 2_556
O2 O3 Ga2 157.9(5) 4_655 2_556
O2 O3 Ga2 7.4(3) 3_655 2_556
O2 O3 Ga2 53.2(3) 5_656 2_556
O1 O3 Ga2 76.3(3) . 2_556
O3 O3 Ga2 74.3(3) 6 2_556
O3 O3 Ga2 49.41(18) 6_556 2_556
O2 O3 Ga2 82.0(3) 5_655 2_556
Ga2 O3 Ga2 69.7(2) 1_545 2_556
Ga3 O3 Ga2 74.94(18) 4_765 2_556
O2 O3 Ga2 129.0(3) 1_545 2_556
La1 O3 Ga2 46.72(14) . 2_556
Ga2 O3 Ga2 141.3(3) 2_546 2_556
O3 O3 Ga2 107.34(14) 5_765 2_556
O3 O3 Ga2 88.3(2) 5_766 2_556
Ga3 O3 Ga2 86.4(2) 1_554 2_556
Nb O3 Ga2 76.33(19) 1_656 2_556
Ga1 O3 Ga2 76.33(19) 1_656 2_556
O2 O3 Ga2 91.4(3) 2_546 2_556
La1 O3 Ga2 91.8(2) 4_656 2_556
La1 O3 Ga2 45.09(11) 2_655 2_556
O1 O3 Ga2 154.5(4) 2_645 2_556
O2 O3 Ga2 125.4(4) 6_656 2_556
Ga3 O3 Ga2 128.9(3) 2_645 2_556
O2 O3 Ga2 107.6(3) 2_545 2_556
Ga3 O3 O2 151.2(5) . 6_655
Nb O3 O2 45.4(3) 1_655 6_655
Ga1 O3 O2 45.4(3) 1_655 6_655
La1 O3 O2 70.8(3) 4_655 6_655
Ga3 O3 O2 67.5(3) 2_646 6_655
O3 O3 O2 31.5(4) 2_645 6_655
O3 O3 O2 106.2(6) 2_646 6_655
O3 O3 O2 88.8(4) 4_765 6_655
O3 O3 O2 45.4(4) 3_645 6_655
O2 O3 O2 53.8(5) 4_655 6_655
O2 O3 O2 140.3(5) 3_655 6_655
O2 O3 O2 162.0(5) 5_656 6_655
O1 O3 O2 121.4(4) . 6_655
O3 O3 O2 71.8(4) 6 6_655
O3 O3 O2 128.5(2) 6_556 6_655
O2 O3 O2 85.6(5) 5_655 6_655
Ga2 O3 O2 142.1(3) 1_545 6_655
Ga3 O3 O2 87.0(3) 4_765 6_655
O2 O3 O2 84.7(3) 1_545 6_655
La1 O3 O2 124.0(4) . 6_655
Ga2 O3 O2 74.4(3) 2_546 6_655
O3 O3 O2 37.1(2) 5_765 6_655
O3 O3 O2 89.0(3) 5_766 6_655
Ga3 O3 O2 68.2(3) 1_554 6_655
Nb O3 O2 113.7(3) 1_656 6_655
Ga1 O3 O2 113.7(3) 1_656 6_655
O2 O3 O2 124.0(3) 2_546 6_655
La1 O3 O2 121.2(3) 4_656 6_655
La1 O3 O2 98.9(3) 2_655 6_655
O1 O3 O2 46.0(2) 2_645 6_655
O2 O3 O2 67.6(2) 6_656 6_655
Ga3 O3 O2 22.67(19) 2_645 6_655
O2 O3 O2 81.3(4) 2_545 6_655
Ga2 O3 O2 144.0(3) 2_556 6_655
Ga3 O3 La1 146.8(6) . 2_645
Nb O3 La1 74.2(3) 1_655 2_645
Ga1 O3 La1 74.2(3) 1_655 2_645
La1 O3 La1 61.3(2) 4_655 2_645
Ga3 O3 La1 51.2(2) 2_646 2_645
O3 O3 La1 53.1(5) 2_645 2_645
O3 O3 La1 84.2(5) 2_646 2_645
O3 O3 La1 110.8(4) 4_765 2_645
O3 O3 La1 53.1(5) 3_645 2_645
O2 O3 La1 24.4(3) 4_655 2_645
O2 O3 La1 170.3(5) 3_655 2_645
O2 O3 La1 132.2(5) 5_656 2_645
O1 O3 La1 111.8(3) . 2_645
O3 O3 La1 101.4(3) 6 2_645
O3 O3 La1 126.3(3) 6_556 2_645
O2 O3 La1 101.0(4) 5_655 2_645
Ga2 O3 La1 118.4(3) 1_545 2_645
Ga3 O3 La1 97.2(3) 4_765 2_645
O2 O3 La1 59.2(2) 1_545 2_645
La1 O3 La1 138.4(3) . 2_645
Ga2 O3 La1 44.56(12) 2_546 2_645
O3 O3 La1 65.63(14) 5_765 2_645
O3 O3 La1 85.76(18) 5_766 2_645
Ga3 O3 La1 92.7(2) 1_554 2_645
Nb O3 La1 100.9(3) 1_656 2_645
Ga1 O3 La1 100.9(3) 1_656 2_645
O2 O3 La1 96.0(3) 2_546 2_645
La1 O3 La1 92.1(2) 4_656 2_645
La1 O3 La1 128.1(3) 2_655 2_645
O1 O3 La1 32.26(11) 2_645 2_645
O2 O3 La1 50.8(2) 6_656 2_645
Ga3 O3 La1 47.97(12) 2_645 2_645
O2 O3 La1 78.9(2) 2_545 2_645
Ga2 O3 La1 171.5(2) 2_556 2_645
O2 O3 La1 30.02(18) 6_655 2_645
Ga3 O3 O1 94.6(5) . 2_646
Nb O3 O1 128.7(5) 1_655 2_646
Ga1 O3 O1 128.7(5) 1_655 2_646
La1 O3 O1 75.3(3) 4_655 2_646
Ga3 O3 O1 46.1(2) 2_646 2_646
O3 O3 O1 110.1(5) 2_645 2_646
O3 O3 O1 38.6(3) 2_646 2_646
O3 O3 O1 129.3(4) 4_765 2_646
O3 O3 O1 84.6(4) 3_645 2_646
O2 O3 O1 36.3(3) 4_655 2_646
O2 O3 O1 129.0(5) 3_655 2_646
O2 O3 O1 71.9(4) 5_656 2_646
O1 O3 O1 88.5(3) . 2_646
O3 O3 O1 161.9(4) 6 2_646
O3 O3 O1 88.9(5) 6_556 2_646
O2 O3 O1 129.7(3) 5_655 2_646
Ga2 O3 O1 70.0(2) 1_545 2_646
Ga3 O3 O1 101.0(4) 4_765 2_646
O2 O3 O1 39.1(3) 1_545 2_646
La1 O3 O1 128.2(3) . 2_646
Ga2 O3 O1 20.93(19) 2_546 2_646
O3 O3 O1 121.0(2) 5_765 2_646
O3 O3 O1 74.3(3) 5_766 2_646
Ga3 O3 O1 144.8(3) 1_554 2_646
Nb O3 O1 63.3(3) 1_656 2_646
Ga1 O3 O1 63.3(3) 1_656 2_646
O2 O3 O1 45.7(2) 2_546 2_646
La1 O3 O1 31.7(2) 4_656 2_646
La1 O3 O1 157.6(4) 2_655 2_646
O1 O3 O1 66.49(17) 2_645 2_646
O2 O3 O1 45.2(2) 6_656 2_646
Ga3 O3 O1 107.6(3) 2_645 2_646
O2 O3 O1 91.9(3) 2_545 2_646
Ga2 O3 O1 123.5(3) 2_556 2_646
O2 O3 O1 90.1(3) 6_655 2_646
La1 O3 O1 60.53(19) 2_645 2_646
Ga3 O3 O2 82.8(4) . 1_655
Nb O3 O2 43.0(3) 1_655 1_655
Ga1 O3 O2 43.0(3) 1_655 1_655
La1 O3 O2 139.4(4) 4_655 1_655
Ga3 O3 O2 60.2(2) 2_646 1_655
O3 O3 O2 87.2(3) 2_645 1_655
O3 O3 O2 79.2(3) 2_646 1_655
O3 O3 O2 29.9(3) 4_765 1_655
O3 O3 O2 30.7(3) 3_645 1_655
O2 O3 O2 90.7(3) 4_655 1_655
O2 O3 O2 91.1(3) 3_655 1_655
O2 O3 O2 115.4(4) 5_656 1_655
O1 O3 O2 163.3(4) . 1_655
O3 O3 O2 69.0(3) 6 1_655
O3 O3 O2 62.2(3) 6_556 1_655
O2 O3 O2 118.9(4) 5_655 1_655
Ga2 O3 O2 146.7(4) 1_545 1_655
Ga3 O3 O2 19.2(2) 4_765 1_655
O2 O3 O2 136.9(4) 1_545 1_655
La1 O3 O2 121.9(3) . 1_655
Ga2 O3 O2 111.1(3) 2_546 1_655
O3 O3 O2 44.8(3) 5_765 1_655
O3 O3 O2 37.6(3) 5_766 1_655
Ga3 O3 O2 92.4(3) 1_554 1_655
Nb O3 O2 63.6(2) 1_656 1_655
Ga1 O3 O2 63.6(2) 1_656 1_655
O2 O3 O2 142.4(4) 2_546 1_655
La1 O3 O2 109.2(3) 4_656 1_655
La1 O3 O2 59.9(2) 2_655 1_655
O1 O3 O2 112.8(3) 2_645 1_655
O2 O3 O2 61.2(3) 6_656 1_655
Ga3 O3 O2 78.4(2) 2_645 1_655
O2 O3 O2 144.8(3) 2_545 1_655
Ga2 O3 O2 88.2(2) 2_556 1_655
O2 O3 O2 68.6(3) 6_655 1_655
La1 O3 O2 83.5(2) 2_645 1_655
O1 O3 O2 105.6(3) 2_646 1_655
Ga3 O3 Ga2 117.3(5) . 1_544
Nb O3 Ga2 91.4(4) 1_655 1_544
Ga1 O3 Ga2 91.4(4) 1_655 1_544
La1 O3 Ga2 41.1(2) 4_655 1_544
Ga3 O3 Ga2 144.0(3) 2_646 1_544
O3 O3 Ga2 56.4(4) 2_645 1_544
O3 O3 Ga2 147.12(16) 2_646 1_544
O3 O3 Ga2 117.0(3) 4_765 1_544
O3 O3 Ga2 129.7(2) 3_645 1_544
O2 O3 Ga2 105.8(4) 4_655 1_544
O2 O3 Ga2 83.9(4) 3_655 1_544
O2 O3 Ga2 100.6(4) 5_656 1_544
O1 O3 Ga2 42.4(4) . 1_544
O3 O3 Ga2 65.9(3) 6 1_544
O3 O3 Ga2 139.7(2) 6_556 1_544
O2 O3 Ga2 16.4(2) 5_655 1_544
Ga2 O3 Ga2 73.5(2) 1_545 1_544
Ga3 O3 Ga2 144.9(3) 4_765 1_544
O2 O3 Ga2 74.4(3) 1_545 1_544
La1 O3 Ga2 44.46(14) . 1_544
Ga2 O3 Ga2 98.1(2) 2_546 1_544
O3 O3 Ga2 91.9(4) 5_765 1_544
O3 O3 Ga2 170.9(4) 5_766 1_544
Ga3 O3 Ga2 41.05(14) 1_554 1_544
Nb O3 Ga2 159.2(3) 1_656 1_544
Ga1 O3 Ga2 159.2(3) 1_656 1_544
O2 O3 Ga2 84.3(3) 2_546 1_544
La1 O3 Ga2 117.4(2) 4_656 1_544
La1 O3 Ga2 87.8(3) 2_655 1_544
O1 O3 Ga2 64.4(2) 2_645 1_544
O2 O3 Ga2 143.4(3) 6_656 1_544
Ga3 O3 Ga2 66.43(18) 2_645 1_544
O2 O3 Ga2 22.01(17) 2_545 1_544
Ga2 O3 Ga2 90.9(2) 2_556 1_544
O2 O3 Ga2 86.3(3) 6_655 1_544
La1 O3 Ga2 94.0(2) 2_645 1_544
O1 O3 Ga2 113.4(2) 2_646 1_544
O2 O3 Ga2 133.3(3) 1_655 1_544
Ga3 O3 Ga3 98.5(4) . 4_655
Nb O3 Ga3 147.9(4) 1_655 4_655
Ga1 O3 Ga3 147.9(4) 1_655 4_655
La1 O3 Ga3 46.8(2) 4_655 4_655
Ga3 O3 Ga3 88.5(3) 2_646 4_655
O3 O3 Ga3 101.86(17) 2_645 4_655
O3 O3 Ga3 73.55(16) 2_646 4_655
O3 O3 Ga3 164.0(2) 4_765 4_655
O3 O3 Ga3 123.4(6) 3_645 4_655
O2 O3 Ga3 63.0(3) 4_655 4_655
O2 O3 Ga3 109.8(4) 3_655 4_655
O2 O3 Ga3 62.8(3) 5_656 4_655
O1 O3 Ga3 46.4(2) . 4_655
O3 O3 Ga3 139.8(4) 6 4_655
O3 O3 Ga3 109.5(5) 6_556 4_655
O2 O3 Ga3 89.9(3) 5_655 4_655
Ga2 O3 Ga3 39.88(11) 1_545 4_655
Ga3 O3 Ga3 141.0(4) 4_765 4_655
O2 O3 Ga3 19.56(19) 1_545 4_655
La1 O3 Ga3 88.1(2) . 4_655
Ga2 O3 Ga3 39.98(9) 2_546 4_655
O3 O3 Ga3 140.5(3) 5_765 4_655
O3 O3 Ga3 114.8(4) 5_766 4_655
Ga3 O3 Ga3 113.9(3) 1_554 4_655
Nb O3 Ga3 94.7(2) 1_656 4_655
Ga1 O3 Ga3 94.7(2) 1_656 4_655
O2 O3 Ga3 21.17(19) 2_546 4_655
La1 O3 Ga3 46.72(11) 4_656 4_655
La1 O3 Ga3 149.3(3) 2_655 4_655
O1 O3 Ga3 59.7(2) 2_645 4_655
O2 O3 Ga3 87.6(3) 6_656 4_655
Ga3 O3 Ga3 106.9(2) 2_645 4_655
O2 O3 Ga3 55.4(2) 2_545 4_655
Ga2 O3 Ga3 109.5(2) 2_556 4_655
O2 O3 Ga3 104.1(3) 6_655 4_655
La1 O3 Ga3 78.50(16) 2_645 4_655
O1 O3 Ga3 42.95(11) 2_646 4_655
O2 O3 Ga3 148.5(3) 1_655 4_655
Ga2 O3 Ga3 73.94(15) 1_544 4_655
Ga3 O3 La1 116.5(4) . 1_655
Nb O3 La1 34.8(3) 1_655 1_655
Ga1 O3 La1 34.8(3) 1_655 1_655
La1 O3 La1 105.3(3) 4_655 1_655
Ga3 O3 La1 53.0(2) 2_646 1_655
O3 O3 La1 59.7(3) 2_645 1_655
O3 O3 La1 88.6(4) 2_646 1_655
O3 O3 La1 59.7(3) 4_765 1_655
O3 O3 La1 14.64(15) 3_645 1_655
O2 O3 La1 65.5(3) 4_655 1_655
O2 O3 La1 121.6(4) 3_655 1_655
O2 O3 La1 143.7(5) 5_656 1_655
O1 O3 La1 155.7(4) . 1_655
O3 O3 La1 70.99(16) 6 1_655
O3 O3 La1 94.09(16) 6_556 1_655
O2 O3 La1 108.6(4) 5_655 1_655
Ga2 O3 La1 164.6(4) 1_545 1_655
Ga3 O3 La1 52.33(14) 4_765 1_655
O2 O3 La1 109.7(3) 1_545 1_655
La1 O3 La1 136.1(3) . 1_655
Ga2 O3 La1 89.1(2) 2_546 1_655
O3 O3 La1 29.02(19) 5_765 1_655
O3 O3 La1 57.5(3) 5_766 1_655
Ga3 O3 La1 83.2(2) 1_554 1_655
Nb O3 La1 85.2(2) 1_656 1_655
Ga1 O3 La1 85.2(2) 1_656 1_655
O2 O3 La1 140.2(4) 2_546 1_655
La1 O3 La1 116.0(3) 4_656 1_655
La1 O3 La1 81.77(17) 2_655 1_655
O1 O3 La1 78.39(19) 2_645 1_655
O2 O3 La1 53.6(2) 6_656 1_655
Ga3 O3 La1 49.80(12) 2_645 1_655
O2 O3 La1 115.5(3) 2_545 1_655
Ga2 O3 La1 120.5(2) 2_556 1_655
O2 O3 La1 34.75(18) 6_655 1_655
La1 O3 La1 51.08(12) 2_645 1_655
O1 O3 La1 94.7(2) 2_646 1_655
O2 O3 La1 34.49(18) 1_655 1_655
Ga2 O3 La1 115.6(3) 1_544 1_655
Ga3 O3 La1 128.2(3) 4_655 1_655
Ga3 O3 O1 72.0(4) . 2_655
Nb O3 O1 74.2(4) 1_655 2_655
Ga1 O3 O1 74.2(4) 1_655 2_655
La1 O3 O1 101.9(5) 4_655 2_655
Ga3 O3 O1 150.7(3) 2_646 2_655
O3 O3 O1 85.6(7) 2_645 2_655
O3 O3 O1 135.3(6) 2_646 2_655
O3 O3 O1 62.9(4) 4_765 2_655
O3 O3 O1 116.5(4) 3_645 2_655
O2 O3 O1 161.9(5) 4_655 2_655
O2 O3 O1 33.3(4) 3_655 2_655
O2 O3 O1 87.1(4) 5_656 2_655
O1 O3 O1 72.8(3) . 2_655
O3 O3 O1 39.8(2) 6 2_655
O3 O3 O1 85.4(3) 6_556 2_655
O2 O3 O1 46.9(3) 5_655 2_655
Ga2 O3 O1 87.4(3) 1_545 2_655
Ga3 O3 O1 89.8(2) 4_765 2_655
O2 O3 O1 130.6(4) 1_545 2_655
La1 O3 O1 31.13(10) . 2_655
Ga2 O3 O1 156.9(3) 2_546 2_655
O3 O3 O1 81.8(3) 5_765 2_655
O3 O3 O1 114.0(2) 5_766 2_655
Ga3 O3 O1 46.2(3) 1_554 2_655
Nb O3 O1 113.5(3) 1_656 2_655
Ga1 O3 O1 113.5(3) 1_656 2_655
O2 O3 O1 112.0(3) 2_546 2_655
La1 O3 O1 128.0(3) 4_656 2_655
La1 O3 O1 31.53(9) 2_655 2_655
O1 O3 O1 121.3(6) 2_645 2_655
O2 O3 O1 151.6(3) 6_656 2_655
Ga3 O3 O1 90.6(3) 2_645 2_655
O2 O3 O1 82.4(3) 2_545 2_655
Ga2 O3 O1 40.2(2) 2_556 2_655
O2 O3 O1 110.6(4) 6_655 2_655
La1 O3 O1 138.5(4) 2_645 2_655
O1 O3 O1 157.2(3) 2_646 2_655
O2 O3 O1 91.3(2) 1_655 2_655
Ga2 O3 O1 60.8(3) 1_544 2_655
Ga3 O3 O1 119.2(2) 4_655 2_655
La1 O3 O1 107.8(2) 1_655 2_655
Ga3 O3 O3 43.8(4) . 1_556
Nb O3 O3 128.6(4) 1_655 1_556
Ga1 O3 O3 128.6(4) 1_655 1_556
La1 O3 O3 120.8(3) 4_655 1_556
Ga3 O3 O3 59.5(3) 2_646 1_556
O3 O3 O3 157.7(6) 2_645 1_556
O3 O3 O3 21.2(5) 2_646 1_556
O3 O3 O3 90.000(2) 4_765 1_556
O3 O3 O3 90.000(1) 3_645 1_556
O2 O3 O3 82.5(4) 4_655 1_556
O2 O3 O3 82.4(4) 3_655 1_556
O2 O3 O3 40.5(4) 5_656 1_556
O1 O3 O3 96.4(4) . 1_556
O3 O3 O3 140.6(4) 6 1_556
O3 O3 O3 37.9(4) 6_556 1_556
O2 O3 O3 146.1(3) 5_655 1_556
Ga2 O3 O3 65.4(2) 1_545 1_556
Ga3 O3 O3 69.0(2) 4_765 1_556
O2 O3 O3 84.5(3) 1_545 1_556
La1 O3 O3 108.96(19) . 1_556
Ga2 O3 O3 73.27(19) 2_546 1_556
O3 O3 O3 129.1(4) 5_765 1_556
O3 O3 O3 49.4(3) 5_766 1_556
Ga3 O3 O3 161.70(16) 1_554 1_556
Nb O3 O3 21.96(15) 1_656 1_556
Ga1 O3 O3 21.96(15) 1_656 1_556
O2 O3 O3 58.1(3) 2_546 1_556
La1 O3 O3 28.32(13) 4_656 1_556
La1 O3 O3 106.92(18) 2_655 1_556
O1 O3 O3 118.8(3) 2_645 1_556
O2 O3 O3 59.4(3) 6_656 1_556
Ga3 O3 O3 149.66(18) 2_645 1_556
O2 O3 O3 128.4(3) 2_545 1_556
Ga2 O3 O3 75.36(18) 2_556 1_556
O2 O3 O3 127.0(3) 6_655 1_556
La1 O3 O3 105.08(17) 2_645 1_556
O1 O3 O3 52.3(2) 2_646 1_556
O2 O3 O3 85.6(2) 1_655 1_556
Ga2 O3 O3 138.87(14) 1_544 1_556
Ga3 O3 O3 74.69(16) 4_655 1_556
La1 O3 O3 104.57(16) 1_655 1_556
O1 O3 O3 115.6(3) 2_655 1_556
Ga3 O3 O3 136.2(4) . 1_554
Nb O3 O3 51.4(4) 1_655 1_554
Ga1 O3 O3 51.4(4) 1_655 1_554
La1 O3 O3 59.2(3) 4_655 1_554
Ga3 O3 O3 120.5(3) 2_646 1_554
O3 O3 O3 22.3(6) 2_645 1_554
O3 O3 O3 158.8(5) 2_646 1_554
O3 O3 O3 90.000(1) 4_765 1_554
O3 O3 O3 90.000(1) 3_645 1_554
O2 O3 O3 97.5(4) 4_655 1_554
O2 O3 O3 97.6(4) 3_655 1_554
O2 O3 O3 139.5(4) 5_656 1_554
O1 O3 O3 83.6(4) . 1_554
O3 O3 O3 39.4(4) 6 1_554
O3 O3 O3 142.1(4) 6_556 1_554
O2 O3 O3 33.9(3) 5_655 1_554
Ga2 O3 O3 114.6(2) 1_545 1_554
Ga3 O3 O3 111.0(2) 4_765 1_554
O2 O3 O3 95.5(3) 1_545 1_554
La1 O3 O3 71.05(19) . 1_554
Ga2 O3 O3 106.73(19) 2_546 1_554
O3 O3 O3 50.9(4) 5_765 1_554
O3 O3 O3 130.6(3) 5_766 1_554
Ga3 O3 O3 18.30(17) 1_554 1_554
Nb O3 O3 158.04(15) 1_656 1_554
Ga1 O3 O3 158.04(15) 1_656 1_554
O2 O3 O3 121.9(3) 2_546 1_554
La1 O3 O3 151.68(13) 4_656 1_554
La1 O3 O3 73.08(18) 2_655 1_554
O1 O3 O3 61.2(3) 2_645 1_554
O2 O3 O3 120.6(3) 6_656 1_554
Ga3 O3 O3 30.34(18) 2_645 1_554
O2 O3 O3 51.6(3) 2_545 1_554
Ga2 O3 O3 104.64(18) 2_556 1_554
O2 O3 O3 53.0(3) 6_655 1_554
La1 O3 O3 74.92(17) 2_645 1_554
O1 O3 O3 127.7(2) 2_646 1_554
O2 O3 O3 94.4(2) 1_655 1_554
Ga2 O3 O3 41.13(14) 1_544 1_554
Ga3 O3 O3 105.31(16) 4_655 1_554
La1 O3 O3 75.43(16) 1_655 1_554
O1 O3 O3 64.4(3) 2_655 1_554
O3 O3 O3 179.999(3) 1_556 1_554
Ga3 O3 Ga3 114.2(4) . 4_764
Nb O3 Ga3 12.1(3) 1_655 4_764
Ga1 O3 Ga3 12.1(3) 1_655 4_764
La1 O3 Ga3 98.6(4) 4_655 4_764
Ga3 O3 Ga3 99.3(3) 2_646 4_764
O3 O3 Ga3 43.5(2) 2_645 4_764
O3 O3 Ga3 131.1(3) 2_646 4_764
O3 O3 Ga3 50.90(15) 4_765 4_764
O3 O3 Ga3 59.41(15) 3_645 4_764
O2 O3 Ga3 103.2(4) 4_655 4_764
O2 O3 Ga3 90.1(4) 3_655 4_764
O2 O3 Ga3 146.9(4) 5_656 4_764
O1 O3 Ga3 120.7(4) . 4_764
O3 O3 Ga3 24.99(16) 6 4_764
O3 O3 Ga3 105.3(4) 6_556 4_764
O2 O3 Ga3 67.5(3) 5_655 4_764
Ga2 O3 Ga3 148.5(4) 1_545 4_764
Ga3 O3 Ga3 68.98(17) 4_765 4_764
O2 O3 Ga3 129.6(3) 1_545 4_764
La1 O3 Ga3 89.8(3) . 4_764
Ga2 O3 Ga3 124.7(3) 2_546 4_764
O3 O3 Ga3 17.83(17) 5_765 4_764
O3 O3 Ga3 90.6(3) 5_766 4_764
Ga3 O3 Ga3 40.27(12) 1_554 4_764
Nb O3 Ga3 116.3(2) 1_656 4_764
Ga1 O3 Ga3 116.3(2) 1_656 4_764
O2 O3 Ga3 163.9(4) 2_546 4_764
La1 O3 Ga3 161.3(3) 4_656 4_764
La1 O3 Ga3 48.97(13) 2_655 4_764
O1 O3 Ga3 88.1(3) 2_645 4_764
O2 O3 Ga3 99.9(3) 6_656 4_764
Ga3 O3 Ga3 39.79(11) 2_645 4_764
O2 O3 Ga3 93.6(3) 2_545 4_764
Ga2 O3 Ga3 93.8(2) 2_556 4_764
O2 O3 Ga3 50.3(2) 6_655 4_764
La1 O3 Ga3 80.22(18) 2_645 4_764
O1 O3 Ga3 138.4(3) 2_646 4_764
O2 O3 Ga3 53.2(2) 1_655 4_764
Ga2 O3 Ga3 80.4(2) 1_544 4_764
Ga3 O3 Ga3 145.1(3) 4_655 4_764
La1 O3 Ga3 46.41(10) 1_655 4_764
O1 O3 Ga3 64.3(2) 2_655 4_764
O3 O3 Ga3 138.00(14) 1_556 4_764
O3 O3 Ga3 42.00(14) 1_554 4_764
Ga3 O3 O2 50.4(3) . 2_656
Nb O3 O2 68.9(3) 1_655 2_656
Ga1 O3 O2 68.9(3) 1_655 2_656
La1 O3 O2 171.8(5) 4_655 2_656
Ga3 O3 O2 71.5(3) 2_646 2_656
O3 O3 O2 116.4(2) 2_645 2_656
O3 O3 O2 68.1(3) 2_646 2_656
O3 O3 O2 26.4(2) 4_765 2_656
O3 O3 O2 59.5(3) 3_645 2_656
O2 O3 O2 109.8(5) 4_655 2_656
O2 O3 O2 65.6(4) 3_655 2_656
O2 O3 O2 84.3(4) 5_656 2_656
O1 O3 O2 135.6(4) . 2_656
O3 O3 O2 79.4(4) 6 2_656
O3 O3 O2 31.5(3) 6_556 2_656
O2 O3 O2 124.5(4) 5_655 2_656
Ga2 O3 O2 115.2(3) 1_545 2_656
Ga3 O3 O2 14.72(15) 4_765 2_656
O2 O3 O2 144.5(4) 1_545 2_656
La1 O3 O2 104.3(3) . 2_656
Ga2 O3 O2 121.4(4) 2_546 2_656
O3 O3 O2 73.5(3) 5_765 2_656
O3 O3 O2 33.5(2) 5_766 2_656
Ga3 O3 O2 105.8(3) 1_554 2_656
Nb O3 O2 44.7(2) 1_656 2_656
Ga1 O3 O2 44.7(2) 1_656 2_656
O2 O3 O2 120.3(5) 2_546 2_656
La1 O3 O2 92.1(3) 4_656 2_656
La1 O3 O2 52.74(18) 2_655 2_656
O1 O3 O2 143.5(3) 2_645 2_656
O2 O3 O2 72.3(3) 6_656 2_656
Ga3 O3 O2 108.9(3) 2_645 2_656
O2 O3 O2 162.4(5) 2_545 2_656
Ga2 O3 O2 60.62(18) 2_556 2_656
O2 O3 O2 101.0(2) 6_655 2_656
La1 O3 O2 111.7(3) 2_645 2_656
O1 O3 O2 105.5(4) 2_646 2_656
O2 O3 O2 32.4(3) 1_655 2_656
Ga2 O3 O2 140.4(3) 1_544 2_656
Ga3 O3 O2 138.6(4) 4_655 2_656
La1 O3 O2 66.5(2) 1_655 2_656
O1 O3 O2 80.5(2) 2_655 2_656
O3 O3 O2 64.0(2) 1_556 2_656
O3 O3 O2 116.0(2) 1_554 2_656
Ga3 O3 O2 75.3(2) 4_764 2_656
Ga3 O3 O2 57.3(4) . 6_556
Nb O3 O2 154.1(6) 1_655 6_556
Ga1 O3 O2 154.1(6) 1_655 6_556
La1 O3 O2 80.5(3) 4_655 6_556
Ga3 O3 O2 116.5(4) 2_646 6_556
O3 O3 O2 130.3(5) 2_645 6_556
O3 O3 O2 80.2(4) 2_646 6_556
O3 O3 O2 119.6(5) 4_765 6_556
O3 O3 O2 154.1(3) 3_645 6_556
O2 O3 O2 109.5(4) 4_655 6_556
O2 O3 O2 60.8(3) 3_655 6_556
O2 O3 O2 26.1(2) 5_656 6_556
O1 O3 O2 33.7(4) . 6_556
O3 O3 O2 118.4(2) 6 6_556
O3 O3 O2 78.1(3) 6_556 6_556
O2 O3 O2 82.7(3) 5_655 6_556
Ga2 O3 O2 9.54(16) 1_545 6_556
Ga3 O3 O2 120.9(3) 4_765 6_556
O2 O3 O2 68.8(3) 1_545 6_556
La1 O3 O2 53.7(2) . 6_556
Ga2 O3 O2 85.9(2) 2_546 6_556
O3 O3 O2 161.2(4) 5_765 6_556
O3 O3 O2 112.1(5) 5_766 6_556
Ga3 O3 O2 108.0(3) 1_554 6_556
Nb O3 O2 84.2(3) 1_656 6_556
Ga1 O3 O2 84.2(3) 1_656 6_556
O2 O3 O2 33.2(2) 2_546 6_556
La1 O3 O2 53.4(2) 4_656 6_556
La1 O3 O2 102.7(3) 2_655 6_556
O1 O3 O2 105.0(2) 2_645 6_556
O2 O3 O2 116.0(4) 6_656 6_556
Ga3 O3 O2 140.0(3) 2_645 6_556
O2 O3 O2 73.09(16) 2_545 6_556
Ga2 O3 O2 60.1(2) 2_556 6_556
O2 O3 O2 150.8(4) 6_655 6_556
La1 O3 O2 127.9(3) 2_645 6_556
O1 O3 O2 77.2(3) 2_646 6_556
O2 O3 O2 139.9(3) 1_655 6_556
Ga2 O3 O2 75.2(2) 1_544 6_556
Ga3 O3 O2 49.41(18) 4_655 6_556
La1 O3 O2 168.7(4) 1_655 6_556
O1 O3 O2 80.0(2) 2_655 6_556
O3 O3 O2 64.3(2) 1_556 6_556
O3 O3 O2 115.7(2) 1_554 6_556
Ga3 O3 O2 143.4(3) 4_764 6_556
O2 O3 O2 107.7(4) 2_656 6_556
Ga3 O3 La1 25.9(2) . 1_556
Nb O3 La1 138.0(4) 1_655 1_556
Ga1 O3 La1 138.0(4) 1_655 1_556
La1 O3 La1 112.3(3) 4_655 1_556
Ga3 O3 La1 102.6(4) 2_646 1_556
O3 O3 La1 158.0(7) 2_645 1_556
O3 O3 La1 63.9(4) 2_646 1_556
O3 O3 La1 91.8(4) 4_765 1_556
O3 O3 La1 127.38(17) 3_645 1_556
O2 O3 La1 118.0(4) 4_655 1_556
O2 O3 La1 47.2(3) 3_655 1_556
O2 O3 La1 11.4(2) 5_656 1_556
O1 O3 La1 64.5(4) . 1_556
O3 O3 La1 116.2(3) 6 1_556
O3 O3 La1 46.0(2) 6_556 1_556
O2 O3 La1 104.0(3) 5_655 1_556
Ga2 O3 La1 39.39(13) 1_545 1_556
Ga3 O3 La1 88.8(2) 4_765 1_556
O2 O3 La1 92.6(3) 1_545 1_556
La1 O3 La1 65.84(17) . 1_556
Ga2 O3 La1 99.0(2) 2_546 1_556
O3 O3 La1 145.7(2) 5_765 1_556
O3 O3 La1 83.3(3) 5_766 1_556
Ga3 O3 La1 121.6(3) 1_554 1_556
Nb O3 La1 57.38(15) 1_656 1_556
Ga1 O3 La1 57.38(15) 1_656 1_556
O2 O3 La1 52.9(2) 2_546 1_556
La1 O3 La1 50.24(13) 4_656 1_556
La1 O3 La1 86.69(19) 2_655 1_556
O1 O3 La1 133.5(3) 2_645 1_556
O2 O3 La1 102.5(3) 6_656 1_556
Ga3 O3 La1 167.2(3) 2_645 1_556
O2 O3 La1 104.7(3) 2_545 1_556
Ga2 O3 La1 42.33(11) 2_556 1_556
O2 O3 La1 170.1(4) 6_655 1_556
La1 O3 La1 142.3(3) 2_645 1_556
O1 O3 La1 81.8(3) 2_646 1_556
O2 O3 La1 107.9(3) 1_655 1_556
Ga2 O3 La1 102.2(2) 1_544 1_556
Ga3 O3 La1 73.81(16) 4_655 1_556
La1 O3 La1 139.8(3) 1_655 1_556
O1 O3 La1 78.3(2) 2_655 1_556
O3 O3 La1 43.12(16) 1_556 1_556
O3 O3 La1 136.88(16) 1_554 1_556
Ga3 O3 La1 135.6(2) 4_764 1_556
O2 O3 La1 75.8(2) 2_656 1_556
O2 O3 La1 32.13(19) 6_556 1_556
Ga3 O3 O2 128.7(5) . 3_645
Nb O3 O2 106.2(4) 1_655 3_645
Ga1 O3 O2 106.2(4) 1_655 3_645
La1 O3 O2 51.0(3) 4_655 3_645
Ga3 O3 O2 54.2(2) 2_646 3_645
O3 O3 O2 76.1(5) 2_645 3_645
O3 O3 O2 69.3(4) 2_646 3_645
O3 O3 O2 137.5(5) 4_765 3_645
O3 O3 O2 77.7(5) 3_645 3_645
O2 O3 O2 17.1(3) 4_655 3_645
O2 O3 O2 157.2(5) 3_655 3_645
O2 O3 O2 101.6(3) 5_656 3_645
O1 O3 O2 89.1(2) . 3_645
O3 O3 O2 129.4(5) 6 3_645
O3 O3 O2 120.6(5) 6_556 3_645
O2 O3 O2 105.9(3) 5_655 3_645
Ga2 O3 O2 87.1(2) 1_545 3_645
Ga3 O3 O2 114.5(3) 4_765 3_645
O2 O3 O2 29.9(2) 1_545 3_645
La1 O3 O2 128.7(3) . 3_645
Ga2 O3 O2 13.90(18) 2_546 3_645
O3 O3 O2 97.68(19) 5_765 3_645
O3 O3 O2 92.5(2) 5_766 3_645
Ga3 O3 O2 111.8(3) 1_554 3_645
Nb O3 O2 92.8(3) 1_656 3_645
Ga1 O3 O2 92.8(3) 1_656 3_645
O2 O3 O2 64.0(3) 2_546 3_645
La1 O3 O2 64.7(2) 4_656 3_645
La1 O3 O2 160.2(3) 2_655 3_645
O1 O3 O2 33.2(3) 2_645 3_645
O2 O3 O2 53.4(2) 6_656 3_645
Ga3 O3 O2 74.7(2) 2_645 3_645
O2 O3 O2 70.8(3) 2_545 3_645
Ga2 O3 O2 154.7(3) 2_556 3_645
O2 O3 O2 61.3(2) 6_655 3_645
La1 O3 O2 32.07(18) 2_645 3_645
O1 O3 O2 34.1(3) 2_646 3_645
O2 O3 O2 107.6(3) 1_655 3_645
Ga2 O3 O2 92.1(2) 1_544 3_645
Ga3 O3 O2 47.78(17) 4_655 3_645
La1 O3 O2 80.4(2) 1_655 3_645
O1 O3 O2 152.7(3) 2_655 3_645
O3 O3 O2 86.1(2) 1_556 3_645
O3 O3 O2 93.9(2) 1_554 3_645
Ga3 O3 O2 111.5(3) 4_764 3_645
O2 O3 O2 125.7(3) 2_656 3_645
O2 O3 O2 96.5(3) 6_556 3_645
La1 O3 O2 112.7(3) 1_556 3_645
Ga3 O3 O1 13.0(3) . 2_656
Nb O3 O1 110.1(4) 1_655 2_656
Ga1 O3 O1 110.1(4) 1_655 2_656
La1 O3 O1 132.8(4) 4_655 2_656
Ga3 O3 O1 108.5(4) 2_646 2_656
O3 O3 O1 144.3(7) 2_645 2_656
O3 O3 O1 76.4(5) 2_646 2_656
O3 O3 O1 65.2(4) 4_765 2_656
O3 O3 O1 114.3(3) 3_645 2_656
O2 O3 O1 138.6(5) 4_655 2_656
O2 O3 O1 26.4(4) 3_655 2_656
O2 O3 O1 39.4(3) 5_656 2_656
O1 O3 O1 80.5(4) . 2_656
O3 O3 O1 91.7(4) 6 2_656
O3 O3 O1 34.23(19) 6_556 2_656
O2 O3 O1 99.4(4) 5_655 2_656
Ga2 O3 O1 63.90(18) 1_545 2_656
Ga3 O3 O1 69.83(18) 4_765 2_656
O2 O3 O1 120.5(3) 1_545 2_656
La1 O3 O1 61.4(2) . 2_656
Ga2 O3 O1 124.9(4) 2_546 2_656
O3 O3 O1 118.05(18) 5_765 2_656
O3 O3 O1 75.8(3) 5_766 2_656
Ga3 O3 O1 105.6(3) 1_554 2_656
Nb O3 O1 58.8(2) 1_656 2_656
Ga1 O3 O1 58.8(2) 1_656 2_656
O2 O3 O1 80.8(3) 2_546 2_656
La1 O3 O1 74.2(3) 4_656 2_656
La1 O3 O1 59.5(2) 2_655 2_656
O1 O3 O1 159.9(3) 2_645 2_656
O2 O3 O1 108.9(4) 6_656 2_656
Ga3 O3 O1 146.4(3) 2_645 2_656
O2 O3 O1 118.1(3) 2_545 2_656
Ga2 O3 O1 19.21(19) 2_556 2_656
O2 O3 O1 154.0(3) 6_655 2_656
La1 O3 O1 159.6(4) 2_645 2_656
O1 O3 O1 105.4(4) 2_646 2_656
O2 O3 O1 86.9(2) 1_655 2_656
Ga2 O3 O1 105.6(3) 1_544 2_656
Ga3 O3 O1 101.4(2) 4_655 2_656
La1 O3 O1 121.4(2) 1_655 2_656
O1 O3 O1 59.44(13) 2_655 2_656
O3 O3 O1 56.1(3) 1_556 2_656
O3 O3 O1 123.9(3) 1_554 2_656
Ga3 O3 O1 108.0(2) 4_764 2_656
O2 O3 O1 55.2(2) 2_656 2_656
O2 O3 O1 54.9(2) 6_556 2_656
La1 O3 O1 28.01(13) 1_556 2_656
O2 O3 O1 138.8(3) 3_645 2_656
Ga3 O3 O1 125.1(5) . 1_655
Nb O3 O1 60.9(4) 1_655 1_655
Ga1 O3 O1 60.9(4) 1_655 1_655
La1 O3 O1 89.5(3) 4_655 1_655
Ga3 O3 O1 34.4(3) 2_646 1_655
O3 O3 O1 64.9(6) 2_645 1_655
O3 O3 O1 73.4(5) 2_646 1_655
O3 O3 O1 85.2(4) 4_765 1_655
O3 O3 O1 25.4(4) 3_645 1_655
O2 O3 O1 37.4(3) 4_655 1_655
O2 O3 O1 147.2(4) 3_655 1_655
O2 O3 O1 132.6(5) 5_656 1_655
O1 O3 O1 139.9(3) . 1_655
O3 O3 O1 96.0(2) 6 1_655
O3 O3 O1 101.7(2) 6_556 1_655
O2 O3 O1 118.9(4) 5_655 1_655
Ga2 O3 O1 137.2(3) 1_545 1_655
Ga3 O3 O1 68.9(2) 4_765 1_655
O2 O3 O1 82.9(3) 1_545 1_655
La1 O3 O1 157.2(4) . 1_655
Ga2 O3 O1 60.88(17) 2_546 1_655
O3 O3 O1 53.4(2) 5_765 1_655
O3 O3 O1 60.0(2) 5_766 1_655
Ga3 O3 O1 100.2(3) 1_554 1_655
Nb O3 O1 81.3(3) 1_656 1_655
Ga1 O3 O1 81.3(3) 1_656 1_655
O2 O3 O1 112.4(3) 2_546 1_655
La1 O3 O1 94.1(3) 4_656 1_655
La1 O3 O1 110.0(2) 2_655 1_655
O1 O3 O1 60.4(2) 2_645 1_655
O2 O3 O1 34.6(3) 6_656 1_655
Ga3 O3 O1 55.9(3) 2_645 1_655
O2 O3 O1 106.2(3) 2_545 1_655
Ga2 O3 O1 143.7(2) 2_556 1_655
O2 O3 O1 33.4(3) 6_655 1_655
La1 O3 O1 28.36(13) 2_645 1_655
O1 O3 O1 67.8(2) 2_646 1_655
O2 O3 O1 56.13(19) 1_655 1_655
Ga2 O3 O1 117.5(3) 1_544 1_655
Ga3 O3 O1 100.3(2) 4_655 1_655
La1 O3 O1 28.29(12) 1_655 1_655
O1 O3 O1 135.0(2) 2_655 1_655
O3 O3 O1 93.8(2) 1_556 1_655
O3 O3 O1 86.2(2) 1_554 1_655
Ga3 O3 O1 71.1(2) 4_764 1_655
O2 O3 O1 83.4(2) 2_656 1_655
O2 O3 O1 145.0(3) 6_556 1_655
La1 O3 O1 136.9(3) 1_556 1_655
O2 O3 O1 53.02(18) 3_645 1_655
O1 O3 O1 135.6(2) 2_656 1_655
Ga3 O3 O2 94.5(4) . 2_655
Nb O3 O2 21.9(3) 1_655 2_655
Ga1 O3 O2 21.9(3) 1_655 2_655
La1 O3 O2 116.9(5) 4_655 2_655
Ga3 O3 O2 100.3(3) 2_646 2_655
O3 O3 O2 63.1(3) 2_645 2_655
O3 O3 O2 121.8(2) 2_646 2_655
O3 O3 O2 32.1(2) 4_765 2_655
O3 O3 O2 61.3(3) 3_645 2_655
O2 O3 O2 116.4(5) 4_655 2_655
O2 O3 O2 74.6(4) 3_655 2_655
O2 O3 O2 128.6(3) 5_656 2_655
O1 O3 O2 124.7(4) . 2_655
O3 O3 O2 25.5(2) 6 2_655
O3 O3 O2 86.4(4) 6_556 2_655
O2 O3 O2 75.7(4) 5_655 2_655
Ga2 O3 O2 142.7(4) 1_545 2_655
Ga3 O3 O2 54.8(2) 4_765 2_655
O2 O3 O2 149.3(3) 1_545 2_655
La1 O3 O2 85.8(3) . 2_655
Ga2 O3 O2 139.8(3) 2_546 2_655
O3 O3 O2 30.39(19) 5_765 2_655
O3 O3 O2 79.9(3) 5_766 2_655
Ga3 O3 O2 50.3(2) 1_554 2_655
Nb O3 O2 101.7(3) 1_656 2_655
Ga1 O3 O2 101.7(3) 1_656 2_655
O2 O3 O2 167.4(4) 2_546 2_655
La1 O3 O2 149.8(3) 4_656 2_655
La1 O3 O2 32.16(15) 2_655 2_655
O1 O3 O2 107.8(4) 2_645 2_655
O2 O3 O2 101.2(2) 6_656 2_655
Ga3 O3 O2 59.5(2) 2_645 2_655
O2 O3 O2 108.4(4) 2_545 2_655
Ga2 O3 O2 77.0(2) 2_556 2_655
O2 O3 O2 67.2(3) 6_655 2_655
La1 O3 O2 96.0(2) 2_645 2_655
O1 O3 O2 145.9(3) 2_646 2_655
O2 O3 O2 43.5(3) 1_655 2_655
Ga2 O3 O2 91.0(3) 1_544 2_655
Ga3 O3 O2 163.4(3) 4_655 2_655
La1 O3 O2 52.14(17) 1_655 2_655
O1 O3 O2 55.8(2) 2_655 2_655
O3 O3 O2 121.9(2) 1_556 2_655
O3 O3 O2 58.1(2) 1_554 2_655
Ga3 O3 O2 19.77(16) 4_764 2_655
O2 O3 O2 57.92(18) 2_656 2_655
O2 O3 O2 134.2(3) 6_556 2_655
La1 O3 O2 117.2(2) 1_556 2_655
O2 O3 O2 128.1(3) 3_645 2_655
O1 O3 O2 89.2(2) 2_656 2_655
O1 O3 O2 80.1(2) 1_655 2_655
Ga3 O3 O2 99.4(5) . 6
Nb O3 O2 105.6(5) 1_655 6
Ga1 O3 O2 105.6(5) 1_655 6
La1 O3 O2 50.6(3) 4_655 6
Ga3 O3 O2 153.8(3) 2_646 6
O3 O3 O2 75.4(5) 2_645 6
O3 O3 O2 135.1(4) 2_646 6
O3 O3 O2 117.9(5) 4_765 6
O3 O3 O2 148.3(2) 3_645 6
O2 O3 O2 115.9(4) 4_655 6
O2 O3 O2 70.2(3) 3_655 6
O2 O3 O2 82.0(3) 5_656 6
O1 O3 O2 26.9(4) . 6
O3 O3 O2 74.3(3) 6 6
O3 O3 O2 122.7(2) 6_556 6
O2 O3 O2 26.5(2) 5_655 6
Ga2 O3 O2 57.0(2) 1_545 6
Ga3 O3 O2 145.2(3) 4_765 6
O2 O3 O2 75.4(3) 1_545 6
La1 O3 O2 30.25(18) . 6
Ga2 O3 O2 101.6(2) 2_546 6
O3 O3 O2 107.9(5) 5_765 6
O3 O3 O2 164.4(3) 5_766 6
Ga3 O3 O2 53.6(2) 1_554 6
Nb O3 O2 140.3(3) 1_656 6
Ga1 O3 O2 140.3(3) 1_656 6
O2 O3 O2 72.65(17) 2_546 6
La1 O3 O2 104.9(2) 4_656 6
La1 O3 O2 86.3(3) 2_655 6
O1 O3 O2 78.1(3) 2_645 6
O2 O3 O2 152.9(4) 6_656 6
Ga3 O3 O2 85.4(3) 2_645 6
O2 O3 O2 31.2(2) 2_545 6
Ga2 O3 O2 76.4(2) 2_556 6
O2 O3 O2 105.3(4) 6_655 6
La1 O3 O2 109.8(3) 2_645 6
O1 O3 O2 111.2(2) 2_646 6
O2 O3 O2 142.8(3) 1_655 6
Ga2 O3 O2 19.07(16) 1_544 6
Ga3 O3 O2 68.33(19) 4_655 6
La1 O3 O2 133.9(3) 1_655 6
O1 O3 O2 55.4(2) 2_655 6
O3 O3 O2 121.5(2) 1_556 6
O3 O3 O2 58.5(2) 1_554 6
Ga3 O3 O2 93.8(3) 4_764 6
O2 O3 O2 134.2(3) 2_656 6
O2 O3 O2 57.24(16) 6_556 6
La1 O3 O2 83.1(2) 1_556 6
O2 O3 O2 99.8(3) 3_645 6
O1 O3 O2 88.6(3) 2_656 6
O1 O3 O2 135.5(3) 1_655 6
O2 O3 O2 99.6(4) 2_655 6
Ga3 O3 O2 43.3(4) . 4_665
Nb O3 O2 79.9(3) 1_655 4_665
Ga1 O3 O2 79.9(3) 1_655 4_665
La1 O3 O2 133.4(5) 4_655 4_665
Ga3 O3 O2 122.0(3) 2_646 4_665
O3 O3 O2 111.9(5) 2_645 4_665
O3 O3 O2 103.3(4) 2_646 4_665
O3 O3 O2 43.9(4) 4_765 4_665
O3 O3 O2 103.7(4) 3_645 4_665
O2 O3 O2 160.8(5) 4_655 4_665
O2 O3 O2 18.6(4) 3_655 4_665
O2 O3 O2 71.3(3) 5_656 4_665
O1 O3 O2 90.4(3) . 4_665
O3 O3 O2 58.5(3) 6 4_665
O3 O3 O2 52.3(3) 6_556 4_665
O2 O3 O2 80.1(3) 5_655 4_665
Ga2 O3 O2 88.3(3) 1_545 4_665
Ga3 O3 O2 63.6(2) 4_765 4_665
O2 O3 O2 147.3(3) 1_545 4_665
La1 O3 O2 53.3(2) . 4_665
Ga2 O3 O2 158.2(3) 2_546 4_665
O3 O3 O2 88.40(19) 5_765 4_665
O3 O3 O2 83.4(2) 5_766 4_665
Ga3 O3 O2 76.0(2) 1_554 4_665
Nb O3 O2 80.3(2) 1_656 4_665
Ga1 O3 O2 80.3(2) 1_656 4_665
O2 O3 O2 110.3(4) 2_546 4_665
La1 O3 O2 107.4(3) 4_656 4_665
La1 O3 O2 26.61(16) 2_655 4_665
O1 O3 O2 154.3(4) 2_645 4_665
O2 O3 O2 122.8(3) 6_656 4_665
Ga3 O3 O2 113.1(3) 2_645 4_665
O2 O3 O2 113.5(4) 2_545 4_665
Ga2 O3 O2 18.99(15) 2_556 4_665
O2 O3 O2 125.3(3) 6_655 4_665
La1 O3 O2 153.3(3) 2_645 4_665
O1 O3 O2 137.9(4) 2_646 4_665
O2 O3 O2 73.1(3) 1_655 4_665
Ga2 O3 O2 93.0(3) 1_544 4_665
Ga3 O3 O2 128.2(3) 4_655 4_665
La1 O3 O2 102.9(2) 1_655 4_665
O1 O3 O2 33.4(3) 2_655 4_665
O3 O3 O2 86.0(2) 1_556 4_665
O3 O3 O2 94.0(2) 1_554 4_665
Ga3 O3 O2 75.6(2) 4_764 4_665
O2 O3 O2 51.05(16) 2_656 4_665
O2 O3 O2 78.8(3) 6_556 4_665
La1 O3 O2 60.08(19) 1_556 4_665
O2 O3 O2 172.0(4) 3_645 4_665
O1 O3 O2 33.4(3) 2_656 4_665
O1 O3 O2 129.0(2) 1_655 4_665
O2 O3 O2 58.1(2) 2_655 4_665
O2 O3 O2 83.2(3) 6 4_665
Ga3 O3 Ga2 167.6(5) . 2_545
Nb O3 Ga2 76.7(3) 1_655 2_545
Ga1 O3 Ga2 76.7(3) 1_655 2_545
La1 O3 Ga2 29.95(19) 4_655 2_545
Ga3 O3 Ga2 91.4(3) 2_646 2_545
O3 O3 Ga2 31.0(2) 2_645 2_545
O3 O3 Ga2 118.6(5) 2_646 2_545
O3 O3 Ga2 124.1(2) 4_765 2_545
O3 O3 Ga2 85.3(4) 3_645 2_545
O2 O3 Ga2 56.8(3) 4_655 2_545
O2 O3 Ga2 136.1(5) 3_655 2_545
O2 O3 Ga2 132.8(3) 5_656 2_545
O1 O3 Ga2 80.6(3) . 2_545
O3 O3 Ga2 82.6(4) 6 2_545
O3 O3 Ga2 166.7(3) 6_556 2_545
O2 O3 Ga2 61.5(3) 5_655 2_545
Ga2 O3 Ga2 102.8(2) 1_545 2_545
Ga3 O3 Ga2 128.2(3) 4_765 2_545
O2 O3 Ga2 55.6(3) 1_545 2_545
La1 O3 Ga2 98.0(3) . 2_545
Ga2 O3 Ga2 62.34(14) 2_546 2_545
O3 O3 Ga2 70.4(3) 5_765 2_545
O3 O3 Ga2 125.3(2) 5_766 2_545
Ga3 O3 Ga2 62.00(17) 1_554 2_545
Nb O3 Ga2 140.0(3) 1_656 2_545
Ga1 O3 Ga2 140.0(3) 1_656 2_545
O2 O3 Ga2 92.7(3) 2_546 2_545
La1 O3 Ga2 110.7(2) 4_656 2_545
La1 O3 Ga2 116.8(3) 2_655 2_545
O1 O3 Ga2 16.8(2) 2_645 2_545
O2 O3 Ga2 90.9(3) 6_656 2_545
Ga3 O3 Ga2 35.36(9) 2_645 2_545
O2 O3 Ga2 41.43(19) 2_545 2_545
Ga2 O3 Ga2 143.5(3) 2_556 2_545
O2 O3 Ga2 41.2(2) 6_655 2_545
La1 O3 Ga2 40.45(9) 2_645 2_545
O1 O3 Ga2 83.3(2) 2_646 2_545
O2 O3 Ga2 109.6(3) 1_655 2_545
Ga2 O3 Ga2 53.57(12) 1_544 2_545
Ga3 O3 Ga2 71.61(13) 4_655 2_545
La1 O3 Ga2 75.90(16) 1_655 2_545
O1 O3 Ga2 105.8(4) 2_655 2_545
O3 O3 Ga2 135.62(14) 1_556 2_545
O3 O3 Ga2 44.38(14) 1_554 2_545
Ga3 O3 Ga2 74.25(17) 4_764 2_545
O2 O3 Ga2 141.9(3) 2_656 2_545
O2 O3 Ga2 110.4(2) 6_556 2_545
La1 O3 Ga2 142.2(2) 1_556 2_545
O2 O3 Ga2 49.80(18) 3_645 2_545
O1 O3 Ga2 158.9(3) 2_656 2_545
O1 O3 Ga2 65.4(2) 1_655 2_545
O2 O3 Ga2 94.0(3) 2_655 2_545
O2 O3 Ga2 70.3(2) 6 2_545
O2 O3 Ga2 137.9(3) 4_665 2_545
Ga3 O3 O3 63.1(5) . 3_545
Nb O3 O3 122.7(5) 1_655 3_545
Ga1 O3 O3 122.7(5) 1_655 3_545
La1 O3 O3 81.0(2) 4_655 3_545
Ga3 O3 O3 147.7(3) 2_646 3_545
O3 O3 O3 110.1(5) 2_645 3_545
O3 O3 O3 109.2(4) 2_646 3_545
O3 O3 O3 103.7(6) 4_765 3_545
O3 O3 O3 163.7(6) 3_645 3_545
O2 O3 O3 134.9(4) 4_655 3_545
O2 O3 O3 42.2(4) 3_655 3_545
O2 O3 O3 49.7(4) 5_656 3_545
O1 O3 O3 30.62(8) . 3_545
O3 O3 O3 86.62(14) 6 3_545
O3 O3 O3 86.72(15) 6_556 3_545
O2 O3 O3 56.3(3) 5_655 3_545
Ga2 O3 O3 38.08(14) 1_545 3_545
Ga3 O3 O3 120.8(4) 4_765 3_545
O2 O3 O3 88.7(2) 1_545 3_545
La1 O3 O3 21.84(19) . 3_545
Ga2 O3 O3 112.0(2) 2_546 3_545
O3 O3 O3 129.3(3) 5_765 3_545
O3 O3 O3 128.3(3) 5_766 3_545
Ga3 O3 O3 78.1(2) 1_554 3_545
Nb O3 O3 105.0(2) 1_656 3_545
Ga1 O3 O3 105.0(2) 1_656 3_545
O2 O3 O3 62.46(19) 2_546 3_545
La1 O3 O3 85.03(12) 4_656 3_545
La1 O3 O3 77.2(3) 2_655 3_545
O1 O3 O3 110.08(18) 2_645 3_545
O2 O3 O3 147.2(3) 6_656 3_545
Ga3 O3 O3 119.71(17) 2_645 3_545
O2 O3 O3 64.73(19) 2_545 3_545
Ga2 O3 O3 45.9(2) 2_556 3_545
O2 O3 O3 141.3(2) 6_655 3_545
La1 O3 O3 142.0(2) 2_645 3_545
O1 O3 O3 108.08(16) 2_646 3_545
O2 O3 O3 133.1(4) 1_655 3_545
Ga2 O3 O3 55.28(11) 1_544 3_545
Ga3 O3 O3 72.12(11) 4_655 3_545
La1 O3 O3 157.2(3) 1_655 3_545
O1 O3 O3 49.6(2) 2_655 3_545
O3 O3 O3 90.0 1_556 3_545
O3 O3 O3 90.000(1) 1_554 3_545
Ga3 O3 O3 111.5(3) 4_764 3_545
O2 O3 O3 106.2(3) 2_656 3_545
O2 O3 O3 31.9(2) 6_556 3_545
La1 O3 O3 47.87(17) 1_556 3_545
O2 O3 O3 118.6(2) 3_645 3_545
O1 O3 O3 53.3(3) 2_656 3_545
O1 O3 O3 170.4(3) 1_655 3_545
O2 O3 O3 105.3(3) 2_655 3_545
O2 O3 O3 36.54(19) 6 3_545
O2 O3 O3 60.1(3) 4_665 3_545
Ga2 O3 O3 105.91(13) 2_545 3_545
Ga3 O3 O3 103.1(3) . 4_655
Nb O3 O3 139.4(4) 1_655 4_655
Ga1 O3 O3 139.4(4) 1_655 4_655
La1 O3 O3 35.9(3) 4_655 4_655
Ga3 O3 O3 106.2(3) 2_646 4_655
O3 O3 O3 92.02(5) 2_645 4_655
O3 O3 O3 91.93(5) 2_646 4_655
O3 O3 O3 163.7(6) 4_765 4_655
O3 O3 O3 136.3(6) 3_645 4_655
O2 O3 O3 75.6(4) 4_655 4_655
O2 O3 O3 101.5(4) 3_655 4_655
O2 O3 O3 67.8(3) 5_656 4_655
O1 O3 O3 30.62(8) . 4_655
O3 O3 O3 121.2(3) 6 4_655
O3 O3 O3 120.1(3) 6_556 4_655
O2 O3 O3 71.1(3) 5_655 4_655
Ga2 O3 O3 38.08(14) 1_545 4_655
Ga3 O3 O3 158.8(2) 4_765 4_655
O2 O3 O3 29.1(2) 1_545 4_655
La1 O3 O3 72.12(15) . 4_655
Ga2 O3 O3 54.9(2) 2_546 4_655
O3 O3 O3 134.9(3) 5_765 4_655
O3 O3 O3 133.6(3) 5_766 4_655
Ga3 O3 O3 95.90(14) 1_554 4_655
Nb O3 O3 111.31(15) 1_656 4_655
Ga1 O3 O3 111.31(15) 1_656 4_655
O2 O3 O3 32.0(3) 2_546 4_655
La1 O3 O3 63.43(15) 4_656 4_655
La1 O3 O3 134.1(3) 2_655 4_655
O1 O3 O3 58.2(2) 2_645 4_655
O2 O3 O3 105.2(3) 6_656 4_655
Ga3 O3 O3 99.40(18) 2_645 4_655
O2 O3 O3 38.5(3) 2_545 4_655
Ga2 O3 O3 103.6(2) 2_556 4_655
O2 O3 O3 104.1(3) 6_655 4_655
La1 O3 O3 84.9(2) 2_645 4_655
O1 O3 O3 61.6(2) 2_646 4_655
O2 O3 O3 166.0(4) 1_655 4_655
Ga2 O3 O3 55.28(11) 1_544 4_655
Ga3 O3 O3 19.03(15) 4_655 4_655
La1 O3 O3 135.7(3) 1_655 4_655
O1 O3 O3 102.6(2) 2_655 4_655
O3 O3 O3 90.000(1) 1_556 4_655
O3 O3 O3 90.000(1) 1_554 4_655
Ga3 O3 O3 131.92(14) 4_764 4_655
O2 O3 O3 151.6(2) 2_656 4_655
O2 O3 O3 46.7(2) 6_556 4_655
La1 O3 O3 77.18(13) 1_556 4_655
O2 O3 O3 58.7(2) 3_645 4_655
O1 O3 O3 101.61(19) 2_656 4_655
O1 O3 O3 111.1(3) 1_655 4_655
O2 O3 O3 146.2(2) 2_655 4_655
O2 O3 O3 49.57(17) 6 4_655
O2 O3 O3 119.9(3) 4_665 4_655
Ga2 O3 O3 65.15(17) 2_545 4_655
O3 O3 O3 60.0 3_545 4_655
Ga3 O3 Ga2 108.8(5) . 1_645
Nb O3 Ga2 74.4(4) 1_655 1_645
Ga1 O3 Ga2 74.4(4) 1_655 1_645
La1 O3 Ga2 99.1(3) 4_655 1_645
Ga3 O3 Ga2 15.57(16) 2_646 1_645
O3 O3 Ga2 83.6(5) 2_645 1_645
O3 O3 Ga2 54.6(4) 2_646 1_645
O3 O3 Ga2 85.3(4) 4_765 1_645
O3 O3 Ga2 29.1(3) 3_645 1_645
O2 O3 Ga2 35.8(3) 4_655 1_645
O2 O3 Ga2 140.4(4) 3_655 1_645
O2 O3 Ga2 114.1(5) 5_656 1_645
O1 O3 Ga2 140.9(3) . 1_645
O3 O3 Ga2 110.60(13) 6 1_645
O3 O3 Ga2 86.6(2) 6_556 1_645
O2 O3 Ga2 137.5(4) 5_655 1_645
Ga2 O3 Ga2 125.1(3) 1_545 1_645
Ga3 O3 Ga2 62.29(19) 4_765 1_645
O2 O3 Ga2 81.3(3) 1_545 1_645
La1 O3 Ga2 175.6(3) . 1_645
Ga2 O3 Ga2 55.65(16) 2_546 1_645
O3 O3 Ga2 68.1(2) 5_765 1_645
O3 O3 Ga2 45.97(12) 5_766 1_645
Ga3 O3 Ga2 118.6(3) 1_554 1_645
Nb O3 Ga2 63.39(18) 1_656 1_645
Ga1 O3 Ga2 63.39(18) 1_656 1_645
O2 O3 Ga2 101.4(3) 2_546 1_645
La1 O3 Ga2 77.5(2) 4_656 1_645
La1 O3 Ga2 115.2(2) 2_655 1_645
O1 O3 Ga2 71.2(2) 2_645 1_645
O2 O3 Ga2 15.83(19) 6_656 1_645
Ga3 O3 Ga2 74.79(18) 2_645 1_645
O2 O3 Ga2 118.1(3) 2_545 1_645
Ga2 O3 Ga2 134.3(2) 2_556 1_645
O2 O3 Ga2 52.2(2) 6_655 1_645
La1 O3 Ga2 39.91(10) 2_645 1_645
O1 O3 Ga2 55.69(14) 2_646 1_645
O2 O3 Ga2 55.64(18) 1_655 1_645
Ga2 O3 Ga2 133.7(2) 1_544 1_645
Ga3 O3 Ga2 95.0(2) 4_655 1_645
La1 O3 Ga2 39.62(10) 1_655 1_645
O1 O3 Ga2 145.5(2) 2_655 1_645
O3 O3 Ga2 74.90(14) 1_556 1_645
O3 O3 Ga2 105.10(14) 1_554 1_645
Ga3 O3 Ga2 85.83(17) 4_764 1_645
O2 O3 Ga2 75.3(2) 2_656 1_645
O2 O3 Ga2 130.7(3) 6_556 1_645
La1 O3 Ga2 118.0(3) 1_556 1_645
O2 O3 Ga2 52.82(18) 3_645 1_645
O1 O3 Ga2 120.7(3) 2_656 1_645
O1 O3 Ga2 18.9(2) 1_655 1_645
O2 O3 Ga2 90.3(2) 2_655 1_645
O2 O3 Ga2 149.3(3) 6 1_645
O2 O3 Ga2 125.9(2) 4_665 1_645
Ga2 O3 Ga2 80.15(16) 2_545 1_645
O3 O3 Ga2 162.54(19) 3_545 1_645
O3 O3 Ga2 110.4(3) 4_655 1_645
Ga3 O3 O2 166.9(6) . 4_654
Nb O3 O2 58.1(3) 1_655 4_654
Ga1 O3 O2 58.1(3) 1_655 4_654
La1 O3 O2 46.6(2) 4_655 4_654
Ga3 O3 O2 93.7(3) 2_646 4_654
O3 O3 O2 12.4(3) 2_645 4_654
O3 O3 O2 128.6(6) 2_646 4_654
O3 O3 O2 105.3(2) 4_765 4_654
O3 O3 O2 75.5(3) 3_645 4_654
O2 O3 O2 66.5(3) 4_655 4_654
O2 O3 O2 128.5(5) 3_655 4_654
O2 O3 O2 150.0(4) 5_656 4_654
O1 O3 O2 92.3(4) . 4_654
O3 O3 O2 65.7(4) 6 4_654
O3 O3 O2 156.7(3) 6_556 4_654
O2 O3 O2 58.1(4) 5_655 4_654
Ga2 O3 O2 118.8(3) 1_545 4_654
Ga3 O3 O2 113.7(3) 4_765 4_654
O2 O3 O2 74.4(3) 1_545 4_654
La1 O3 O2 97.3(3) . 4_654
Ga2 O3 O2 77.9(2) 2_546 4_654
O3 O3 O2 52.4(3) 5_765 4_654
O3 O3 O2 119.3(4) 5_766 4_654
Ga3 O3 O2 49.3(2) 1_554 4_654
Nb O3 O2 142.9(3) 1_656 4_654
Ga1 O3 O2 142.9(3) 1_656 4_654
O2 O3 O2 111.4(3) 2_546 4_654
La1 O3 O2 128.2(3) 4_656 4_654
La1 O3 O2 99.7(3) 2_655 4_654
O1 O3 O2 33.8(3) 2_645 4_654
O2 O3 O2 93.6(4) 6_656 4_654
Ga3 O3 O2 16.89(12) 2_645 4_654
O2 O3 O2 52.17(18) 2_545 4_654
Ga2 O3 O2 135.6(3) 2_556 4_654
O2 O3 O2 30.3(3) 6_655 4_654
La1 O3 O2 44.46(19) 2_645 4_654
O1 O3 O2 98.4(3) 2_646 4_654
O2 O3 O2 94.5(2) 1_655 4_654
Ga2 O3 O2 56.25(19) 1_544 4_654
Ga3 O3 O2 90.49(19) 4_655 4_654
La1 O3 O2 63.4(2) 1_655 4_654
O1 O3 O2 95.4(4) 2_655 4_654
O3 O3 O2 149.0(2) 1_556 4_654
O3 O3 O2 31.0(2) 1_554 4_654
Ga3 O3 O2 55.31(18) 4_764 4_654
O2 O3 O2 125.6(3) 2_656 4_654
O2 O3 O2 125.1(3) 6_556 4_654
La1 O3 O2 156.8(3) 1_556 4_654
O2 O3 O2 64.34(17) 3_645 4_654
O1 O3 O2 154.9(4) 2_656 4_654
O1 O3 O2 61.7(3) 1_655 4_654
O2 O3 O2 75.1(3) 2_655 4_654
O2 O3 O2 75.2(2) 6 4_654
O2 O3 O2 123.7(4) 4_665 4_654
Ga2 O3 O2 18.95(13) 2_545 4_654
O3 O3 O2 111.52(18) 3_545 4_654
O3 O3 O2 82.6(2) 4_655 4_654
Ga2 O3 O2 79.6(2) 1_645 4_654
Ga3 O3 O2 45.6(4) . .
Nb O3 O2 103.3(4) 1_655 .
Ga1 O3 O2 103.3(4) 1_655 .
La1 O3 O2 108.5(4) 4_655 .
Ga3 O3 O2 141.2(4) 2_646 .
O3 O3 O2 116.0(7) 2_645 .
O3 O3 O2 107.2(5) 2_646 .
O3 O3 O2 73.9(5) 4_765 .
O3 O3 O2 133.8(5) 3_645 .
O2 O3 O2 161.4(5) 4_655 .
O2 O3 O2 12.3(4) 3_655 .
O2 O3 O2 54.6(4) 5_656 .
O1 O3 O2 60.6(3) . .
O3 O3 O2 71.8(2) 6 .
O3 O3 O2 66.0(2) 6_556 .
O2 O3 O2 66.6(3) 5_655 .
Ga2 O3 O2 61.1(2) 1_545 .
Ga3 O3 O2 91.8(3) 4_765 .
O2 O3 O2 117.9(3) 1_545 .
La1 O3 O2 29.37(18) . .
Ga2 O3 O2 138.0(3) 2_546 .
O3 O3 O2 111.6(2) 5_765 .
O3 O3 O2 105.9(2) 5_766 .
Ga3 O3 O2 76.6(3) 1_554 .
Nb O3 O2 91.5(2) 1_656 .
Ga1 O3 O2 91.5(2) 1_656 .
O2 O3 O2 85.3(3) 2_546 .
La1 O3 O2 95.6(2) 4_656 .
La1 O3 O2 50.69(19) 2_655 .
O1 O3 O2 136.9(3) 2_645 .
O2 O3 O2 141.6(3) 6_656 .
Ga3 O3 O2 122.4(3) 2_645 .
O2 O3 O2 89.9(3) 2_545 .
Ga2 O3 O2 17.65(16) 2_556 .
O2 O3 O2 143.1(3) 6_655 .
La1 O3 O2 167.6(3) 2_645 .
O1 O3 O2 126.1(3) 2_646 .
O2 O3 O2 103.1(3) 1_655 .
Ga2 O3 O2 73.8(2) 1_544 .
Ga3 O3 O2 99.8(2) 4_655 .
La1 O3 O2 132.0(2) 1_655 .
O1 O3 O2 32.5(3) 2_655 .
O3 O3 O2 86.1(2) 1_556 .
O3 O3 O2 93.9(2) 1_554 .
Ga3 O3 O2 95.1(2) 4_764 .
O2 O3 O2 77.8(2) 2_656 .
O2 O3 O2 52.1(3) 6_556 .
La1 O3 O2 45.98(19) 1_556 .
O2 O3 O2 147.5(2) 3_645 .
O1 O3 O2 32.8(3) 2_656 .
O1 O3 O2 159.1(2) 1_655 .
O2 O3 O2 82.2(2) 2_655 .
O2 O3 O2 58.8(3) 6 .
O2 O3 O2 30.09(18) 4_665 .
Ga2 O3 O2 127.2(3) 2_545 .
O3 O3 O2 30.1(2) 3_545 .
O3 O3 O2 89.8(2) 4_655 .
Ga2 O3 O2 151.9(3) 1_645 .
O2 O3 O2 123.7(4) 4_654 .
Ga3 O3 O2 105.7(5) . 3_654
Nb O3 O2 58.6(4) 1_655 3_654
Ga1 O3 O2 58.6(4) 1_655 3_654
La1 O3 O2 77.6(4) 4_655 3_654
Ga3 O3 O2 144.7(4) 2_646 3_654
O3 O3 O2 52.4(5) 2_645 3_654
O3 O3 O2 168.0(4) 2_646 3_654
O3 O3 O2 76.2(3) 4_765 3_654
O3 O3 O2 105.7(2) 3_645 3_654
O2 O3 O2 128.2(5) 4_655 3_654
O2 O3 O2 66.9(4) 3_655 3_654
O2 O3 O2 115.4(6) 5_656 3_654
O1 O3 O2 75.1(4) . 3_654
O3 O3 O2 25.7(3) 6 3_654
O3 O3 O2 116.7(5) 6_556 3_654
O2 O3 O2 24.9(3) 5_655 3_654
Ga2 O3 O2 102.2(3) 1_545 3_654
Ga3 O3 O2 103.8(3) 4_765 3_654
O2 O3 O2 114.3(4) 1_545 3_654
La1 O3 O2 46.0(2) . 3_654
Ga2 O3 O2 133.6(3) 2_546 3_654
O3 O3 O2 63.1(3) 5_765 3_654
O3 O3 O2 130.3(3) 5_766 3_654
Ga3 O3 O2 12.76(14) 1_554 3_654
Nb O3 O2 143.6(3) 1_656 3_654
Ga1 O3 O2 143.6(3) 1_656 3_654
O2 O3 O2 121.3(3) 2_546 3_654
La1 O3 O2 151.9(3) 4_656 3_654
La1 O3 O2 49.5(2) 2_655 3_654
O1 O3 O2 89.4(4) 2_645 3_654
O2 O3 O2 145.2(3) 6_656 3_654
Ga3 O3 O2 58.7(2) 2_645 3_654
O2 O3 O2 61.7(3) 2_545 3_654
Ga2 O3 O2 74.0(2) 2_556 3_654
O2 O3 O2 80.7(3) 6_655 3_654
La1 O3 O2 105.4(3) 2_645 3_654
O1 O3 O2 153.0(3) 2_646 3_654
O2 O3 O2 94.7(2) 1_655 3_654
Ga2 O3 O2 41.09(17) 1_544 3_654
Ga3 O3 O2 114.8(3) 4_655 3_654
La1 O3 O2 92.1(2) 1_655 3_654
O1 O3 O2 33.8(3) 2_655 3_654
O3 O3 O2 149.30(18) 1_556 3_654
O3 O3 O2 30.70(18) 1_554 3_654
Ga3 O3 O2 46.47(18) 4_764 3_654
O2 O3 O2 101.2(3) 2_656 3_654
O2 O3 O2 98.7(3) 6_556 3_654
La1 O3 O2 109.1(3) 1_556 3_654
O2 O3 O2 122.6(3) 3_645 3_654
O1 O3 O2 93.2(3) 2_656 3_654
O1 O3 O2 111.8(3) 1_655 3_654
O2 O3 O2 51.2(3) 2_655 3_654
O2 O3 O2 48.73(19) 6 3_654
O2 O3 O2 64.9(2) 4_665 3_654
Ga2 O3 O2 73.0(2) 2_545 3_654
O3 O3 O2 67.6(2) 3_545 3_654
O3 O3 O2 95.90(18) 4_655 3_654
Ga2 O3 O2 129.7(3) 1_645 3_654
O2 O3 O2 61.7(3) 4_654 3_654
O2 O3 O2 63.9(2) . 3_654
Ga3 O3 La1 97.3(4) . 2_545
Nb O3 La1 128.2(5) 1_655 2_545
Ga1 O3 La1 128.2(5) 1_655 2_545
La1 O3 La1 42.0(2) 4_655 2_545
Ga3 O3 La1 131.2(3) 2_646 2_545
O3 O3 La1 88.0(3) 2_645 2_545
O3 O3 La1 111.4(2) 2_646 2_545
O3 O3 La1 140.2(5) 4_765 2_545
O3 O3 La1 154.8(5) 3_645 2_545
O2 O3 La1 98.6(3) 4_655 2_545
O2 O3 La1 81.9(4) 3_655 2_545
O2 O3 La1 68.5(3) 5_656 2_545
O1 O3 La1 10.3(2) . 2_545
O3 O3 La1 99.6(3) 6 2_545
O3 O3 La1 119.9(2) 6_556 2_545
O2 O3 La1 50.2(2) 5_655 2_545
Ga2 O3 La1 38.18(13) 1_545 2_545
Ga3 O3 La1 160.4(3) 4_765 2_545
O2 O3 La1 53.3(2) 1_545 2_545
La1 O3 La1 47.72(12) . 2_545
Ga2 O3 La1 79.54(16) 2_546 2_545
O3 O3 La1 128.2(5) 5_765 2_545
O3 O3 La1 152.0(5) 5_766 2_545
Ga3 O3 La1 77.2(2) 1_554 2_545
Nb O3 La1 124.4(3) 1_656 2_545
Ga1 O3 La1 124.4(3) 1_656 2_545
O2 O3 La1 48.1(2) 2_546 2_545
La1 O3 La1 81.08(16) 4_656 2_545
La1 O3 La1 109.2(3) 2_655 2_545
O1 O3 La1 70.76(15) 2_645 2_545
O2 O3 La1 130.3(3) 6_656 2_545
Ga3 O3 La1 97.5(2) 2_645 2_545
O2 O3 La1 30.6(2) 2_545 2_545
Ga2 O3 La1 85.91(19) 2_556 2_545
O2 O3 La1 111.3(3) 6_655 2_545
La1 O3 La1 102.10(17) 2_645 2_545
O1 O3 La1 86.09(16) 2_646 2_545
O2 O3 La1 168.3(3) 1_655 2_545
Ga2 O3 La1 36.84(9) 1_544 2_545
Ga3 O3 La1 43.14(9) 4_655 2_545
La1 O3 La1 146.0(2) 1_655 2_545
O1 O3 La1 77.71(19) 2_655 2_545
O3 O3 La1 102.67(14) 1_556 2_545
O3 O3 La1 77.33(14) 1_554 2_545
Ga3 O3 La1 117.1(3) 4_764 2_545
O2 O3 La1 145.7(3) 2_656 2_545
O2 O3 La1 42.51(19) 6_556 2_545
La1 O3 La1 74.06(15) 1_556 2_545
O2 O3 La1 81.51(19) 3_645 2_545
O1 O3 La1 90.77(19) 2_656 2_545
O1 O3 La1 130.4(2) 1_655 2_545
O2 O3 La1 125.0(3) 2_655 2_545
O2 O3 La1 25.53(15) 6 2_545
O2 O3 La1 98.9(3) 4_665 2_545
Ga2 O3 La1 70.40(13) 2_545 2_545
O3 O3 La1 39.99(9) 3_545 2_545
O3 O3 La1 25.01(9) 4_655 2_545
Ga2 O3 La1 134.3(2) 1_645 2_545
O2 O3 La1 82.8(2) 4_654 2_545
O2 O3 La1 69.6(2) . 2_545
O2 O3 La1 74.0(2) 3_654 2_545
Ga3 O3 La1 19.6(2) . 2_656
Nb O3 La1 96.9(3) 1_655 2_656
Ga1 O3 La1 96.9(3) 1_655 2_656
La1 O3 La1 157.3(4) 4_655 2_656
Ga3 O3 La1 84.9(3) 2_646 2_656
O3 O3 La1 143.6(2) 2_645 2_656
O3 O3 La1 61.4(3) 2_646 2_656
O3 O3 La1 49.7(2) 4_765 2_656
O3 O3 La1 87.9(3) 3_645 2_656
O2 O3 La1 121.4(4) 4_655 2_656
O2 O3 La1 47.1(3) 3_655 2_656
O2 O3 La1 54.1(3) 5_656 2_656
O1 O3 La1 106.5(4) . 2_656
O3 O3 La1 94.2(4) 6 2_656
O3 O3 La1 10.2(2) 6_556 2_656
O2 O3 La1 121.1(3) 5_655 2_656
Ga2 O3 La1 84.4(2) 1_545 2_656
Ga3 O3 La1 44.57(12) 4_765 2_656
O2 O3 La1 129.3(3) 1_545 2_656
La1 O3 La1 86.5(2) . 2_656
Ga2 O3 La1 119.2(3) 2_546 2_656
O3 O3 La1 102.8(3) 5_765 2_656
O3 O3 La1 49.2(2) 5_766 2_656
Ga3 O3 La1 116.8(2) 1_554 2_656
Nb O3 La1 38.28(9) 1_656 2_656
Ga1 O3 La1 38.28(9) 1_656 2_656
O2 O3 La1 93.6(3) 2_546 2_656
La1 O3 La1 73.16(18) 4_656 2_656
La1 O3 La1 60.32(13) 2_655 2_656
O1 O3 La1 163.5(4) 2_645 2_656
O2 O3 La1 85.4(3) 6_656 2_656
Ga3 O3 La1 138.2(2) 2_645 2_656
O2 O3 La1 145.1(3) 2_545 2_656
Ga2 O3 La1 40.03(10) 2_556 2_656
O2 O3 La1 131.6(3) 6_655 2_656
La1 O3 La1 134.9(3) 2_645 2_656
O1 O3 La1 98.5(3) 2_646 2_656
O2 O3 La1 63.2(2) 1_655 2_656
Ga2 O3 La1 130.9(3) 1_544 2_656
Ga3 O3 La1 114.4(2) 4_655 2_656
La1 O3 La1 96.88(18) 1_655 2_656
O1 O3 La1 75.2(2) 2_655 2_656
O3 O3 La1 46.60(13) 1_556 2_656
O3 O3 La1 133.40(13) 1_554 2_656
Ga3 O3 La1 100.16(16) 4_764 2_656
O2 O3 La1 30.86(18) 2_656 2_656
O2 O3 La1 76.8(2) 6_556 2_656
La1 O3 La1 45.03(10) 1_556 2_656
O2 O3 La1 130.7(3) 3_645 2_656
O1 O3 La1 27.01(11) 2_656 2_656
O1 O3 La1 108.6(2) 1_655 2_656
O2 O3 La1 80.6(2) 2_655 2_656
O2 O3 La1 115.2(3) 6 2_656
O2 O3 La1 42.08(18) 4_665 2_656
Ga2 O3 La1 172.7(2) 2_545 2_656
O3 O3 La1 80.3(2) 3_545 2_656
O3 O3 La1 121.90(16) 4_655 2_656
Ga2 O3 La1 94.9(2) 1_645 2_656
O2 O3 La1 155.0(2) 4_654 2_656
O2 O3 La1 57.15(19) . 2_656
O2 O3 La1 106.7(2) 3_654 2_656
La1 O3 La1 116.7(2) 2_545 2_656
Ga3 O3 O1 47.7(3) . 1_556
Nb O3 O1 159.4(4) 1_655 1_556
Ga1 O3 O1 159.4(4) 1_655 1_556
La1 O3 O1 96.6(3) 4_655 1_556
Ga3 O3 O1 86.5(3) 2_646 1_556
O3 O3 O1 152.96(13) 2_645 1_556
O3 O3 O1 48.9(4) 2_646 1_556
O3 O3 O1 112.6(3) 4_765 1_556
O3 O3 O1 122.8(2) 3_645 1_556
O2 O3 O1 92.2(4) 4_655 1_556
O2 O3 O1 73.5(4) 3_655 1_556
O2 O3 O1 16.0(3) 5_656 1_556
O1 O3 O1 62.6(3) . 1_556
O3 O3 O1 142.1(3) 6 1_556
O3 O3 O1 59.2(3) 6_556 1_556
O2 O3 O1 114.0(4) 5_655 1_556
Ga2 O3 O1 31.51(19) 1_545 1_556
Ga3 O3 O1 99.6(3) 4_765 1_556
O2 O3 O1 68.4(3) 1_545 1_556
La1 O3 O1 82.7(2) . 1_556
Ga2 O3 O1 72.34(19) 2_546 1_556
O3 O3 O1 162.6(5) 5_765 1_556
O3 O3 O1 83.1(4) 5_766 1_556
Ga3 O3 O1 139.1(3) 1_554 1_556
Nb O3 O1 55.22(17) 1_656 1_556
Ga1 O3 O1 55.22(17) 1_656 1_556
O2 O3 O1 30.7(2) 2_546 1_556
La1 O3 O1 25.47(9) 4_656 1_556
La1 O3 O1 113.2(2) 2_655 1_556
O1 O3 O1 110.0(3) 2_645 1_556
O2 O3 O1 86.1(3) 6_656 1_556
Ga3 O3 O1 158.2(2) 2_645 1_556
O2 O3 O1 97.3(3) 2_545 1_556
Ga2 O3 O1 69.01(16) 2_556 1_556
O2 O3 O1 146.0(3) 6_655 1_556
La1 O3 O1 116.2(2) 2_645 1_556
O1 O3 O1 55.91(18) 2_646 1_556
O2 O3 O1 117.9(3) 1_655 1_556
Ga2 O3 O1 105.0(2) 1_544 1_556
Ga3 O3 O1 51.54(13) 4_655 1_556
La1 O3 O1 137.4(3) 1_655 1_556
O1 O3 O1 102.7(3) 2_655 1_556
O3 O3 O1 33.84(15) 1_556 1_556
O3 O3 O1 146.16(15) 1_554 1_556
Ga3 O3 O1 161.8(2) 4_764 1_556
O2 O3 O1 90.5(3) 2_656 1_556
O2 O3 O1 31.4(2) 6_556 1_556
La1 O3 O1 26.71(6) 1_556 1_556
O2 O3 O1 86.0(2) 3_645 1_556
O1 O3 O1 53.85(17) 2_656 1_556
O1 O3 O1 119.2(3) 1_655 1_556
O2 O3 O1 142.3(3) 2_655 1_556
O2 O3 O1 88.1(2) 6 1_556
O2 O3 O1 86.7(2) 4_665 1_556
Ga2 O3 O1 123.14(19) 2_545 1_556
O3 O3 O1 61.16(12) 3_545 1_556
O3 O3 O1 61.16(12) 4_655 1_556
Ga2 O3 O1 101.7(2) 1_645 1_556
O2 O3 O1 142.0(2) 4_654 1_556
O2 O3 O1 70.4(2) . 1_556
O2 O3 O1 128.6(3) 3_654 1_556
La1 O3 O1 69.17(16) 2_545 1_556
La1 O3 O1 62.95(14) 2_656 1_556
Ga3 O3 O3 34.3(3) . 4_766
Nb O3 O3 103.6(5) 1_655 4_766
Ga1 O3 O3 103.6(5) 1_655 4_766
La1 O3 O3 148.6(4) 4_655 4_766
Ga3 O3 O3 62.1(2) 2_646 4_766
O3 O3 O3 148.4(5) 2_645 4_766
O3 O3 O3 37.6(3) 2_646 4_766
O3 O3 O3 62.14(16) 4_765 4_766
O3 O3 O3 76.49(7) 3_645 4_766
O2 O3 O3 97.0(4) 4_655 4_766
O2 O3 O3 70.5(4) 3_655 4_766
O2 O3 O3 55.1(3) 5_656 4_766
O1 O3 O3 114.8(5) . 4_766
O3 O3 O3 113.7(5) 6 4_766
O3 O3 O3 14.3(2) 6_556 4_766
O2 O3 O3 145.1(4) 5_655 4_766
Ga2 O3 O3 85.7(2) 1_545 4_766
Ga3 O3 O3 43.3(2) 4_765 4_766
O2 O3 O3 111.7(3) 1_545 4_766
La1 O3 O3 107.9(3) . 4_766
Ga2 O3 O3 96.0(2) 2_546 4_766
O3 O3 O3 106.5(5) 5_765 4_766
O3 O3 O3 32.5(3) 5_766 4_766
Ga3 O3 O3 139.0(3) 1_554 4_766
Nb O3 O3 13.76(8) 1_656 4_766
Ga1 O3 O3 13.76(8) 1_656 4_766
O2 O3 O3 84.7(3) 2_546 4_766
La1 O3 O3 56.16(12) 4_656 4_766
La1 O3 O3 81.9(3) 2_655 4_766
O1 O3 O3 139.0(4) 2_645 4_766
O2 O3 O3 62.5(3) 6_656 4_766
Ga3 O3 O3 138.8(3) 2_645 4_766
O2 O3 O3 153.5(4) 2_545 4_766
Ga2 O3 O3 63.1(2) 2_556 4_766
O2 O3 O3 121.5(4) 6_655 4_766
La1 O3 O3 113.3(3) 2_645 4_766
O1 O3 O3 75.9(2) 2_646 4_766
O2 O3 O3 61.7(3) 1_655 4_766
Ga2 O3 O3 151.4(3) 1_544 4_766
Ga3 O3 O3 102.5(2) 4_655 4_766
La1 O3 O3 89.3(3) 1_655 4_766
O1 O3 O3 99.7(3) 2_655 4_766
O3 O3 O3 27.86(16) 1_556 4_766
O3 O3 O3 152.14(16) 1_554 4_766
Ga3 O3 O3 111.2(3) 4_764 4_766
O2 O3 O3 36.2(3) 2_656 4_766
O2 O3 O3 81.2(3) 6_556 4_766
La1 O3 O3 50.91(16) 1_556 4_766
O2 O3 O3 106.5(3) 3_645 4_766
O1 O3 O3 46.5(2) 2_656 4_766
O1 O3 O3 91.1(3) 1_655 4_766
O2 O3 O3 94.1(3) 2_655 4_766
O2 O3 O3 132.9(3) 6 4_766
O2 O3 O3 66.5(3) 4_665 4_766
Ga2 O3 O3 153.3(3) 2_545 4_766
O3 O3 O3 96.4(3) 3_545 4_766
O3 O3 O3 116.65(19) 4_655 4_766
Ga2 O3 O3 74.4(2) 1_645 4_766
O2 O3 O3 151.8(4) 4_654 4_766
O2 O3 O3 79.1(3) . 4_766
O2 O3 O3 130.4(3) 3_654 4_766
La1 O3 O3 123.6(3) 2_545 4_766
La1 O3 O3 24.52(14) 2_656 4_766
O1 O3 O3 56.32(19) 1_556 4_766
Ga3 O3 O3 116.8(5) . 4_764
Nb O3 O3 29.8(3) 1_655 4_764
Ga1 O3 O3 29.8(3) 1_655 4_764
La1 O3 O3 87.0(3) 4_655 4_764
Ga3 O3 O3 115.5(4) 2_646 4_764
O3 O3 O3 38.3(4) 2_645 4_764
O3 O3 O3 148.9(4) 2_646 4_764
O3 O3 O3 62.14(16) 4_765 4_764
O3 O3 O3 76.49(7) 3_645 4_764
O2 O3 O3 110.7(4) 4_655 4_764
O2 O3 O3 84.3(5) 3_655 4_764
O2 O3 O3 140.6(5) 5_656 4_764
O1 O3 O3 102.8(4) . 4_764
O3 O3 O3 15.5(3) 6 4_764
O3 O3 O3 115.2(5) 6_556 4_764
O2 O3 O3 49.6(3) 5_655 4_764
Ga2 O3 O3 131.5(4) 1_545 4_764
Ga3 O3 O3 84.6(3) 4_765 4_764
O2 O3 O3 122.6(3) 1_545 4_764
La1 O3 O3 74.5(3) . 4_764
Ga2 O3 O3 127.8(3) 2_546 4_764
O3 O3 O3 33.8(3) 5_765 4_764
O3 O3 O3 107.9(4) 5_766 4_764
Ga3 O3 O3 22.43(11) 1_554 4_764
Nb O3 O3 132.0(3) 1_656 4_764
Ga1 O3 O3 132.0(3) 1_656 4_764
O2 O3 O3 147.3(4) 2_546 4_764
La1 O3 O3 178.4(3) 4_656 4_764
La1 O3 O3 49.1(2) 2_655 4_764
O1 O3 O3 84.3(3) 2_645 4_764
O2 O3 O3 116.1(3) 6_656 4_764
Ga3 O3 O3 39.32(9) 2_645 4_764
O2 O3 O3 78.3(3) 2_545 4_764
Ga2 O3 O3 89.7(3) 2_556 4_764
O2 O3 O3 57.2(2) 6_655 4_764
La1 O3 O3 86.33(18) 2_645 4_764
O1 O3 O3 146.8(3) 2_646 4_764
O2 O3 O3 70.3(3) 1_655 4_764
Ga2 O3 O3 63.0(2) 1_544 4_764
Ga3 O3 O3 133.0(3) 4_655 4_764
La1 O3 O3 62.74(18) 1_655 4_764
O1 O3 O3 53.5(3) 2_655 4_764
O3 O3 O3 152.14(16) 1_556 4_764
O3 O3 O3 27.86(16) 1_554 4_764
Ga3 O3 O3 17.87(13) 4_764 4_764
O2 O3 O3 88.3(3) 2_656 4_764
O2 O3 O3 127.9(4) 6_556 4_764
La1 O3 O3 131.3(3) 1_556 4_764
O2 O3 O3 113.9(3) 3_645 4_764
O1 O3 O3 107.3(3) 2_656 4_764
O1 O3 O3 84.4(3) 1_655 4_764
O2 O3 O3 30.4(2) 2_655 4_764
O2 O3 O3 75.9(3) 6 4_764
O2 O3 O3 74.0(3) 4_665 4_764
Ga2 O3 O3 68.28(13) 2_545 4_764
O3 O3 O3 96.4(3) 3_545 4_764
O3 O3 O3 116.65(19) 4_655 4_764
Ga2 O3 O3 101.1(2) 1_645 4_764
O2 O3 O3 50.63(17) 4_654 4_764
O2 O3 O3 86.0(3) . 4_764
O2 O3 O3 29.3(2) 3_654 4_764
La1 O3 O3 99.5(3) 2_545 4_764
La1 O3 O3 107.8(2) 2_656 4_764
O1 O3 O3 156.1(3) 1_556 4_764
O3 O3 O3 124.3(3) 4_766 4_764
Ga3 O3 O3 59.7(3) . 3_646
Nb O3 O3 103.6(5) 1_655 3_646
Ga1 O3 O3 103.6(5) 1_655 3_646
La1 O3 O3 129.4(5) 4_655 3_646
Ga3 O3 O3 36.3(3) 2_646 3_646
O3 O3 O3 133.2(7) 2_645 3_646
O3 O3 O3 17.84(18) 2_646 3_646
O3 O3 O3 76.49(7) 4_765 3_646
O3 O3 O3 62.14(16) 3_645 3_646
O2 O3 O3 70.1(5) 4_655 3_646
O2 O3 O3 97.4(4) 3_655 3_646
O2 O3 O3 68.0(4) 5_656 3_646
O1 O3 O3 123.4(4) . 3_646
O3 O3 O3 128.8(4) 6 3_646
O3 O3 O3 41.2(3) 6_556 3_646
O2 O3 O3 171.9(4) 5_655 3_646
Ga2 O3 O3 92.5(2) 1_545 3_646
Ga3 O3 O3 49.58(19) 4_765 3_646
O2 O3 O3 93.2(4) 1_545 3_646
La1 O3 O3 132.8(3) . 3_646
Ga2 O3 O3 72.1(3) 2_546 3_646
O3 O3 O3 102.4(5) 5_765 3_646
O3 O3 O3 24.4(3) 5_766 3_646
Ga3 O3 O3 154.2(3) 1_554 3_646
Nb O3 O3 13.76(8) 1_656 3_646
Ga1 O3 O3 13.76(8) 1_656 3_646
O2 O3 O3 80.4(3) 2_546 3_646
La1 O3 O3 47.29(16) 4_656 3_646
La1 O3 O3 103.6(2) 2_655 3_646
O1 O3 O3 112.2(5) 2_645 3_646
O2 O3 O3 36.5(3) 6_656 3_646
Ga3 O3 O3 123.6(3) 2_645 3_646
O2 O3 O3 145.8(4) 2_545 3_646
Ga2 O3 O3 90.0(2) 2_556 3_646
O2 O3 O3 101.8(4) 6_655 3_646
La1 O3 O3 87.1(3) 2_645 3_646
O1 O3 O3 54.3(3) 2_646 3_646
O2 O3 O3 62.0(2) 1_655 3_646
Ga2 O3 O3 164.7(3) 1_544 3_646
Ga3 O3 O3 91.4(3) 4_655 3_646
La1 O3 O3 76.7(3) 1_655 3_646
O1 O3 O3 126.2(3) 2_655 3_646
O3 O3 O3 27.86(16) 1_556 3_646
O3 O3 O3 152.14(16) 1_554 3_646
Ga3 O3 O3 114.8(2) 4_764 3_646
O2 O3 O3 51.3(2) 2_656 3_646
O2 O3 O3 92.1(3) 6_556 3_646
La1 O3 O3 68.80(13) 1_556 3_646
O2 O3 O3 80.8(3) 3_645 3_646
O1 O3 O3 72.5(2) 2_656 3_646
O1 O3 O3 68.7(3) 1_655 3_646
O2 O3 O3 104.0(3) 2_655 3_646
O2 O3 O3 149.3(3) 6 3_646
O2 O3 O3 92.8(2) 4_665 3_646
Ga2 O3 O3 126.4(3) 2_545 3_646
O3 O3 O3 116.65(19) 3_545 3_646
O3 O3 O3 109.7(2) 4_655 3_646
Ga2 O3 O3 50.3(2) 1_645 3_646
O2 O3 O3 129.8(4) 4_654 3_646
O2 O3 O3 105.3(3) . 3_646
O2 O3 O3 152.5(3) 3_654 3_646
La1 O3 O3 128.1(2) 2_545 3_646
La1 O3 O3 51.32(13) 2_656 3_646
O1 O3 O3 61.22(16) 1_556 3_646
O3 O3 O3 27.02(14) 4_766 3_646
O3 O3 O3 132.3(3) 4_764 3_646
Ga3 O3 O3 140.6(5) . 3_644
Nb O3 O3 29.8(3) 1_655 3_644
Ga1 O3 O3 29.8(3) 1_655 3_644
La1 O3 O3 74.2(3) 4_655 3_644
Ga3 O3 O3 95.3(4) 2_646 3_644
O3 O3 O3 17.84(16) 2_645 3_644
O3 O3 O3 134.2(6) 2_646 3_644
O3 O3 O3 76.49(7) 4_765 3_644
O3 O3 O3 62.14(16) 3_645 3_644
O2 O3 O3 83.7(5) 4_655 3_644
O2 O3 O3 111.3(5) 3_655 3_644
O2 O3 O3 166.1(5) 5_656 3_644
O1 O3 O3 110.6(4) . 3_644
O3 O3 O3 42.3(3) 6 3_644
O3 O3 O3 130.0(5) 6_556 3_644
O2 O3 O3 61.4(3) 5_655 3_644
Ga2 O3 O3 141.4(3) 1_545 3_644
Ga3 O3 O3 89.1(3) 4_765 3_644
O2 O3 O3 103.0(4) 1_545 3_644
La1 O3 O3 96.0(2) . 3_644
Ga2 O3 O3 101.6(3) 2_546 3_644
O3 O3 O3 25.8(4) 5_765 3_644
O3 O3 O3 103.9(4) 5_766 3_644
Ga3 O3 O3 38.90(8) 1_554 3_644
Nb O3 O3 132.0(3) 1_656 3_644
Ga1 O3 O3 132.0(3) 1_656 3_644
O2 O3 O3 140.2(4) 2_546 3_644
La1 O3 O3 151.4(4) 4_656 3_644
La1 O3 O3 73.7(2) 2_655 3_644
O1 O3 O3 61.7(3) 2_645 3_644
O2 O3 O3 95.6(3) 6_656 3_644
Ga3 O3 O3 13.46(13) 2_645 3_644
O2 O3 O3 74.3(3) 2_545 3_644
Ga2 O3 O3 116.6(3) 2_556 3_644
O2 O3 O3 30.7(2) 6_655 3_644
La1 O3 O3 59.3(2) 2_645 3_644
O1 O3 O3 119.8(3) 2_646 3_644
O2 O3 O3 70.5(3) 1_655 3_644
Ga2 O3 O3 68.45(13) 1_544 3_644
Ga3 O3 O3 119.4(3) 4_655 3_644
La1 O3 O3 47.6(2) 1_655 3_644
O1 O3 O3 80.0(3) 2_655 3_644
O3 O3 O3 152.14(16) 1_556 3_644
O3 O3 O3 27.86(16) 1_554 3_644
Ga3 O3 O3 26.52(14) 4_764 3_644
O2 O3 O3 98.7(3) 2_656 3_644
O2 O3 O3 143.5(3) 6_556 3_644
La1 O3 O3 158.3(3) 1_556 3_644
O2 O3 O3 87.8(3) 3_645 3_644
O1 O3 O3 133.2(4) 2_656 3_644
O1 O3 O3 61.3(3) 1_655 3_644
O2 O3 O3 46.3(2) 2_655 3_644
O2 O3 O3 86.3(2) 6 3_644
O2 O3 O3 99.9(3) 4_665 3_644
Ga2 O3 O3 47.90(18) 2_545 3_644
O3 O3 O3 116.65(19) 3_545 3_644
O3 O3 O3 109.7(2) 4_655 3_644
Ga2 O3 O3 79.7(2) 1_645 3_644
O2 O3 O3 29.0(2) 4_654 3_644
O2 O3 O3 112.5(3) . 3_644
O2 O3 O3 50.70(18) 3_654 3_644
La1 O3 O3 103.23(19) 2_545 3_644
La1 O3 O3 126.2(3) 2_656 3_644
O1 O3 O3 170.8(3) 1_556 3_644
O3 O3 O3 132.3(3) 4_766 3_644
O3 O3 O3 27.02(14) 4_764 3_644
O3 O3 O3 124.3(3) 3_646 3_644
Ga3 O3 O1 64.9(3) . 1_665
Nb O3 O1 48.9(3) 1_655 1_665
Ga1 O3 O1 48.9(3) 1_655 1_665
La1 O3 O1 145.4(5) 4_655 1_665
Ga3 O3 O1 96.0(3) 2_646 1_665
O3 O3 O1 93.6(3) 2_645 1_665
O3 O3 O1 99.8(3) 2_646 1_665
O3 O3 O1 8.2(3) 4_765 1_665
O3 O3 O1 67.5(3) 3_645 1_665
O2 O3 O1 128.4(4) 4_655 1_665
O2 O3 O1 55.7(3) 3_655 1_665
O2 O3 O1 100.4(4) 5_656 1_665
O1 O3 O1 125.5(3) . 1_665
O3 O3 O1 48.1(4) 6 1_665
O3 O3 O1 56.5(4) 6_556 1_665
O2 O3 O1 93.7(3) 5_655 1_665
Ga2 O3 O1 124.2(3) 1_545 1_665
Ga3 O3 O1 36.01(18) 4_765 1_665
O2 O3 O1 174.7(3) 1_545 1_665
La1 O3 O1 84.4(2) . 1_665
Ga2 O3 O1 148.3(3) 2_546 1_665
O3 O3 O1 56.4(3) 5_765 1_665
O3 O3 O1 62.4(2) 5_766 1_665
Ga3 O3 O1 74.3(2) 1_554 1_665
Nb O3 O1 76.1(2) 1_656 1_665
Ga1 O3 O1 76.1(2) 1_656 1_665
O2 O3 O1 142.1(3) 2_546 1_665
La1 O3 O1 121.7(3) 4_656 1_665
La1 O3 O1 23.47(14) 2_655 1_665
O1 O3 O1 137.1(3) 2_645 1_665
O2 O3 O1 96.9(3) 6_656 1_665
Ga3 O3 O1 89.4(2) 2_645 1_665
O2 O3 O1 131.4(4) 2_545 1_665
Ga2 O3 O1 54.86(13) 2_556 1_665
O2 O3 O1 92.6(3) 6_655 1_665
La1 O3 O1 116.8(2) 2_645 1_665
O1 O3 O1 136.6(3) 2_646 1_665
O2 O3 O1 37.82(17) 1_655 1_665
Ga2 O3 O1 110.0(3) 1_544 1_665
Ga3 O3 O1 163.1(3) 4_655 1_665
La1 O3 O1 65.94(13) 1_655 1_665
O1 O3 O1 54.73(17) 2_655 1_665
O3 O3 O1 93.5(2) 1_556 1_665
O3 O3 O1 86.5(2) 1_554 1_665
Ga3 O3 O1 50.1(2) 4_764 1_665
O2 O3 O1 31.7(3) 2_656 1_665
O2 O3 O1 114.7(3) 6_556 1_665
La1 O3 O1 89.3(2) 1_556 1_665
O2 O3 O1 145.2(3) 3_645 1_665
O1 O3 O1 61.8(2) 2_656 1_665
O1 O3 O1 92.34(16) 1_655 1_665
O2 O3 O1 30.5(3) 2_655 1_665
O2 O3 O1 109.8(3) 6 1_665
O2 O3 O1 37.04(14) 4_665 1_665
Ga2 O3 O1 124.4(3) 2_545 1_665
O3 O3 O1 96.3(3) 3_545 1_665
O3 O3 O1 156.0(3) 4_655 1_665
Ga2 O3 O1 93.41(16) 1_645 1_665
O2 O3 O1 105.4(3) 4_654 1_665
O2 O3 O1 66.82(18) . 1_665
O2 O3 O1 69.7(2) 3_654 1_665
La1 O3 O1 132.0(2) 2_545 1_665
La1 O3 O1 50.1(2) 2_656 1_665
O1 O3 O1 112.3(3) 1_556 1_665
O3 O3 O1 65.9(3) 4_766 1_665
O3 O3 O1 58.9(3) 4_764 1_665
O3 O3 O1 82.8(3) 3_646 1_665
O3 O3 O1 76.5(2) 3_644 1_665
Ga3 O3 La1 92.9(5) . 2_646
Nb O3 La1 108.2(4) 1_655 2_646
Ga1 O3 La1 108.2(4) 1_655 2_646
La1 O3 La1 93.1(3) 4_655 2_646
Ga3 O3 La1 21.76(16) 2_646 2_646
O3 O3 La1 108.0(6) 2_645 2_646
O3 O3 La1 29.4(4) 2_646 2_646
O3 O3 La1 106.4(3) 4_765 2_646
O3 O3 La1 61.6(4) 3_645 2_646
O2 O3 La1 33.5(3) 4_655 2_646
O2 O3 La1 132.1(4) 3_655 2_646
O2 O3 La1 83.6(4) 5_656 2_646
O1 O3 La1 113.0(3) . 2_646
O3 O3 La1 144.39(11) 6 2_646
O3 O3 La1 78.5(4) 6_556 2_646
O2 O3 La1 148.9(3) 5_655 2_646
Ga2 O3 La1 91.3(3) 1_545 2_646
Ga3 O3 La1 78.2(2) 4_765 2_646
O2 O3 La1 60.8(2) 1_545 2_646
La1 O3 La1 150.4(3) . 2_646
Ga2 O3 La1 35.91(13) 2_546 2_646
O3 O3 La1 102.0(3) 5_765 2_646
O3 O3 La1 52.35(16) 5_766 2_646
Ga3 O3 La1 147.5(3) 1_554 2_646
Nb O3 La1 50.39(15) 1_656 2_646
Ga1 O3 La1 50.39(15) 1_656 2_646
O2 O3 La1 68.6(3) 2_546 2_646
La1 O3 La1 44.14(13) 4_656 2_646
La1 O3 La1 137.5(3) 2_655 2_646
O1 O3 La1 74.8(3) 2_645 2_646
O2 O3 La1 20.94(18) 6_656 2_646
Ga3 O3 La1 101.6(2) 2_645 2_646
O2 O3 La1 112.0(3) 2_545 2_646
Ga2 O3 La1 124.8(3) 2_556 2_646
O2 O3 La1 79.8(3) 6_655 2_646
La1 O3 La1 55.03(14) 2_645 2_646
O1 O3 La1 24.62(10) 2_646 2_646
O2 O3 La1 81.0(2) 1_655 2_646
Ga2 O3 La1 133.98(19) 1_544 2_646
Ga3 O3 La1 67.52(15) 4_655 2_646
La1 O3 La1 73.43(17) 1_655 2_646
O1 O3 La1 163.9(3) 2_655 2_646
O3 O3 La1 50.05(11) 1_556 2_646
O3 O3 La1 129.95(11) 1_554 2_646
Ga3 O3 La1 119.7(2) 4_764 2_646
O2 O3 La1 85.5(3) 2_656 2_646
O2 O3 La1 96.8(3) 6_556 2_646
La1 O3 La1 90.5(2) 1_556 2_646
O2 O3 La1 43.03(17) 3_645 2_646
O1 O3 La1 105.8(3) 2_656 2_646
O1 O3 La1 50.0(2) 1_655 2_646
O2 O3 La1 122.1(3) 2_655 2_646
O2 O3 La1 135.4(2) 6 2_646
O2 O3 La1 130.5(3) 4_665 2_646
Ga2 O3 La1 90.13(17) 2_545 2_646
O3 O3 La1 128.73(14) 3_545 2_646
O3 O3 La1 85.9(2) 4_655 2_646
Ga2 O3 La1 33.89(9) 1_645 2_646
O2 O3 La1 99.3(2) 4_654 2_646
O2 O3 La1 135.9(3) . 2_646
O2 O3 La1 160.2(3) 3_654 2_646
La1 O3 La1 110.65(17) 2_545 2_646
La1 O3 La1 88.67(19) 2_656 2_646
O1 O3 La1 69.21(16) 1_556 2_646
O3 O3 La1 64.15(14) 4_766 2_646
O3 O3 La1 134.4(3) 4_764 2_646
O3 O3 La1 37.8(2) 3_646 2_646
O3 O3 La1 110.2(3) 3_644 2_646
O1 O3 La1 114.2(2) 1_665 2_646
Ga3 O3 O2 71.1(4) . 4_656
Nb O3 O2 124.0(5) 1_655 4_656
Ga1 O3 O2 124.0(5) 1_655 4_656
La1 O3 O2 103.5(4) 4_655 4_656
Ga3 O3 O2 38.6(2) 2_646 4_656
O3 O3 O2 131.1(7) 2_645 4_656
O3 O3 O2 10.2(2) 2_646 4_656
O3 O3 O2 103.7(2) 4_765 4_656
O3 O3 O2 77.0(3) 3_645 4_656
O2 O3 O2 55.1(3) 4_655 4_656
O2 O3 O2 109.8(5) 3_655 4_656
O2 O3 O2 61.1(4) 5_656 4_656
O1 O3 O2 102.8(4) . 4_656
O3 O3 O2 155.4(3) 6 4_656
O3 O3 O2 61.1(4) 6_556 4_656
O2 O3 O2 154.3(4) 5_655 4_656
Ga2 O3 O2 75.0(3) 1_545 4_656
Ga3 O3 O2 76.5(3) 4_765 4_656
O2 O3 O2 66.5(3) 1_545 4_656
La1 O3 O2 130.7(3) . 4_656
Ga2 O3 O2 48.4(2) 2_546 4_656
O3 O3 O2 119.8(4) 5_765 4_656
O3 O3 O2 50.3(3) 5_766 4_656
Ga3 O3 O2 170.7(3) 1_554 4_656
Nb O3 O2 34.85(15) 1_656 4_656
Ga1 O3 O2 34.85(15) 1_656 4_656
O2 O3 O2 56.8(2) 2_546 4_656
La1 O3 O2 25.35(14) 4_656 4_656
La1 O3 O2 129.2(3) 2_655 4_656
O1 O3 O2 93.2(4) 2_645 4_656
O2 O3 O2 38.1(3) 6_656 4_656
Ga3 O3 O2 124.9(3) 2_645 4_656
O2 O3 O2 118.6(3) 2_545 4_656
Ga2 O3 O2 102.8(2) 2_556 4_656
O2 O3 O2 102.9(4) 6_655 4_656
La1 O3 O2 78.0(2) 2_645 4_656
O1 O3 O2 28.4(3) 2_646 4_656
O2 O3 O2 86.6(3) 1_655 4_656
Ga2 O3 O2 138.5(2) 1_544 4_656
Ga3 O3 O2 64.58(19) 4_655 4_656
La1 O3 O2 90.9(2) 1_655 4_656
O1 O3 O2 143.0(3) 2_655 4_656
O3 O3 O2 27.42(16) 1_556 4_656
O3 O3 O2 152.58(16) 1_554 4_656
Ga3 O3 O2 136.1(3) 4_764 4_656
O2 O3 O2 78.1(3) 2_656 4_656
O2 O3 O2 78.2(3) 6_556 4_656
La1 O3 O2 67.32(19) 1_556 4_656
O2 O3 O2 59.95(18) 3_645 4_656
O1 O3 O2 83.6(3) 2_656 4_656
O1 O3 O2 71.7(3) 1_655 4_656
O2 O3 O2 130.0(3) 2_655 4_656
O2 O3 O2 129.5(2) 6 4_656
O2 O3 O2 112.4(3) 4_665 4_656
Ga2 O3 O2 109.7(2) 2_545 4_656
O3 O3 O2 109.15(16) 3_545 4_656
O3 O3 O2 83.34(17) 4_655 4_656
Ga2 O3 O2 53.68(19) 1_645 4_656
O2 O3 O2 121.6(3) 4_654 4_656
O2 O3 O2 112.6(3) . 4_656
O2 O3 O2 176.4(3) 3_654 4_656
La1 O3 O2 104.5(2) 2_545 4_656
La1 O3 O2 70.95(18) 2_656 4_656
O1 O3 O2 48.01(17) 1_556 4_656
O3 O3 O2 47.59(15) 4_766 4_656
O3 O3 O2 153.5(3) 4_764 4_656
O3 O3 O2 27.18(19) 3_646 4_656
O3 O3 O2 132.8(3) 3_644 4_656
O1 O3 O2 109.8(3) 1_665 4_656
La1 O3 O2 23.31(14) 2_646 4_656
Ga3 O3 O2 17.2(3) . 3_656
Nb O3 O2 124.6(4) 1_655 3_656
Ga1 O3 O2 124.6(4) 1_655 3_656
La1 O3 O2 131.2(4) 4_655 3_656
Ga3 O3 O2 83.5(3) 2_646 3_656
O3 O3 O2 171.4(3) 2_645 3_656
O3 O3 O2 47.8(4) 2_646 3_656
O3 O3 O2 77.7(3) 4_765 3_656
O3 O3 O2 104.03(18) 3_645 3_656
O2 O3 O2 109.6(5) 4_655 3_656
O2 O3 O2 55.3(3) 3_655 3_656
O2 O3 O2 28.6(3) 5_656 3_656
O1 O3 O2 87.5(4) . 3_656
O3 O3 O2 118.4(4) 6 3_656
O3 O3 O2 24.9(3) 6_556 3_656
O2 O3 O2 124.5(4) 5_655 3_656
Ga2 O3 O2 59.9(2) 1_545 3_656
Ga3 O3 O2 67.6(2) 4_765 3_656
O2 O3 O2 102.0(4) 1_545 3_656
La1 O3 O2 85.3(2) . 3_656
Ga2 O3 O2 98.0(3) 2_546 3_656
O3 O3 O2 129.9(4) 5_765 3_656
O3 O3 O2 60.0(3) 5_766 3_656
Ga3 O3 O2 134.7(3) 1_554 3_656
Nb O3 O2 35.01(15) 1_656 3_656
Ga1 O3 O2 35.01(15) 1_656 3_656
O2 O3 O2 65.7(3) 2_546 3_656
La1 O3 O2 47.81(16) 4_656 3_656
La1 O3 O2 84.4(2) 2_655 3_656
O1 O3 O2 142.2(4) 2_645 3_656
O2 O3 O2 83.6(3) 6_656 3_656
Ga3 O3 O2 165.2(2) 2_645 3_656
O2 O3 O2 127.3(3) 2_545 3_656
Ga2 O3 O2 48.25(18) 2_556 3_656
O2 O3 O2 148.5(3) 6_655 3_656
La1 O3 O2 132.0(3) 2_645 3_656
O1 O3 O2 77.5(3) 2_646 3_656
O2 O3 O2 86.8(2) 1_655 3_656
Ga2 O3 O2 125.1(3) 1_544 3_656
Ga3 O3 O2 86.4(2) 4_655 3_656
La1 O3 O2 116.7(2) 1_655 3_656
O1 O3 O2 88.5(3) 2_655 3_656
O3 O3 O2 27.14(17) 1_556 3_656
O3 O3 O2 152.86(17) 1_554 3_656
Ga3 O3 O2 128.1(2) 4_764 3_656
O2 O3 O2 56.4(3) 2_656 3_656
O2 O3 O2 54.2(2) 6_556 3_656
La1 O3 O2 23.35(14) 1_556 3_656
O2 O3 O2 111.5(3) 3_645 3_656
O1 O3 O2 29.0(3) 2_656 3_656
O1 O3 O2 116.2(3) 1_655 3_656
O2 O3 O2 108.4(3) 2_655 3_656
O2 O3 O2 106.1(3) 6 3_656
O2 O3 O2 60.41(19) 4_665 3_656
Ga2 O3 O2 157.6(2) 2_545 3_656
O3 O3 O2 70.1(2) 3_545 3_656
O3 O3 O2 95.27(16) 4_655 3_656
Ga2 O3 O2 98.0(2) 1_645 3_656
O2 O3 O2 175.9(3) 4_654 3_656
O2 O3 O2 59.62(19) . 3_656
O2 O3 O2 122.2(3) 3_654 3_656
La1 O3 O2 96.7(2) 2_545 3_656
La1 O3 O2 28.02(14) 2_656 3_656
O1 O3 O2 34.99(16) 1_556 3_656
O3 O3 O2 27.57(19) 4_766 3_656
O3 O3 O2 133.4(3) 4_764 3_656
O3 O3 O2 47.67(15) 3_646 3_656
O3 O3 O2 154.2(3) 3_644 3_656
O1 O3 O2 78.0(2) 1_665 3_656
La1 O3 O2 77.07(19) 2_646 3_656
O2 O3 O2 54.5(2) 4_656 3_656
Ga3 O3 La1 137.1(4) . 1_545
Nb O3 La1 108.5(4) 1_655 1_545
Ga1 O3 La1 108.5(4) 1_655 1_545
La1 O3 La1 27.7(2) 4_655 1_545
Ga3 O3 La1 77.5(2) 2_646 1_545
O3 O3 La1 66.3(3) 2_645 1_545
O3 O3 La1 88.9(3) 2_646 1_545
O3 O3 La1 152.8(5) 4_765 1_545
O3 O3 La1 95.2(5) 3_645 1_545
O2 O3 La1 39.2(3) 4_655 1_545
O2 O3 La1 142.9(4) 3_655 1_545
O2 O3 La1 102.3(3) 5_656 1_545
O1 O3 La1 70.17(18) . 1_545
O3 O3 La1 117.6(5) 6 1_545
O3 O3 La1 139.3(5) 6_556 1_545
O2 O3 La1 83.3(3) 5_655 1_545
Ga2 O3 La1 78.12(17) 1_545 1_545
Ga3 O3 La1 136.7(3) 4_765 1_545
O2 O3 La1 21.0(2) 1_545 1_545
La1 O3 La1 106.4(2) . 1_545
Ga2 O3 La1 30.73(9) 2_546 1_545
O3 O3 La1 100.7(2) 5_765 1_545
O3 O3 La1 115.92(15) 5_766 1_545
Ga3 O3 La1 94.4(2) 1_554 1_545
Nb O3 La1 113.4(3) 1_656 1_545
Ga1 O3 La1 113.4(3) 1_656 1_545
O2 O3 La1 60.5(2) 2_546 1_545
La1 O3 La1 75.20(15) 4_656 1_545
La1 O3 La1 151.4(3) 2_655 1_545
O1 O3 La1 20.6(2) 2_645 1_545
O2 O3 La1 76.7(2) 6_656 1_545
Ga3 O3 La1 68.90(14) 2_645 1_545
O2 O3 La1 47.39(17) 2_545 1_545
Ga2 O3 La1 145.8(2) 2_556 1_545
O2 O3 La1 64.6(2) 6_655 1_545
La1 O3 La1 42.59(8) 2_645 1_545
O1 O3 La1 50.5(2) 2_646 1_545
O2 O3 La1 125.8(3) 1_655 1_545
Ga2 O3 La1 68.84(13) 1_544 1_545
Ga3 O3 La1 39.77(7) 4_655 1_545
La1 O3 La1 93.41(18) 1_655 1_545
O1 O3 La1 129.6(3) 2_655 1_545
O3 O3 La1 101.59(13) 1_556 1_545
O3 O3 La1 78.41(13) 1_554 1_545
Ga3 O3 La1 108.7(2) 4_764 1_545
O2 O3 La1 149.0(3) 2_656 1_545
O2 O3 La1 87.5(2) 6_556 1_545
La1 O3 La1 113.47(18) 1_556 1_545
O2 O3 La1 23.42(15) 3_645 1_545
O1 O3 La1 141.1(2) 2_656 1_545
O1 O3 La1 69.77(14) 1_655 1_545
O2 O3 La1 128.3(3) 2_655 1_545
O2 O3 La1 76.78(19) 6 1_545
O2 O3 La1 159.7(3) 4_665 1_545
Ga2 O3 La1 35.54(6) 2_545 1_545
O3 O3 La1 100.78(17) 3_545 1_545
O3 O3 La1 42.34(17) 4_655 1_545
Ga2 O3 La1 74.38(14) 1_645 1_545
O2 O3 La1 53.95(16) 4_654 1_545
O2 O3 La1 130.8(2) . 1_545
O2 O3 La1 103.0(2) 3_654 1_545
La1 O3 La1 61.21(10) 2_545 1_545
La1 O3 La1 148.1(3) 2_656 1_545
O1 O3 La1 89.39(16) 1_556 1_545
O3 O3 La1 126.4(2) 4_766 1_545
O3 O3 La1 103.78(17) 4_764 1_545
O3 O3 La1 102.7(3) 3_646 1_545
O3 O3 La1 82.2(2) 3_644 1_545
O1 O3 La1 157.1(3) 1_665 1_545
La1 O3 La1 65.55(12) 2_646 1_545
O2 O3 La1 78.83(19) 4_656 1_545
O2 O3 La1 122.3(2) 3_656 1_545
Ga3 O3 La1 76.0(4) . 1_656
Nb O3 La1 81.8(4) 1_655 1_656
Ga1 O3 La1 81.8(4) 1_655 1_656
La1 O3 La1 129.6(4) 4_655 1_656
Ga3 O3 La1 25.00(15) 2_646 1_656
O3 O3 La1 111.4(5) 2_645 1_656
O3 O3 La1 37.4(2) 2_646 1_656
O3 O3 La1 66.1(3) 4_765 1_656
O3 O3 La1 38.97(11) 3_645 1_656
O2 O3 La1 63.8(4) 4_655 1_656
O2 O3 La1 108.1(4) 3_655 1_656
O2 O3 La1 90.9(4) 5_656 1_656
O1 O3 La1 145.6(4) . 1_656
O3 O3 La1 112.3(2) 6 1_656
O3 O3 La1 53.27(17) 6_556 1_656
O2 O3 La1 161.1(4) 5_655 1_656
Ga2 O3 La1 115.4(3) 1_545 1_656
Ga3 O3 La1 37.95(15) 4_765 1_656
O2 O3 La1 101.1(3) 1_545 1_656
La1 O3 La1 148.1(3) . 1_656
Ga2 O3 La1 75.5(2) 2_546 1_656
O3 O3 La1 79.7(4) 5_765 1_656
O3 O3 La1 13.65(10) 5_766 1_656
Ga3 O3 La1 133.9(2) 1_554 1_656
Nb O3 La1 33.03(10) 1_656 1_656
Ga1 O3 La1 33.03(10) 1_656 1_656
O2 O3 La1 100.3(3) 2_546 1_656
La1 O3 La1 67.72(18) 4_656 1_656
La1 O3 La1 97.28(18) 2_655 1_656
O1 O3 La1 103.8(3) 2_645 1_656
O2 O3 La1 25.8(2) 6_656 1_656
Ga3 O3 La1 101.4(2) 2_645 1_656
O2 O3 La1 149.5(3) 2_545 1_656
Ga2 O3 La1 101.4(2) 2_556 1_656
O2 O3 La1 80.8(3) 6_655 1_656
La1 O3 La1 73.22(18) 2_645 1_656
O1 O3 La1 63.8(2) 2_646 1_656
O2 O3 La1 43.40(19) 1_655 1_656
Ga2 O3 La1 166.7(2) 1_544 1_656
Ga3 O3 La1 106.1(2) 4_655 1_656
La1 O3 La1 53.53(13) 1_655 1_656
O1 O3 La1 127.2(2) 2_655 1_656
O3 O3 La1 51.05(11) 1_556 1_656
O3 O3 La1 128.95(11) 1_554 1_656
Ga3 O3 La1 93.63(17) 4_764 1_656
O2 O3 La1 46.78(18) 2_656 1_656
O2 O3 La1 115.3(3) 6_556 1_656
La1 O3 La1 90.41(19) 1_556 1_656
O2 O3 La1 79.0(2) 3_645 1_656
O1 O3 La1 87.5(2) 2_656 1_656
O1 O3 La1 49.26(19) 1_655 1_656
O2 O3 La1 86.9(2) 2_655 1_656
O2 O3 La1 172.4(3) 6 1_656
O2 O3 La1 97.0(2) 4_665 1_656
Ga2 O3 La1 113.5(2) 2_545 1_656
O3 O3 La1 137.81(16) 3_545 1_656
O3 O3 La1 125.1(2) 4_655 1_656
Ga2 O3 La1 33.34(8) 1_645 1_656
O2 O3 La1 110.6(3) 4_654 1_656
O2 O3 La1 118.8(2) . 1_656
O2 O3 La1 138.0(2) 3_654 1_656
La1 O3 La1 148.0(2) 2_545 1_656
La1 O3 La1 61.66(13) 2_656 1_656
O1 O3 La1 84.31(19) 1_556 1_656
O3 O3 La1 41.83(16) 4_766 1_656
O3 O3 La1 111.5(3) 4_764 1_656
O3 O3 La1 23.20(14) 3_646 1_656
O3 O3 La1 101.1(2) 3_644 1_656
O1 O3 La1 73.94(16) 1_665 1_656
La1 O3 La1 40.29(9) 2_646 1_656
O2 O3 La1 43.55(15) 4_656 1_656
O2 O3 La1 67.78(18) 3_656 1_656
La1 O3 La1 102.40(19) 1_545 1_656
Ga3 O3 O2 152.0(5) . 1_544
Nb O3 O2 83.4(4) 1_655 1_544
Ga1 O3 O2 83.4(4) 1_655 1_544
La1 O3 O2 20.9(2) 4_655 1_544
Ga3 O3 O2 107.4(3) 2_646 1_544
O3 O3 O2 35.88(16) 2_645 1_544
O3 O3 O2 129.0(4) 2_646 1_544
O3 O3 O2 128.33(17) 4_765 1_544
O3 O3 O2 101.1(4) 3_645 1_544
O2 O3 O2 70.7(4) 4_655 1_544
O2 O3 O2 120.6(5) 3_655 1_544
O2 O3 O2 122.5(4) 5_656 1_544
O1 O3 O2 65.5(3) . 1_544
O3 O3 O2 78.7(4) 6 1_544
O3 O3 O2 175.6(2) 6_556 1_544
O2 O3 O2 46.80(18) 5_655 1_544
Ga2 O3 O2 91.3(2) 1_545 1_544
Ga3 O3 O2 141.3(3) 4_765 1_544
O2 O3 O2 56.1(2) 1_545 1_544
La1 O3 O2 81.4(2) . 1_544
Ga2 O3 O2 70.6(2) 2_546 1_544
O3 O3 O2 78.9(4) 5_765 1_544
O3 O3 O2 142.2(3) 5_766 1_544
Ga3 O3 O2 54.14(18) 1_554 1_544
Nb O3 O2 153.1(3) 1_656 1_544
Ga1 O3 O2 153.1(3) 1_656 1_544
O2 O3 O2 87.1(4) 2_546 1_544
La1 O3 O2 112.5(2) 4_656 1_544
La1 O3 O2 111.3(3) 2_655 1_544
O1 O3 O2 28.5(3) 2_645 1_544
O2 O3 O2 106.9(3) 6_656 1_544
Ga3 O3 O2 43.83(15) 2_645 1_544
O2 O3 O2 25.4(3) 2_545 1_544
Ga2 O3 O2 127.7(3) 2_556 1_544
O2 O3 O2 55.91(19) 6_655 1_544
La1 O3 O2 57.08(15) 2_645 1_544
O1 O3 O2 90.8(3) 2_646 1_544
O2 O3 O2 122.0(3) 1_655 1_544
Ga2 O3 O2 36.96(14) 1_544 1_544
Ga3 O3 O2 67.61(18) 4_655 1_544
La1 O3 O2 90.3(2) 1_655 1_544
O1 O3 O2 93.1(3) 2_655 1_544
O3 O3 O2 140.58(17) 1_556 1_544
O3 O3 O2 39.42(17) 1_554 1_544
Ga3 O3 O2 77.7(2) 4_764 1_544
O2 O3 O2 152.3(3) 2_656 1_544
O2 O3 O2 97.6(3) 6_556 1_544
La1 O3 O2 129.6(2) 1_556 1_544
O2 O3 O2 60.28(14) 3_645 1_544
O1 O3 O2 142.0(3) 2_656 1_544
O1 O3 O2 82.3(2) 1_655 1_544
O2 O3 O2 96.2(2) 2_655 1_544
O2 O3 O2 53.38(19) 6 1_544
O2 O3 O2 126.5(3) 4_665 1_544
Ga2 O3 O2 16.95(11) 2_545 1_544
O3 O3 O2 89.15(14) 3_545 1_544
O3 O3 O2 56.14(18) 4_655 1_544
Ga2 O3 O2 96.94(19) 1_645 1_544
O2 O3 O2 27.6(2) 4_654 1_544
O2 O3 O2 110.8(3) . 1_544
O2 O3 O2 63.0(3) 3_654 1_544
La1 O3 O2 55.65(16) 2_545 1_544
La1 O3 O2 167.7(3) 2_656 1_544
O1 O3 O2 117.2(2) 1_556 1_544
O3 O3 O2 166.6(3) 4_766 1_544
O3 O3 O2 66.85(17) 4_764 1_544
O3 O3 O2 140.6(3) 3_646 1_544
O3 O3 O2 53.62(19) 3_644 1_544
O1 O3 O2 125.7(3) 1_665 1_544
La1 O3 O2 102.95(19) 2_646 1_544
O2 O3 O2 119.0(2) 4_656 1_544
O2 O3 O2 151.0(2) 3_656 1_544
La1 O3 O2 40.28(15) 1_545 1_544
La1 O3 O2 130.3(2) 1_656 1_544
Ga3 O3 O3 78.2(3) . 5_665
Nb O3 O3 98.4(5) 1_655 5_665
Ga1 O3 O3 98.4(5) 1_655 5_665
La1 O3 O3 77.9(5) 4_655 5_665
Ga3 O3 O3 173.0(5) 2_646 5_665
O3 O3 O3 88.1(7) 2_645 5_665
O3 O3 O3 133.9(6) 2_646 5_665
O3 O3 O3 93.2(4) 4_765 5_665
O3 O3 O3 145.1(3) 3_645 5_665
O2 O3 O3 143.4(4) 4_655 5_665
O2 O3 O3 43.7(3) 3_655 5_665
O2 O3 O3 74.4(4) 5_656 5_665
O1 O3 O3 42.3(3) . 5_665
O3 O3 O3 62.3(2) 6 5_665
O3 O3 O3 99.44(14) 6_556 5_665
O2 O3 O3 34.6(3) 5_655 5_665
Ga2 O3 O3 62.0(3) 1_545 5_665
Ga3 O3 O3 118.51(17) 4_765 5_665
O2 O3 O3 100.3(4) 1_545 5_665
La1 O3 O3 4.67(7) . 5_665
Ga2 O3 O3 126.7(3) 2_546 5_665
O3 O3 O3 104.2(4) 5_765 5_665
O3 O3 O3 138.4(2) 5_766 5_665
Ga3 O3 O3 52.9(2) 1_554 5_665
Nb O3 O3 124.0(3) 1_656 5_665
Ga1 O3 O3 124.0(3) 1_656 5_665
O2 O3 O3 84.8(3) 2_546 5_665
La1 O3 O3 110.5(3) 4_656 5_665
La1 O3 O3 62.15(10) 2_655 5_665
O1 O3 O3 104.4(4) 2_645 5_665
O2 O3 O3 172.7(4) 6_656 5_665
Ga3 O3 O3 96.8(4) 2_645 5_665
O2 O3 O3 58.2(3) 2_545 5_665
Ga2 O3 O3 50.51(6) 2_556 5_665
O2 O3 O3 119.4(4) 6_655 5_665
La1 O3 O3 134.3(4) 2_645 5_665
O1 O3 O3 130.0(3) 2_646 5_665
O2 O3 O3 122.0(2) 1_655 5_665
Ga2 O3 O3 40.4(2) 1_544 5_665
Ga3 O3 O3 88.7(3) 4_655 5_665
La1 O3 O3 133.1(3) 1_655 5_665
O1 O3 O3 30.72(6) 2_655 5_665
O3 O3 O3 113.6(2) 1_556 5_665
O3 O3 O3 66.4(2) 1_554 5_665
Ga3 O3 O3 86.7(3) 4_764 5_665
O2 O3 O3 106.78(17) 2_656 5_665
O2 O3 O3 57.1(2) 6_556 5_665
La1 O3 O3 70.45(18) 1_556 5_665
O2 O3 O3 127.0(3) 3_645 5_665
O1 O3 O3 65.80(18) 2_656 5_665
O1 O3 O3 152.6(4) 1_655 5_665
O2 O3 O3 84.0(2) 2_655 5_665
O2 O3 O3 27.5(2) 6 5_665
O2 O3 O3 55.74(15) 4_665 5_665
Ga2 O3 O3 93.8(3) 2_545 5_665
O3 O3 O3 25.6(2) 3_545 5_665
O3 O3 O3 71.9(3) 4_655 5_665
Ga2 O3 O3 171.4(4) 1_645 5_665
O2 O3 O3 92.7(4) 4_654 5_665
O2 O3 O3 33.43(18) . 5_665
O2 O3 O3 42.0(2) 3_654 5_665
La1 O3 O3 47.1(2) 2_545 5_665
La1 O3 O3 90.47(13) 2_656 5_665
O1 O3 O3 86.7(3) 1_556 5_665
O3 O3 O3 112.3(3) 4_766 5_665
O3 O3 O3 70.9(3) 4_764 5_665
O3 O3 O3 137.4(3) 3_646 5_665
O3 O3 O3 91.7(3) 3_644 5_665
O1 O3 O3 84.98(12) 1_665 5_665
La1 O3 O3 153.3(3) 2_646 5_665
O2 O3 O3 134.7(3) 4_656 5_665
O2 O3 O3 89.9(2) 3_656 5_665
La1 O3 O3 104.2(3) 1_545 5_665
La1 O3 O3 151.8(2) 1_656 5_665
O2 O3 O3 77.4(3) 1_544 5_665
Ga3 O3 O3 134.1(5) . 5_655
Nb O3 O3 109.9(5) 1_655 5_655
Ga1 O3 O3 109.9(5) 1_655 5_655
La1 O3 O3 7.38(14) 4_655 5_655
Ga3 O3 O3 100.1(2) 2_646 5_655
O3 O3 O3 62.4(2) 2_645 5_655
O3 O3 O3 106.5(3) 2_646 5_655
O3 O3 O3 156.0(2) 4_765 5_655
O3 O3 O3 113.1(5) 3_645 5_655
O2 O3 O3 61.6(3) 4_655 5_655
O2 O3 O3 122.8(4) 3_655 5_655
O2 O3 O3 98.8(4) 5_656 5_655
O1 O3 O3 51.7(3) . 5_655
O3 O3 O3 104.8(6) 6 5_655
O3 O3 O3 149.4(6) 6_556 5_655
O2 O3 O3 62.5(3) 5_655 5_655
Ga2 O3 O3 69.0(2) 1_545 5_655
Ga3 O3 O3 157.5(3) 4_765 5_655
O2 O3 O3 30.0(2) 1_545 5_655
La1 O3 O3 84.3(3) . 5_655
Ga2 O3 O3 51.09(6) 2_546 5_655
O3 O3 O3 104.2(4) 5_765 5_655
O3 O3 O3 138.4(2) 5_766 5_655
Ga3 O3 O3 78.8(3) 1_554 5_655
Nb O3 O3 130.8(3) 1_656 5_655
Ga1 O3 O3 130.8(3) 1_656 5_655
O2 O3 O3 60.0(2) 2_546 5_655
La1 O3 O3 85.2(2) 4_656 5_655
La1 O3 O3 134.0(4) 2_655 5_655
O1 O3 O3 29.25(7) 2_645 5_655
O2 O3 O3 99.3(2) 6_656 5_655
Ga3 O3 O3 68.8(2) 2_645 5_655
O2 O3 O3 25.2(2) 2_545 5_655
Ga2 O3 O3 127.5(3) 2_556 5_655
O2 O3 O3 73.7(2) 6_655 5_655
La1 O3 O3 60.35(8) 2_645 5_655
O1 O3 O3 68.28(19) 2_646 5_655
O2 O3 O3 141.9(3) 1_655 5_655
Ga2 O3 O3 47.06(19) 1_544 5_655
Ga3 O3 O3 39.96(12) 4_655 5_655
La1 O3 O3 107.4(2) 1_655 5_655
O1 O3 O3 107.5(3) 2_655 5_655
O3 O3 O3 113.6(2) 1_556 5_655
O3 O3 O3 66.4(2) 1_554 5_655
Ga3 O3 O3 105.2(3) 4_764 5_655
O2 O3 O3 171.4(3) 2_656 5_655
O2 O3 O3 77.2(3) 6_556 5_655
La1 O3 O3 108.3(3) 1_556 5_655
O2 O3 O3 45.90(15) 3_645 5_655
O1 O3 O3 131.2(3) 2_656 5_655
O1 O3 O3 88.69(16) 1_655 5_655
O2 O3 O3 123.9(4) 2_655 5_655
O2 O3 O3 54.3(2) 6 5_655
O2 O3 O3 137.5(3) 4_665 5_655
Ga2 O3 O3 34.07(13) 2_545 5_655
O3 O3 O3 81.7(2) 3_545 5_655
O3 O3 O3 31.1(2) 4_655 5_655
Ga2 O3 O3 96.17(12) 1_645 5_655
O2 O3 O3 51.9(2) 4_654 5_655
O2 O3 O3 110.5(3) . 5_655
O2 O3 O3 84.7(3) 3_654 5_655
La1 O3 O3 41.80(15) 2_545 5_655
La1 O3 O3 152.9(3) 2_656 5_655
O1 O3 O3 90.6(3) 1_556 5_655
O3 O3 O3 141.3(3) 4_766 5_655
O3 O3 O3 94.2(3) 4_764 5_655
O3 O3 O3 122.5(3) 3_646 5_655
O3 O3 O3 80.2(3) 3_644 5_655
O1 O3 O3 152.8(4) 1_665 5_655
La1 O3 O3 86.93(14) 2_646 5_655
O2 O3 O3 96.3(2) 4_656 5_655
O2 O3 O3 125.5(3) 3_656 5_655
La1 O3 O3 22.55(6) 1_545 5_655
La1 O3 O3 124.9(2) 1_656 5_655
O2 O3 O3 27.7(2) 1_544 5_655
O3 O3 O3 81.8(3) 5_665 5_655
Ga3 O3 O3 37.7(2) . 5_666
Nb O3 O3 130.7(4) 1_655 5_666
Ga1 O3 O3 130.7(4) 1_655 5_666
La1 O3 O3 102.1(4) 4_655 5_666
Ga3 O3 O3 124.8(5) 2_646 5_666
O3 O3 O3 136.1(7) 2_645 5_666
O3 O3 O3 85.9(6) 2_646 5_666
O3 O3 O3 93.2(4) 4_765 5_666
O3 O3 O3 144.4(3) 3_645 5_666
O2 O3 O3 133.6(5) 4_655 5_666
O2 O3 O3 34.5(3) 3_655 5_666
O2 O3 O3 27.7(3) 5_656 5_666
O1 O3 O3 50.0(4) . 5_666
O3 O3 O3 99.67(15) 6 5_666
O3 O3 O3 61.3(2) 6_556 5_666
O2 O3 O3 82.0(3) 5_655 5_666
Ga2 O3 O3 36.4(2) 1_545 5_666
Ga3 O3 O3 100.5(2) 4_765 5_666
O2 O3 O3 95.7(3) 1_545 5_666
La1 O3 O3 43.66(12) . 5_666
Ga2 O3 O3 111.0(3) 2_546 5_666
O3 O3 O3 139.21(17) 5_765 5_666
O3 O3 O3 102.2(4) 5_766 5_666
Ga3 O3 O3 100.1(3) 1_554 5_666
Nb O3 O3 78.5(3) 1_656 5_666
Ga1 O3 O3 78.5(3) 1_656 5_666
O2 O3 O3 58.7(3) 2_546 5_666
La1 O3 O3 68.3(3) 4_656 5_666
La1 O3 O3 76.93(7) 2_655 5_666
O1 O3 O3 129.7(3) 2_645 5_666
O2 O3 O3 124.6(4) 6_656 5_666
Ga3 O3 O3 145.0(4) 2_645 5_666
O2 O3 O3 89.1(3) 2_545 5_666
Ga2 O3 O3 33.27(5) 2_556 5_666
O2 O3 O3 167.6(5) 6_655 5_666
La1 O3 O3 154.6(3) 2_645 5_666
O1 O3 O3 98.0(3) 2_646 5_666
O2 O3 O3 117.5(3) 1_655 5_666
Ga2 O3 O3 81.9(3) 1_544 5_666
Ga3 O3 O3 76.3(2) 4_655 5_666
La1 O3 O3 151.9(2) 1_655 5_666
O1 O3 O3 59.96(18) 2_655 5_666
O3 O3 O3 65.3(2) 1_556 5_666
O3 O3 O3 114.7(2) 1_554 5_666
Ga3 O3 O3 123.2(2) 4_764 5_666
O2 O3 O3 85.9(2) 2_656 5_666
O2 O3 O3 26.9(2) 6_556 5_666
La1 O3 O3 22.19(13) 1_556 5_666
O2 O3 O3 122.7(3) 3_645 5_666
O1 O3 O3 30.71(9) 2_656 5_666
O1 O3 O3 159.0(4) 1_655 5_666
O2 O3 O3 109.07(18) 2_655 5_666
O2 O3 O3 63.0(3) 6 5_666
O2 O3 O3 52.08(13) 4_665 5_666
Ga2 O3 O3 130.4(3) 2_545 5_666
O3 O3 O3 26.6(3) 3_545 5_666
O3 O3 O3 72.1(3) 4_655 5_666
Ga2 O3 O3 140.2(4) 1_645 5_666
O2 O3 O3 138.1(4) 4_654 5_666
O2 O3 O3 28.10(17) . 5_666
O2 O3 O3 87.9(3) 3_654 5_666
La1 O3 O3 60.3(2) 2_545 5_666
La1 O3 O3 56.55(15) 2_656 5_666
O1 O3 O3 42.8(2) 1_556 5_666
O3 O3 O3 69.9(2) 4_766 5_666
O3 O3 O3 113.3(3) 4_764 5_666
O3 O3 O3 90.6(2) 3_646 5_666
O3 O3 O3 138.5(3) 3_644 5_666
O1 O3 O3 87.89(12) 1_665 5_666
La1 O3 O3 111.3(3) 2_646 5_666
O2 O3 O3 88.5(3) 4_656 5_666
O2 O3 O3 43.5(2) 3_656 5_666
La1 O3 O3 114.0(2) 1_545 5_666
La1 O3 O3 111.2(3) 1_656 5_666
O2 O3 O3 114.3(3) 1_544 5_666
O3 O3 O3 48.26(12) 5_665 5_666
O3 O3 O3 100.6(3) 5_655 5_666
Ga3 O3 O3 95.9(5) . 5_656
Nb O3 O3 147.7(4) 1_655 5_656
Ga1 O3 O3 147.7(4) 1_655 5_656
La1 O3 O3 55.54(17) 4_655 5_656
Ga3 O3 O3 76.1(3) 2_646 5_656
O3 O3 O3 107.1(2) 2_645 5_656
O3 O3 O3 61.5(3) 2_646 5_656
O3 O3 O3 154.9(3) 4_765 5_656
O3 O3 O3 112.9(5) 3_645 5_656
O2 O3 O3 54.7(3) 4_655 5_656
O2 O3 O3 115.4(4) 3_655 5_656
O2 O3 O3 62.1(4) 5_656 5_656
O1 O3 O3 58.5(3) . 5_656
O3 O3 O3 151.8(6) 6 5_656
O3 O3 O3 102.2(6) 6_556 5_656
O2 O3 O3 102.6(4) 5_655 5_656
Ga2 O3 O3 46.0(2) 1_545 5_656
Ga3 O3 O3 128.7(4) 4_765 5_656
O2 O3 O3 20.6(2) 1_545 5_656
La1 O3 O3 99.5(3) . 5_656
Ga2 O3 O3 31.05(6) 2_546 5_656
O3 O3 O3 139.21(17) 5_765 5_656
O3 O3 O3 102.2(4) 5_766 5_656
Ga3 O3 O3 125.5(3) 1_554 5_656
Nb O3 O3 83.8(3) 1_656 5_656
Ga1 O3 O3 83.8(3) 1_656 5_656
O2 O3 O3 22.2(2) 2_546 5_656
La1 O3 O3 36.99(18) 4_656 5_656
La1 O3 O3 157.7(3) 2_655 5_656
O1 O3 O3 61.8(2) 2_645 5_656
O2 O3 O3 75.2(3) 6_656 5_656
Ga3 O3 O3 110.13(19) 2_645 5_656
O2 O3 O3 66.9(2) 2_545 5_656
Ga2 O3 O3 113.4(3) 2_556 5_656
O2 O3 O3 102.2(2) 6_655 5_656
La1 O3 O3 73.82(6) 2_645 5_656
O1 O3 O3 30.22(10) 2_646 5_656
O2 O3 O3 135.8(4) 1_655 5_656
Ga2 O3 O3 86.4(2) 1_544 5_656
Ga3 O3 O3 12.93(9) 4_655 5_656
La1 O3 O3 120.1(2) 1_655 5_656
O1 O3 O3 130.5(3) 2_655 5_656
O3 O3 O3 65.3(2) 1_556 5_656
O3 O3 O3 114.7(2) 1_554 5_656
Ga3 O3 O3 149.9(3) 4_764 5_656
O2 O3 O3 128.5(4) 2_656 5_656
O2 O3 O3 55.0(2) 6_556 5_656
La1 O3 O3 73.5(2) 1_556 5_656
O2 O3 O3 41.79(16) 3_645 5_656
O1 O3 O3 101.5(3) 2_656 5_656
O1 O3 O3 91.78(14) 1_655 5_656
O2 O3 O3 169.3(3) 2_655 5_656
O2 O3 O3 81.2(2) 6 5_656
O2 O3 O3 132.4(3) 4_665 5_656
Ga2 O3 O3 76.16(14) 2_545 5_656
O3 O3 O3 81.7(2) 3_545 5_656
O3 O3 O3 31.9(2) 4_655 5_656
Ga2 O3 O3 83.94(17) 1_645 5_656
O2 O3 O3 95.0(2) 4_654 5_656
O2 O3 O3 107.0(3) . 5_656
O2 O3 O3 127.5(3) 3_654 5_656
La1 O3 O3 55.92(17) 2_545 5_656
La1 O3 O3 108.8(3) 2_656 5_656
O1 O3 O3 48.2(2) 1_556 5_656
O3 O3 O3 93.1(2) 4_766 5_656
O3 O3 O3 142.4(3) 4_764 5_656
O3 O3 O3 79.2(3) 3_646 5_656
O3 O3 O3 123.5(3) 3_644 5_656
O1 O3 O3 158.6(4) 1_665 5_656
La1 O3 O3 54.84(16) 2_646 5_656
O2 O3 O3 52.1(2) 4_656 5_656
O2 O3 O3 81.4(3) 3_656 5_656
La1 O3 O3 41.25(10) 1_545 5_656
La1 O3 O3 93.2(3) 1_656 5_656
O2 O3 O3 75.6(2) 1_544 5_656
O3 O3 O3 100.6(3) 5_665 5_656
O3 O3 O3 48.26(12) 5_655 5_656
O3 O3 O3 80.9(3) 5_666 5_656
Ga3 O3 O1 123.9(5) . 1_554
Nb O3 O1 80.7(4) 1_655 1_554
Ga1 O3 O1 80.7(4) 1_655 1_554
La1 O3 O1 43.6(3) 4_655 1_554
Ga3 O3 O1 140.0(3) 2_646 1_554
O3 O3 O1 46.4(4) 2_645 1_554
O3 O3 O1 155.63(12) 2_646 1_554
O3 O3 O1 110.4(2) 4_765 1_554
O3 O3 O1 119.27(18) 3_645 1_554
O2 O3 O1 104.2(4) 4_655 1_554
O2 O3 O1 87.5(4) 3_655 1_554
O2 O3 O1 111.1(5) 5_656 1_554
O1 O3 O1 53.4(3) . 1_554
O3 O3 O1 57.7(3) 6 1_554
O3 O3 O1 144.2(3) 6_556 1_554
O2 O3 O1 13.3(2) 5_655 1_554
Ga2 O3 O1 84.4(3) 1_545 1_554
Ga3 O3 O1 136.8(3) 4_765 1_554
O2 O3 O1 79.8(3) 1_545 1_554
La1 O3 O1 50.24(18) . 1_554
Ga2 O3 O1 101.0(2) 2_546 1_554
O3 O3 O1 81.0(4) 5_765 1_554
O3 O3 O1 160.5(4) 5_766 1_554
Ga3 O3 O1 31.76(11) 1_554 1_554
Nb O3 O1 169.1(3) 1_656 1_554
Ga1 O3 O1 169.1(3) 1_656 1_554
O2 O3 O1 94.4(3) 2_546 1_554
La1 O3 O1 127.3(2) 4_656 1_554
La1 O3 O1 83.5(2) 2_655 1_554
O1 O3 O1 62.0(3) 2_645 1_554
O2 O3 O1 139.6(3) 6_656 1_554
Ga3 O3 O1 56.34(16) 2_645 1_554
O2 O3 O1 27.4(2) 2_545 1_554
Ga2 O3 O1 94.8(2) 2_556 1_554
O2 O3 O1 77.2(3) 6_655 1_554
La1 O3 O1 88.76(18) 2_645 1_554
O1 O3 O1 118.7(3) 2_646 1_554
O2 O3 O1 123.2(3) 1_655 1_554
Ga2 O3 O1 10.91(11) 1_544 1_554
Ga3 O3 O1 82.20(18) 4_655 1_554
La1 O3 O1 105.0(2) 1_655 1_554
O1 O3 O1 60.1(3) 2_655 1_554
O3 O3 O1 149.78(14) 1_556 1_554
O3 O3 O1 30.22(14) 1_554 1_554
Ga3 O3 O1 70.04(17) 4_764 1_554
O2 O3 O1 135.7(3) 2_656 1_554
O2 O3 O1 85.9(3) 6_556 1_554
La1 O3 O1 111.8(2) 1_556 1_554
O2 O3 O1 92.7(2) 3_645 1_554
O1 O3 O1 111.5(3) 2_656 1_554
O1 O3 O1 109.5(3) 1_655 1_554
O2 O3 O1 82.1(2) 2_655 1_554
O2 O3 O1 29.1(2) 6 1_554
O2 O3 O1 93.4(2) 4_665 1_554
Ga2 O3 O1 48.70(11) 2_545 1_554
O3 O3 O1 64.16(12) 3_545 1_554
O3 O3 O1 64.16(12) 4_655 1_554
Ga2 O3 O1 127.1(2) 1_645 1_554
O2 O3 O1 47.80(18) 4_654 1_554
O2 O3 O1 78.8(2) . 1_554
O2 O3 O1 34.51(15) 3_654 1_554
La1 O3 O1 47.50(15) 2_545 1_554
La1 O3 O1 134.3(2) 2_656 1_554
O1 O3 O1 115.94(18) 1_556 1_554
O3 O3 O1 157.9(3) 4_766 1_554
O3 O3 O1 53.03(16) 4_764 1_554
O3 O3 O1 173.0(3) 3_646 1_554
O3 O3 O1 57.63(13) 3_644 1_554
O1 O3 O1 104.1(3) 1_665 1_554
La1 O3 O1 135.74(18) 2_646 1_554
O2 O3 O1 146.0(2) 4_656 1_554
O2 O3 O1 134.1(3) 3_656 1_554
La1 O3 O1 70.48(12) 1_545 1_554
La1 O3 O1 157.8(2) 1_656 1_554
O2 O3 O1 33.52(13) 1_544 1_554
O3 O3 O1 45.8(2) 5_665 1_554
O3 O3 O1 50.5(2) 5_655 1_554
O3 O3 O1 90.7(3) 5_666 1_554
O3 O3 O1 94.2(3) 5_656 1_554
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
La1 O3 2.404(10) 5_665
La1 O3 2.404(10) 3_545
La1 O2 2.446(14) 3_655
La1 O2 2.446(14) 5_655
La1 O1 2.554(7) .
La1 O1 2.554(7) 2_655
La1 O2 2.874(14) 6
La1 O2 2.874(14) .
La1 Ga2 3.381(2) 2_556
La1 Ga2 3.381(2) 1_544
La1 Ga1 3.4617(11) .
La1 Nb 3.4617(11) .
Ga1 O3 1.976(11) 4_665
Ga1 O3 1.976(11) 6_455
Ga1 O3 1.976(11) 1_455
Ga1 O3 1.976(11) 5_665
Ga1 O3 1.976(11) 2_545
Ga1 O3 1.976(11) 3_545
Ga1 La1 3.4617(11) 2
Ga1 La1 3.4618(11) 4
Ga1 O2 3.610(13) 2
Ga1 O2 3.610(13) 3
Ga1 O2 3.610(13) 5
Nb O3 1.976(11) 4_665
Nb O3 1.976(11) 6_455
Nb O3 1.976(11) 1_455
Nb O3 1.976(11) 5_665
Nb O3 1.976(11) 2_545
Nb O3 1.976(11) 3_545
Nb Ga3 3.1590(15) 4_665
Nb Ga3 3.1590(15) 1_454
Nb Ga3 3.1590(15) 1_455
Nb Ga3 3.1590(15) 4_664
Nb Ga3 3.1591(15) 2_545
Nb Ga3 3.1591(15) 2_546
Ga2 O1 1.80(2) 1_565
Ga2 O2 1.802(12) 6_566
Ga2 O2 1.802(12) 5_666
Ga2 O2 1.802(12) 2_556
Ga2 O1 3.26(2) 1_566
Ga2 La1 3.381(2) 1_566
Ga2 La1 3.381(2) 2_556
Ga2 La1 3.381(2) 4_666
Ga2 O3 3.472(11) 3
Ga2 O3 3.472(11) 1_565
Ga2 O3 3.472(11) 4_665
Ga2 La1 3.597(2) 1_565
Ga3 O3 1.799(12) .
Ga3 O3 1.799(12) 6_556
Ga3 O2 1.815(13) 3_655
Ga3 O2 1.815(13) 5_656
Ga3 O3 2.557(14) 4_765
Ga3 O3 2.557(14) 2_646
Ga3 Nb 3.1591(15) 1_656
Ga3 Nb 3.1591(15) 1_655
Ga3 O1 3.572(9) 2_656
Ga3 O1 3.572(9) .
Ga3 O3 3.629(11) 5_766
Ga3 O3 3.629(11) 3_645
O1 Ga2 1.80(2) 1_545
O1 La1 2.554(7) 2_545
O1 La1 2.554(7) 4_655
O1 O2 2.96(2) 6
O1 O2 2.96(2) 5_655
O1 O2 2.96(2) 2_545
O1 O2 3.05(2) 6_556
O1 O2 3.05(2) 5_656
O1 O2 3.05(2) 2_546
O1 O3 3.176(11) 3_545
O1 O3 3.176(11) 4_655
O1 O3 3.176(11) .
O1 Ga2 3.26(2) 1_544
O1 O2 3.563(13) 4
O1 O2 3.563(13) 3_655
O1 O2 3.563(13) 1_545
O1 Ga3 3.572(9) 2_546
O1 Ga3 3.572(9) 4_655
O1 O3 4.370(14) 5_665
O1 O3 4.370(14) 6_445
O1 O3 4.370(14) 2_645
O1 Ga3 4.651(15) 2_545
O1 Ga3 4.651(15) 1_554
O1 Ga3 4.651(15) 4_654
O1 O3 4.84(2) 5_666
O1 O3 4.84(2) 6_446
O1 O3 4.84(2) 2_646
O1 Nb 4.740(4) 1_655
O1 Ga1 4.740(4) 1_655
O1 Ga1 4.740(4) 1_545
O1 Nb 4.740(4) 1_545
O1 La1 4.824(17) 1_556
O1 La1 4.824(17) 2_546
O1 La1 4.824(17) 4_656
O1 O2 4.813(14) .
O1 O2 4.813(14) 3_545
O1 O2 4.813(14) 4_655
O1 Ga2 4.896(6) 2_556
O1 Ga2 4.896(6) 2_446
O1 Ga2 4.896(6) 2_546
O1 O3 4.882(17) 2_545
O1 O3 4.882(17) 6
O1 O3 4.882(17) 5_655
O1 O1 4.977(14) 2_655
O1 O1 4.977(14) 2_545
O1 O1 4.977(14) 2_645
O1 O1 5.0620 1_556
O1 O1 5.0620 1_554
O1 Ga3 5.293(6) 4_665
O1 Ga3 5.293(6) 1_445
O1 Ga3 5.293(6) 2_646
O1 O3 5.303(16) 2_546
O1 O3 5.303(16) 6_556
O1 O3 5.303(16) 5_656
O1 O3 5.377(13) 1_455
O1 O3 5.377(13) 4_765
O1 O3 5.377(13) 3_535
O1 O1 5.71(2) 2_656
O1 O1 5.71(2) 2_546
O1 O1 5.71(2) 2_646
O1 O2 5.56(2) 4_554
O1 O2 5.56(2) 3_654
O1 O2 5.56(2) 1_544
O1 O3 5.67(2) 3_544
O1 O3 5.67(2) 4_654
O1 O3 5.67(2) 1_554
O1 O3 5.801(10) 4_665
O1 O3 5.801(10) 1_445
O1 O3 5.801(10) 3_645
O1 La1 5.870(3) 4
O1 La1 5.870(3) 2_655
O1 La1 5.870(3) 1_545
O1 O2 6.225(12) 1_445
O1 O2 6.225(12) 4_665
O1 O2 6.225(12) 3_645
O1 O3 6.270(19) 3_546
O2 Ga2 1.802(12) 2_556
O2 Ga3 1.815(13) 4_665
O2 La1 2.446(14) 4_665
O2 O3 2.843(18) 3_545
O2 O2 2.814(19) 4_665
O2 O2 2.814(19) 3_655
O2 O2 2.76(3) 2_556
O2 O3 2.810(17) 4_665
O2 O1 2.96(2) 2_655
O2 O3 2.929(19) 5_666
O2 O1 3.05(2) 2_656
O2 O3 3.41(2) 5_665
O2 O1 3.563(13) 1_565
O2 O2 3.80(3) 2
O2 O3 3.873(17) 1_565
O2 La1 3.922(16) 4_666
O2 Ga3 4.165(13) 2_546
O2 O3 4.215(19) 2_656
O2 Ga3 4.205(13) 2_656
O2 La1 4.202(14) 1_556
O2 La1 4.318(12) 2_655
O2 Ga3 4.419(15) 4_664
O2 O3 4.371(19) 6_456
O2 La1 4.530(11) 2
O2 O3 4.565(19) 2_655
O2 Ga2 4.581(15) 2
O2 O2 4.488(13) 5_666
O2 O2 4.488(13) 5_656
O2 O3 4.710(17) 6_455
O2 O2 4.68(3) 6_556
O2 Nb 4.736(14) 1_556
O2 Ga1 4.736(14) 1_556
O2 O3 4.793(16) 1_455
O2 Ga2 4.878(13) 1_545
O2 Ga3 4.904(12) 1_455
O2 Ga3 4.938(14) 1_565
O2 O2 5.0620 1_554
O2 O2 5.0620 1_556
O2 O2 5.194(19) 5_665
O2 O2 5.194(19) 5_655
O2 O3 5.073(17) 2_546
O2 O3 5.132(16) 6_556
O2 Ga2 5.296(14) 1_554
O2 O2 5.36(3) 6
O2 O2 5.195(19) 6_566
O2 O2 5.195(19) 6_666
O2 O3 5.405(16) 4_765
O2 Nb 5.350(13) 1_665
O2 Ga1 5.350(13) 1_665
O2 La1 5.296(13) 2_656
O2 O3 5.368(19) 2_545
O2 O3 5.423(19) 6
O2 O3 5.330(17) 3_655
O2 La1 5.470(13) 2_556
O2 O3 5.473(18) 3_546
O2 O3 5.496(16) .
O2 O3 5.456(19) 4_666
O2 O2 5.60(2) 3
O2 O2 5.60(2) 4
O2 O1 5.56(2) 1_566
O2 O2 5.82(2) 6_565
O2 O2 5.82(2) 6_665
O2 Ga3 5.795(15) 2_545
O2 O2 5.792(9) 4_664
O2 O2 5.792(9) 4_666
O2 O2 5.792(9) 3_654
O2 O2 5.792(9) 3_656
O2 La1 5.914(13) 1_565
O2 O3 6.12(2) 3_544
O2 O2 6.04(2) 3_665
O2 O2 6.04(2) 4_565
O2 O3 6.106(18) 4_664
O2 O3 6.072(19) 1_566
O2 O1 6.225(12) 1_665
O3 Nb 1.976(11) 1_655
O3 Ga1 1.976(11) 1_655
O3 La1 2.404(10) 4_655
O3 Ga3 2.557(14) 2_646
O3 O3 2.66(3) 2_645
O3 O3 2.79(3) 2_646
O3 O3 2.675(18) 4_765
O3 O3 2.675(18) 3_645
O3 O2 2.843(18) 4_655
O3 O2 2.810(17) 3_655
O3 O2 2.929(19) 5_656
O3 O3 3.19(3) 6
O3 O3 3.29(2) 6_556
O3 O2 3.41(2) 5_655
O3 Ga2 3.472(11) 1_545
O3 Ga3 3.629(11) 4_765
O3 O2 3.874(17) 1_545
O3 Ga2 3.997(12) 2_546
O3 O3 3.91(2) 5_765
O3 O3 3.99(3) 5_766
O3 Ga3 3.963(14) 1_554
O3 Nb 4.130(14) 1_656
O3 Ga1 4.130(14) 1_656
O3 O2 4.215(19) 2_546
O3 La1 4.351(13) 4_656
O3 La1 4.233(11) 2_655
O3 O1 4.370(14) 2_645
O3 O2 4.372(19) 6_656
O3 Ga3 4.360(12) 2_645
O3 O2 4.565(19) 2_545
O3 Ga2 4.551(12) 2_556
O3 O2 4.710(17) 6_655
O3 La1 4.736(12) 2_645
O3 O1 4.84(2) 2_646
O3 O2 4.793(16) 1_655
O3 Ga2 4.798(14) 1_544
O3 Ga3 4.920(10) 4_655
O3 La1 4.895(12) 1_655
O3 O1 4.882(17) 2_655
O3 O3 5.0620 1_556
O3 O3 5.0620 1_554
O3 Ga3 5.063(12) 4_764
O3 O2 5.073(17) 2_656
O3 O2 5.132(16) 6_556
O3 La1 5.247(12) 1_556
O3 O2 5.405(16) 3_645
O3 O1 5.303(16) 2_656
O3 O1 5.377(13) 1_655
O3 O2 5.368(18) 2_655
O3 O2 5.423(19) 6
O3 O2 5.330(17) 4_665
O3 Ga2 5.473(12) 2_545
O3 O3 5.466(19) 3_545
O3 O3 5.466(19) 4_655
O3 Ga2 5.557(13) 1_645
O3 O2 5.473(18) 4_654
O3 O2 5.456(19) 3_654
O3 La1 5.615(11) 2_545
O3 La1 5.574(11) 2_656
O3 O1 5.67(2) 1_556
O3 O3 5.726(8) 4_766
O3 O3 5.726(8) 4_764
O3 O3 5.726(8) 3_646
O3 O3 5.726(8) 3_644
O3 O1 5.801(10) 1_665
O3 La1 5.965(14) 2_646
O3 O2 6.12(2) 4_656
O3 O2 6.106(18) 3_656
O3 La1 6.130(10) 1_545
O3 La1 6.092(14) 1_656
O3 O2 6.072(19) 1_544
O3 O3 6.163(19) 5_665
O3 O3 6.163(19) 5_655
O3 O3 6.219(17) 5_666
O3 O3 6.219(17) 5_656
O3 O1 6.270(19) 1_554
